Springer Series in Optical Sciences 189
Gerd Marowsky Editor
Planar Waveguides and other Confined Geometries Theory, T...

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

Springer Series in Optical Sciences 189

Gerd Marowsky Editor

Planar Waveguides and other Confined Geometries Theory, Technology, Production, and Novel Applications

Springer Series in Optical Sciences Volume 189 Founded by H. K. V. Lotsch Editor-in-Chief: W. T. Rhodes Editorial Board: Ali Adibi, Atlanta Toshimitsu Asakura, Sapporo Theodor W. Hänsch, Garching Ferenc Krausz, Garching Bo A. J. Monemar, Linköping Herbert Venghaus, Berlin Horst Weber, Berlin Harald Weinfurter, München

More information about this series at http://www.springer.com/series/624

Springer Series in Optical Sciences The Springer Series in Optical Sciences, under the leadership of Editor-in-Chief William T. Rhodes, Georgia Institute of Technology, USA, provides an expanding selection of research monographs in all major areas of optics: lasers and quantum optics, ultrafast phenomena, optical spectroscopy techniques, optoelectronics, quantum information, information optics, applied laser technology, industrial applications, and other topics of contemporary interest. With this broad coverage of topics, the series is of use to all research scientists and engineers who need up-to-date reference books. The editors encourage prospective authors to correspond with them in advance of submitting a manuscript. Submission of manuscripts should be made to the Editor-in-Chief or one of the Editors. See also www.springer.com/series/624 Editor-in-Chief William T. Rhodes School of Electrical and Computer Engineering Georgia Institute of Technology Atlanta, GA 30332-0250, USA e-mail: [email protected] Editorial Board Ali Adibi School of Electrical and Computer Engineering Georgia Institute of Technology Atlanta, GA 30332-0250, USA e-mail: [email protected] Toshimitsu Asakura Faculty of Engineering Hokkai-Gakuen University 1-1, Minami-26, Nishi 11, Chuo-ku Sapporo, Hokkaido 064-0926, Japan e-mail: [email protected] Theodor W. Hänsch Max-Planck-Institut für Quantenoptik Hans-Kopfermann-Straße 1 85748 Garching, Germany e-mail: [email protected] Ferenc Krausz Ludwig-Maximilians-Universität München Lehrstuhl für Experimentelle Physik Am Coulombwall 1 85748 Garching, Germany and Max-Planck-Institut für Quantenoptik Hans-Kopfermann-Straße 1 85748 Garching, Germany e-mail: [email protected]

Bo A. J. Monemar Department of Physics and Measurement Technology Materials Science Division Linköping University 58183 Linköping, Sweden e-mail: [email protected] Herbert Venghaus Fraunhofer Institut für Nachrichtentechnik Heinrich-Hertz-Institut Einsteinufer 37 10587 Berlin, Germany e-mail: [email protected] Horst Weber Optisches Institut Technische Universität Berlin Straße des 17. Juni 135 10623 Berlin, Germany e-mail: [email protected] Harald Weinfurter Sektion Physik Ludwig-Maximilians-Universität München Schellingstraße 4/III 80799 München, Germany e-mail: [email protected]

Gerd Marowsky Editor

Planar Waveguides and other Confined Geometries Theory, Technology, Production, and Novel Applications

123

Editor Gerd Marowsky Laser-Laboratorium Göttingen e.V. Göttingen, Germany

ISSN 0342-4111 ISSN 1556-1534 (electronic) ISBN 978-1-4939-1178-3 ISBN 978-1-4939-1179-0 (eBook) DOI 10.1007/978-1-4939-1179-0 Springer New York Heidelberg Dordrecht London Library of Congress Control Number: 2014948197 © Springer Science+Business Media New York 2015 This work is subject to copyright. All rights are reserved by the Publisher, whether the whole or part of the material is concerned, specifically the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microfilms or in any other physical way, and transmission or information storage and retrieval, electronic adaptation, computer software, or by similar or dissimilar methodology now known or hereafter developed. Exempted from this legal reservation are brief excerpts in connection with reviews or scholarly analysis or material supplied specifically for the purpose of being entered and executed on a computer system, for exclusive use by the purchaser of the work. Duplication of this publication or parts thereof is permitted only under the provisions of the Copyright Law of the Publisher’s location, in its current version, and permission for use must always be obtained from Springer. Permissions for use may be obtained through RightsLink at the Copyright Clearance Center. Violations are liable to prosecution under the respective Copyright Law. The use of general descriptive names, registered names, trademarks, service marks, etc. in this publication does not imply, even in the absence of a specific statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. While the advice and information in this book are believed to be true and accurate at the date of publication, neither the authors nor the editors nor the publisher can accept any legal responsibility for any errors or omissions that may be made. The publisher makes no warranty, express or implied, with respect to the material contained herein. Printed on acid-free paper Springer is part of Springer Science+Business Media (www.springer.com)

Preface

The aim of this book is to provide an actual collection of highlights in the technology, production, and novel applications of waveguides and other confined geometries, in particular optical fibers. It is well known that waveguide phenomena are nowadays a textbook subject and some energy is needed to prove that waveguide problems are still of great scientific and commercial interest. Any textbook approach should go back to the books by Theodor Tamir,1 who always considered waveguiding as the heart of any integrated optics. It is very interesting to study the details of his first book on this subject in as early as 1975. There he dated the beginning of integrated optics to the late 1960s and mentioned as primary applications signal processing and optical communications. It is striking to note that he did not mention at this time any analytical applications (lab-on-chip) or sensors. However, he already did mention the possible chances of novel optical phenomena opened by the concentration of high intensity fields in thin films and effects due to attendant enhancement of nonlinear and/or active properties of such films. It should be emphasized that at least two contributions in this book deal with nonlinear phenomena in waveguiding structures and potential applications. Contributions came from Europe, Canada, and Israel. The manuscripts have been arranged as follows: • Theoretical considerations for semi-infinite planar waveguides. Unusual, novel ways of efficient frequency conversion in structured fibers and nanoplasmonic waveguides • Five contributions on laser writing of waveguiding structures in various geometries and materials • Channel formation in cluster targets as an example of self-organization of waveguiding structures

1

Still available is the second corrected and updated edition of the book “Integrated Optics,” T. Tamir editor, Springer-Verlag, Berlin, Heidelberg, New York, 1979. v

vi

Preface

• An example of a novel application of Bragg grating technology using optical fibers for 3D shape sensing The contributions are beyond the normal textbook style, representing cuttingedge research results. A short preview/summary of some of the selected contributions is given below: In Chap. 1 of this book radiation emerging from an open-ended waveguide is studied in theory. The idealized case of a planar waveguide open to an infinite half space is considered. An iterative scheme is constructed in analogy to the exact solution of reflection from a step-potential in one-dimensional quantum mechanics and Fresnel reflection of electromagnetic radiation from a half space. For the planar waveguide, the first step in the iterative scheme is evaluated. This yields an approximation to the radiation pattern emerging from the waveguide, as well as the amplitude of the wave reflected back into the waveguide. Another selected example, Chap. 2, considers second-harmonic generation in a circular cylindrical waveguide with embedded periodically arranged tubelets of high nonlinear susceptibility. The configuration is similar to usual quasi-phasematched arrangements, but places the nonlinear polarization sheet at intensity peaks of the guided fundamental wave. This leads (yet only in theory) under optimized conditions to high conversion efficiencies and hence pump depletion has to be considered in the framework of mode-coupling theory. A major advance on femtosecond laser structuring inside optical fibers in Chap. 4 presents powerful new directions for inscribing optical, microfluidic, and mechanical structure devices in the fiber cladding that efficiently interconnect with the fiber core waveguide. This all-fiber platform circumvents tedious packaging and assembly process steps to enable highly functional photonic microsystems and labin-fiber devices to form into a compact and flexible optical fiber system that greatly enhances the value of today’s widely deployed fiber cables. The modification of optical properties of dielectrics has led to the fabrication of waveguides in a variety of glasses and crystals as shown in Chap. 6. UV photosensitivity of germanium-doped glass led to a new technology of fiber Bragg gratings; now femtosecond lasers have allowed yet another aspect of laser-material interaction to be exploited, bordering in the twilight zone between optical damage and plasma formation. This not fully understood process has also led to the production of 3D waveguides and holds the promise of easing the process of waveguide fabrication in all sorts of transparent media, provided the optical loss can be tamed. At the other end of the spectrum, the brute force of carbon dioxide lasers has also been used to cut glass to form delicate, yet complex, low-loss optical devices for fast prototyping and integration. These technologies are reviewed by examining the induction of refractive index changes and waveguides in several different materials. An unusual case of waveguide generation is discussed in Chap. 9: channel formation due to focusing of high-power laser radiation in a self-generated rare gas plasma. The discovery of a stable highly nonlinear mechanism that can compress power to a density exceeding thermonuclear values led to a new era of power

Preface

vii

compression. The associated steps, increasing by a factor of 1010 in power density, mark different stages of technological breakthroughs. Chapter 10 discusses a novel method for direct femtosecond laser-based writing of Bragg gratings and micro-waveguides not only inside the core but also in the cladding of a standard telecom fiber. This enables an optical 3D shape monitoring system using just a single one-core optical fiber. For a 1.5 m long fiber, the tip position can be tracked with an accuracy of less than 1 mm for the x,y,z-coordinates. Applications of this new technology range from medical tracking systems to longterm inspection of boreholes and drilling wells in the oil and gas industry. Göttingen, Germany March 2014

Gerd Marowsky

Acknowledgments

The editor wishes to thank Jaydev Jethwa (Max Planck Institute for Biophysical Chemistry), Charles K. Rhodes (University of Illinois at Chicago), and Anke Düker (Laser-Laboratorium Göttingen) for critical reading of part of the manuscripts and many practical hints and fruitful discussions. Valuable coordination and constant technical assistance of Dirk Born, Jutta Steckel, and Tatjana Kasten (all from LaserLaboratory Göttingen) is gratefully acknowledged. The editor owes particular thanks to Ho Ying Fan from Springer USA in New York for his very engaged and continuous interest in timely finalization of the book-project. The editor took the liberty to make appropriate changes in some of the manuscripts for better readability of the book.

ix

Contents

1

2

Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide .. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . B.U. Felderhof Optimizing Second-Harmonic Generation in a Circular Cylindrical Waveguide with Embedded Periodically Arranged Tubelets of Nonlinear Susceptibility . . . . . .. . . . . . . . . . . . . . . . . . . . B.U. Felderhof, G. Marowsky, and J. Troe

3

Nanoplasmonic Metal –Insulator –Metal Waveguides . . . . . . . . . . . . . . . . . Moshik Cohen, Reuven Shavit, and Zeev Zalevsky

4

Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber Cladding . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . Jason R. Grenier, Moez Haque, Luís A. Fernandes, Kenneth K.C. Lee, and Peter R. Herman

1

21 45

67

5

Fabrication of Channel Waveguides in Chalcogenide Glass Films by a Focused Laser Beam . . . . . . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . 111 K. Shemesh, Yu. Kaganovskii, and M. Rosenbluh

6

Laser Processed Photonic Devices . . . . . . . . . . . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . 129 Jerome Lapointe and Raman Kashyap

7

Advanced Coupling Technologies for Planar and Strip Waveguides .. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . 169 Thomas Fricke-Begemann and Jürgen Ihlemann

8

Nonlinear Light Propagation in Laser-Written Waveguide Arrays ... . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . 185 Matthias Heinrich, Stefan Nolte, and Alexander Szameit

xi

xii

9

Contents

Stable Power Compression with Efficient Relativistic UV Channel Formation in Cluster Targets . . . . . . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . 207 Alex B. Borisov and Charles K. Rhodes

10 Fiber-Optical 3D Shape Sensing . . . . . . . . . . . . . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . 227 Christian Waltermann, Jan Koch, Martin Angelmahr, Jörg Burgmeier, Markus Thiel, and Wolfgang Schade 11 Polarized Fiber Lasers and Amplifiers . . . . . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . 251 Oliver Fitzau Index . . . . . . . . .. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . 265

Chapter 1

Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide B.U. Felderhof

PACS numbers: 41.20.Jb, 42.25.Bs, 42.79.Gn, 43.20.+g

1.1 Introduction In a classic paper Levine and Schwinger [1] studied the radiation of sound from an unflanged circular pipe. Later they extended their theory to electromagnetic radiation [2]. Their work constituted the first major advance in the theory of diffraction after Sommerfeld’s exact solution of the problem of plane wave diffraction by an ideally conducting half plane [3]. In the theory of diffraction of sound, microwaves, or light, the radiation is assumed to propagate in uniform space with reflection by rigid objects or idealized boundaries. For a lucid introduction to the theory of diffraction we refer to Sommerfeld’s lecture notes [4]. The early theory of diffraction was reviewed by Bouwkamp [5]. Later developments are discussed by Born and Wolf [6]. A brief review of the principles and applications of open-ended waveguides with idealized walls was presented by Gardiol [7]. The invention of the dielectric waveguide by Hondros and Debye [8] has led to the development of optical fibers and the subsequent advances in telecommunication. In the theoretical determination of running wave solutions to Maxwell’s equations in a spatially inhomogeneous medium the radiation is assumed to propagate in a guiding structure of infinite length. The problem of emergence of radiation from a semi-infinite waveguide into a half-space is of obvious technical interest. In the case of sound the analysis is based on the exact solution of Levine and Schwinger [1,9–12]. For a dielectric waveguide the observation of the emerging radiation can be used as a tool to study the nature of the driving incident wave [13].

B.U. Felderhof () Institut für Theorie der Statistischen Physik, RWTH Aachen University, Templergraben 55, 52056 Aachen, Germany e-mail: [email protected] G. Marowsky (ed.), Planar Waveguides and other Confined Geometries: Theory, Technology, Production, and Novel Applications, Springer Series in Optical Sciences 189, DOI 10.1007/978-1-4939-1179-0__1, © Springer ScienceCBusiness Media New York 2015

1

2

B.U. Felderhof

It is advantageous to simplify the theoretical analysis by the use of planar symmetry. The theory of Levine and Schwinger was extended to planar geometry by Heins [14,15]. In the following we study radiation emerging from a semi-infinite planar dielectric waveguide. As an intermediate step the wave function in the exit plane must be calculated. In this case the integral equation technique of Schwinger [16] cannot be implemented, because of the complicated nature of the integral kernel. We evaluate the emitted radiation and the coefficients of reflection back into the waveguide approximately in a first step of an iterative scheme. We show in two appendices that the iterative scheme converges to the exact solution in the related problems of reflection by a step potential in one-dimensional quantum mechanics and of Fresnel reflection of an electromagnetic plane wave by a half-space. For the planar dielectric waveguide it does not seem practically possible to go beyond the first step of the iterative scheme. In a numerical example we study a planar waveguide consisting of a slab of uniform dielectric constant, bounded on both sides by a medium with a smaller dielectric constant [17–19]. In the case studied the first step of the iterative scheme leads to a modification of the wave function at the exit plane which is relatively small in comparison with the incident wave. Hence we may expect that the calculation provides a reasonable approximation to the exact solution.

1.2 Planar Open End Geometry We employ Cartesian coordinates .x; y; z/ and consider a planar waveguide in the half-space z < 0 with stratified dielectric constant ".x/ and uniform magnetic permeability 1 . In the half-space z > 0 the dielectric constant is uniform with value "0 and the magnetic permeability is 1 . We consider solutions of Maxwell’s equations which do not depend on the coordinate y and depend on time t through a factor exp.i !t/. Waves traveling to the right in the left half-space will be partly reflected at the plane z D 0 and partly transmitted into the right halfspace. The solutions of Maxwell’s equations may be decomposed according to two polarizations. For TE polarization the components Ex ; Ez , and Hy vanish, and the equations may be combined into the single equation @2 Ey @2 Ey C C "1 ! 2 Ey D 0 2 @x @z2

.TE/:

(1.1)

We have used SI units. For TM polarization the components Ey ; Hx , and Hz vanish, and the equations may be combined into the single equation @2 Hy @2 Hy 1 d " @Hy C "1 ! 2 Hy D 0 C 2 2 @x @z " dx @x

.TM/:

(1.2)

1 Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide

3

Fig. 1.1 Geometry of the planar waveguide

x ⑀1

d

⑀2

0

⑀' z

⑀2 ⑀1

d

⑀'

y

We assume that the profile ".x/ is symmetric, ".x/ D ".x/, and has a simple form with ".x/ increasing monotonically for x < 0 from value "1 to a maximum value "2 at x D 0. An example of the geometry under consideration is shown in Fig. 1.1. In the example the dielectric constant in the left half-space equals a constant "2 for d < x < d and a constant "1 < "2 for x < d and x > d . For definiteness we consider only TM polarization. It is convenient to denote the magnetic field component Hy .x; z/ for z < 0 as u.x; z/ and for z > 0 as v.x; z/. The continuity conditions at z D 0 are u.x; 0/ D v.x; 0C/;

ˇ ˇ 1 @v.x; z/ ˇˇ 1 @u.x; z/ ˇˇ D 0 : ".x/ @z ˇzD0 " @z ˇzD0C

(1.3)

We consider a solution u0n .x; z/ of Eq. (1.2) given by a guided mode solution u0n .x; z/ D

n .x/ exp.ipn z/;

(1.4)

where n .x/ is the guided mode wave function and pn the guided mode wavenumber. We assume pn > 0, so that the wave u0n .x; z/ exp.i !t/ is traveling to the right. The complete solution takes the form un .x; z/ D u0n .x; z/ C u1n .x; z/;

vn .x; z/;

(1.5)

where u1n .x; z/ and vn .x; z/ must be determined such that the continuity conditions Eq. (1.3) are satisfied. The function u1n .x; z/ describes the reflected wave, and vn .x; z/ describes the wave radiated into the right-hand half-space. Since the right-hand half-space is uniform the solution vn .x; z/ takes a simple form and can be expressed as Z 1 p Fn .q/ exp.i qx C i "0 1 ! 2 q 2 z/ dq: (1.6) vn .x; z/ D 1

p p The contribution from the interval "0 1 j!j < q < p"0 1 j!j corresponds to waves traveling to the right; the contribution from jqj > "0 1 j!j corresponds to evanescent waves.

4

B.U. Felderhof

Similarly the solution u1n .x; z/ in the left half-space can be expressed as nX m 1

u1n .x; z/ D

Z Rmn

m .x/ exp.ipm z/

1

C

Rn .q/ .q; x/ exp.i

p

"1 1 ! 2 q 2 z/ dq;

0

mD0

(1.7)

where the sum corresponds to guided waves traveling to the left, with nm the number of such guided modes possible at the given frequency !, and the integral corresponds to waves radiating towards the left. We require that the mode solutions are normalized such that [20] Z Z

1

1 1 1

m .x/ n .x/

".x/

Z dx D ımn ;

1

m .x/

.q; x/ dx D 0; ".x/

1

.q; x/ .q 0 ; x/ dx D ı.q q 0 /: ".x/

(1.8)

The guided mode solutions f m .x/g can be taken to be real. Orthogonality follows from Eq. (1.2). We show in the next section how the functions u1n .x; z/ and vn .x; z/ may in principle be evaluated from an iterative scheme. The coefficients fRmn g and the amplitude function Rn .q/ also follow from the scheme.

1.3 Iterative Scheme The iterative scheme is based on successive approximations to the scattering solution. Thus we write the exact solution as infinite sums un .x; z/ D

1 X

vn .x; z/ D

/ u.j n .x; z/;

j D0

1 X

/ v.j n .x; z/;

(1.9)

j D0

.j C1/

.j C1/

.x; z/; vn .x; z/ determined from the previous with the terms un .j / .j / .0/ un .x; z/; vn .x; z/. In zeroth approximation we identify un .x; z/ with the incident wave, u.0/ n .x; z/ D

n .x/ exp.ipn z/:

(1.10)

.0/

The corresponding vn .x; z/ will be determined by continuity at the exit plane z D 0. .0/ From Eq. (1.10) we have un .x; 0/ D n .x/. This has the Fourier transform n .q/ D

1 2

Z

1 1

n .x/ exp.i qx/

dx:

(1.11)

1 Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide

5

Using continuity of the wave function at z D 0 and the expression Eq. (1.6) we find correspondingly Z v.0/ n .x; z/ D

1 1

n .q/ exp.i qx C i

p "0 1 ! 2 q 2 z/ dq;

(1.12)

.0/

so that in zeroth approximation Fn .q/ D n .q/. Clearly the zeroth approximation does not satisfy the second continuity equation in Eq. (1.3), and we must take care of this in the next approximation. For the difference of terms in Eq. (1.3) we find n.0/ .x/ D

i pn ".x/

n .x/ C

i "0

Z

p "0 1 ! 2 q 2 n .q/ exp.i qx/ dq:

1

1

(1.13)

.0/

By symmetry n .x/ is symmetric in x for n even and antisymmetric in x for n odd. .1/ The next approximation un .x; z/ can be found by comparison with the solution of the problem where the profile ".x/ extends over all space and radiation is generated by a source ".x/.x/ı.z/ with a Sommerfeld radiation condition, so that radiation is emitted to the right for z > 0 and to the left for z < 0. This antenna solution can be expressed as Z uA .x; z/ D

1

K.x; x 0 ; z/.x 0 / dx 0 ;

(1.14)

1

with kernel K.x; x 0 ; z/. The latter can be calculated from the Fourier decomposition 1 ı.z/ D 2

Z

1

e ipz dp;

(1.15)

1

in terms of the integral K.x; x 0 ; z/ D

1 2

Z

1

G.x; x 0 ; p/ e ipz dp;

(1.16)

1

with the prescription that the path of integration in the complex p plane runs just above the negative real axis and just below the positive real axis. The Green function G.x; x 0 ; p/ can be found from the solution of the one-dimensional wave equation, d 2 G 1 d " dG C ."1 ! 2 p 2 /G D ".x/ı.x x 0 /: dx 2 " dx dx

(1.17)

The solution takes the form [20] G.x; x 0 ; p/ D

p

".x/

f2 .x< ; p/f3 .x> ; p/ p 0 ".x /; .f2 ; f3 ; p/

(1.18)

6

B.U. Felderhof

where x< .x> / is the smaller (larger) of x and x 0 and the remaining quantities will be specified in the next section. The Green function satisfies the symmetry properties G.x; x 0 ; p/ D G.x; x 0 ; p/;

G.x; x 0 ; p/ D G.x; x 0 ; p/;

(1.19)

and the reciprocity relation G.x; x 0 ; p/ D G.x 0 ; x; p/:

(1.20)

Consequently the kernel K.x; x 0 ; z/ has the properties K.x; x 0 ; z/ D K.x; x 0 ; z/;

K.x; x 0 ; z/ D K.x; x 0 ; z/;

(1.21)

as well as K.x; x 0 ; z/ D K.x 0 ; x; z/:

(1.22)

.1/

The function un .x; z/ is now identified as Z u.1/ n .x; z/ D

1 1

K.x; x 0 ; z/n.0/ .x 0 / dx 0 :

(1.23)

The minus sign is needed to provide near cancellation of the source density between .0/ .1/ the zeroth and first order solutions, n .x/ C n .x/ 0. We find the first order .1/ function Fn .q/ by Fourier transform from the value at z D 0 in the form Fn.1/ .q/

1 D 2

Z

1

1

i qx u.1/ dx: n .x; 0/e

(1.24)

.1/

The corresponding function vn .x; z/ is found from Eq. (1.6). The first order source .1/ density n .x/ is found to be n.1/ .x/

ˇ Z 1p .1/ 1 @un .x; z/ ˇˇ i D C "0 1 ! 2 q 2 Fn.1/ .q/ exp.i qx/ dq: ˇ ".x/ @z "0 1 zD0 (1.25) .1/

In principle the first order function un .x; 0/ in the exit plane z D 0 may be regarded as the result of a linear operator R.1/ acting on the state n .x/ given by the incident wave. The iterated solution then corresponds to the action with the operator R D R.1/ .I R.1/ /1 , where I is the identity operator. In order j of the .j / geometric series corresponding to the operator R the wave functions u1n .x; z/ and .j / vn .x; z/ in the left and right half-space can be found by completing the function .j / .j / u1n .x; 0/ D v1n .x; 0/ in the exit plane by left and right running waves, respectively.

1 Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide

7

Assuming that the scheme has been extended to all orders we obtain the solutions .0/ u1n .x; z/ D un .x; z/ un .x; z/ and vn .x; z/ given by Eq. (1.9). By construction at .j / .j / each step un .x; 0/ D vn .x; 0/. In the limit we must have 1 X

n.j / .x/ D 0;

(1.26)

j D0

so that the continuity conditions Eq. (1.3) are exactly satisfied. In Appendix 1 we show how the iterative scheme reproduces the exact solution for reflection from a step potential in one-dimensional quantum mechanics. In Appendix 2 we show the same for Fresnel reflection. In the integral in Eq. (1.23) it is convenient to perform the integral over p first, .0/ since n .x 0 / does not depend on p. The pole at pm , arising from a zero of the denominator in Eq. (1.18), yields the first order reflection coefficient [20] Z 1 i .1/ .0/ Rmn D (1.27) m .x/n .x/ dx: 2pm 1 The second term in Eq. (1.2) corresponds to the remainder of the integral, after .1/ subtraction of the simple pole contributions. The function Rn .q/ will be discussed .1/ in the next section. In the calculation of Fn .q/ from Eq. (1.24) we find Fn.1/ .q/ D

nX m 1

.1/ Rmn m .q/ C ıFn.1/ .q/;

(1.28)

mD0 .1/

where ıFn .q/ is the contribution from the remainder of the integral over p, after subtraction of the simple pole contributions. Formally, in the complete solution Eq. (1.2), the reflection coefficients Rmn and the amplitude function Rn .q/ are found as Rmn D .

m ; u1n .0//;

Rn .q/ D . .q/; u1n .0//:

(1.29)

with the scalar product as given by Eq. (1.8). The first step of the iterative scheme yields .1/ D. Rmn

.1/ m ; un .0//;

Rn.1/ .q/ D . .q/; u.1/ n .0//:

(1.30)

The continuum states .q/ can be discretized in the usual way, so that the expressions in Eq. (1.30) can be regarded as elements of a matrix R.1/ . As indicated above, the iterative scheme corresponds to a geometric series, so that the reflection coefficients in Eq. (1.29) can be found as elements of the matrix R D .I R.1/ /1 I; where I is the identity matrix.

(1.31)

8

B.U. Felderhof

Finally the function Fn .q/ can be found from the corresponding state un .0/ as in Eq. (1.24). The function Fn .q/ can be related to the radiation scattered into the right half-space. The scattering angle is related to the component q by p sin D q= "0 1 ! 2 :

(1.32)

Defining the scattering cross section n ./ by n ./ sin d D jFn .q/j2 qdq;

(1.33)

we find the relation n ./ D

p p "0 1 ! 2 "0 1 ! 2 q 2 jFn .q/j2 :

(1.34)

In lowest approximation the cross section is proportional to the absolute square of the Fourier transform of the guided mode n .x/. To higher order the cross section is affected by the reflection into other modes.

1.4 Continuous Spectrum .1/

The calculation of the function Rn .q/ corresponding to the contribution from the continuous spectrum requires a separate discussion. The wave equation (1.17) is related to a quantum mechanical Schrödinger equation for a particle in a potential. The bound states of the Schrödinger problem correspond to the guided modes, and the scattering states correspond to a continuous spectrum of radiation modes. The eigenstates of the Hamilton operator of the Schrödinger problem satisfy a completeness relation which can be usefully employed in the waveguide problem. Explicitly the homogeneous one-dimensional Schrödinger equation correspondp ing to Eq. (1.17) via the relation .x/ D ".x/f .x/ reads [20] d 2f V .x/f D p 2 f; dx 2

(1.35)

where the function V .x/ is given by V .x/ D "1 ! 2 C

p d2 1 " 2p : dx "

(1.36)

By comparison with the quantum mechanical Schrödinger equation we see that U.x/ D N1 C V .x/;

(1.37)

where N1 D "1 1 ! 2 may be identified as the potential. The bound state energies correspond to fN1 pn2 g.

1 Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide

9

It is convenient to assume that the dielectric profile ".x/ equals "1 for x < x1 and x > x1 , so that the potential U.x/ vanishes for jxj > x1 . We define three independent solutions of the Schrödinger equation (1.35) with specified behavior for jxj > x1 . The behavior of the function f1 .x; p/ is specified as f1 .x; p/ D e i q1 x ; f1 .x; p/ D W11 e

for x < x1 ;

i q1 x

C W21 e i q1 x ;

with wavenumber q1 D

for x > x1 ;

p N1 p 2 :

(1.38)

(1.39)

The behavior of the function f2 .x; p/ is specified as f2 .x; p/ D e i q1 x ;

for x < x1 ;

f2 .x; p/ D W12 e i q1 x C W22 e i q1 x ;

for x > x1 :

(1.40)

Similarly, the behavior of the function f3 .x; p/ is specified as f3 .x; p/ D W22 e i q1 x C W12 e i q1 x ; f3 .x; p/ D e

i q1 x

;

for x < x1 ;

for x > x1 :

(1.41)

The coefficients W12 and W22 are elements of the transfer matrix of the planar structure, WD

W11 W12 W21 W22

1 D 0 T

T T 0 RR0 R0 R 1

:

(1.42)

Because of the assumed symmetry of the dielectric profile we have in the present case R0 D R and T 0 D T , so that W21 D W12 . Moreover W11 W22 C W122 D 1:

(1.43)

The functions f2 .x; p/ and f3 .x; p/ were used in the calculation of the Green function in Eq. (1.18). The denominator in that expression is the Wronskian of f2 ; f3 given by .f2 ; f3 / D 2i q1 W22 .p; !/:

(1.44)

From the solution of the inhomogeneous Schrödinger equation it follows that the completeness relation of the normal mode solutions may be expressed as [21] p p Z 1 nX m 1 0 f2 .x; N1 q 2 /f2 .x 0 ; N1 q 2 / 1 n .x/ n .x / p C p dq D ı.xx 0 /: 0/ 2 ; !/j2 2 ".x/".x jW . N q 1 22 1 nD0 (1.45)

10

B.U. Felderhof

Correspondingly the Green function may be decomposed as G.x; x 0 ; p/ D

nX m 1 nD0

n .x/ n .x pn2 p 2

0

/

1 p C ".x/".x 0 / 2

Z

p N1 q 2 /f2 .x 0 ; N1 q 2 / p dq: .N1 q 2 p 2 / jW22 . N1 q 2 ; !/j2 (1.46)

1

f2 .x;

1

p

Hence we find for the antenna kernel K.x; x 0 ; z/ from Eq. (1.16) by use of the integration prescription 0

K.x; x ; z/ D

nX m 1 nD0

i 2pn

i p ".x/".x 0 / 4

Z

1 0

n .x/ n .x

0

/ e ipn jzj

p p f2 .x; N1 q 2 /f2 .x 0 ; N1 q 2 / i pN1 q 2 jzj e dq: p p N1 q 2 jW22 . N1 q 2 ; !/j2 (1.47)

The first order left-hand wave function is therefore found from Eq. (1.23) as u.1/ n .x; z/ D

nX m 1 mD0

i . 2pm

.0/ m ; "n / m .x/

e ipm z

p p Z 1 .0/ . "f2 . N1 q 2 /; "n / i p 0 p C ".x/".x / p 4 N1 q 2 jW22 . N1 q 2 ; !/j2 0 p p 2 f2 .x; N1 q 2 /e i N1 q z dq; (1.48) with scalar product as given by Eq. (1.8). The wave function is the sum of guided modes running to the left and of radiation into the left-hand half-space. The first term agrees with the reflection coefficient given by Eq. (1.27). By symmetry the .0/ matrix element . m ; "n / vanishes unless m and n are both even or both odd. The .1/ integral provides an alternative expression for the remainder ıun .x; z/. From Eq. (1.45) we may identify p p 1 .q; x/ D p p ".x/f2 .x; N1 q 2 /: 2jW22 . N1 q 2 ; !/j

(1.49)

.1/

With this definition the function Rn .q/ is given by p p .0/ . "f2 . N1 q 2 /; "n / i .1/ p p Rn .q/ D p 2 2 N1 q 2 jW22 . N1 q 2 ; !/j i D p . .q/; "n.0/ /: 2 N1 q 2

(1.50)

1 Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide

11

The second line has the same structure as Eq. (1.27). Although the decomposition .1/ in Eq. (1.48) is of theoretical interest, the calculation of the function un .x; z/ is performed more conveniently as indicated in Eq. (1.23), with the integral over p performed first.

1.5 Numerical Example We demonstrate the effectiveness of the scheme on a numerical example. We consider a flat dielectric profile defined by ".x/ D "2 for d < x < d and ".x/ D "1 for jxj > d with values "2 D 2:25"0 and "1 D 2:13"0 . In the right half-space we put "0 D "0 , and we put 1 D 0 everywhere. The geometry is shown in Fig. 1.1. By symmetry the guided modes in infinite space are either symmetric or antisymmetric in x. The explicit expressions for the mode wave functions can be found by the transfer matrix method [20]. At each of the two discontinuities the coefficients of the plane waves exp.i qi x/ and exp.i qi x/ are transformed into coefficients of the plane waves exp.i qj x/ and exp.i qj x/ by a matrix involving Fresnel coefficients given by tij D

2"j qi ; "i qj C "j qi

rij D

"j qi "i qj ; "i qj C "j qi

.i; j / D .1; 2/;

(1.51)

with wavenumbers qj D

q

kj2 p 2 ;

kj D

p "j 1 !:

(1.52)

The wavenumbers pn .!/ of the guided modes are found as zeros of the transfer matrix element W22 .p; !/, which takes the explicit form "2 q 2 C "22 q12 W22 .p; !/ D e 2i q1 d cos 2q2 d i 1 2 sin 2q2 d : 2"1 "2 q1 q2

(1.53)

The guided mode wave functions f n .x/g, their Fourier transforms fn .q/g, and the Green function G.x; x 0 ; p/ can be found in explicit form. In Fig. 1.2 we show the ratio of wavenumbers pn .k/=k as a function of kd for the first few guided modes, p with k D !=c, where c D 1= "0 0 is the velocity of light in vacuum. We choose the frequency corresponding to kd D 12. In that case there are two symmetric modes, denoted as TM0 and TM2, and one antisymmetric mode, denoted as TM1. We assume the incident wave to be symmetric in x. Then it is not necessary to consider the antisymmetric mode. In Fig. 1.3 we show the corresponding normalized wave functions 0 .x/ and 2 .x/. In Fig. 1.4 we show their Fourier transforms 0 .q/ and 2 .q/. The wavenumbers at kd D 12 are

12

B.U. Felderhof

1.5

n=0

pn(k)/k

1.49

n=1

n=2

1.48 1.47 1.46 0

5

10

15 kd

20

25

30

Fig. 1.2 Plot of the reduced wavenumber pn .k/=k of the lowest order guided waves for n D 0; 1; 2, as functions of kd for values of the dielectric constant given in the text

1.5

2(x)

1

0(x),

Fig. 1.3 Plot of the wave functions 0 .x/ and 2 .x/ of the guided modes with n D 0 (no nodes) and n D 2 (two nodes) as functions of x=d

0.5 0 −0.5 −1 −1.5 −3

−2

−1

0 x/d

1

2

3

p0 D 17:955=d and p2 D 17:624=d . The edge of the continuum is given by k1 d D 17:513, and the corresponding value for "2 is k2 d D 18. .0/ In Fig. 1.5 we show the source density in .x/ of the zeroth approximation for n D 0; 2 as a function of x, as given by Eq. (1.13). The coefficients of the simple pole contributions can be calculated from Eq. (1.27). We find numerically for the .1/ discrete part Rd of the matrix R.1/ .1/ Rd

.1/

D

.1/

R00 R02 .1/ .1/ R20 R22

!

D

0:2477 0:0004 : 0:0013 0:2312

(1.54)

For the first correction to the emitted radiation we need to calculate the function .1/ un .x; 0/. The kernel K.x; x 0 ; 0/ in Eq. (1.23) can be evaluated numerically. On account of the symmetry in ˙p it is sufficient to calculate twice the integral along the positive real p axis, with path of integration just below the axis. In the numerical integration over p in Eq. (1.16) the simple poles at fpm g cause problems.

1 Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide

13

0.3 f0(q),f2(q)

0.2 0.1 0 −0.1 −0.2 −0.3 −10

−5

0 qd

5

10

Fig. 1.4 Plot of the Fourier transform 0 .q/ and 2 .q/ of the wave functions of the guided modes with n D 0 (solid curve) and n D 2 (dashed curve) as functions of qd

6 4 −ir0(0)(x), −ir2(0)(x)

Fig. 1.5 Plot of the source .0/ densities i0 .x/ and .0/ i2 .x/, as given by Eq. (1.13), as functions of x=d

2 0 −2 −4 −2

−1

0

1

2

x/d

In order to avoid the simple poles we therefore integrate instead along a contour consisting of the line from 0 to k1 just below the axis, a semicircle in the lower half of the complex p plane centered at .k1 C k2 /=2 and of radius .k2 k1 /=2, and the line just below the real axis from k2 to C1. In Fig. 1.6 we plot as an example the real part of K.x; 0; 0/ as a function of x. The plot of the imaginary part is similar. .1/ In Fig. 1.7 we show the imaginary part of the function u0 .x; 0/, as calculated from Eq. (1.23). This is nearly identical with the contribution from the simple poles at p0 and p2 , which is also shown in Fig. 1.7. In Fig. 1.8 we show the real part of .1/ the function u0 .x; 0/. Here the simple poles do not contribute. The magnitude of .1/ the wave function at the origin u0 .0; 0/ D 0:149 0:005i may be compared with .0/ that of the zeroth approximation u0 .0; 0/ D 1:346. This shows that the first order correction is an order of magnitude smaller than the zeroth order approximation. .0/ .1/ Consequently we may expect that the sum u0 .x; 0/ C u0 .x; 0/ provides a close approximation to the exact value.

14

B.U. Felderhof

Fig. 1.6 Plot of the real part of the kernel K.x; 0; 0/, as given by Eq. (1.16), as a function of x=d

0.3

Re K(x,0,0)

0.2 0.1 0 −0.1 −0.2 −0.3 −3

−2

−1

0

1

2

3

x/d 0.35 0.3 −Re u(1) 0 (x,0)

Fig. 1.7 Plot of the real part of the first order wave .1/ function u0 .x; 0/ at the exit plane as a function of x=d (solid curve), compared with the contribution of the two guided waves .1/ .1/ R00 u0 .x/ C R20 u2 .x/ (dashed curve)

0.25 0.2 0.15 0.1 0.05 0

−2

−1

.0/

0 x/d

1

2

.1/

In Fig. 1.9 we show the absolute value jF0 .q/ C F0 .q/j of the Fourier trans.0/ .1/ form of the sum u0 .x; 0/ C u0 .x; 0/ and compare with the zeroth approximation .0/ jF0 .q/j D j0 .q/j. By use of Eq. (1.34) the absolute square of the transform yields the angular distribution of radiation emitted into the right-hand half-space.

1.6 Discussion In the above we have employed an iterative scheme inspired by the exact solution of two fundamental scattering problems, reflection by a step potential in onedimensional quantum mechanics, shown in Appendix 1, and Fresnel reflection of electromagnetic radiation by a half-space, shown in Appendix 2. For the planar dielectric waveguide we have implemented only the first step of the iterative scheme. In the numerical example shown in Sect. 1.5 even this first step leads to interesting results. The method is sufficiently successful that it encourages application in other situations.

1 Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide

15

0.015

(1)

−Im u0 (x,0)

0.0125 0.01 0.0075 0.005 0.0025 0 −2

−1

0 x/d

1

2

.1/

Fig. 1.8 Plot of the imaginary part of the first order wave function u0 .x; 0/ at the exit plane as a function of x=d

0.35 0.3 F0(q)

0.25 0.2 0.15 0.1 0.05 0

0

2

4

6

8

10

qd .0/

.1/

Fig. 1.9 Plot of the absolute value of the Fourier transform jF0 .q/ C F0 .q/j of the sum of zero order and first order wave function at the exit plane (solid curve), compared with the Fourier .0/ transform jF0 .q/j (dashed curve)

In particular it will be of interest to apply the method to a circular cylindrical dielectric waveguide or optical fiber. The mathematics of the method carries over straightforwardly to this more complicated geometry, with the plane wave behavior in the transverse direction replaced by Bessel functions. Due to symmetry the problem for both planar and cylindrical geometry can be reduced to an equation for a scalar wave function, so that the theory is similar to that for sound propagation. This suggests that an interesting comparison can be made with a lattice Boltzmann simulation. For a rigid circular pipe such a simulation has already been performed by da Silva and Scavone [22], with interesting results. A finite element method has been applied to a rigid open-ended duct of more general cross section [23].

16

B.U. Felderhof

Appendix 1 In this Appendix we show how the iterative scheme reproduces the exact solution of the time-independent one-dimensional Schrödinger equation with a step potential. We consider the equation

d 2u C V .z/u D p 2 u; d z2

(1.55)

with potential V .z/ D 0 for z < 0 and V .z/ D V for z > 0. In proper units p 2 is the energy. We denote the solution for z > 0 as v.z/. For a wave incident from the left the exact solution reads 0

u.z/ D e ipz C Be ipz ;

v.z/ D C e ip z ;

(1.56)

p where p 0 D p 2 V and the reflection coefficient B and transmission coefficient C are given by p p0 ; p C p0

BD

C D

2p : p C p0

(1.57)

The wave function and its derivative are continuous at z D 0. We apply the iterative scheme and put to zeroth order 0

u.0/ .z/ D e ipz ;

v.0/ .z/ D e ip z :

(1.58)

The antenna solution uA .z/ solves the equation d 2 uA C p 2 uA D ı.z/ d z2

(1.59)

for all z. It is given by uA .z/ D K.z/;

K.z/ D

1 ipjzj e : 2ip

(1.60)

To zeroth order the source is .0/ D

ˇ ˇ d u.0/ ˇˇ d v.0/ ˇˇ C D i.p p 0 /: d z ˇzD0 d z ˇzD0

(1.61)

We put the first order solution equal to u.1/ .z/ D K.z/.0/ D

p p 0 ipz ; e 2p

v.1/ .z/ D

p p 0 ip0 z e : 2p

(1.62)

1 Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide

17

Note the minus sign in K.z/.0/ . The value at the exit z D 0 is sufficient to calculate the coefficients B and C from the geometric series BD

1 X p p0 j j D1

2p

C D

;

1 X p p0 j 2p

j D0

:

(1.63)

By continuation one finds for the wave function at order j for j 1 u

.j /

.z/ D

p p0 2p

j e

ipz

;

v

.j /

.z/ D

p p0 2p

j

0

e ip z :

(1.64)

Hence for j 1 the source at order j is

.j /

p p0 D i.p C p / 2p 0

j ;

.j 1/

(1.65)

so that the sum over all j vanishes, 1 X

.j / D 0;

(1.66)

j D0

as it should. Alternatively one can write directly from Eq. (1.62) u1 .z/ D

.p p 0 /=.2p/ p p 0 ipz ipz e D e ; 1 .p p 0 /=.2p/ p C p0

v1 .z/ D

p p 0 ip0 z e : p C p0 (1.67)

Adding this to u.0/ .z/; v.0/ .z/ one reproduces Eq. (1.56).

Appendix 2 In this Appendix we show how the iterative scheme reproduces the exact solution for Fresnel reflection from a half-space. We consider infinite space with dielectric constant " for z < 0 and "0 for z > 0. The magnetic permeability equals 1 everywhere. We consider waves independent of y and TM polarization. Then the magnetic field component Hy .x; z/ satisfies the scalar equation (1.2). We put Hy .x; z/ D u.x; z/ for z < 0 and Hy .x; z/ D v.x; z/ for z > 0. The continuity conditions at z D 0 are ˇ ˇ 1 @u.x; z/ ˇˇ 1 @v.x; z/ ˇˇ u.x; 0/ D v.x; 0C/; D 0 : (1.68) " @z ˇzD0 " @z ˇzD0C

18

B.U. Felderhof

For a plane wave incident from the left the exact solution reads u.x; z/ D e i qx e ipz C Be ipz ;

0

v.x; z/ D C e i qxCip z ;

(1.69)

p p 0 N1 q 2 ; p 0 D N1 q 2 , and reflection coefficient B and with p D transmission coefficient C given by BD

"0 p "p 0 ; "0 p C "p 0

C D

2"0 p : "0 p C "p 0

(1.70)

We apply the iterative scheme and put to zeroth order u.0/ .x; z/ D e i qxCipz ;

0

v.0/ .x; z/ D e i qxCip z :

(1.71)

The antenna solution uA .x; z/ solves the equation @2 uA @2 uA C C "1 k 2 uA D ".x/ı.z/ @x 2 @z2

(1.72)

for all .x; z/. For .x/ D q e i qx it is given by uA .x; z/ D e i qx K.z/q ;

K.z/ D

" ipjzj e : 2ip

(1.73)

To zeroth order the source q is q.0/

De

i qx

ˇ ˇ 1 @u.0/ ˇˇ p p0 1 @v.0/ ˇˇ 0 : D i C " @z ˇzD0 "0 @z ˇzD0 " "

(1.74)

We put the first order solution equal to u.1/ .x; z/ D e i qx K.z/q.0/ D v.1/ .x; z/ D

"0 p "p 0 i qxipz ; e 2"0 p

"0 p "p 0 i qxCip0 z e : 2"0 p

(1.75)

.0/

Note the minus sign in e i qx K.z/q . The value at the exit z D 0 is sufficient to calculate the coefficients B and C from the geometric series BD

1 0 X " p "p 0 j j D1

2"0 p

;

C D

1 0 X " p "p 0 j j D0

2"0 p

By continuation one finds for the wave function at order j for j 1

:

(1.76)

1 Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide

u.j /.x; z/ D

"0 p "p 0 2"0 p

j

v.j / .x; z/ D

e i qxipz ;

"0 p "p 0 2"0 p

19

j

0

e i qxCip z : (1.77)

Hence for j 1 the source at order j is q.j / D i

p0 p C 0 " "

"0 p "p 0 2"0 p

j ;

.j 1/

(1.78)

so that the sum over all j vanishes, 1 X

q.j / D 0;

(1.79)

j D0

as it should. Alternatively one can write directly from Eq. (1.75) u1 .x; z/ D

."0 p "p 0 /=.2"0 p/ "0 p "p 0 i qxipz i qxipz e D e ; 1 ."0 p "p 0 /=.2"0 p/ "0 p C "p 0

v1 .x; z/ D

"0 p "p 0 i qxCip0 z e : "0 p C "p 0

(1.80)

Adding this to u.0/ .x; z/; v.0/ .x; z/ one reproduces Eq. (1.69). We note that the zeroth and first order source densities are related by q.1/ D Mq.0/ ;

M D

"0 p C "p 0 : 2"0 p

(1.81)

Hence we find B D 1 M 1 ;

C D 1 C B:

(1.82)

This suggests that more generally the complete solution of the scattering problem may be found from the relation between the zeroth and first order source densities.

References 1. 2. 3. 4. 5. 6. 7.

H. Levine, J. Schwinger, Phys. Rev. 73, 383 (1948) H. Levine, J. Schwinger, Commun. Pure Appl. Math. 3, 355 (1950) A. Sommerfeld, Math. Ann. 47, 317 (1896) A. Sommerfeld, Optics (Akademische Verlagsgesellschaft, Leipzig, 1964) H. Bouwkamp, Rep. Prog. Phys. 17, 35 (1954) M. Born, E. Wolf, Principles of Optics (Pergamon Press, Oxford, 1975) F.E. Gardiol, in Advances in Electronics and Electron Physics, vol. 63, ed. by P.W. Hawkes (Academic, London, 1985), p. 139

20

B.U. Felderhof

8. D. Hondros, P. Debye, Ann. d. Phys. 32, 465 (1910) 9. G.F. Homicz, J.A. Lordi, J. Sound Vib. 41, 283 (1975) 10. P. Joseph, C.L. Morfey, J. Acoust. Soc. Am. 105, 2590 (1999) 11. M.S. Howe, Hydrodynamics and Sound (Cambridge University Press, Cambridge, 2007) 12. S.W. Rienstra, A. Hirschberg, An Introduction to Acoustics 2014, www.win.tue.nl/~sjoerdr/ papers/boek.pdf 13. D.M.S. Soh, J. Nilsson, S. Baek, C. Codemard, Y. Jeong, V. Philippov, J. Opt. Soc. Am. A21, 1241 (2004) 14. A.E. Heins, Q. Appl. Math. 6, 157 (1948) 15. P.C. Clemmow, Proc. R. Soc. A 205, 286 (1951) 16. F.E. Borgnis, C.H. Papas, Electromagnetic Waveguides and Resonators (Springer, Berlin, 1958) 17. D. Marcuse, Theory of Dielectric Optical Waveguides (Academic, New York, 1974) 18. H. Kogelnik, in Integrated Optics, Topics Appl. Phys. 7, ed. by T. Tamir (Springer, Berlin, 1979) 19. P. Lorrain, D.R. Corson, F. Lorrain, Electromagnetic Fields and Waves (Freeman, New York, 1988) 20. A. Bratz, B.U. Felderhof, G. Marowsky, Appl. Phys. B 50, 393 (1990) 21. R.G. Newton, Scattering Theory of Waves and Particles (McGraw-Hill, New York, 1966) 22. A.R. da Silva, G.P. Scavone, J. Phys. A 40, 397 (2007) 23. W. Duan, R. Kirby, J. Acoust. Soc. Am. 131, 3638 (2012)

Chapter 2

Optimizing Second-Harmonic Generation in a Circular Cylindrical Waveguide with Embedded Periodically Arranged Tubelets of Nonlinear Susceptibility B.U. Felderhof, G. Marowsky, and J. Troe

2.1 Introduction An efficient method of generating second-harmonic radiation (SHG) can find use in a variety of technical applications. Confined geometry—such as in fibers or film waveguides—allows concentration of the fundamental radiation at the position of the material with nonlinear susceptibility. In earlier work [1] we have investigated SHG in a planar geometry and studied the dependence on the position of nonlinear material with respect to the planar device that guides the fundamental radiation. SHG was enhanced by a judicious use of periodicity of the nonlinear material in the direction of propagation of the fundamental wave. In this paper we consider instead confinement of radiation in a circular waveguide or optical fiber. This geometry has the advantage of confinement in both transverse dimensions, thus avoiding diffraction and the corresponding dispersion of the fundamental beam in a transverse direction. The following calculations show that the circular geometry is preferable to the planar one, even when in the latter case the beam has infinite width, so that diffraction no longer plays a role. In the following we analyze SHG in a circular waveguide for an idealized situation of high symmetry. The nonlinear material—representing an idealized polarization sheet [2]—is assumed to be arranged in a periodic array of cylindrical tubelets centered around the axis of the waveguide. The period in the axial direction can be optimized by use of a Bragg condition involving the wavenumbers of both

B.U. Felderhof () Institut für Theorie der Statistischen Physik, RWTH Aachen University Templergraben 55, 52056 Aachen, Germany e-mail: [email protected] G. Marowsky • J. Troe Laser-Laboratorium Göttingen e.V. Hans-Adolf-Krebs-Weg 1, 37077 Göttingen, Germany e-mail: [email protected] G. Marowsky (ed.), Planar Waveguides and other Confined Geometries: Theory, Technology, Production, and Novel Applications, Springer Series in Optical Sciences 189, DOI 10.1007/978-1-4939-1179-0__2, © Springer ScienceCBusiness Media New York 2015

21

22

B.U. Felderhof et al.

the fundamental and the doubled frequency. In addition one can optimize the axial width of the tubelets and their transverse radius. By integration over the radius the calculation can be extended to cover the case of tubelets of finite thickness, or of an array of solid cylindrical pieces. Admittedly, the idealized situation under consideration may be difficult to realize experimentally. The intention of our model calculation is to elucidate the principles, and to serve as a guide for the analysis of more realistic but less symmetric situations. Due to the high symmetry of the model situation we can limit attention to a small number of modes. This advantage is lost in more realistic situations. The paper is organized as follows: First we perform a calculation in analogy to that for planar geometry [1] for a finite length L of nonlinear material distributed in N tubelets, where N is much larger than unity. For optimum phase matching the intensity of the generated SHG grows in proportion to L2 . In the circular waveguide the efficiency is sufficiently high so that it is necessary to consider depletion of the fundamental. On a large length scale the effect of depletion may be studied by use of mode-coupling theory. The situation is mathematically analogous to that of SHG in anisotropic crystals, so that the mode-coupling theory of Armstrong et al. [3] can be used. Apparently this was not realized by Zhao et al. [4], who formulated mode-coupling equations on the much smaller length scale of the period of the array. Second-harmonic generation in poled optical fibers using gratings optically written by mode interference was studied experimentally by Fermann et al. [5]. Analogous experiments in thermally poled twin-hole glass fibers were performed by Mizunami et al. [6, 7]. Pump depletion in a waveguide filled with periodically poled lithium niobate was observed by Parameswaran et al. [8] to be in good agreement with theory.

2.2 Circular Waveguide Theory We consider a circular waveguide of radius b filled with material which is uniform in the axial direction z and with electric and magnetic permeability, which depend only on the radial direction r. We use cylindrical coordinates .r; '; z/. The dielectric profile ".r; !/ and magnetic profile .r; !/ depend also on frequency !. We assume that for the frequencies of interest " and are real. Also we assume that " and tend to constants "i ; i for small r and to constants "f ; f for r ! b. In later application we consider in particular a two-layer situation with "; D "2 ; 2 for 0 < r < d and "; D "1 ; 1 for d < r < b. We consider plane wave solutions of Maxwell’s equations which depend on z and t through a factor exp.ipz i !t/ and which do not depend on the azimuthal angle '. Maxwell’s equations for the electric and magnetic field amplitudes then read in SI units [9–11]

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

drHr d "rEr C ip"rEz D 0; C iprHz D 0; dr dr E' H' dH' dE' C D i !Hz ; C D i !"Ez ; dr r dr r dHz dEz ipEr D i !H' ; ipHr D i !"E' ; dr dr pE' D !Hr ; pH' D !"Er :

23

(2.1)

The solutions of these equations may be decomposed according to two polarizations. For TE-polarization the components Er ; Ez , and H' vanish, and the equations may be combined into the single equation d 2 E' 1 r d.=r/ dE' 1 d 2 C "! 2 E' D p 2 E' dr 2 dr dr r dr r

.TE/: (2.2)

For TM-polarization the components Hr ; Hz , and E' vanish, and the equations may be combined into the single equation d 2 H' r d."=r/ dH' 1 1 d" 2 C "! H' D p 2 H' dr 2 " dr dr "r dr r 2

.TM/: (2.3)

We consider first TE-polarization. We assume that for 0 < r < ri the permeabilities "; equal "i ; i and that for r > rf they equal "f ; f . We write the solution of Eq. (2.2) in these two regions: E' .r/ D J1 .qi r/

for r < ri ;

E' .r/ D Af J1 .qf r/ C Bf Y1 .qf r/

for r > rf ;

with Bessel-functions J1 .qr/; Y1 .qr/ and wavenumbers q qj D "j j ! 2 p 2 :

(2.4)

(2.5)

The coefficients Af and Bf are related by the boundary conditions at r D b. The p wavenumbers fqi ; qf g are real only up to a maximum value of p given by "j j ! in either case and are pure imaginary beyond this value. For such wavenumbers we rewrite the second equation in (2.4) as E' .r/ D AI1 . f r/ C BK1 . f r/

for r > rf ; (2.6) p with modified Bessel-functions I1 . r/ and K1 . r/ and D p 2 "! 2 . The p guided mode solutions occur at discrete values fpj g of p larger than "f f !. We assume that the radius b is sufficiently large that the waveguide condition can be approximated by A.p; !/ D 0:

(2.7)

24

B.U. Felderhof et al.

At fixed ! the roots of this equation determine the discrete values fpj g for which a guided mode solution exists. We call A.p; !/ the dispersion function. The explicit expressions for the coefficients A.p; !/ and B.p; !/ in the analogous case of TM-polarization will be given in Eq. (2.54). The one-dimensional wave equation (2.2) can be transformed to a form resembling the one-dimensional time-independent Schrödinger equation by use of the transformation r f .r/: (2.8) E' .r/ D r By substitution we find that Eq. (2.2) is transformed to d 2f V .r/f D p 2 f; dr 2

(2.9)

where the function V .r/ is given by r V .r/ D "! 2 C

d2 r dr 2

r

1 d log.r/ r C : r dr

(2.10)

It is of interest to derive an expression for the norm of the eigensolutions. Differentiating Eq. (2.9) with respect to p 2 one derives the identity @ @f @f @f @ f D f 2: 2 (2.11) @r @r @p 2 @p @r Applying this identity to guided mode solutions normalized as in Eq. (2.4) we find by integration over r and use of the waveguide condition (2.7) ˇ Z b 1 @A.p; !/ ˇˇ r E 2 E'j .r/ dr D B.pj ; !/ : (2.12) Nj D 2f pj @p ˇpj 0 .r/ We shall show in the next section that the norm is related to the intensity of the mode. It follows from Eq. (2.3) that for TM-polarization exactly the same relations hold if we replace E' by H' , " by , and by ". Where necessary the symbols corresponding to the two types of solution will be distinguished by a superscript E or M.

2.3 Excitation of Guided Modes In this section we describe how the eigenmodes may be excited by an oscillating dipole density. We begin by relating the norm of an eigenmode, given by Eq. (2.12), to the physical intensity. The energy current density averaged over a time period 2=! is given by the Poynting vector S D

1 Re.E H /: 2

(2.13)

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

25

The z-component of this expression may be decomposed into Sz D SzE C SzM ;

(2.14)

with the separate terms for TE- and TM-polarizations SzE D

p jE' j2 ; 2!

SzM D

p jH' j2 : 2!"

(2.15)

We define the total intensity by the integrals Z

Z

b

I E D 2 0

SzE .r/r dr;

b

I M D 2 0

SzM .r/r dr:

(2.16)

The intensity does not depend on z. For a single eigenmode of either TE- or TM-type the expressions (2.15) become E Szj D

pjE 2!

jE'j j2 ;

M Szj D

pjM 2!"

jH'j j2 :

(2.17)

By comparison with Eq. (2.12) we find that for a single eigenmode excited with amplitude aj the intensity is related to the norm of the mode by Ij D

pj Nj jaj j2 : !

(2.18)

This expression is formally the same for both polarizations. Using orthogonality of the eigenmodes [9–11] we find that for a linear superposition of guided modes, all oscillating at the same frequency !, the total intensity is given by I D

X .IjE C IjM /;

(2.19)

j

which again does not depend on z. Next we investigate how radiation is emitted by an antenna embedded in the waveguide. We consider a surface polarization [12–14] P S .z/ of finite extent in the z-direction, independent of ', located at radius r D r0 , and oscillating at frequency !. The corresponding charge and current densities are .r/ D

@PzS @ ı.r r0 / PzS ı.r r0 /; @z @r j .r/ D i !P S .z/ı.r r0 /;

(2.20)

26

B.U. Felderhof et al.

which must be added as source terms to Maxwell’s equations. The charge and current densities are related by the continuity equation i ! C r j D 0. A Fourier analysis of the surface polarization yields Z

S PO .p/e ipz dp:

P S .z/ D

(2.21)

From Maxwell’s equations we now find instead of Eq. (2.2) d 2 EO ' 1 O r d.=r/ d EO ' 1 d 2 2 C "! p 2 E' dr 2 dr dr r dr r D ! 2 PO'S ı.r r0 /:

(2.22)

Similarly instead of Eq. (2.3) d 2 HO ' 1 O r .d "=r/ d HO ' 1 d" 2 2 C "! H' D p dr 2 " dr dr "r dr r 2 d 1 d" OS Pz ı.r r0 / !p POrS ı.r r0 /: ı.r r0 / i ! POzS dr " dr

(2.23)

The solution of these equations may be found with the aid of the Green’s functions G E .r; r0 / and G M .r; r0 / defined by the equation d 2G V .r/G D p 2 G C ı.r r0 /: dr 2

(2.24)

The Green’s function may be expressed as G.r; r0 / D

f1 .r< /f2 .r> / ; .f1 ; f2 /

(2.25)

where r< .r> / is the smaller (larger) of r and r0 , in terms of the two fundamental solutions f1 ; f2 defined by r f1E .r/

D r

f2E .r/ D

r J1 .qi r/; i r K1 . f r/; f

r

r J1 .qi r/; for r < ri ; "i r r f2M .r/ D K1 . f r/; for r > rf ; (2.26) "f

f1M .r/

D

with the Wronskian ˇ ˇ ˇ f1 f2 ˇ ˇ .f1 ; f2 / D ˇ 0 0 ˇˇ: f1 f2

(2.27)

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

27

The Wronskian takes the value .f1E ; f2E / D

1 E A .p; !/; f

.f1M ; f2M / D

1 M A .p; !/: "f

(2.28)

The solution of Eq. (2.22) is given by EO ' .p; r/ D ! 2 Œ.r/=r 1=2 G E .r; r0 /Œ.r0 /r0 1=2 PO'S :

(2.29)

The solution of Eq. (2.23) is given by HO ' .p; r/ D i !Œ".r/=r 1=2

@G M .r;r0 / @r0

C

1 d ln ".r0 / M 2 dr0 G .r; r0 /

C 2r10 G M .r; r0 / Œ".r0 /=r0 1=2 POzS !pŒ".r/=r 1=2 G M .r; r0 /Œ".r0 /=r0 1=2 POrS : (2.30) For a surface polarization P S .z/ with arbitrary variation in the z-direction the fields E' .r; z/ and H' .r; z/ are now obtained by Fourier superposition. Thus we find Z Z E' .r; z/ D EO ' .p; r/e ipz dp; H' .r; z/ D HO ' .p; r/e ipz dp; (2.31) S where EO ' .p; r/ and HO ' .p; r/ are given by Eqs. (2.29) and (2.30) in terms of PO .p/. The Wronskian, given by Eq. (2.28), vanishes at the eigenvalues fpjE g and fpjM g. For large z the contribution from the corresponding poles dominates the integrals in Eq. (2.31). This allows us to evaluate the amplitude of the various guided modes excited by the oscillating surface polarization.

2.4 Emitted Radiation In this section we analyze the radiation emitted by a circular cylindrical antenna, as introduced in the preceding section, in more detail. We are interested in the radiation channeled into the waveguide and detected at large positive z. At sufficiently large distance from the antenna, i.e., after the decay of transients corresponding to evanescent wave solutions, the behavior of the fields is dominated by pole contributions to the integrals, corresponding to roots of the waveguide condition (2.7). The contributions may be found by contour integration in Eq. (2.31) with the poles at positive fpj g shifted slightly upwards into the complex plane and those at fpj g shifted slightly downwards. We note that it follows from Eq. (2.6) that for values fpj g for which the waveguide condition is satisfied f1 .pj ; r/ D B.pj ; !/f2 .pj ; r/:

(2.32)

28

B.U. Felderhof et al.

Thus we find for large positive z, far from the source P S .z/, X E E E a1j E' .r; z/ j .r/ exp.ipj z/;

(2.33)

j

where we employ the notation E j .r/

D

p .r/=rf1jE .r/:

(2.34)

The amplitudes are given by E OS E j .r0 /P' .pj /;

E a1j D i ! 2 .pjE NjE /1 r0

(2.35)

where we have used Eq. (2.12). From Eq. (2.33) we may evaluate the intensity defined in Eq. (2.16). Because of the orthogonality of the different modes [9–11] there are no cross terms, and we find by use of Eq. (2.18) X X IjE D 3 ! 3 .pjE NjE /1 r02 Œ jE .r0 / 2 jPO'S .pjE /j2 : (2.36) IE D j

j

Similarly we find for large positive z X M a1j H' .r; z/

M M j .r/ exp.ipj z/;

(2.37)

j

with the notation M j .r/

D

p ".r/=rf1jM .r/:

(2.38)

The amplitudes are given by M D !.pjM NjM /1 Rj .r0 /POrS .pjM / C Zj .r0 /POzS .pjM / ; a1j

(2.39)

with the abbreviations Rj .r/ D Zj .r/ D

ir M p ".r/ j @ r

M j .r/

".r/

@r

M j .r/;

1 C r

M j .r/

:

(2.40)

This yields for the intensity IM D

X

IjM

j

D 3!

X j

ˇ2 ˇ .pjM NjM /1 ˇRj .r0 /POrS .pjM / C Zj .r0 /POzS .pjM /ˇ : (2.41)

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

29

The expressions (2.36) and (2.41) have a fairly simple structure. The efficiency with which a surface polarization P S .z/ excites the guided modes is determined by its Fourier component at the wavenumber pj , as well as by its radial location r0 via the eigenfunction j .r0 /, which appears quadratically with its proper normalization Nj .

2.5 Phase Matching In this section we discuss the principle of second-harmonic generation by use of a phase-matched adsorbate embedded in a circular cylindrical waveguide. We shall assume that the adsorbate either is located as a thin layer directly outside the core or is embedded in the core. We consider a surface polarization P S .z/ located at radius r0 and induced by an incident fundamental wave. The polarization acts as an antenna emitting waves at the second-harmonic frequency. Thus we put P S .r0 ; z/ D .2/ .z/ W E 10 .r0 ; z/E 10 .r0 ; z/;

(2.42)

where E 10 .r0 ; z/ is the incident fundamental field at the location of the adsorbate. If the fundamental field oscillates at frequency !, then the surface polarization oscillates at frequency 2!, and this must be taken into account in the expressions of the preceding sections. We assume that the adsorbate is so weak that it does not disturb the fundamental wave. This is expressed by the subscript zero in (2.42). The fundamental wave is a linear combination of guided modes with z-dependence exp.ipj z/ with wavenumber pj .!/. We shall assume that the susceptibility .2/ depends on z via the density of adsorbed molecules. If the adsorbate has a periodicity in the z-direction with period a characterized by the wavenumber K D 2=a, then we may expect resonance when the phasematching condition pj .2!/ D 2pk .!/ C nK;

n D 0; ˙1; ˙2; : : :

(2.43)

is satisfied. More specifically it is natural to aim at satisfying the condition p0 .2!/ D 2p0 .!/ ˙ K;

(2.44)

for the lowest mode j D 0. We shall call this the Bragg condition. We consider in particular a grating of period a consisting of N adsorbate tubelets of width w < a. An example of the grating and waveguide is shown in Figs. 2.1 and 2.2. The susceptibility function is given by .z/ D .2/ gN .z/;

(2.45)

30

B.U. Felderhof et al.

Fig. 2.1 Axial cross section of the waveguide and adsorbate structure. The figure should be rotated about the z axis to get the three-dimensional picture

r d 0 d

⑀1 ⑀2 ⑀2

z

⑀1

Fig. 2.2 Three-dimensional picture of the waveguide and adsorbate structure

with the Bragg function gN .z/ D

N 1 X

1 .w; z na w/; 2 nD0

(2.46)

where .w; z/ D 1

for D0

w w : 2

(2.47)

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

31

The prefactor .2/ in (2.45) is a third rank tensor independent of z. We shall assume that .2/ has the characteristics of a layer isotropic about the surface normal in the radial direction. We also assume that there exists a mirror plane containing the radial normal to exclude chirality. From these assumptions it follows that .2/ has only three independent components (for details see [14–17]). The Fourier-component O S .p/ is proportional to P Z 1 1 GO N .p 2pk .!// D gN .z/e 2ipk .!/zipz d z 2 1 D

exp.i sk w/ 1 1 exp .iN sk a/ ; 2 i sk 1 exp.i sk a/

(2.48)

where we have introduced the variable sk D 2pk .!/ p:

(2.49)

For real p the absolute square of the second factor in Eq. (2.48) is given by ˇ ˇ 2 ˇ 1 e iN sa ˇ2 ˇ D sin .N sa=2/ ; ˇ (2.50) FN .sa/ D ˇ 1 e i sa ˇ sin2 .sa=2/ which takes the values N 2 at sa D 2n, where n D 0; ˙1; ˙2; : : :. Since we wish O S .p/ to be maximum at p0 .2!/ we choose the lattice distance a such that P a D 2j2p0 .!/ p0 .2!/j1

(2.51)

corresponding to n D 1 or n D 1. In this way we satisfy the Bragg condition (2.44). The width of the function in Eq. (2.50) at s D ˙2=a is of order 1=Na. Hence the area of the peak is proportional to N . The larger N , the more precisely the condition (2.51) must be satisfied. An error a in the value of a implies an error p D 2a=a2 in p-space. If we require this to be at most 1=Na, then N cannot be larger than a=2a. Ideally one would use a tunable laser and adjust the frequency ! such that the condition (2.51) is precisely satisfied. With that choice the absolute square of the first factor in Eq. (2.48) is maximal at w D 12 a.

2.6 Second-Harmonic Generation In this section we investigate the effect of geometry on the efficiency for secondharmonic generation. We consider the core of the waveguide to be a cylinder of radius d with dielectric constant "2 surrounded by an outer mantle with uniform dielectric constant "1 < "2 . The grating of adsorbed molecules is located at radius r0 , either inside or outside the core (r0 < d or r0 > d ). We put the magnetic permeability equal to 0 everywhere and consider guided mode solutions of TM type. We study the dependence of the efficiency for second-harmonic generation on the radius r0 .

32

B.U. Felderhof et al.

The discontinuity of the dielectric constant at r D d corresponds to jump conditions for the tangential component H' .r/. The first condition is that H' .r/ is continuous at r D d . The wave equation (2.3) may be rewritten as ".r/

H' 1 dH' d C C "! 2 H' D p 2 H' : dr ".r/ dr r".r/

(2.52)

Hence the second condition is that .dH' =dr C H' =r/=" is continuous at the interface. In analogy to Eqs. (2.4) and (2.6) we write the solution as H' .r/ D J1 .q2 r/;

for 0 < r < d;

D A I1 . 1 r/ C B M K1 . 1 r/; M

for d < r < b;

(2.53)

p p where q2 D "2 0 ! 2 p 2 and 1 D p 2 "1 0 ! 2 . From the two continuity equations we find for the coefficients AM and B M "1 q2 dJ0 .q2 d /K1 . 1 d / C 1 dJ1 .q2 d /K0 . 1 d /; "2 "1 B M .p; !/ D q2 dJ0 .q2 d /I1 . 1 d / C 1 dJ1 .q2 d /I0 . 1 d /: "2 AM .p; !/ D

(2.54)

Putting AM .p; !/ D 0 for fixed ! one finds the wavenumbers pjM .k/ of the guided modes. The guided mode solutions take the form M j .r/

D J1 .q2j r/;

for 0 < r < d;

D B M .pjM ; !/K1 . 1j r/;

for d < r < b:

(2.55)

From Eq. (2.12) one finds for their norm Z NjM

b

D 0

r Œ ".r/

M 2 j .r/

ˇ 1 @AM .p; !/ ˇˇ M dr D B .pj ; !/ ˇ M: @p 2"1 pjM pj

(2.56)

The electrical field has components Er .r/ D

p H' ; !"

Ez .r/ D

H' i dH' C : !" dr r

(2.57)

We assume that the fundamental is present as a single mode oscillating at frequency M ! with amplitude a1k .!/. Hence the electrical field vector is E .!I r; z/ D

M .!/ M a1k p !".r/ k

M k .r/e r

Ci

d

M k .r/

dr

C

M k .r/ r

e z exp.ipkM z/: (2.58)

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

33

We assume an isotropic tensor .2/ with mirror symmetry. The induced surface polarization is P SM .2!; z/ D gN .z/

2

M .!/ a1k !".!; r0 /

X k .!; r0 / exp.2ipkM z/;

(2.59)

with Bragg factor given by Eq. (2.46) and vector X k .!; r0 / given by X k .!; r/ D 1 pkM

2 M k .!; r/

2

C2i3 pkM .2/

M k .!; r/

.2/

d

M k .r/

d

dr

M k .r/

dr .2/

C

C

2 M k .r/

er

r M k .r/ ez; r

(2.60)

.2/

where 1 D rrr ; 2 D rzz , and 3 D zrz D zzr are the relevant components of the nonlinear susceptibility tensor .2/ . We assume that the layer of second-order susceptibility is locally flat, so that the subscript r corresponds to the locally normal component and z to the locally tangential component. For a representation of the tensor in the local Cartesian frame see Roders et al. [17]. The emitted secondharmonic radiation is TM-polarized. The intensity of the emitted second-harmonic radiation is given by Eq. (2.41), with the right-hand side taken at frequency 2! instead of !. We find by use of Eq. (2.18)

IjM .2!/ D

1 2 jGO N .pjM .2!/ 2pkM .!//j2 M !".!; r0 /4 pj .2!/NjM .2!/pkM .!/2 NkM .!/2 ˇ ˇ2 2 ˇRj .2!; r0 /Xkr .!; r0 / C Zj .2!; r0 /Xkz .!; r0 /ˇ IkM .!/ :

(2.61)

The conversion coefficient is defined by M M MM j k D Ij .2!/=Ik .!/:

(2.62)

We write the conversion coefficient in the form MM jk D

2 O jGN .pjM .2!/ 2pkM .!//j2 Aj k .r0 /IkM .!/; c

(2.63)

with coefficient Aj k .r0 / D

ˇ ˇ ˇRj .2!; r0 /Xkr .!; r0 / C Zj .2!; r0 /Xkz .!; r0 /ˇ2 k".!; r0 /4 pjM .2!/NjM .2!/pkM .!/2 NkM .!/2

;

(2.64)

and write the latter as Aj k .r0 / D

1 X "30 d 6

C .j jkI r0 / ;

(2.65)

34

B.U. Felderhof et al.

1.5 p2(k)/k,p1(k)/k,p0(k)/k

Fig. 2.3 Plot of the wavenumber p0 .k/ of the lowest order guided wave (solid curve), of the wavenumber p1 .k/ of the first-order guided wave (long dashes), of the wavenumber p2 .k/ of the second-order guided wave (short dashes), as functions of kd for values of the dielectric constant given in the text

1.49 1.48 1.47 1.46 10

20

30

40

50

kd

with dimensionless coefficients C .j jkI r0 /. The factors Rj and Zj are given by Eq. (2.40), and Xr and Xz are given by Eq. (2.60). The coupling coefficients C .j jk/ depend on the radius r0 and the geometry of the waveguide. The efficiency of second-harmonic generation for the chosen geometry is characterized by the Bragg prefactor jGO N j2 and the coefficients C .j jkI r0 /. We consider the width d to be fixed, and vary the frequency !. The input laser is tuned in a narrow frequency range, so that dispersion of the dielectric constant near ! and 2! may be neglected. We put "2 .!/ D 2:25"0, "2 .2!/ D 2:28"0 , in combination with "1 .!/ D 2:13"0 and "1 .2!/ D 2:17"0 . In Fig. 2.3 we plot the reduced wavenumbers p0 .k/=k; p1 .k/=k, and p2 .k/=k at the fundamental p frequency as functionspof kd . The ratios fpn .k/=kg are larger than "1 ="0 D 1:4595 and less than "2 ="0 D 1:5. The corresponding plots at the secondharmonic frequency are very similar. In Fig. 2.4 we plot the coefficient C11 .0j0I r0/ at kd =24 as a function of the fraction r0 =d . In Figs. 2.5 and 2.6 we present similar plots for the coefficients .2/ C22 .0j0I r0/ and C33 .0j0I r0/. The plot in Fig. 2.4 for susceptibility 1 D rrr shows the largest rate of conversion. It is of interest to compare the optimal situation with that for a planar waveguide. We have found earlier that for a planar waveguide consisting of a slab of dielectric constant "2 of thickness 2d surrounded by a medium of dielectric constant "1 second-harmonic generation is optimal for a thin polarization layer midway between the two interfaces (in Ref. 1 this was called geometry III). For the planar waveguide the conversion coefficient took the form X 4 2

MM j kP D GNj kP Bj k JkM .!/; (2.66) !

with Bragg factor GNj kP D jGO N .pjM .2!/ 2pkM .!//j2 :

(2.67)

Here the wavenumbers p must be calculated for the guided modes of the planar waveguide, so that the lattice distance a and the Bragg factor GNj kP differ from

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

35

4000 3000 C11(0 0)

2000 1000 0

0

0.2

0.4

0.6 r0/d

0.8

1

Fig. 2.4 Plot of the coupling coefficient C11 .0j0I r0 / for kd D 24 as a function of r0 =d . The coefficient characterizes the efficiency of conversion, as given by Eqs. (2.63) and (2.65), of the lowest order guided wave with largest wavenumber p0 .k/ at the fundamental frequency ! D kc to the mode with largest wavenumber p0 .2k/ at the second-harmonic frequency 2! D 2kc. The radius of the tubelet of nonlinear susceptibility is r0 , and d is the radius of the core of the waveguide. The subscripts 11 indicate the contribution which is quadratic in the component .2/ 1 D rrr of the second-order susceptibility tensor

0.2 0.15 C22(0 0) 0.1 0.05 0

0

0.2

0.4

0.6 r0/d

0.8

1

Fig. 2.5 Plot of the coupling coefficient C22 .0j0I r0 / for kd D 24 as a function of r0 =d . The coefficient characterizes the efficiency of conversion, as given by Eqs. (2.63) and (2.65), of the lowest order guided wave with largest wavenumber p0 .k/ at the fundamental frequency ! D kc to the mode with largest wavenumber p0 .2k/ at the second-harmonic frequency 2! D 2kc. The radius of the tubelet of nonlinear susceptibility is r0 , and d is the radius of the core of the waveguide. The subscripts 22 indicate the contribution which is quadratic in the component .2/ 2 D rzz of the second-order susceptibility tensor

the lattice distance and corresponding factor GNj kC for a cylindrical waveguide appearing in Eq. (2.63). The intensity JkM .!/ is defined from the integral of the Poynting vector along the transverse coordinate. In order to compare the two geometries we put IkM .!/ D d 2 S C ;

JkM .!/ D 2d S P ;

(2.68)

36

B.U. Felderhof et al.

0.175 0.15 0.125 0.1 C33(0 0) 0.075 0.05 0.025 0

0

0.2

0.4

0.6

0.8

1

r0/d Fig. 2.6 Plot of the coupling coefficient C33 .0j0I r0 / for kd D 24 as a function of r0 =d . The coefficient characterizes the efficiency of conversion, as given by Eqs. (2.63) and (2.65), of the lowest order guided wave with largest wavenumber p0 .k/ at the fundamental frequency ! D kc to the mode with largest wavenumber p0 .2k/ at the second-harmonic frequency 2! D 2kc. The radius of the tubelet of nonlinear susceptibility is r0 , and d is the radius of the core of the waveguide. The subscripts 33 indicate the contribution which is quadratic in the component .2/ 1 D zzr of the second-order susceptibility tensor

and write the conversion coefficient (2.63) for the cylindrical waveguide in the form MM j kC D

2 2 GNj kC Aj kC .r0 /d 2 S C ; c

(2.69)

where GNj kC is the Bragg factor defined as in Eq. (2.67). The conversion coefficient for the planar waveguide is written similarly as MM j kP D

2 2 GNj kP Aj kP d 2 S P : c

(2.70)

4 X Bj k : kd

(2.71)

By comparison with Eq. (2.66) Aj kP D

We consider kd D 24, as in the experiment of Parameswaran et al. [8], with wavelength of the fundamental D 2=k D 1550 nm and d 6m, and use the same dielectric constants as above. Then we find for the cylindrical waveguide p0 .!/d D 35:837 and p0 .2!/d D 72:388, and for the planar waveguide p0 .!/d D 35:972 and p0 .2!/d D 72:463. The lattice distance a, given by Eq. (2.51), in the two cases takes the value aC D 8:79 d;

aP D 12:12 d:

(2.72)

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

37

5000 4000 C11(0 0) 3000 2000 1000 0 7.5

10

12.5

15

17.5 kd

20

22.5

25

Fig. 2.7 Plot of the coupling coefficient C11 .0j0/ for the circular waveguide as a function of kd (solid curve). For each value of kd , the optimal radius r0 has been chosen. For comparison we also plot the coupling coefficient C11 .0j0/ for the planar waveguide as a function of kd (dashed curve). The notation is explained in the caption to Fig. 2.4

Correspondingly we find for the coupling factors in Eqs. (2.69) and (2.70) for 2 D 3 D 0 A00C .rm / D 4275 j1 j2 =."30 d 6 /;

A00P D 32:47 j1 j2 =."30 d 6 /:

(2.73)

for the value rm D 0:593 d corresponding to the maximum in Fig. 2.4. The prefactors in Eq. (2.73) are the values of the coupling coefficients C11C .0j0/ D 4275 and C11P .0j0/ D 32:47. In Fig. 2.7 we show the coupling coefficient C11C .0j0/ as a function of kd . At each value of kd the optimal radius r0 has been chosen. For comparison we show also the coupling coefficient C11P .0j0/ as a function of kd for the planar waveguide. This shows a decrease with increasing frequency of the fundamental. Clearly the circular waveguide geometry is to be preferred for most frequencies . For large N the Bragg factors G in Eqs. (2.69) and (2.70) vary rapidly with frequency. It makes sense to compare the two geometries at their peak values for second-harmonic generation. Hence we put the factor FN in Eq. (2.50) equal to N 2 in both cases. Then the Bragg factors differ only by the first factor in Eq. (2.48). Taking w D a=2 in both cases we get for the two Bragg factors at the peak value GN 00C D 0:198 N 2 ;

GN 00P D 0:377 N 2 :

(2.74)

The prefactors for the two geometries in the conversion coefficients (2.68) and (2.69) take similar values. The circular geometry may have an advantage over the planar geometry in the efficiency of input of the fundamental wave. In the above numerical example we find for the circular waveguide with susceptibility 1 D 1013 esu the conversion factor in SI units 5 2 M MM 00C D 2:7 10 L I .!/;

(2.75)

38

B.U. Felderhof et al.

Table 2.1 Selected conversion efficiencies (for details, cf. text) SHG-experiment

P .2!/=P .!/ in %

Reference

Surface-SHG simple reflection

1012

KDP-crystal in transmission

1:72 104

Planar waveguide

1 104

G.T. Boyd, Y. R. Shen, T.W. Hänsch Second-harmonic generation from sub-monolayer molecular adsorbates using a CW diode laser Seventh International Conference Laser Spectroscopy VII Maui, HI, USA, 24–28 June 1985 A. Yariv Quantum Electronics Third Edition, Wiley, New York, 1988 Chapter 16.7: Second-Harmonic Generation with Gaussian Beams, pp. 402 A. Bratz, B. U. Felderhof, G. Marowsky Second-harmonic generation in planar waveguides Appl. Phys. B 50, 393–404 (1990) This work

optimized geometry III

Quasi-phase-matched SHG in a fiber under optimized conditions

2.7

where L D Na is the length of material with nonlinear susceptibility 1 . For an 2 input power of the fundamental I M .!/ D 100 mW this becomes MM 00C D 2:7L with L in cm. By definition the conversion factor is less than unity. This implies that for a length 1 cm we must take depletion into account. In Table 2.1 we have summarized some relevant conversion data from reliable literature sources. The table shows that SHG conversion varies by many orders of magnitude, depending on the experiment. The conversion efficiency 1012 % concerns the famous Maui surface experiment of Boyd, Shen, and Hänsch, demonstrating surface SHG of a sub-monolayer of pyridine adsorbed on a silver electrode. The other SHG conversion data concern KDP, an optimized planar waveguide geometry of Bratz et al. [1], and the proposed configuration of Fig. 2.2 in this work. Due to strong spatial confinement and Bragg interference the conversion efficiency is strongly enhanced and pump depletion has to be considered even for device lengths as short as 1 cm. Therefore the device length was taken to be 0.1 cm to avoid depletion and make the data comparable. It should be noted that for the KDP-case SHG was considered with Gaussian beams; hence the efficiency increases only linearly with crystal thickness.

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

39

2.7 Depletion For a sufficiently long stretch of nonlinear susceptibility depletion of the fundamental must be taken into account. We consider a stretch with M periods of nonlinear susceptibility .2/ , where M is a large multiple of N . It is assumed that N is sufficiently small that the preceding theory, with neglect of depletion, may be applied. In the experiment of Parameswaran et al. [8] with a planar waveguide the number of periods is about M D 4000. The period a is assumed to be adjusted to the frequency of the fundamental by use of Eq. (2.51). Due to the Bragg factor, conversion is then limited to the lowest mode with wavenumber p0 .2!/. We assume first that the input laser is tuned to the peak value, so that the Bragg factor is proportional to N 2 , as in Eq. (2.74). On a large length scale the intensity of the fundamental I0M .!I z/ decreases with distance along the waveguide, and the intensity of the second harmonic I0M .2!I z/ increases. For brevity we denote I1 .z/ D I0M .!I z/ and I2 .z/ D I0M .2!I z/. We define corresponding slowly varying wave amplitudes A1 .z/ and A2 .z/ by [3] I1 .z/ D p1 A1 .z/2 I1 .0/;

I2 .z/ D

1 p2 A2 .z/2 I1 .0/; 2

(2.76)

with the abbreviations p1 D p0 .!/;

p2 D p0 .2!/:

(2.77)

The amplitudes A1 .z/ and A2 .z/ are assumed to satisfy the mode-coupling equations dA1 D A1 A2 ; dz p1 dA2 D 2 A21 ; dz p2

(2.78)

where the coefficient can be evaluated from the preceding theory for the behavior at small z. The mode-coupling equations imply the conservation law I1 .z/ C I2 .z/ D I1 .0/:

(2.79)

The equations have the solution s 1 A1 .z/ D p sech z; p1 with

A2 .z/ D

2 tanh z; p2

(2.80)

s D p1

2 ; p2

(2.81)

40

B.U. Felderhof et al.

so that correspondingly I1 .z/ D I1 .0/sech2 z;

I2 .z/ D I1 .0/ tanh2 z:

(2.82)

Comparison with Eq. (2.62) yields 2 D 8

a2 2 i w=a je 1j2 A00 I1 .0/; c

(2.83)

with coupling factor A00 given by Eq. (2.65). The decay length 1= decreases with increasing intensity of the incident laser light. We note the identity

dA1 dz

2 C 2 A21 .p1 A21 1/ D 0:

(2.84)

This shows that the solution may be interpreted as the motion of a particle in a quartic potential at zero energy, or as the interface profile between two phases of a fluid [18]. The identity is equivalent with the conservation law (2.79). If the input laser is not tuned to the peak value we must use complex amplitudes A1 .z/; A2 .z/ and generalize the mode-coupling equations to [3, 19] dA1 D A1 A2 e i p z ; dz p1 dA2 D 2 A21 e i p z ; dz p2

(2.85)

with phase mismatch p D p2 2p1 nK:

(2.86)

With the normalization B1 D

p p1 A1 ;

B2 D

1p p2 A2 2

(2.87)

the mode-coupling equations can be expressed as dB1 D B1 B2 e i p z ; dz 1 dB2 D B12 e i p z ; dz 2

(2.88)

with coefficient p D 2:

(2.89)

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

41

With the complex notation B1 D b1 e i'1 ;

B2 D i b2 e i'2 ;

(2.90)

the mode-coupling equations (2.88) can be cast in the standard form with real variables [3] db1 D b1 b2 sin ; dz 1 db2 D b12 sin ; dz 2

d'1 D b2 cos ; dz 1 b2 d'2 D 1 cos ; dz 2 b2

(2.91)

with phase difference D p z C '2 2'1 :

(2.92)

The mode-coupling equations imply the energy conservation law, which may be expressed as b12 .z/ C 2b22 .z/ D 1:

(2.93)

With a final change of variables p v D b2 2;

u D b1 ;

D z

(2.94)

the equations become du D uv sin ; d dv D u2 sin ; d d d D s C cot ln.u2 v/; d d

s D

p :

(2.95)

These equations have the two conservation laws u2 C v2 D 1;

u2 v cos C

p 2 p 2 v DC v; 2 2 0

(2.96)

where the constant is determined by the initial values at z D 0 according to D u0 v20 cos 0 . In our case D 0, since v0 D 0. The equations can be solved in terms of the elliptic integral D

1 2

Z

v2

q 0

1 x.1 x/2 14 s 2 x 2

dx:

(2.97)

42

B.U. Felderhof et al.

0.6 0.5 0.4 v2 0.3 0.2 0.1 0.0 −20

−10

0

10

20

Δs Fig. 2.8 Plot of the reduced second-harmonic intensity v2 at fixed length L D 1= as a function of the reduced detuning parameter s D p= , where p is the phase mismatch. The notation is explained in Sect. 2.7

Explicitly D

p p F .arcsin.v= /j 2 /;

D 8=.8 C s 2 C

p s 4 C 16s 2 /; (2.98)

where F .'j 2 / is the elliptic integral of the first kind [20]. In particular F .'j1/ D 2 arctanh.tan.'=2// leads to v D tanh in agreement with Eq. (2.82). The expression Eq. (2.98) can be inverted to v./ D

p p sn.= ; /;

(2.99)

p with Jacobian elliptic function sn.= ; /. In Fig. 2.8 we plot the reduced second2 harmonic intensity v for fixed length D 1 as a function of the detuning parameter s. The plot shows a spectral line with sidewings. For fixed detuning parameter s the second-harmonic intensity varies periodically as a function of distance . Note that in the present theory the mode-coupling equations are assumed to hold on a length scale much larger than the period of the grating. This is in contrast to the theory of Zhao et al. [4], who assume mode-coupling equations on the scale of the period. The present formulation allows understanding of the effect of depletion in the framework of the well-known theory developed by Armstrong et al. [3] for second-harmonic generation in anisotropic crystals. Finally we note that it follows from Eq. (2.82) that for optimal phase matching the stretch of nonlinear susceptibility L1=2 over which the second-harmonic intensity I2 is one half of the input fundamental intensity I1 .0/ is given by L1=2 D

0:881 1 1 arctanh p D : 2

(2.100)

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

43

For the numerical example used in Eq. (2.75) we have 2 D 2:7 105 I1 .0/, so that L1=2 D

5:36 1013 cm; p 1 I1 .0/

(2.101)

p with 1 in esu and I1 .0/ in mW. The prefactor follows from 5:36 D 0:881= 0:027. Thus the half-length varies inversely with the second-order susceptibility and the square root of the input fundamental intensity. In Eq. (2.101) it is assumed that the radius of the tubelet r0 has the optimal value shown in Fig. 2.4.

2.8 Discussion We have presented a model calculation of second-harmonic generation in a circular cylindrical waveguide or optical fiber for a situation where the nonlinear material is isotropic and distributed in a radially symmetric manner. Though the geometry is not easy to realize experimentally, the calculation shows the essential features of the mechanism. A comparison with an earlier calculation for a planar waveguide [1] shows that the confinement in cylindrical geometry has distinct advantages. The work of Parameswaran et al. [8] shows that second-harmonic generation in cylindrical geometry can be realized experimentally and is quite effective. The conversion efficiency is sufficiently high that depletion of the fundamental must be taken into account. We have shown that depletion can be described in terms of the mode-coupling formalism developed by Armstrong et al. [3] for secondharmonic generation in anisotropic crystals.

References 1. A. Bratz, B.U. Felderhof, G. Marowsky, Appl. Phys. B 50, 393 (1990) 2. B.U. Felderhof, G. Marowsky, Appl. Phys. B 43, 161 (1987) 3. J.A. Armstrong, N. Bloembergen, J. Ducuing, P. S. Pershan, Phys. Rev. 127, 1918 (1962); reprinted in N. Bloembergen Nonlinear Optics (Addison-Wesley, Redwood City, 1992) 4. L.-M. Zhao, G.-K. Yue, Y.-S. Zhou, EPL 99, 34002 (2012) 5. M.E. Fermann, L. Li, M.C. Farries, L.J. Poyntz-Wright, L. Dong, Optics Lett. 14, 748 (1989) 6. T. Mizunami, T. Tsukuda, Y. Noi, K. Horimoto, Proc. Soc. Photo-Opt. Instrum. Eng. 5350, 115 (2004) 7. T. Mizunami, Y. Sadakane, Y. Tatsumoto, Thin Solid Films 516, 5890 (2008) 8. K.R. Parameswaran, J.R. Kurz, R.V. Roussev, M.M. Fejer, Optics Lett. 27, 43 (2002) 9. D. Marcuse, Theory of Dielectric Optical Waveguides (Academic, New York, 1974) 10. H. Kogelnik, in Integrated Optics, Topics Appllied Physics 7, ed. by T. Tamir (Springer, Berlin, 1979), p. 13 11. H.A. Haus Waves and Fields in Optoelectronics (Prentice Hall, Englewood Cliffs, 1974) 12. B.U. Felderhof, G. Marowsky, Appl. Phys. B 43, 161 (1991). 13. V. Mizrahi, J.E. Sipe, J. Opt. Soc. Am. B 5, 660 (1988)

44

B.U. Felderhof et al.

14. J.M. Chen, J. R. Bower, C. S. Wang, C. H. Lee, Opt. Commun. 9, 132 (1973) 15. C.K. Chen, T.F. Heinz, D. Ricard, Y.R. Shen, Phys. Rev. Lett. 46, 1010 (1981) 16. B. Dick, Chem. Phys. 96, 199 (1985) 17. O. Roders, O. Befort, G. Marowsky, D. Möbius, A. Bratz, Appl. Phys. B 59, 537 (1994) 18. N.G. van Kampen, Phys. Rev. A 135, 362 (1964) 19. H. Paul, Nichtlineare Optik II (Akademie-Verlag, Berlin, 1973) 20. M. Abramowitz, I.A. Stegun, Handbook of Mathematical Functions (Dover, New York, 1970)

Chapter 3

Nanoplasmonic Metal–Insulator–Metal Waveguides Moshik Cohen, Reuven Shavit, and Zeev Zalevsky

3.1 Introduction With the rapidly growing demand for higher data processing rates, silicon-based electronic devices approach fundamental speed and bandwidth limitations, which is an increasingly serious problem that impedes further progress in numerous fields of modern science and technology. These limitations arise from interconnect delays and from increased power dissipation of transistors as their gate lengths approach single-nanometer scale [1–4]. Possible solution for these setbacks may lay in photonics devices, as photons provide considerably superior information bandwidth and improved thermal properties compared with electrons [5, 6]. Although semiconductor-based optical devices were previously introduced [7–10], largescale integration of photonic circuitry has been fundamentally limited by their large, diffraction-limited size and by the poor optical response of silicon at optical frequencies. Recently, it has been suggested that surface plasmon nanophotonics may overcome these limitation [11–14]. Newly introduced plasmonic nanoantennas [12, 15–17], waveguides [18–21], and devices [18, 22–24] unlock an enormous potential for exciting new applications based on SPPs. Predominantly, nanometric

M. Cohen () Faculty of Engineering, Bar-Ilan University, Ramat-Gan 52900, Israel Department of Electrical and Computer Engineering, Ben-Gurion University of the Negev, Beer-Sheva 84105, Israel e-mail: [email protected] R. Shavit Department of Electrical and Computer Engineering, Ben-Gurion University of the Negev, Beer-Sheva 84105, Israel e-mail: [email protected] Z. Zalevsky Faculty of Engineering, Bar-Ilan University, Ramat-Gan 52900, Israel Bar-Ilan Institute for Nanotechnology and Advanced Materials, Ramat-Gan 52900, Israel e-mail: [email protected] G. Marowsky (ed.), Planar Waveguides and other Confined Geometries: Theory, Technology, Production, and Novel Applications, Springer Series in Optical Sciences 189, DOI 10.1007/978-1-4939-1179-0__3, © Springer ScienceCBusiness Media New York 2015

45

46

M. Cohen et al.

all-optical logic devices that use plasmonics as data carriers are of prime importance for future information processing and photonic computing technologies. Still, although plasmonic-based logic devices were recently introduced [10, 25], logic devices which operate directly on SPPs in deep nanoscale have not been reported. In Sect. 3.1, we design, fabricate, and characterize a novel, silicon-based alloptical nanoplasmonic exclusive or (XOR) gate. The device achieves smallest reported dimensions for plasmonic logic gate and therefore achieves significantly low losses and small delay times. The logic operation is obtained by interference of SPPs through ultrathin Ag film with measured lateral dimensions of 4 20 nm, achieving the smallest reported dimensions for all-optical logic gate. Additional logic and Boolean functionalities can be realized by engineering the interferometer dimensions. We propose a special excitation and waveguiding scheme which facilitates the launch of nanometric SPPs from laser illumination and rout them toward the gate. High-resolution (HR) atomic force microscopy (AFM) system with He–Ne laser at wavelength of 633 nm is used to excite and trace the nanoplasmonic waves along the structure and particularly at the device’s area. We theoretically and experimentally show full logic XOR functionality of the reported gate, with device operating at broad frequency range which enables multi-tera-bits per second (Tbit s1 ) data processing rates. In Sect. 3.2 we show that Kelvin probe force microscopy (KPFM) can image and characterize SPPs achieving molecular-scale resolution. Since SPPs are bound to the surface and confined to deep subwavelength scales, high-resolution imaging of nanoplasmonic modes using conventional optical microscopy is nearly impossible [26–29]. Subdiffraction optical imaging of surface plasmons can be achieved using near-field techniques, as scanning near-field optical microscope (SNOM) and its modifications that use metal tips [30–36]. In SNOM, a subwavelength optical aperture samples the average optical signal intensity as a function of position. However, spatial resolution and collection efficiency are both limited by the aperture size and by the distance between a sample and the tip. This is mainly because SNOM samples only the decaying or evanescent part of the optical signal outside the nanoscale object [37]. To date the smallest commercially available SNOM tips achieve aperture diameters of 50–100 nm ([CSL STYLE ERROR: reference with no printed form.]). Plasmonic imaging with nanometric spatial resolution can also be achieved using electron energy loss spectroscopy (EELS) [38–40], with time-resolved measurements that are also demonstrated using laser-excited photocathodes in electric microscopy [41, 42]. KPFM, also known as surface potential microscopy, is a variant of AFM which was first introduced in 1991 [43]. KPFM enables to measure the work function difference between a scanning tip and a surface with submolecular resolution and submilivolt sensitivity [44–49]. When a scanning probe tip is electrically connected to a conductive sample, a contact potential difference (CPD) will arise due to the different work functions of the tip and the sample. KPFM measures local variations in the CPD by applying a voltage between the sample and the tapping AFM tip so that the electric field caused by the CPD and the resulting force on the tip are compensated. For a certain tip position, the compensating voltage represents the local contact potential difference (LCPD) and can be determined either with a feedback loop or by measuring the

3 Nanoplasmonic Metal–Insulator–Metal Waveguides

47

voltage dependence frequency shift [43, 46, 50–52]. Recently, we used KPFM and space–time Fourier analysis to characterize SPP modes with resolution of 10 nm [53, 54]. Here, we show that KPFM can image and characterize surface plasmon polaritons with resolution at the single-nanometer scale. A theoretical model is proposed to define the relation between CPD and SPPs and provide an in-depth understanding of the imaging mechanism. We characterize plasmonic nanoantenna and waveguiding structures achieving resolution of only 2 nm. Additionally, we observe that the sign of the CPD can be used to obtain information on the electric field’s directionality, toward full-vector characterization of SPPs.

3.2 Nanoplasmonic Logic Circuitry Based on Multilayer Gap Waveguides The proposed system is comprised of two metal–insulator–metal (MIM) SPP waveguides connected to the dipole nanoantennas at one end and to the logic device in their other end. Figure 3.1a illustrates the operational concept of the proposed nanoplasmonic system. Each nanoantenna is illuminated by a laser and converts the incident light to propagating SPPs along the corresponding waveguide. The modes are guided to the device, where they undergo all-optical logic operation. The XOR

Fig. 3.1 Nanoplasmonic interferometer-based XOR gate integrated with SPP excitation and waveguiding system. (a) Schematic illustration of the reported nanoplasmonic system. Micronscale optical excitation is converted to nanoscale plasmonic waves by the resonant dipole nanoantennas, confined and guided via plasmonic MIM waveguides toward the plasmonic XOR device, which performs the logic operation. The inset shows a 3D illustration of the nanoplasmonic interferometer which is used to realize XOR logic functionality. s D 20 nm, the thickness of the internal metallic layer is • D 4 nm, and LI D 300 nm represents the overall interferometer length. (b) SEM image of the fabricated nanoplasmonic system

48

M. Cohen et al.

logic device consists of two MIM waveguides separated by a 4 nm (• D 4 nm)-thick metallic layer. The MIM waveguides comprising the nanoplasmonic interferometer are integrated with identical dielectric cores of two independent MIM plasmonic waveguides. In the other perimeter of the system, the waveguides are connected to resonant dipole nanoantennas to achieve efficient excitation of propagating SPPs from laser illumination. To fabricate nanoplasmonic devices, 20 nm Ag layer was sputtered on top of chemically cleaned wafers, via ion sputtering at vacuum levels of less than 9e-7 Torr without cooling. The structures were patterned using gallium focused ion beam (Ga FIB) with 7 nm ion beam spot size. The acceleration voltage was set to 5 KV and currents as low as 0.69 nA were applied. Figure 3.1b shows scanning electron microscopy (SEM) image of the fabricated nanometric interferometer, integrated with the plasmonic system. The silver structures are shown in bright colors, and the gray background represents the SOI substrate. We respectively mark the inputs and outputs of the device as “I1 ”, “I2 ”, and “Out”. The overall area occupied by the nanoplasmonic gate with the excitation system is 1 1 m, which is more than 200 times smaller compared with the system reported in [25]. The average surface roughness measured on the internal faces of the system is 2 nm, obtained by experimental optimization of the lithography process. The theoretical operation principle of the nanoplasmonic interferometer may be explained using the coupled-mode theory [55], which suggests that a structure built out of two identical slab waveguides with a subwavelength separation transfers light between the two waveguides with a constant phase shift of /2. The spatial periodicity of the power transfer between the two MIM waveguides depends on the magnitude of the wave number k D 2 /œSPP , where œSPP is the wavelength of the propagating plasmonic mode within the waveguide. In optical frequencies, the refractive index of metals can be expressed as n D ni C jnj , where the real part ni governs the phase of a signal and the imaginary part nj origins absorption. From the refractive index, we extract the relative permittivity by " D "0 C j"00 "0 D n2i n2j I

"00 D 2ni nj

(3.1)

where "0 and "00 are the real and imaginary part of ", respectively. The thickness of the silver metallic layer is numerically designed to accomplish relative phase shift of between the plasmonic modes, which is required to realize XOR operation [56]. The MIM waveguides comprising the interferometer are integrated with identical dielectric cores of two independent MIM plasmonic waveguides. In the other perimeter of the system, the waveguides are connected to resonant dipole nanoantennas to achieve efficient excitation of propagating SPPs from laser illumination. It was recently observed that excitation of MIM SPP waveguides using dipole nanoantennas achieves coupling efficiencies which are orders of magnitude

3 Nanoplasmonic Metal–Insulator–Metal Waveguides

49

higher compared with direct illumination of bare waveguide [57]. To achieve maximum excitation efficiency, we maximize the intensity of the electric field in the dipole gap and simultaneously minimize the impedance mismatch between the dipole and the waveguide by geometry optimization. These requirements are met by maximization of the net power flowing through the waveguide cross section, which also ensures flow of propagating SPPs toward the device. The net power flow is given by “ W D

n! o n dS Re P !

(3.2)

! where P is the Poynting vector for the propagating SPPs and ! n is a vector in the direction of wave propagation. The dimensions of the nanoantennas are optimized to achieve maximum W in the MIM waveguides. The numerical analysis and optimization of the structures were carried out using finite element method (FEM) commercial SW package HFSS V14 [58]. Figure 3.2a shows the 3D electromagnetic model for analysis and optimization of the system. The model is comprised of Ag plasmonic nanostructures deposited on SOI substrate, with the materials properties obtained from [53, 54]. Each nanoantenna is illuminated by a laser at a wavelength of 1.55 m, linearly polarized in the dipole direction and with parameterized incident angle. Each laser beam is focused to a radius of 1 m, centered at the origin of the corresponding nanoantenna. Selectively dense meshing at a maximum of 1 nm cell size was assigned at the metallic regions to precisely capture the plasmonic logic operation obtained by the device. The model was terminated by PML absorbing boundaries, matched to the material at the boundary of each computational domain. Convergence criterion was set to less than 1 % energy variation between three successive iterations of adaptive mesh refinement. The results are presented at the optical frequency, i.e., 194.55 THz. Figure 3.2c shows the numerically calculated electric field magnitude for XOR(“1”, “1”) D “0” logic operation, in which both nanoantennas are illuminated. The optical laser radiation is efficiently coupled to SPP modes that propagate through MIM waveguides toward the nanoplasmonic XOR device. Zoom in-to the area of the device shows destructive plasmon interference, which results in logic zero (“0”) at the output of the device, as emphasized in the inset. Figure 3.2d illustrates XOR(“1”, “0”) D “1” logic operation, with zoom in-to the area of the device shown in the inset shows the high field value which corresponds to logic “1”. For this case, a portion of the propagating SPPs is reflected from the device’s input and coupled to the other waveguide. The intensity of the undesired reflected field is 20 dB lower compared with that of the plasmon in the excited waveguide, i.e., S12 D 20 dB. Full modulation, i.e., 30 dB extinction ratio at the device’s output, is achieved after less than 300 nm of interference length (LI < 300 nm, as defined in Fig. 3.1a). This indicates a high-speed phase accumulation through tunneling of the plasmonic modes, until relative phase shift of between the waveguides is accomplished. Figure 3.2e, f shows the electric

50

M. Cohen et al.

a

b

c

d

f

e 4.00

3.50

I1

3.00

3.00

I1

2.50

Electric Field [V/m]

Electric Field [V/m]

3.50

Out

2.00 1.50 1.00 0.50

Out

2.50 2.00 1.50 1.00 0.50

0.00 0.00

0.25

0.50

0.75

1.00 D [mm]

1.25

1.50

1.75

2.00

0.00 0.00

0.25

0.50

0.75

1.00

1.25

1.50

1.75

2.00

D [mm]

Fig. 3.2 Theoretical analysis and design of the nanoplasmonic XOR gate and excitation system. (a) 3D EM model for the analysis and optimization of the nanoplasmonic device. (b) 2D description of the model. The graphs in Fig. 3.2e, f are plotted on the dashed line defined here. (c) 3D numerical calculation results of the system performance for XOR(“1”, “1”) D “0”; the device’s region is shown in the inset. (d) 3D numerical calculation results of the system performance for XOR(“1”, “0”) D “1”; the device’s region is shown in the inset. (e) Electric field magnitude along the system, for the case of XOR(“1”, “1”). The field is presented along the dashed line defined in Fig. 3.2b. The fields are plotted for three different phases of the laser excitation as the red, brown, and blue patterns that correspond to the excitation phases of 450, 500, and 550, respectively. (f) Electric field magnitude for XOR(“1”, “0”), plotted along the same geometry and for the same laser excitation phases as in Fig. 3.2e

3 Nanoplasmonic Metal–Insulator–Metal Waveguides

51

Fig. 3.3 Extinction ratio and power transfer analysis. (a) Extinction ratio as a function of the device’s length. (b) Electric fields in the device’s region for XOR(“1”, “1”) for • D 20 nm (upper image) and for • D 5 nm (lower image)

field magnitude at the center of the MIM waveguide and the device for XOR(“1”, “1”) D “0” and XOR(“1”, “1”) D “1”, respectively. The field is plotted along the dashed line defined in Fig. 3.2b, for three different phases of the illuminating lasers. Figure 3.2e shows the destructive interference results in logic “0” for the case of two active lasers. In Fig. 3.2f we observe similar electric field profiles at the input (located at D D 1.6 m) and output (located at D D 1.9 m) of the device, for logic level “1”, which is an essential property for the realization of logic gates. The black graph in Fig. 3.3a shows the extinction ratio versus the interference length, as the blue and red curves are XOR(“1”, “0”) and XOR(“1”, “1”), respectively. It is observed that the extinction ratio has two peaks, at L D 130 nm and L D 280 nm, corresponding to the peaks appearing in XOR(“1”, “0”). Extinction ratio of 35 dB is obtained for L D 280 nm; this high value is achieved due to strong destructive interference in XOR(“1”, “1”) response. The dependence of the power transfer as a function of the separation width was rigorously changing for values of • varying from 3 to 20 nm (• D S). Figure 3.3b shows the fields in the XOR device’s area for • D 20 nm and for • D 5 nm. We observe very low coupling between the waveguides for • D 20 nm, yielding luck in destructive interference. For • D 5 nm the coupling between the waveguides is higher, which results in destructive interference, and XOR(“1”, “1”) D “0” is accomplished. However, the observed “0” logic level achieved for • D 5 nm is significantly higher than the “0” logic level in the optimal design (• D 5 nm). The higher level of “0” results in degradation in the extinction ratio to a maximum of 12 dB, compared with 35 dB obtained in the optimal design. We use the surface electric potential measurement in frequency-modulated scanning Kelvin probe microscopy (FMSKPM) for experimental characterization of the reported nanoplasmonic structures. Surface potential microscopy measures the CPD, between the scanning tip and the characterized device. Generally, CPD is highly material dependent and related to the work functions of pure material and to additional surface dipole moments [59]. The contributions of bulk and surface plasmons to the work functions of materials [60–64] as well as to the van der Waals force [65, 66] were previously

52

M. Cohen et al.

Fig. 3.4 Performance characterization of the nanoplasmonic logic XOR gate, integrated with the excitation and waveguiding system. (a) 2D measurement of XOR(“1”, “1”) D “0” logic functionality. (b) HR SEM image of the fabricated structure for characterization of XOR(“1”, “1”) D “0” logic functionality. (c) 2D measurement of XOR(“0”, “1”) D “1” logic functionality. (d) HR SEM image of the fabricated structure for characterization of XOR(“0”, “1”) D “1” logic functionality

reported. Our AFM system includes He–Ne laser at wavelength of 633 nm which illuminates the entire sample to excite propagating SPPs from the nanoantenna gaps toward the XOR device. Figure 3.4a presents a 2D image of the surface electric potential on the sample for XOR(I1 D “1”, I2 D “1”) D “0” experiment, obtained for the structure shown in Fig. 3.4b. High field values are measured at both I1 and I2 , i.e., “1”. The XOR device realizes destructive interference between the SPPs at I1 and I2 , which results in low field values at the device’s output, i.e., “0”, as shown in Fig. 3.3b. Additional “hot spots” appear on the sample outside the plasmonic system. These “hot spots” represent localized surface plasmons excited by the interaction of the laser light and residual Ag nanoparticles, which remained on the sample after the lithography process. We note that even though the laser

3 Nanoplasmonic Metal–Insulator–Metal Waveguides

53

Fig. 3.5 Measured electric potential along the nanoplasmonic XOR device. (a) The blue line represents the measured field for XOR(I1 D ‘1’, I2 D “0”) D “1”. The black line represents the measured electric potential for XOR(I1 D ‘1’, I2 D ‘1’) D “0”. Dashed points correspond to discrete measured values. The length of the XOR gate is defined by the interference length for which 10 dB extinction ratio is observed, i.e., 150 nm. (b) The line along which the fields are presented for the two experimental setups

illuminates the whole structure, the dominant effect which governs the device operation is caused by propagating SPPs from the nanoantennas. Therefore we neglect effects caused by localized plasmons as well as by direct illumination of the device [67]. The ultrasmall size of the introduced nanoplasmonic structures poses strong limitation on the capability to precisely confine the laser beam to separately excite each nanoantenna. Therefore, we fabricated the identical device integrated with a single nanoantenna and MIM waveguide, as shown in Fig. 3.4d. Figure 3.4c shows the experimental results of XOR(I1 D “0”, I2 D “1”) D “1”, obtained by the characterization of the structure depicted in Fig. 3.4d. We observe low (“0”) field values at I1 and high field values (“1”) at I2 . For this combination of inputs, the device yields high field values at the output “Out”, as emphasized in Fig. 3.4d, resulting it XOR(“0”, “1”) D “1”. The reported nanoplasmonic gate implements Boolean XOR function on the propagating SPPs at inputs “I1 ”and “I2 ”. Hence, signal level of “1” at the device’s output “Out” results if only one of the inputs to the gate is at logic level “1”. Otherwise, logic “0” shall be measured at “Out”.

54

M. Cohen et al. Table 3.1 Experimental results at the output of the plasmonic logic XOR gate I1 0 0 1 1

I2 0 1 0 1

Out D XOR(I1 , I2 ) 0 1 1 0

Logic level of “1” at the inputs I1 and I2 is observed only when the corresponding nanoantenna is illuminated. A 10 dB extinction ratio between the logic levels at the device’s output “Out” is obtained at the device’s length of 150 nm, increasing up to 30 dB for the device’s length of 280 nm

Figure 3.5a shows the measured surface electric potential along the device for XOR(I1 D “1”, I2 D “1”) and XOR(I1 D “0”, I2 D “1”). The fields are presented from the inputs to the gate (L D 0) to the boundary of the physical device (L D 300 nm), as a function of the distance, L. The quanta are presented along a dashed line as described in Fig. 3.4b. We define an electric potential at the output of > 16 [mV] as the “1” or ‘ON’ state and potential < 6 [mV] as “0” or “OFF” state. For the case of XOR(I1 D “1”, I2 D “1”), destructive interference between the plasmonic modes along the device leads to rapid attenuation of the signal which results in “0” logic level at the output, as shown in the black graph of Fig. 3.5a. For the case of XOR(I1 D “0”, I2 D “1”) the field maintains high level through the device, achieving “1” at the output, as shown in the blue graph of Fig. 3.5a. The average surface roughness measured at the internal faces of the waveguides is 2 nm, with measured average periodicity of 10 nm. These values are much smaller than the wavelength of the propagating SPP, thus introducing small additional loss mechanism. These losses have little effect on the XOR performance, as the SPPs are attenuated for both XOR(“1”, “0”) and XOR(“1”, “1”) scenarios, thus having negligible effect on the extinction ratio. The experimental results are summarized in Table 3.1, which is in perfect agreement with the true table of a XOR device. Extinction ratio of 10 dB between the logic levels at the device’s output is accomplished after of only 150 nm, increasing up to 30 dB for the device’s length of 280 nm. The extremely small size of the device is achieved due to the introduced interferometry structure. Tunneling of the SPP modes through the nanometric separation layer leads to rapid phase accumulation, until relative phase shift of between the waveguides is accomplished. This architecture achieves the required phase accumulation much faster and after smaller interference length compared with the linear interference mechanism used in [25], where the phase accumulation is based on propagation length. As a result, the XOR device reported in this paper is more than three orders of magnitude smaller than the one reported in [25]. As micron-scale plasmonic devices [10, 25] suffer from high propagation loss, longer delay times, and huge size mismatch with CMOS electronics, the current concept can be the first nanoplasmonic architectural solution for all of these setbacks.

3 Nanoplasmonic Metal–Insulator–Metal Waveguides

a

55

b

62.50

Potential [dBmV]

50.00 37.50 25.00

13dB

12.50 0.00 -12.50 0.00

100.00

200.00

300.00

400.00

500.00 550.00

-1

Re {kx} [nm ]

Fig. 3.6 Spatial Fourier analysis of the measured surface electric potential on the sample. (a) The red curve shows the spatial FFT performed on the field along the XOR device, defined as “Line 1” in Fig. 3.5b. The blue curve presents spatial FFT analysis of the field outside the XOR device, performed on “Line 2” in Fig. 3.5b. (b) Definition of the lines on which we performed spatial FFT

We provide further experimental evidence for the existence of propagating SPPs along the device by observing the spatial frequency content of the measured fields on the sample. Since the gate exhibits imperfect impedance matching at its boundaries, partial standing waves are excited along the system. These standing waves are characterized by stationary spatial behavior, which is identical to the spatial frequency of the propagating SPPs and therefore can be detected via surface potential measurement in FM KPFM. To examine the spatial frequency content of the fields along the XOR gate, we performed spatial fast Fourier transform (FFT) on the surface electric potential measured along the sample. Figure 3.6a presents the spatial FFT results for two different measurements of the surface electric potential on the sample. The lines on which the FFT was calculated are detailed in Fig. 3.6b. The blue curve shows the spatial FFT of the surface potential along a line, which is outside the device (Line 1 in Fig. 3.6b), as the red curve is the spatial FFT of the surface potential along the center of the device (Line 2 in Fig. 3.6b). For both measurements shown in Fig. 3.6a the dominant field component appears at low spatial frequencies, a result which is in good agreement with the general electrostatic character of the measured potential and is due to the standing waves in the structure. However, we observe a strong spatial frequency component in the field along the device, at Re fkSPP g D 125 m1 . The amplitude of this component is 13 dB higher than the corresponding component in the measurement described by the blue curve. This result confirms the existence of propagating SPPs with wave vector of Re fkSPP g D 125 m1 inside the device, which is in excellent agreement with Dione [19] and Chen [68]. This further substantiates our theoretical analysis and experiments.

56

M. Cohen et al.

3.3 Molecular-Scale Imaging of Modes in Nanoplasmonic Slot Waveguides with Scanning Kelvin Probe Microscopy In this section we introduce for the first time, the imaging of surface plasmon polaritons with KPFM. Although traditionally considered as electrostatic measurement, we show that KPFM can characterize near fields at optical frequencies within single-nanometer scale. The experimental results are supported by 3D numerical calculations as well as analytical model. Figure 3.7 illustrates the process of SPP characterization with scanning KPFM. The origin of nanoplasmonic sensing with KPFM lies in the fact that KPFM measures the CPD between the scanning probe tip and the surface [46, 69]. The CPD is closely related with the charge distribution on the surface as well as with the surface plasmon polaritons [70–76]. When nanometallic structures are illuminated with optical radiation, coherent oscillations of free electrons are excited on the surface. These highly confined optically induced charge density waves preserve the frequency of incident photons and strongly affect the work function in the vicinity of the device. Optically excited variations in the work function of CdSe nanowires [77] and 2D array of subwavelength apertures [78] were recently characterized by electric force microscopy and KPFM. According to the Lorentz model, the motion of electrons in metals is governed by a second-order partial differential equation: 2 @ x @x 2 m C x D eE C (3.3) @t 2 @t

Fig. 3.7 Illustration of nanoplasmonic characterization with KPFM. Dipole nanoantenna is connected to MIM waveguide with nanometric gap width. The device is illuminated by a laser and the excited plasmons change the CPD between the tip and the surface, which is measured by KPFM with molecular-scale resolution

3 Nanoplasmonic Metal–Insulator–Metal Waveguides

57

Here m and e are the electron mass and charge, respectively; x is the electron displacement from the nucleus, D 1/ is the damping rate, is the spring constant, and E is the electric field. Assuming time harmonic behavior for the electric field and displacement, neglecting in the free electron region yields the Drude polarizability: P D Nex D

1 Ne 2 E .x; t/ m ¨2 C i ¨

(3.4)

where ! D 2f is the optical angular frequency of the electric field. The inplane relative permittivity ("k "r C i"i ) can be extracted from (3.4), using " D 1 C P/E.The real and imaginary parts of "k are attributed to intraband and interband transitions, respectively. Extended Drude model which considers the restoration force () is a preferred analytical description at the bound electron region. This model achieves excellent agreement for Au within 500–1,000 nm wavelength range [79]. Further improvement to the extended Drude model can be obtained by adding terms which carefully p describe the critical points (CP) [80, 81]. Near the plasma frequency, ! !p D Ne 2 =m"0, the relative permittivity is very small ("(! p ) ! 0). Hence, E(x, t) becomes a pure depolarization field with quanta of these charge oscillations referred to as plasmons. Using the relation between polarization and charge density Pol D r P, the surface electric potential is calculated by integrating the charge density function over the computational surface: “ V .r/ D

P ol .r/ ds 0 4"0 jr r 0 j

(3.5)

The charge density function may also be obtained by solving the Fock equations using an exchange potential operator [82, 83], a more accurate solution but computationally expensive when obtained numerically. The experimental setup used in this work is depicted in Fig. 3.8a. The sample is illuminated from above by a He–Ne laser at wavelength of 633 nm (! D 2.98 1015 r/s) linearly polarized in parallel with the dipole orientation. Since ¨ 1013 , the in-plane relative permittivity can be written as "k D "B ! 2p /! 2 C i! 3p /! 2 , with "B as the contribution of bound electrons and ! p as the plasma frequency. In our measurements topography and KPFM images are recorded sequentially using the lift mode technique to minimize cross talk between the measurements [84]. To this end, we first acquire the surface topography of a single line in tapping mode and then retrace this topography over the same line at a set lift height from the surface to measure the KPFM signal. To map the work function of the sample, we apply both AC voltage (VAC ) and DC voltage (VDC ) to the AFM tip. VAC generates oscillating electrical forces between the AFM tip and sample surface, and VDC nullifies the oscillating electrical forces that originated from CPD between the tip and sample surface. In our study, the tip–sample distance (H) significantly influences the resolution and sensitivity of the measurements. For small values of H, the KPFM image is dominated by short-range forces ( H6 ) like

58

M. Cohen et al.

Fig. 3.8 Schematic description of our KPFM experimental process and fabricated devices. (a) Schematic of the measurement principle. First the topography is acquired in tapping mode, and then the tip elevates to a set lift height, H, to create the CPD map. (b) Description of the analyzed nanoplasmonic devices. Dipole nanoantenna with arm length “LA” and gap “g” are connected to MIM waveguide of length LW. The thickness and width of all metal strips are 12 nm

van der Waals and capillary interactions. However, for larger values of H, long-range electrostatic and magnetic interactions ( H2 ) govern the results. Therefore, it is critical to optimize the lift height for high-quality imaging. To demonstrate unambiguously that we can measure and image plasmonic waves with molecular resolution, we chose to investigate hybrid devices of dipole nanoantennas integrated with MIM plasmonic waveguides, as shown in Fig. 3.8b. These devices are of prime importance for a large variety of applications and have several advantages for our study. First, the combination of nanoantenna and plasmonic waveguide enables to image both localized SPs and propagating SPPs. Localized SPs are optically excited at the nanoantenna and are coupled to propagating modes along the waveguide. Furthermore, by comparing CPD images with calculated vector fields, we show that KPFM measurements provide information on the directionality of the optical fields. The devices were fabricated by electron beam lithography (EBL), ion beam sputtering (Ag, 10 nm), and lift-off. Figure 3.9a presents a SEM image of the analyzed device, with geometrical dimensions of LW D 750 nm, LA D 100 nm, and g D 12 nm. The image was recorded at beam current of 0.4 nA and low accelerating voltage of 5 kV. Figure 3.9b shows an AFM topography image of the device in 3D, obtained using Si tip with 2 nm diameter. Subsequently, KPFM characterization of the same device was performed in lift mode while the device is illuminated by a He–Ne laser. The KPFM measurements were performed for tip–sample distances ranging from 10 to 250 nm. We observe that for small values of H, short-range interactions strongly affect the KPFM image. For larger tip–sample distances, the results are governed by the long-range interactions. The range of distances for which we obtained the best resolution was between 30 and 50 nm. Figure 3.9c shows the KPFM image recorded for tip–sample distance of H D 35 nm, which exhibits clear nanometric resolution. We observe two dipolar-like modes on the

3 Nanoplasmonic Metal–Insulator–Metal Waveguides

59

Fig. 3.9 SEM, AFM, KPFM, and numerical analysis of MIM nanoplasmonic device. (a) Highresolution SEM image of the fabricated and analyzed device. (b) 3D AFM topography image of the device. The image was recorded with Si super sharp tip with 2 nm aperture. (c) CPD image of the device under optical illumination with He–Ne laser at frequency of 474 THz, recorded with the same tip as (a). KPFM signal scale bar, 1.7–C1.7 V. (d) 3D numerical calculation (FEM) results of the analyzed device under optical illumination of He–Ne laser, similar to the experimental setup used to obtain the results in (c). Scale bar, 50 nm

antenna segments, with strong fields at the antenna ends and at the gap, as expected for a dipole plasmonic nanoantenna in the visible [53, 54]. The localized fields at the nanoantenna gap extend along the MIM waveguide, periodically changing their polarity. The modal behavior of the propagating SPPs along the waveguide is clearly observed in the KPFM image (Fig. 3.9c). Four periods of modes appear along the waveguide, represented by four spots with similar spatial dimensionality. The shapes of the waveguide as well as the field decay into its metallic arms are very well captured. This provides direct experimental evidence of a propagating surface plasmon polariton wave, obtained for the first time for SPPs confined to 12 10 nm mode area. Strong localized fields are observed also on the exterior metal–insulator interfaces of the waveguides, as predicted by the theory of SPPs ([CSL STYLE ERROR: reference with no printed form.]).

60

M. Cohen et al.

We observe that the measured KPFM fields on the ends of the nanoantenna are inversely polarized, with the field on the left edge as positive C1.5 V and the field on the right edge as negative –1.5 V. This important property of the KPFM signal is directly related with the direction of the optical field, as will be further discussed herein. This behavior is reproduced in 3D numerical calculation results, which were obtained using FEM commercial SW package HFSS V15 [53, 54]; see Fig. 3.9d. The calculated vector electric field along the sample is plotted at frequency of 474 THz (wavelength of 633 nm), with the arrows representing the direction of the field. KPFM signal of C1.5 V is measured at the left end of the nanoantenna (see Fig. 3.9c) that corresponds to the optical field direction of b z (see Fig. 3.9d). Consistently, a signal of 1.5 V is measured at the right end of the nanoantenna (see Fig. 3.9c) that corresponds to the optical field direction of Cb z (see Fig. 3.9d). These results contribute valuable information on the polarization of the electrical field, which cannot be obtained with standard SNOM which measures the average field’s magnitude. The high correlation between the calculated electric field and KPFM maps is a direct evidence that KPFM can measure fields at optical frequencies. Now, we show that KPFM can characterize SPPs with 2 nm spatial resolution, by resolving the propagation properties of MIM waveguide with gap (g) difference of 2 nm. Figure 3.10a presents the configuration of the analyzed devices. Figure 3.10b shows the calculated electric field at frequency of 474 THz (œ D 633 nm) for devices with LW D 900 nm, g D 10, 20, 30, and 60 nm. We observe inverse relation between the wavelength of the propagating SPPs, œSPP , and the gap width. As the gap width decreases, the plasmons are confined in both dimensions and vice versa; a confinement which increases the propagation loss. This nonlinear dispersion behavior is evidenced by the difference number of SPP periods that propagate within the waveguide. For g D 10 nm, seven periods of SPP modes are contained inside the waveguide, as for g D 60 nm only four periods are observed (see Fig. 3.10b). The calculated electric field along the center of the waveguide (dashed line in Fig. 3.10a) is shown in Fig. 3.10c, which further demonstrate the change in œSPP as the gap width increases. Figure 3.10d shows the KPFM signal map for g D 30 nm and the tip–sample distance of H D 35 nm, selected for maximum resolution. This image has similar characteristics to Fig. 3.9c with two main differences. First, only three periods of SPPs are contained within the waveguide (compared with four periods in Fig. 3.9c), this is due to the increase in gap width from 12 to 30 nm, a result which is in very good agreement with our calculations (Fig. 3.10b). Second, lower field intensities are observed at the gap and on both nanoantenna ends, mainly caused by impedance mismatch between the dipole and the waveguide and by geometrical shift from resonance. The exact spatial frequency of the propagating SPPs is detected by analyzing the frequency content of the KPFM measurements along the waveguide via spatial FFT. The black graph in Fig. 3.10e presents the results of spatial FFT performed on the KPFM signal inside the waveguide (marked by Line 1 in Fig. 3.10d), with the blue curve corresponding to the spatial FFT performed outside the device (Line 2). Both measurements shown

3 Nanoplasmonic Metal–Insulator–Metal Waveguides

61

Fig. 3.10 (a) Spatial frequency analysis of the nanoplasmonic devices using KPFM, spatial FFT, and numerical calculations. (b) Numerical analysis of the nanoplasmonic devices with g D 10 nm, 20, 30, and 60 nm, under optical illumination. Decrease in the spatial frequency (higher œSPP ) is observed when g is increased. (c) Calculated electric field at 474 THz plotted along the center of the MIM waveguides (dashed line in (a)) corresponding to the 3D results in (b). (d) CPD image of the device under optical illumination with He–Ne laser at frequency of 474 THz, recorded with Si super sharp tip at H D 35 nm. KPFM signal scale bar, 1.2–C1.2 V. (e) Spatial FFT results of the KPFM signal inside the waveguide (black graph, calculated along Line 1 in (d)) and outside the waveguide (Line 2 in (d)). Scale bars, 100 nm in (a) and 50 nm in (d)

in Fig. 3.10e have dominant field component at low frequencies, a result which is in good agreement with the general electrostatic character of KPFM and can be referred to the standing waves in the structure. However, we observe a strong spatial frequency component in the field along the device, œSPP D 248 nm. The amplitude of this component is 15 dB higher than the corresponding component in the measurement described by the blue curve, providing solid evidence for the existence of propagating SPPs inside the waveguide. We used this method to characterize the propagation properties in a series of fabricated nanoplasmonic devices with gap width varying between 10 and 30 nm in steps of only 2 nm (i.e., g D 10, 12, : : : ,30 nm), LA D 100 nm, and LW D 3,000 nm. For each KPFM measurement, we found œSPP by performing spatial FFT and measuring the plasmon wavelength at the peak of the curve (see Fig. 3.10e).

62

M. Cohen et al.

Fig. 3.11 SPP characterization with 2 nm resolution and experimental results for the device with an 8 nm gap width. (a) œSPP as a function of the gap width, g, obtained experimentally (black dots) and theoretically (continuous blue curve). (b) Topography image of the device with g D 8 nm, obtained with our AFM using supersharp Si tip. (c) KPFM image of the device in (b). Scale bars, 100 nm. KPFM signal scale bar, 1.3–C1.3 V

We use long waveguides (LW œSPP ) in order to minimize the standing waves in the device and improve the resolution. Figure 3.11a shows the experimentally obtained dispersion curve (blue graph), with the calculation results presented in the black curve. We observe different experimentally obtained plasmon propagation wavelength (œSPP ) for waveguides with gap difference of 2 nm, which confirm that KPFM can resolve SPPs with 2 nm resolution, currently limited by the aperture dimensions of the scanning probe. The maximum deviation between the calculated and experimental dispersion curves is • D 2.5 nm, less than 1 % from the mean œSPP . Figure 3.11b shows the fabrication result of a similar device with a gap width of g D 8 nm, with the KPFM measurement of this device presented in Fig. 3.11c. We see that for a gap width of 8 nm and smaller the waveguide does not support propagating SPP modes. Instead, the localized SPPs at the antenna gap decay exponentially, similar to a single interface plasmonic waveguide. This can be explained by the very small gap width, which prevents mode hybridation from the two metal–air interfaces of the waveguide. This behavior is attributed also to the metal roughness (1 nm in each face, overall 2 nm) which size is now 25 % of the gap width.

3.4 Summary This chapter provides a deep insight into highly confined MIM plasmonic waveguides, including two sections with novel contributions. In the first section we propose as well as validate theoretically and experimentally for the first time the capability to compress all-optical logic devices into volumes smaller than œ3 /15,500. By employing extremely confined SPPs as information carriers in optical frequencies, the reported nanoplasmonic binary XOR gate exhibits the speed and bandwidth performances of photonics, with dimensions of integrated electronics.

3 Nanoplasmonic Metal–Insulator–Metal Waveguides

63

Extinction ratio of 10 dB is measured at the output for the device’s length of 150 nm, rising up to 30 dB for the device’s length of only 280 nm. The introduced interferometry architecture can be used to realize a variety of plasmonic logic in deep nanoscale. In the second section, we used AFM and KPFM to image MIM nanoplasmonic devices with smallest reported gap dimensions of 8 nm, providing first ever experimental evidence for propagating SPP modes in these dimensions. We have shown that KPFM can achieve SPP imaging resolution of 2 nm and provide 2D images which are in good agreement with theoretical calculations obtained at optical frequencies. Our findings and results advance the scientific frontier and establish MIM geometry and SPPs as future nanoscale technologies for a huge variety of applications: applications ranging from nanoscale optical microscopy and spectroscopy, integrated optical nanocircuitry, optoelectronics engineering to ultrasensitive sensing and quantum nanoplasmonics.

References 1. M.L. Brongersma, V.M. Shalaev, The case for plasmonics. Science 328, 440–441 (2010). doi:10.1126/science.1186905 2. J.A. Dionne, L.A. Sweatlock, M.T. Sheldon et al., Silicon-based plasmonics for on-chip photonics. IEEE J. Sel. Top. Quant. Electron. 16, 295–306 (2010). doi:10.1109/JSTQE.2009.2034983 3. E. Ozbay, Plasmonics: merging photonics and electronics at nanoscale dimensions. Science 311, 189–193 (2006). doi:10.1126/science.1114849 4. J.A. Schuller, E.S. Barnard, W. Cai et al., Plasmonics for extreme light concentration and manipulation. Nat. Mater. 9, 193–204 (2010). doi:10.1038/nmat2630 5. N. Engheta, Circuits with light at nanoscales: optical nanocircuits inspired by metamaterials. Science 317, 1698–1702 (2007). doi:10.1126/science.1133268 6. R. Kirchain, L. Kimerling, A roadmap for nanophotonics. Nat. Photonics 1, 303–305 (2007). doi:10.1038/nphoton.2007.84 7. V.R. Almeida, C.A. Barrios, R.R. Panepucci, M. Lipson, All-optical control of light on a silicon chip. Nature 431, 1081–1084 (2004). doi:10.1038/nature02921 8. L. Bi, J. Hu, P. Jiang et al., On-chip optical isolation in monolithically integrated non-reciprocal optical resonators. Nat. Photonics 5, 758–762 (2011). doi:10.1038/nphoton.2011.270 9. C. Koos, P. Vorreau, T. Vallaitis et al., All-optical high-speed signal processing with silicon–organic hybrid slot waveguides. Nat. Photonics 3, 216–219 (2009). doi:10.1038/nphoton.2009.25 10. H. Wei, Z. Wang, X. Tian et al., Cascaded logic gates in nanophotonic plasmon networks. Nat. Comm. 2, 387 (2011). doi:10.1038/ncomms1388 11. A.G. Curto, G. Volpe, T.H. Taminiau et al., Unidirectional emission of a quantum dot coupled to a nanoantenna. Science 329, 930–933 (2010). doi:10.1126/science.1191922 12. A. Kinkhabwala, Z. Yu, S. Fan et al., Large single-molecule fluorescence enhancements produced by a bowtie nanoantenna. Nat. Photonics 3, 654–657 (2009). doi:10.1038/nphoton.2009.187 13. S. Lal, S. Link, N.J. Halas, Nano-optics from sensing to waveguiding. Nat. Photonics 1, 641–648 (2007). doi:10.1038/nphoton.2007.223 14. M. Schnell, A. García-Etxarri, A.J. Huber et al., Controlling the near-field oscillations of loaded plasmonic nanoantennas. Nat. Photonics 3, 287–291 (2009). doi:10.1038/nphoton.2009.46

64

M. Cohen et al.

15. T. Kosako, Y. Kadoya, H.F. Hofmann, Directional control of light by a nano-optical Yagi–Uda antenna. Nat. Photonics 4, 312–315 (2010). doi:10.1038/nphoton.2010.34 16. T. Pakizeh, M. Käll, Unidirectional ultracompact optical nanoantennas. Nano Lett. 9, 2343–2349 (2009). doi:10.1021/nl900786u 17. T. Shegai, S. Chen, V.D. Miljkovi´c et al., A bimetallic nanoantenna for directional colour routing. Nat. Comm. 2, 481 (2011). doi:10.1038/ncomms1490 18. S.I. Bozhevolnyi, V.S. Volkov, E. Devaux et al., Channel plasmon subwavelength waveguide components including interferometers and ring resonators. Nature 440, 508–511 (2006). doi:10.1038/nature04594 19. J.A. Dionne, L.A. Sweatlock, H.A. Atwater, A. Polman, Plasmon slot waveguides: towards chip-scale propagation with subwavelength-scale localization. Phys. Rev. B 73, 035407 (2006). doi:10.1103/PhysRevB.73.035407 20. J.R. Krenn, Nanoparticle waveguides: watching energy transfer. Nat. Mater. 2, 210–211 (2003). doi:10.1038/nmat865 21. R.F. Oulton, V.J. Sorger, D.A. Genov et al., A hybrid plasmonic waveguide for subwavelength confinement and long-range propagation. Nat. Photonics 2, 496–500 (2008). doi:10.1038/nphoton.2008.131 22. P. Berini, I.D. Leon, Surface plasmon-polariton amplifiers and lasers. Nat. Photonics 6, 16–24 (2012). doi:10.1038/nphoton.2011.285 23. H. Yan, X. Li, B. Chandra et al., Tunable infrared plasmonic devices using graphene/insulator stacks. Nat. Nanotech. 7, 330–334 (2012). doi:10.1038/nnano.2012.59 24. N.I. Zheludev, Photonic–plasmonic devices: a 7-nm light pen makes its mark. Nat. Nanotech. 5, 10–11 (2010). doi:10.1038/nnano.2009.460 25. Y. Fu, X. Hu, C. Lu et al., All-optical logic gates based on nanoscale plasmonic slot waveguides. Nano Lett. 12, 5784–5790 (2012). doi:10.1021/nl303095s 26. E. Abbe, Beiträge zur theorie des mikroskops und der mikroskopischen Wahrnehmung. Arch. ür Mikrosk. Anat. 9, 413–418 (1873). doi:10.1007/BF02956173 27. W. Heisenberg, Über den anschaulichen Inhalt der quantentheoretischen Kinematik und Mechanik. Z. Für Phys. 43, 172–198 (1927). doi:10.1007/BF01397280 28. A. Sommerfeld, Ueber die Fortpflanzung elektrodynamischer Wellen längs eines Drahtes. Ann. Phys. 303, 233–290 (1899). doi:10.1002/andp.18993030202 29. E. Abbe, Beiträge zur Theorie des Mikroskops und der mikroskopischen Wahrnehmung. Arch. Für Mikrosk. Anat. 9, 413–418 (1873). doi:10.1007/BF02956173 30. E. Betzig, A. Lewis, A. Harootunian et al., Near field scanning optical microscopy (NSOM). Biophys. J. 49, 269–279 (1986). doi:10.1016/S0006-3495(86)83640-2 31. J. Chen, M. Badioli, P. Alonso-González et al., Optical nano-imaging of gate-tunable graphene plasmons. Nature 487, 77–81 (2012). doi:10.1038/nature11254 32. R. Esteban, R. Vogelgesang, J. Dorfmüller et al., Direct near-field optical imaging of higher order plasmonic resonances. Nano Lett. 8, 3155–3159 (2008). doi:10.1021/nl801396r 33. Z. Fei, A.S. Rodin, G.O. Andreev et al., Gate-tuning of graphene plasmons revealed by infrared nano-imaging. Nature 487, 82–85 (2012). doi:10.1038/nature11253 34. R. Hillenbrand, T. Taubner, F. Keilmann, Phonon-enhanced light–matter interaction at the nanometre scale. Nature 418, 159–162 (2002). doi:10.1038/nature00899 35. Y. Inouye, S. Kawata, Near-field scanning optical microscope with a metallic probe tip. Opt. Lett. 19, 159–161 (1994). doi:10.1364/OL.19.000159 36. M. Schnell, P. Alonso-González, L. Arzubiaga et al., Nanofocusing of mid-infrared energy with tapered transmission lines. Nat. Photonics 5, 283–287 (2011). doi:10.1038/nphoton.2011.33 37. P.E. Batson, Plasmonic modes revealed. Science 335, 47–48 (2012). doi:10.1126/science.1215588 38. H. Duan, A.I. Fernández-Domínguez, M. Bosman et al., Nanoplasmonics: classical down to the nanometer scale. Nano Lett. 12, 1683–1689 (2012). doi:10.1021/nl3001309 39. V. Iberi, N. Mirsaleh-Kohan, J.P. Camden, understanding plasmonic properties in metallic nanostructures by correlating photonic and electronic excitations. J. Phys. Chem. Lett. 4, 1070–1078 (2013). doi:10.1021/jz302140h

3 Nanoplasmonic Metal–Insulator–Metal Waveguides

65

40. J.A. Scholl, A. García-Etxarri, A.L. Koh, J.A. Dionne, Observation of quantum tunneling between two plasmonic nanoparticles. Nano Lett. 13, 564–569 (2013). doi:10.1021/nl304078v 41. J.S. Kim, T. LaGrange, B.W. Reed et al., Imaging of transient structures using nanosecond in situ TEM. Science 321, 1472–1475 (2008). doi:10.1126/science.1161517 42. A.H. Zewail, Four-dimensional electron microscopy. Science 328, 187–193 (2010). doi:10.1126/science.1166135 43. M. Nonnenmacher, M.P. O’Boyle, H.K. Wickramasinghe, Kelvin probe force microscopy. Appl. Phys. Lett. 58, 2921–2923 (1991). doi:10.1063/1.105227 44. P. Grutter, Scanning probe microscopy: seeing the charge within. Nat. Nanotech. 7, 210–211 (2012). doi:10.1038/nnano.2012.43 45. H. Hoppe, T. Glatzel, M. Niggemann et al., Kelvin Probe force microscopy study on conjugated polymer/fullerene bulk heterojunction organic solar cells. Nano Lett. 5, 269–274 (2005). doi:10.1021/nl048176c 46. H.O. Jacobs, H.F. Knapp, A. Stemmer, Practical aspects of Kelvin probe force microscopy. Rev. Sci. Instr. 70, 1756 (1999). doi:10.1063/1.1149664 47. F. Mohn, L. Gross, N. Moll, G. Meyer, Imaging the charge distribution within a single molecule. Nat. Nanotech. 7, 227–231 (2012). doi:10.1038/nnano.2012.20 48. E.J. Spadafora, R. Demadrille, B. Ratier, B. Grévin, Imaging the carrier photogeneration in nanoscale phase segregated organic heterojunctions by kelvin probe force microscopy. Nano Lett. 10, 3337–3342 (2010). doi:10.1021/nl101001d 49. L. Yan, C. Punckt, I.A. Aksay et al., Local voltage drop in a single functionalized graphene sheet characterized by kelvin probe force microscopy. Nano Lett. 11, 3543–3549 (2011). doi:10.1021/nl201070c 50. S.A. Burke, J.M. LeDue, Y. Miyahara et al., Determination of the local contact potential difference of PTCDA on NaCl: a comparison of techniques. Nanotechnology 20, 264012 (2009). doi:10.1088/0957-4484/20/26/264012 51. L. Nony, A.S. Foster, F. Bocquet, C. Loppacher, Understanding the atomic-scale contrast in Kelvin probe force microscopy. Phys. Rev. Lett. 103, 036802. arXiv:09074015 (2009). doi:10.1103/PhysRevLett.103.036802 52. S. Sadewasser, P. Jelinek, C.-K. Fang et al., New insights on atomic-resolution frequencymodulation kelvin-probe force-microscopy imaging of semiconductors. Phys. Rev. Lett. 103, 266103 (2009). doi:10.1103/PhysRevLett.103.266103 53. M. Cohen, Z. Zalevsky, R. Shavit, Towards integrated nanoplasmonic logic circuitry. Nanoscale 5, 5442–5449 (2013). doi:10.1039/C3NR00830D 54. M. Cohen, Z. Zalevsky, R. Shavit, Towards integrated nanoplasmonic logic circuitry. Nanoscale (2013). doi:10.1039/C3NR00830D 55. A. Yariv, Coupled-mode theory for guided-wave optics. IEEE J. Quant. Electron. 9, 919–933 (1973). doi:10.1109/JQE.1973.1077767 56. O. Limon, Z. Zalevsky, Nanophotonic interferometer realizing all-optical exclusive or gate on a silicon chip. Opt. Eng. 48, 064601–064601 (2009). doi:10.1117/1.3156021 57. A. Andryieuski, R. Malureanu, G. Biagi et al., Compact dipole nanoantenna coupler to plasmonic slot waveguide. Opt. Lett. 37, 1124–1126 (2012). doi:10.1364/OL.37.001124 58. V.G. Kravets, G. Zoriniants, C.P. Burrows et al., Composite Au nanostructures for fluorescence studies in visible light. Nano Lett. 10, 874–879 (2010). doi:10.1021/nl903498h 59. M. Nonnenmacher, M. O’Boyle, H.K. Wickramasinghe, Surface investigations with a Kelvin probe force microscope. Ultramicroscopy 42–44(Part 1), 268–273 (1992). doi:10.1016/03043991(92)90278-R 60. I. Brodie, Uncertainty, topography, and work function. Phys. Rev. B 51, 13660–13668 (1995). doi:10.1103/PhysRevB.51.13660 61. F.J. García de Abajo, The role of surface plasmons in ion-induced kinetic electron emission. Nucl. Instr. Meth. Phys. Res. Sect. B Beam Interact. Mater. Atoms 98, 445–449 (1995). doi:10.1016/0168-583X(95)00164-6 62. F.A. Gutierrez, J. Díaz-Valdés, H. Jouin, Bulk-plasmon contribution to the work function of metals. J. Phys. Condens. Matter 19, 326221 (2007). doi:10.1088/0953-8984/19/32/326221

66

M. Cohen et al.

63. R. Mehrotra, J. Mahanty, Free electron contribution to the workfunction of metals. J. Phys. C Solid State Phys. 11, 2061–2064 (1978). doi:10.1088/0022-3719/11/10/016 64. M. Schmeits, A. Lucas, Physical adsorption and surface plasmons. Surf. Sci. 64, 176–196 (1977). doi:10.1016/0039-6028(77)90265-5 65. E. Gerlach, Equivalence of van der Waals forces between Solids and the surface-plasmon interaction. Phys. Rev. B 4, 393–396 (1971). doi:10.1103/PhysRevB.4.393 66. N.R. Hill, M. Haller, V. Celli, Van der Waals forces and molecular diffraction from metal surfaces, with application to Ag(111). Chem. Phys. 73, 363–375 (1982). doi:10.1016/03010104(82)85175-6 67. J. Wen, S. Romanov, U. Peschel, Excitation of plasmonic gap waveguides by nanoantennas. Opt. Express 17, 5925–5932 (2009). doi:10.1364/OE.17.005925 68. J. Chen, G.A. Smolyakov, S.R. Brueck, K.J. Malloy, Surface plasmon modes of finite, planar, metal-insulator-metal plasmonic waveguides. Opt. Express 16, 14902–14909 (2008). doi:10.1364/OE.16.014902 69. W. Melitz, J. Shen, A.C. Kummel, S. Lee, Kelvin probe force microscopy and its application. Surf. Sci. Rep. 66, 1–27 (2011). doi:10.1016/j.surfrep.2010.10.001 70. C. Barth, C.R. Henry, Surface double layer on (001) surfaces of alkali halide crystals: a scanning force microscopy study. Phys. Rev. Lett. 98, 136804 (2007). doi:10.1103/PhysRevLett.98.136804 71. A.J. Bennett, Influence of the electron charge distribution on surface-plasmon dispersion. Phys. Rev. B 1, 203–207 (1970). doi:10.1103/PhysRevB.1.203 72. W. Ekardt, Work function of small metal particles: self-consistent spherical jellium-background model. Phys. Rev. B 29, 1558–1564 (1984). doi:10.1103/PhysRevB.29.1558 73. L. Gross, F. Mohn, P. Liljeroth et al., Measuring the charge state of an adatom with noncontact atomic force microscopy. Science 324, 1428–1431 (2009). doi:10.1126/science.1172273 74. T. König, G.H. Simon, H.-P. Rust et al., Measuring the charge state of point defects on MgO/Ag(001). J. Am. Chem. Soc. 131, 17544–17545 (2009). doi:10.1021/ja908049n 75. T. Leoni, O. Guillermet, H. Walch et al., Controlling the charge state of a single redox molecular switch. Phys. Rev. Lett. 106, 216103 (2011). doi:10.1103/PhysRevLett.106.216103 76. C. Sommerhalter, T.W. Matthes, T. Glatzel et al., High-sensitivity quantitative Kelvin probe microscopy by noncontact ultra-high-vacuum atomic force microscopy. Appl. Phys. Lett. 75, 286–288 (1999). doi:10.1063/1.124357 77. S. Schäfer, Z. Wang, R. Zierold et al., Laser-induced charge separation in CdSe nanowires. Nano Lett. 11, 2672–2677 (2011). doi:10.1021/nl200770h 78. J.A. Hutchison, A. Liscio, T. Schwartz et al., Tuning the work-function via strong coupling. Adv. Mater. 25, 2481–2485 (2013). doi:10.1002/adma.201203682 79. A. Vial, A.-S. Grimault, D. Macías et al., Improved analytical fit of gold dispersion: application to the modeling of extinction spectra with a finite-difference time-domain method. Phys. Rev. B 71, 085416 (2005). doi:10.1103/PhysRevB.71.085416 80. P.G. Etchegoin, E.C. Le Ru, M. Meyer, An analytic model for the optical properties of gold. J. Chem. Phys. 125, 164705 (2006). doi:10.1063/1.2360270 81. A. Vial, T. Laroche, Description of dispersion properties of metals by means of the critical points model and application to the study of resonant structures using the FDTD method. J. Phys. Appl. Phys. 40, 7152 (2007). doi:10.1088/0022-3727/40/22/043 82. J. Bardeen, Theory of the work function. II. The surface double layer. Phys. Rev. 49, 653–663 (1936). doi:10.1103/PhysRev.49.653 83. J.C. Slater, H.M. Krutter, The Thomas-Fermi method for metals. Phys. Rev. 47, 559–568 (1935). doi:10.1103/PhysRev.47.559 84. H.O. Jacobs, H.F. Knapp, S. Müller, A. Stemmer, Surface potential mapping: a qualitative material contrast in SPM. Ultramicroscopy 69, 39–49 (1997). doi:10.1016/S03043991(97)00027-2

Chapter 4

Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber Cladding Jason R. Grenier, Moez Haque, Luís A. Fernandes, Kenneth K.C. Lee, and Peter R. Herman

4.1 Introduction Over the past forty years, single-mode optical fibers have been used to guide encoded light signals over long distances at fast speeds, high modulation rates (100 GB/s to TB/s), and exceptionally low transmission loss (0.2 dB/km). Today, there is more than 1.8 billion kilometers [1] of fiber deployed around the globe, much of which forms the backbone of today’s Internet. Optical fibers also appear in many other useful forms that include large-core multimode, multicore, coreless, and photonic crystal fibers, finding broad application from the doped fibers that underpin high-power fiber lasers to the facile biomedical tools [2] used for in vivo diagnostic, endoscopic, and surgical procedures. A major challenge in optical fiber technology is creating optical, interconnecting, microfluidic, and sensing devices that can penetrate through the thick cladding layer and reach into the core waveguide. One traditional approach has been to pull on bundled fibers as they are heated and tapered to make fused-fiber directional couplers [3]. A less invasive procedure was discovered by Hill and coworkers in 1978 that imprinted Bragg-grating structures directly within the core waveguide under UV laser exposure [4]. Such in-core fiber Bragg gratings (FBGs) manipulate the spectral response of the waveguide to serve as, for example, wavelength division multiplexing (WDM) filters or dispersion compensators in telecommunication networks, mirrors in fiber lasers, and static or dynamic sensing elements for strain, temperature, and refractive index detection in other applications [5, 6]. However, these and other related methods are directed mainly at the core waveguide at the center of the fiber, where light guiding is typically confined to less than 1% of the total cross-sectional fiber area for the case of single-mode

J.R. Grenier () • M. Haque • L.A. Fernandes • K.K.C. Lee • P.R. Herman Department of Electrical and Computer Engineering, University of Toronto, Institute for Optical Sciences, 10 Kings College Rd., Toronto, Ontario, M5S 3G4, Canada e-mail: [email protected]; [email protected] G. Marowsky (ed.), Planar Waveguides and other Confined Geometries: Theory, Technology, Production, and Novel Applications, Springer Series in Optical Sciences 189, DOI 10.1007/978-1-4939-1179-0__4, © Springer ScienceCBusiness Media New York 2015

67

68

J.R Grenier et al.

a

b

SMF Core

ide

FBG

u eg

v

fs

wa

Fig. 4.1 Femtosecond laser writing of a (a) directional coupler in bulk glass and (b) Bragg grating in a fiber core waveguide

optical fibers. There exists a large and relatively unexplored volume in which to consider cladding devices that promise to add significantly more functionality and improve the value of the optical fiber. Several advances are emerging in the direction of fiber cladding devices, including the surface functionalization of cladding surfaces for label-free chemical, biological, and acoustic sensing [7, 8], acid thinning of fibers for evanescent [9] and interferometric sensing [10, 11], laser writing of long period waveguide gratings to couple and sense from fiber cladding modes [12], and laser drilling of microholes to the core waveguide for sensing [13, 14]. An alternate direction for increasing the performance of optical fiber is the formation of multicore waveguides within a single fiber. Such fibers recently enabled a record 1.05 Petabits/s communication rate [15] while the writing of FBGs into the individual waveguide cores served to define a novel temperature-independent two-axis bend sensor [16]. Here, the core waveguides are independent and isolated from each other and pose significant packaging challenges for efficient light coupling at the fiber facets. To further expand the opportunity for fiber cladding photonic and sensing devices, a threedimensional (3D) internal fabrication technology that can form optical devices and interconnections around and between the waveguides and also embed microfluidic and other microelectromechanical system (MEMS) structures to interact with the guided light is highly desirable. A major opportunity for creating higher-performance fiber cladding devices comes from the rapidly expanding field of ultrashort pulsed laser processing of transparent materials. Such lasers have opened a new realm of opportunities for 3D writing of compact micro-optical systems directly inside the bulk of transparent materials [17, 18] as depicted in Fig. 4.1a. Here, nonlinear optical absorption precisely confines laser interactions within a small focal volume where optical breakdown, multiphoton and/or tunnel ionization, electron avalanche, nonequilibrium heating, dense plasma formation, and micro-explosion evolve on record short-time and small-size scales [19–22]. This highly nonlinear physics regime briefly generates extreme temperatures that, under the right condition,

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

69

can mitigate significant shock- or thermally induced collateral damage [23]. Hence, this physics can be favorably manipulated to fabricate 3D optical devices such as: buried optical waveguides [24], volume gratings [25], Bragg-grating waveguides (BGWs) [26], directional couplers [27, 28], waveguide lasers [29], mode converters [30], and second-harmonic waveguide sources [31] in bulk glasses. One unusual aspect of femtosecond laser interactions in fused silica is the formation of nanogratings [32] that underlie significant new opportunities for creating birefringent optical waveguides [33], polarization-selective diffractive optical elements [34], and buried optical waveplates [35]. The nanogratings further open the way for preferential etching [36–39] to enable 3D fabrication of buried microfluidics with submicron resolution by the method known as femtosecond laser irradiation with chemical etching (FLICE). An etching contrast ratio of up to 280:1 between laser-processed and unmodified volumes in fused silica was demonstrated with a range of 2.5–20 % hydrofluoric acid (HF) solutions [38, 40–42]. The 3D FLICE technique enables unprecedented flexibility in fabricating 3D lab-on-chips (LOCs) in fused silica with optically smooth 10 nm (rms) surface roughness [43] and compares well with the 0.8 nm (rms) surface roughness found without nanograting formation in Foturan® photosensitive glass after post-baking and post-annealing steps [44]. FLICE therefore provides a major opportunity to continue reducing biological and chemical laboratory processes from bulky freespace systems toward dense packaging beyond the current planar LOC geometries as reviewed by Whitesides [45] and new 3D design approaches for highly advanced and packaged optofluidic microsystems as reviewed by Osellame et al. [46] and Xu et al. [47]. The pure fused silica cladding found in most types of standard, multicore, and photonic crystal fiber presents an ideal material platform on which to bring microfluidic and structural components into even more compact size scales. By wrapping microfluidic and optical components around the guiding core waveguide of existing fiber-optic technology, one envisions a new concept for lab-in-fiber (LIF) devices. The fused silica cladding is highly favorable for biocompatibility and resistance to chemical erosion and therefore presents a promising LIF platform. LIF offers superior packaging advantages over LOCs by (1) harnessing the mechanical flexibility and robustness of optical fiber, (2) naturally facilitating intimate optical interrogation of microfluidic and micro-reactor components, and (3) providing a convenient platform for interconnecting with light sources, diagnostics, and fiber interreactors. Lab-in-fiber concepts are only recently emerging for creating multifunctional sensing and actuating devices to probe micro- and nanoscale volumes in optical fiber. Bennion and coworkers [48–51] were first to apply FLICE in glass fiber, taking advantage of the 3D direct laser writing to template and then open up cladding microfluidic networks. Although the rough FLICE surfaces led to significant optical insertion loss, much smoother channel walls of 10 nm (rms) roughness were recently demonstrated in bulk glass [43]. Hence, the 3D direct laser writing and FLICE

70

J.R Grenier et al.

techniques are examined here toward new prospects for creating LIF and smart catheter devices that can efficiently exchange information and combine sensing data for broad opportunity in telecom and local area networks, security and defense systems, medical diagnostic and surgical procedures, and low-cost health-care products. This chapter examines the emerging domain of laser microstructuring and inscribing of optical fibers to embed and integrate highly functional optical, microfluidic, and microelectromechanical devices that interconnect efficiently with the fiber core. In background research, one can find numerous examples of laser processing into the core of optical fiber, such as the writing of FBGs by UV lasers [4] or femtosecond lasers with phase mask [52] or point-by-point [53, 54] methods (Fig. 4.1b). However, the direct laser writing into the fiber cladding has remained elusive due to strong beam distortion caused by the spherical and astigmatic optical aberration at the small fiber diameter, typically 125 m for telecommunication fiber. The approach adopted here for undistorted 3D processing inside optical fiber was met with a 1.25 numerical aperture (NA) oil-immersion lens [55], the topic of Sect. 4.2. This distortion-free writing enabled the formation of numerous fiber cladding devices on which we have sought to improve the functionality of optical fibers. This technique promises to overcome many of the challenges and high costs otherwise seen in connecting and packaging optical fiber with discrete bulk devices. The first devices presented here are aimed at the challenge of coupling light out of the core waveguide of a single-mode fiber (SMF) into laser-written cladding waveguides. Section 4.3 presents the spectral coupling characteristics of laserwritten X-couplers, S-bend couplers, and directional couplers. Coreless optical fiber is further introduced as an alternative platform for harnessing symmetric coupling between laser-written core and cladding waveguides. The polarization properties of the couplers are further examined and directions defined for designing polarization-selective optical taps and polarization beam splitters that exploit a laserinduced waveguide birefringence. Section 4.4 begins with the optical properties of the laser-written waveguides and introduces the following examples of photonic cladding devices: BGW filters comparing formation in the fiber core waveguide and the cladding, an in-fiber Mach-Zehnder interferometer (MZI), and a distributed position-shape-temperature sensor. Section 4.5 shows how laser-written stressing tracks can induce waveguide birefringence into the fiber core and enable submillimeter in-fiber wave retarders. Lastly, the concept of 3D writing of microfluidic networks, reservoirs, and micro-optical resonators with optically smooth sidewall roughness into single-mode and coreless fibers is presented in Sect. 4.6. The facile integration of the open structures with laser-formed waveguides culminates with the demonstration of an in-fiber optofluidic Fabry-Perot refractive index sensor. This chapter therefore describes a new laser processing technology and the outlook for creating 3D optical and optofluidic microsystems inside a compact and flexible optical fiber platform that promise highly functional LIF devices for complex laboratory-level diagnostics.

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

71

4.2 Laser Structuring of Optical Fibers The underlying methodologies for writing optical circuits inside optical fibers are described in this section for the specific case of Corning SMF-28® fiber, selected because of its widespread deployment as the backbone of optical communication networks, as well as its low cost and small optical loss. However, one fundamental challenge with writing optical circuits in SMF is the lower coupling efficiency ( 5 m gap from the glass surface. Further, the orientation of the laser polarization was a useful control parameter on multiple purposes to orient the nanograting alignment preferentially. For example, one could reduce both the waveguide loss and the waveguide birefringence when the laser polarization was parallel and the nanogratings were perpendicular to the waveguide axis. Alternatively, dramatically faster chemical etching rates were found [38] when the laser polarization was perpendicular to the modification track, facilitating rapid acid flow along nanogratings aligned parallel with the track. The concept of using an AOM to create laser burst trains of femtosecond pulses that form segmented waveguides in bulk fused silica glass was previously reported in [18, 26]. Here, the waveguide consists of an array of partially overlapping refractive index voxels that offer a strong first-order Bragg resonance at wavelength

B D 2neff ƒ, where neff is the effective index (1.445) of the waveguide mode and ƒ is the grating period. In the telecommunication band, a Bragg wavelength of B D 1550 nm follows from a grating period of 536 nm, controlled by the ratio of the scan speed (0.268 mm/s) to the AOM modulation frequency (500 Hz). The grating period can be arbitrarily varied on each voxel by the DAQ card (Fig. 4.2) to introduce phase shifts and apodization for the flexible tailoring of BGW spectrum [58, 59]. BGWs were formed in the fused silica cladding of SMF and in the coreless fiber with oil-immersion focusing (Fig. 4.2 inset) under various exposure conditions such as 130 nJ pulse energy, 0.268 mm/s scan speed, and 60 % duty cycle at 500 kHz repetition rate or 71 nJ pulse energy, 0.1 mm/s scan speed, and 60 % duty cycle at 1 MHz repetition rate. Bragg gratings were also written into the preexisting core waveguide of SMF [55, 60] at lower exposures in the range of 10 nJ to 120 nJ, 0.268 mm/s scan speed, and 500 kHz repetition rate. A lower exposure here is the result of the stronger ultrafast laser interaction in the Ge-doped core waveguide volume. A practical objective in writing optical circuits in coreless fiber is facilitating an efficient optical connection with standard fibers or optical systems. A simple assembly and packing approach that we examined here is the fusion splicing of the waveguide-embedded coreless fiber to SMF. In one approach, fusion splicing was completed after the laser writing step. However, the high temperature generated during the arc discharge erased a long 374 m segment of the waveguide in the

74

J.R Grenier et al.

Fig. 4.4 Optical micrographs of coreless optical fiber (left) with a core waveguide inscribed by a femtosecond laser (a) before and (b) after fusion splicing to an SMF (right). The fusion splice is seen to have erased a 374 µm segment of the laser-formed waveguide in (a), leading to a large insertion loss (10 dB) in contrast with low loss (1 dB) in the case of (b)

coreless fiber as shown in Fig. 4.4a, leading to an 10 dB insertion loss with SMF. Alternatively, a much improved insertion loss of 1 dB was found when the coreless fiber was first fusion spliced to SMF and followed with waveguide writing in the coreless fiber to meet the SMF core waveguide as shown in Fig. 4.4b. Hence, this latter approach is more preferable while also offering the advantage of real-time monitoring as optical circuits form and connect with the SMF. The transmission and reflection spectra of the laser-formed waveguides and embedded devices were recorded by probing the device under test via end-coupled SMF or free-space lens launching of various infrared light sources (Thorlabs: ASE-FL7002, 1520 nm to 1610 nm; Agilent: 83437A, 1200 nm to 1700 nm; Photonetics: Tunics-BT, 1520 nm to 1600 nm; and AFC BBS1310, 1275 nm to 1345 nm). Reflection spectra were recorded with an optical fiber circulator. Index-matching oil was applied at all glass-fiber interfaces to reduce the Fresnel reflections and FabryPerot effects. All spectra were normalized relative to a direct fiber-to-fiber transmission and recorded with an optical spectrum analyzer (OSA: Ando AQ6317B, with 0.01 nm resolution) or a spectrometer (Ibsen Photonics: I-MON 512E) suited for real-time measurement during the laser writing. The polarization properties of the laser-formed devices were probed by free-space launching of infrared light through a broadband polarizer (Thorlabs: LPNIR) and a 10 (0.16 NA) lens to excite either horizontally or vertically linearly polarized eigenmodes defined as having electric fields aligned parallel or perpendicular to the sample surface, respectively. The intensity profiles of the propagating modes were captured by imaging the end fiber facet onto a phosphor-coated CCD camera (Spiricon: SP-1550M) with a 60 (0.65 NA) lens.

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

75

The laser writing and device characterization methods described in this section are now applied to build the photonic and optofluidic cladding components described in the following sections.

4.3 Optical Couplers for Fiber Cladding Photonics This section addresses the major challenge of coupling light into and out of the light-guiding structures that are to be written in the cladding of optical fibers. Three approaches of coupling light from an SMF core waveguide into femtosecond laserformed waveguides are investigated by using X-couplers, S-bend couplers, and directional couplers as depicted in Fig. 4.5a, b, c. In each case, the coupling waveguide was formed to intersect with (X, S-bend) or run parallel near (directional) the centered core waveguide and then curved at 30 mm bend radius to meet tangentially with a straight spur cladding waveguide that is parallel to the core waveguide. A 15 mm long BGW was formed along the spur to create a back reflection for probing of the coupler efficiency and also for determining the polarization axis and birefringence of the waveguide. In this way, polarization-selective taps in SMF and polarization beam splitters in coreless fiber were designed and fabricated.

4.3.1 X-Couplers in Single-Mode Fiber X-couplers, also known as cross couplers, are formed by two waveguides that intersect at a given crossing angle (). X-couplers are widely found in commercial planar lightwave circuits made by lithographic patterning. Direct laser writing of

Fig. 4.5 Femtosecond (fs) laser writing of waveguides by focusing through index-matching oil to form an (a) X-coupler, (b) S-bend coupler, and (c) directional coupler in an SMF [64]

76

J.R Grenier et al.

1.0 SMF core

Transmission

0.8 0.6 q =20⬚ 8.3 µm

Core

0.4

fs waveguide 0.2 fs waveguide 0.0

0

10

20

30

40

50

70

90

Angle(⬚) Fig. 4.6 Normalized optical transmission in the through-port (SMF core waveguide; blue squares) and cross-port (fs waveguide; green triangles) as a function of the crossing angle for a X-coupler. The fitted (dashed) lines follow the analytical model of DRurr and Renner [63]. Inset, optical micrograph of a femtosecond laser-formed waveguide crossing an SMF core waveguide at 20ı crossing angle [64]

X-couplers has also been studied to explore more flexible writing options. For example, broadband X-couplers with up to 95 % tapping efficiency and 1 dB loss have been demonstrated in silica-on-silicon with UV direct writing [61] while 50% coupling has been shown in bulk soda lime glass (Corning 0215) with femtosecond laser writing [62]. Such couplers have the advantage of coupling light in short interaction lengths of tens of microns, which is attractive in the limited space of optical fibers. A major challenge of forming X-couplers in SMF is the accurate alignment required to position the crossing waveguide to intercept the center of the core waveguide. As an example, the inset image in Fig. 4.6 shows a femtosecond laserformed waveguide crossing an SMF core waveguide at a 20ı crossing angle, where a statistical alignment error of ˙1 m was estimated. Real-time recording of the optical transmission at 1550 nm wavelength during writing of the X-coupler provided the through-port transmission of the SMF core waveguide (blue squares) as plotted in Fig. 4.6 for 0ı to 90ı coupling angles. A minimum transmission value of 2.9 % is shown at a crossing angle of 2:2ı . Both core and spur waveguides were more fully assessed for X-couplers in the high coupling region with crossing angles of 1:3ı to 3:1ı , bend radius of 30 mm, and offset distance of 45 m from the fiber core. After accounting for a loss of 3.2 dB, attributed to the curved waveguide and straight BGW sections, the optical transmission inferred to couple into the crossport (green triangles) was also plotted in Fig. 4.6 and found to yield a maximum 76 % for a crossing angle of 1:9ı . With 6 % power remaining in the core waveguide,

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

77

1.0

Transmission

fs waveguide 0.8

8.3 µm Core

0.6

SMF Core

0.4 0.2 0.0

fs waveguide 30

40

50

60

70

80

90

100

Bend Radius (mm) Fig. 4.7 Normalized optical transmission in the through-port SMF core waveguide (blue squares) and fs laser cross-port waveguide (green triangles) as a function of the bend radius for an S-bend coupler. Inset, optical micrograph (compressed by a factor of 4 in the horizontal direction) of a femtosecond laser-formed waveguide curving out of the SMF core with a 30 mm bend radius [64]

the X-coupler yielded an 18 % loss that was attributed to optical scattering at the crossing point of the waveguides. Vertical and horizontal linearly polarized spectra (1250 nm to 1650 nm) were recorded for several X-couplers and revealed less than 10 % variation in the coupling ratio over a 400 nm band and with no appreciable polarization dependence.

4.3.2 S-Bend Couplers in Single-Mode Fiber In an alternative approach to couple light out of an SMF core waveguide, a femtosecond laser-formed waveguide was inscribed by starting in the core and curving outwards to a distance of 45 m into the cladding following along two reversing circular arcs that terminated into a straight 15 mm long BGW segment as shown in Fig. 4.5b. The inset in Fig. 4.7 shows an optical micrograph (compressed by a factor of 4 in the horizontal direction) of a femtosecond laser-formed waveguide curving out of the SMF core with a 30 mm bend radius. To vary the degree of light coupling, the bend radius of the arcs was varied from 30 mm to 100 mm, yielding the normalized power splitting shown in Fig. 4.7 for the through-port SMF core waveguide (blue squares) and femtosecond waveguide crossing waveguide port (green triangles). The propagation loss incurred in the curved waveguide and straight BGW sections was removed here, thus revealing a maximum coupling of 33% for a bend radius of 30 mm. This value falls monotonically with longer bend radius to < 2 % coupling at 100 mm bend radius. In this data range, the observed

78

J.R Grenier et al.

1.00 0.98

IL = 5%

Transmission

0.96

Beat length = 13.5 mm

0.94 0.92 0.90 0.88 0.86 0

5

10

15

20

Length (mm) Fig. 4.8 Real-time recording of the normalized optical transmission of 1550 nm light through an SMF core waveguide (blue line) as a femtosecond laser formed a parallel waveguide 10 m away from the core to form an asymmetric directional coupler [64]

net loss of 20–33 % was attributed to optical scattering at the intersection point of the waveguides. As in the case of the X-couplers, the S-bend couplers showed less than 10% variation in the coupling ratio over a 400 nm band (1250 nm to 1650 nm) and with no appreciable polarization dependence.

4.3.3 Direction Couplers in Single-Mode Fiber Directional couplers transfer optical power via evanescent fields between two or more waveguides positioned in close proximity to each other and are widely used in planar lightwave circuits. Directional couplers are readily fabricated by fusing two twisted glass fibers but require femtosecond lasers to write 22 [28, 65], 3 3 [66] symmetric, and broadband asymmetric [67] directional couplers in bulk glass. Directional couplers have the advantage of complete energy transfer over coupler lengths predicted by rigorous coupled mode theory [68, 69]; however, they are highly wavelength and polarization-dependent. Asymmetric directional couplers in SMF are presented here by femtosecond laser writing of waveguides parallel with and offset by 10 m to 12 m from the core waveguide and formed by exposure of 130 nJ pulse energy and 0.268 mm/s scan speed. Figure 4.8 shows the normalized optical transmission measured at 1550 nm in the SMF core waveguide (blue line) as a function of the coupler length, recorded

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

79

in real time over length increasing from 0 to 20.5 mm. The beating of two harmonic functions seen here consists of a fast oscillating component of the usual evanescent coupling and a slower component owing to waveguide birefringence that induces polarization-dependent coupling ratios of rH and rV . The coupling ratio could be well represented for the asymmetric directional coupler by the expression 2 . /sin2 rH;V . / D H;V

H;V . / L ; H;V . /

(4.1)

where the subscripts, H and V, represent the horizontal and vertical linearly polarized eigenmodes, respectively, is the coupling coefficient, L is the coupling length, and . / is the amplitude dephasing term, given by v u H;V . / D u t

1C

1 ˇH;V . / 2 H;V . /

2 :

(4.2)

. /

as For the present case of asymmetric couplers, it is convenient to define H;V H;V . / the effective coupling coefficient. The transmission through the core waveguide in the first complete beat cycle between 6.94 mm and 20.4 mm length in Fig. 4.8 could be well represented by the equation T.L/ D 1

rH C rV 2

;

(4.3)

yielding effective coupling coefficients of 1.53 rad/mm and 1.30 rad/mm for the vertical and horizontal polarization eigenmodes, respectively. The difference in these values produced a beat length of 13.5 mm as labeled in Fig. 4.8 when the differential coupling phases .. V H /L/ accumulated a -phase. The respective amplitude values of V2 D 0:08 and H2 D 0:09 for the vertical and horizontal polarizations align with the 9 % coupling value inferred from the first half cycle transmission (86 %) after accounting for the 5 % insertion loss (IL) resulting from the abrupt starting point of the laser-formed waveguide. In order to minimize device loss, one may consider the design of directional couplers having the shorter lengths ( 350 nm > 350 nm < 73 nm < 175 nm

Negligible Negligible Strong Strong

1.2 1–1.7 0.2 0.04

Based on a coupling length of 0.099 mm; Based on a zero length coupler

In this section, coupling of light from the core waveguide of SMF was demonstrated with X-, S-bend, and directional couplers whose characteristics are summarized and compared in Table 4.1. Despite the asymmetric waveguides (ˇ ¤ 0), coupling ratios from 0 to 76 % were demonstrated. While directional couplers based on evanescent fields had the lowest losses introduced by the coupler (0.2 dB), their wavelength dependence, defined here as the wavelength range over which less than 5 % variation in the coupling ratio was observed, was more limited relative to the higher-loss (1–1.7 dB) broadband .> 350 nm/ S-bend and X-couplers. The design of directional couplers can be further tailored by the waveguide separation to increase or decrease the coupling strength. In this way, weak polarization or non-polarization taps may be designed with large waveguide separation (> 10 m) while shorter separation (i.e., 9 m) increases the overall coupling strength as stronger evanescent coupling ( V;H ) improves the magnitude of the amplitude dephasing term as seen in Eq. 4.2. However, the overall efficiency

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

83

of directional couplers in this weak coupling regime is restricted by the ˇ-mismatch, which can be addressed alternatively by using X- (Sect. 4.3.1) or S-bend (Sect. 4.3.2) couplers. The coupler losses summarized in Table 4.1 only represent the losses introduced by the coupler itself and do not include the propagation loss (Sect. 4.2) encountered in guiding the light in the fiber cladding. S-bend and X-couplers provided polarization-independent coupling while the strong polarization-dependent coupling offered by the directional couplers provided new directions for designing in-fiber polarization-selective taps and polarization beam splitters. In summary, the challenge of coupling light between the SMF core and light-guiding cladding structures has been met with multiple coupler types, whose loss and spectral and polarization coupling characteristics were analyzed.

4.4 Femtosecond Laser-Formed Cladding Photonic Devices Waveguides are the fundamental component for routing light signals in optical circuits in which couplers and gratings offer powerful ways to multiplex signals and tailor their spectral responses. This section discusses the properties of femtosecond laser-written waveguides and BGW devices as formed inside single-mode and coreless optical fibers. An in-line MZI in SMF and a 3D distributed position-shapetemperature sensor in coreless fiber are presented as examples of the powerful integration approaches that are now available given the new coupling techniques presented in Sect. 4.3.

4.4.1 Waveguides and Bragg-Grating Waveguides in the Core and Cladding of Optical Fibers The femtosecond laser oil-immersion writing technique described in Sect. 4.2 was used to extend single-mode waveguide writing from bulk glass to the cladding of SMF and coreless optical fibers, providing waveguides with propagation loss as low as 0.5 dB/cm. The AOM modulation techniques introduced in Sect. 4.2 provided the burst trains of femtosecond laser pulses on which low- and high-strength, first-order gratings were formed both in the core waveguide and cladding waveguides of SMF and coreless fibers. While several laser approaches, including femtosecond direct laser writing, have been developed for writing Bragg gratings into the preexisting germanium-doped SMF core [52–54], their integration into the cladding of optical fibers opens new opportunities for cladding photonic devices that we explore in this section. The spectral response of strong BGWs is first examined for various writing positions in SMF and coreless fiber using nearly identical exposures (120 nJ to

84

J.R Grenier et al.

a

b

c

d

Fig. 4.11 Linearly polarized transmission spectra of 25 mm long BGWs fabricated in (a) the core of an SMF with 130 nJ pulse energy, (b) the cladding of an SMF with 120 nJ, and (c) the center of a coreless fiber with 130 nJ. Insets, optical micrographs of BGW end facets (writing laser from the top) with expanded views of the waveguide zone (image diameter is 12 m). (d) Vertical (V) and horizontal (H) linearly polarized and unpolarized (U) transmission spectra for the BGW in (c) [60]

130 nJ). Transmission spectra are shown in Fig. 4.11a, b, c for the respective cases of positioning the BGW near-center of the preexisting core of SMF, off-center (r D 30 m) in the cladding of an SMF, and centered in the coreless optical fiber. The inset optical micrographs shown in Fig. 4.11a,b,c are of the waveguide end facets with magnified views revealing a dual modification zone of positive increase in refractive index of a larger diameter .3:6 m/ white zone under a smaller diameter zone .2:1 m/ of negative refractive index change that appears dark. The spectra of Fig. 4.11 all show a strong and narrow Bragg resonance ( 3dB D 0:3 nm) near B D 1550 nm with propagation losses varying from 1 dB/cm to 1.9 dB/cm. However, there was a significant difference between the strength of coupling and number of permitted cladding modes. When the BGWs were centered in the core waveguide of the SMF (Fig. 4.11a) and the center of the coreless fiber (Fig. 4.11c), a very open spectrum formed that was dominated by strong coupling to the discrete LP0n cladding modes that matched well with the stick spectra as shown in the SMF case (Fig. 4.11a), calculated in [60]. Moderately strong coupling was also observed in both fiber types to a higher-order azimuthal cladding mode (LP1n ) that arose from imperfect centering of the BGW as reported by [71,72]. Also contributing to the coupling is the asymmetric refractive index profile as seen in

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

1.450 SMF core n =1.44922

1.449

Effective Index

Fig. 4.12 Effective index at 1550 nm wavelength of FBG (black circles) and BGW (black squares) as a function of the laser pulse energy. Horizontal lines indicate the refractive index of the SMF core (green dashed line), fused silica fiber cladding (blue dashed line), and the effective index of the unmodified SMF mode (red dashed line) [74]

85

FBG

1.448 1.447

SMF neff =1.44630

1.446 1.445 1.444

BGW Silica n =1.44402

0

20

40

60

80 100 120 140 160 180

Pulse Energy (nJ)

the higher-resolution optical micrographs inset of Fig. 4.11a, b, c. Coupling to an increasing density of azimuthal cladding modes progressed systematically as the BGW position was increasingly displaced from the center axis, eventually leading to broadening and weaker coupling until the weak (7.3 dB loss) near-continuum in Fig. 4.11b was observed for the 30 m offset. Figure 4.11d shows transmission spectra for vertical (V) and horizontal (H) linear polarization and unpolarized (U) light coupled into the BGW formed in the center of a coreless fiber (Fig. 4.11c). A waveguide birefringence of 1:03 104 was inferred from the spectral shifting of the V and H Bragg resonances that was more than 2 higher than values previously reported with weaker focusing [33]. This higher birefringence is a result of higher asymmetric stresses [73] induced by the 1.25 NA oil-immersion lens. Such large birefringence was harnessed to form polarization beam splitters in coreless fiber (Sect. 4.3.4) and previously in bulk glass [70]. Further tuning of the waveguide birefringence by femtosecond laser-written stressing tracks is discussed in Sect. 4.5. The effective refractive index is a key waveguide parameter required in the design of optical circuits. The effective index value of neff D 1:44630 is defined in Fig. 4.12 for 1550 nm wavelength against the indicated cladding (1.44402) and core (1.44922) refractive index values. The effective refractive index of BGWs formed in the SMF core and cladding was inferred from the measured Bragg wavelength for a range of laser pulse energies applied between 5 nJ and 170 nJ and is plotted in Fig. 4.12 for 1550 nm wavelength along with the SMF cladding (1.44402), core (1.44922), and effective (1.44630) refractive index values. The threshold exposure of 5 nJ pulse energy for forming a grating into the preexisting SMF core waveguide was significantly lower than the 70 nJ pulse energy required to form both the waveguide and the grating structure in the fused silica fiber cladding. Above these threshold values, the laser pulse energy provided a means of tuning the effective refractive index and hence the propagation constants (ˇ) of

86

J.R Grenier et al.

a

b

−5

FSR = 32 nm

L

BGW SMF Core

Transmission (dB)

fs waveguide −10 −15 −20

1300

1350

1400

1450

1500

1550

1600

Wavelength (nm)

Fig. 4.13 (a) Femtosecond laser-formed MZI in an SMF and (b) the resulting transmission spectrum probed with vertical linearly polarized light [64]

the waveguides. Such tunability is useful in the design of directional couplers where the maximum coupling efficiency depends on the propagation constant mismatch (ˇ) as shown in Eq. 4.2.

4.4.2 Mach-Zehnder Interferometer Device Mach-Zehnder interferometers are an important optical component that find application as sensors or as wavelength-dependent filters and wavelength division multiplexers in telecommunications. Femtosecond laser-written MZIs have previously been demonstrated in bulk glass [28] with a 10 m path length difference. In the limited volume of fiber cladding, a large path difference has not been previously demonstrated with the formation of a second waveguide arm, and MZIs were limited to designs based on tapered fibers [75], microcavities [76, 77], and long period gratings [78]. The fabrication of a fiber-integrated MZI is presented here as an example of a more functional photonic in-fiber device. The demonstration is made possible by combining the coupler presented in Sect. 4.3 with the cladding waveguides in Sect. 4.4.1. The MZI design consists of two broadband S-bend couplers (Sect. 4.3.2) with 30 mm bend radius to couple light between the SMF core waveguide and a laser-formed cladding waveguide offset by 40 m from the SMF core as depicted in Fig. 4.13a. A 15 mm length BGW ( B D 1316 nm) was also fabricated in the core of SMF with 20 nJ pulse energy in order to monitor the V and H polarization axes once the fiber had been removed from the fabrication setup. The total length of the cladding waveguide arm was L2 D 38:382 mm, consisting of a 34 mm long straight section and two 2.191 mm long S-bend couplers. Although this design only offers 1 m longer physical path length over the core waveguide section (L1 D 38:381 mm), the large difference in the effective index of the SMF core

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

87

waveguide (neff1 D 1:44630) and the laser-formed cladding waveguide (neff2 D 1:4446 ˙ 0:0003), as seen in Fig. 4.12, is significant in creating a large optical path difference estimated at L2 neff2 L1 neff1 D 1 m) without requiring any large displacement of the cladding waveguide arm. The measured transmission spectrum (Fig. 4.13b) was recorded with vertical linearly polarized light and clearly shows interferometric fringes with a maximum contrast of 16.5 dB at 1445 nm. The S-bend couplers were designed to couple as much light into the cladding waveguide to compensate for their higher propagation loss. The measured free spectral range (FSR) of 32 nm at 1550 nm wavelength agrees with FSR D

2 ; L2 neff2 L1 neff1 C

(4.6)

yielding a value of 33.9 nm that falls within the experimental uncertainty of the cladding BGW effective index (1:4446 ˙ 0:0003) from Fig. 4.12. The FSR can be tuned most strongly with the MZI device length (L), while a smaller degree of tuning is available with coiling the waveguide around the cladding as well as by varying the effective index of the cladding waveguide with the laser exposure.

4.4.3 Bragg-Grating Waveguide Shape Sensor Fiber-optic sensing is broadly applied today with the sensing region typically confined to the core waveguide of an SMF. For the case of laser-inscribed Bragg gratings, optical sensing relies on a shift of the Bragg resonant wavelength that in the case of strain gauging typically requires secure bonding or embedding of the fiber within a host structure in order to strain the grating along the central neutral axis of the fiber. For more flexible applications such as in shape or position sensing and accelerometers, the grating-embedded waveguide should be displaced away from the neutral axis of a bending structure, for example, as demonstrated in multicore optical fibers (MCFs) [79, 80] and further discussed in Chap. 10. However, the coupling of light into each radially distributed waveguide core to interrogate all the Bragg gratings simultaneously remains a challenge with such MCF-based sensors. In this section, we examine femtosecond laser direct writing of optical circuits in a coreless optical fiber that is fusion spliced to an SMF to provide a unique solution for simultaneous FBG interrogation through a single waveguide core of the SMF. This combination of multiple 3D optical components is shown to offer distributed shape, position, and temperature sensing. Figure 4.14a shows a schematic of a fiber-optic shape sensor that is being fabricated with a femtosecond laser focused by an oil-immersion lens as previously described in Sect. 4.2. The laser exposure conditions of 1 MHz repetition rate, 71 nJ pulse energy, 0.1 mm/s scan speed, and 60 % duty cycle were used to form the BGW sensor segments. Prior to laser structuring, the coreless fiber was fusion spliced to the SMF to avoid thermal erasing of laser-written structures as discussed in Sect. 4.2.

88

J.R Grenier et al.

Fig. 4.14 (a) Schematic of a 3D distributed shape and thermal sensor written in coreless fiber by a femtosecond laser focused with an oil-immersion lens. The embedded Bragg-grating sensors are labeled 1 to 9 . Optical micrographs of the fiber cross section (125 m diameter) at (b) the coupling and (c) sensor regions, showing the arrangement of the internal laser-written waveguides [81]

The sensor consisted of three parallel waveguides, one 1 3 directional coupler, two waveguides with S-bends, and nine BGWs, all written in a single exposure step inside the coreless fiber. A nearly equal power splitting at 1310 nm wavelength was obtained with a 500 m long directional coupler by using a waveguide separation of 9 m in a right-angled isosceles triangle arrangement as shown in Fig. 4.14b. The two off-center waveguides were drawn out by S-bends (40 mm radius) to the 40 m radial positions as shown in the cross-sectional image of Fig. 4.14c. Following the S-bends, the three waveguides were formed into straight and parallel paths to define the distributed sensing region, over which three 1 cm long BGWs were written along each waveguide at 2 cm center-to-center separations, forming three groups of axially colocated BGW triplets as illustrated in Fig. 4.14a. Each BGW was tuned to a different Bragg resonance scaled from 1 D 1280 nm to 9 D 1320 nm in 5 nm increments. This short to long wavelength ordering positioned the spectrum of cladding-mode-coupled light from an upstream BGW outside of the Bragg resonance of a downstream BGW [53]. The fiber shape could be inferred from the shifts in Bragg wavelength of all nine BGWs as monitored with a spectrometer (Ibsen Photonics: I-MON 512E) through the single waveguide port of the SMF shown in Fig. 4.14a. The Bragg wavelength shift was first calibrated against strain and temperature according to the conventional FBG response, which relates the Bragg wavelength shift, , to strain, , and thermal variation, T , according to [82] 1 D .1 pe / C .˛ C /T;

n

(4.7)

where pe is the effective strain-optic constant, ˛ is the thermal expansion coefficient, n is the refractive index, and is the thermo-optic coefficient. A strain sensitivity and

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

89

Fig. 4.15 (a) Four superimposed photographs of the fiber sensor bent in various shapes showing scattered light from the laser-formed waveguides in the coreless fiber while end-fired with a red diode laser from the SMF. (b) Fiber profiles calculated from Bragg resonance shift of nine BGWs are shown in dashed lines superimposed onto the fiber shapes of (a). Green lines indicate the BGW triplet locations [81]

thermal response of the sensor was determined to be = D 1:06 ˙ 0:06 pm= and =T D 9:1 ˙ 0:6 pm/ı C, respectively, which is consistent with the response values of 1:2 pm= and 10.0 pm/ı C, respectively, found in traditional FBGs at longer 1550 nm wavelength [82]. An example of fiber shape sensing at uniform room temperature is presented in Fig. 4.15 by the four cases of nonuniform fiber bending. Red diode laser light was launched into the fiber in order to record the scattered light optical images that were superimposed in Fig. 4.15a with the four different images of fiber shape. For each sensor shape, the nine Bragg wavelength shifts were used in Eq. (4.7) to infer the bending radius and azimuthal bending plane at the three BGW axial positions. These values were decomposed into bend radii on orthogonal planes and followed with a cubic spline interpolation to calculate a continuously varying curvature and azimuth along the length of the fiber. The shape and position of the fiber was finally determined by the finite element method of corotational analysis, which discretized the fiber into curved rigid beam elements that were aligned tangentially at each node [83]. The fiber shapes calculated in this way for each of the fibers imaged in Fig. 4.15a are shown in Fig. 4.15b as dashed lines that closely align with the BGW locations highlighted in green. Hence, the fiber shape sensing could precisely follow the lateral BGW displacements up to 26 mm and bending radii as small as 77 mm. Figure 4.16 shows two examples of the calculated fiber shape (top) together with the reflection spectrum (bottom) recorded at different instants of dynamically changing conditions of fiber bending at room temperature (Fig. 4.16a) and nonuniform heating (Fig. 4.16b). The red lines in the reflection spectrum mark the unstrained and room-temperature Bragg wavelengths for the BGWs in each sensing arm (i.e., center and side) further labeled by a different color. As expected, fiber bending induces large wavelength shifts of up to 560 pm in the off-center BGWs relative to the non-shifting center BGWs, corresponding to a minimum bend radius of 75 mm. The present fiber sensor was designed such that the center waveguide is minimally sensitive to any bend-induced strain and therefore can be used to sense

90

J.R Grenier et al.

Fig. 4.16 Fiber shape and temperature profile (top) calculated from the Bragg resonance shift of nine BGWs in corresponding reflection spectrum (bottom), where the red lines indicate the Bragg wavelengths of unstrained gratings at room temperature. Fiber bending with (a) uniform and (b) graded temperature along the fiber length [81]

temperature and to compensate Bragg wavelength shifts in the off-center BGWs due to thermal variations. Figure 4.16b presents simultaneous sensing of fiber shape and temperature for nonuniform bending and heating of the fiber sensor with a hot iron. Temperature over a range of 24 to 100 ıC was determined from the wavelength shift of the center BGWs and extended by linear interpolation to profile the region between axially colocated BGW triplets. Assuming uniform temperature in the fiber’s cross section, the observed wavelength shifts of the center and sidearm BGWs adjusted for temperature to isolate values for the fiber strain and thus offer the real-time measure of the temperature gradient seen along the fiber in false color together with the fiber sensor shape. The BGW spectra line shape could also be broadened into a spectral chirp when heated at a point smaller than the 1 cm long BGW length and give more precise information of thermal gradients along the grating [84]. The successful demonstration of the temperature-compensated fiber-optic 3D shape sensor was predicated on the 3D writing of a balanced 1 3 waveguide coupler from which distributed BGW sensor signals could all be efficiently relayed into a single fusion spliced SMF. This approach offered advantages in facile and flexible fabrication in comparison with shape sensors based on multiple-fiber assemblies [85,86] or in an MCF [79,80]. In combination, the MZI and BGW sensor examples presented here demonstrate the utility of femtosecond laser writing for creating fiber cladding photonics that can be conveniently probing from a single core waveguide such as provided in SMF. The overall compact size and high temperature

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

91

tolerance of the present devices are further attractive for structural, industrial, reactor, and pipeline applications as well as for integration into biomedical and catheter devices. Much more advanced and functional cladding photonic circuits may now be considered for design and application.

4.5 Birefringence Tuning in Fibers Optical fibers are typically desired without having any polarization sensitivity and are therefore manufactured with very small birefringence of 107 for telecommunication and optical sensing applications. However, polarization-sensitive devices are required in new applications such as phase-shift keying for optical communication [87], quantum optics [88,89], strain, pressure, and temperature sensing [90,91], twist and torsion sensing [92], and single polarization fiber lasers [93, 94]. To this end, polarization-maintaining fibers are also widely available with high birefringence values ranging from 104 in commercial fibers to 103 in microstructured optical fibers [95] and up to 102 in photonic crystal fibers [90]. Such polarizationdependent optical systems also require quarter-wave and half-wave plates, Faraday rotators, and other polarization elements to be integrated and packaged into the optical fiber systems. Laser processing is attractive as a more flexible method to replace such lumped elements and directly embed polarization devices such as polarizers, waveplates [33], polarization splitters [70], and high birefringent stresses [74, 96] directly within the optical fiber or circuit. In this section, we examine how laser processing can bypass the cumbersome lumped-element fiber packaging step and facilitate the integration and miniaturization of polarization components directly within optical fiber technology. The presented results report on the control of waveguide birefringence in both the core waveguide of the SMF and in laser-formed waveguides by writing laser-stressing tracks under various geometries, polarization direction, laser pulse energy, and degree of track overwriting. The high birefringence values promise to create more compact submillimeter polarization devices.

4.5.1 Stress-Induced Birefringence Laser writing of waveguides is well known to cause local asymmetric stresses [73, 96] that manifest in a waveguide birefringence of 104 as shown in Fig. 4.11 (Sect. 4.4). This intrinsic waveguide birefringence was also found to include a strong component of form birefringence owing to the laser formation of nanogratings in fused silica glasses [39, 97–99]. One can harness these stress and nanograting effects and manipulate the waveguide birefringence by writing laser modification tracks in close proximity to preexisting waveguides. In this way, the waveguide birefringence can be flexibly tuned to lower birefringence to values of 106 [96]

92

J.R Grenier et al.

Fig. 4.17 Femtosecond laser stress tracks written around a FBG inscribed in the SMF core waveguide. The electric field amplitude vectors, EV and EH , represent the vertical and horizontal orientations of the waveguide polarization eigenmodes. The center-to-center track separation (S) is noted between the fiber waveguide core and the stress-inducing modification tracks. An optical micrograph of the cross section of a finalized device is shown in the bottom right corner [74]

or increase birefringence to values of 8 104 [96, 100, 101] with adjacent pairs of laser modification tracks, or as high as 2:0 103 with multiple overwritten tracks [74]. The schematic shown in Fig. 4.17 shows the high numerical aperture (HNA) oil-immersion writing geometry, as introduced in Sect. 4.2, together with the stressinducing laser tracks being fabricated around the core waveguide of the SMF. The polarization eigenmodes in the center waveguide (y-direction) are defined as EV for vertical and EH for horizontal in the z-axis and x-axis directions, respectively.

4.5.2 Birefringence Tuning An example of the morphology, laser-formed waveguides surrounded by horizontally and vertically positioned stress-inducing tracks is shown in the end-view optical micrographs of Fig. 4.18a and d, respectively. To better assess the center waveguide birefringence, the same waveguides were back-illuminated and viewed through two crossed polarizers aligned vertical (Fig. 4.18b), horizontal (Fig. 4.18e), and diagonal (Fig. 4.18c and f) as indicated by the green crosses. The highest birefringence is inferred from the brightest light patterns, which appeared for the horizontally arranged stressing tracks in Fig. 4.18c. The long horizontal bright strip indicated the presence of long-range ( 10 m) stresses that reached symmetrically from the stress-inducing tracks to overlap at the center waveguide under test.

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

93

Fig. 4.18 Optical micrographs of the facets of waveguides fabricated in fused silica and surrounded horizontally (a–c) and vertically (d–f) by symmetric pairs of stress-inducing tracks. The green crosses indicate the direction of polarizers used to record the cross-polarization image for (b), (c), (e), and (f). A typical optical mode profile of 1560 nm guided light in (d) is shown to scale with guiding lines marking the mode position over the laser-modified structure seen in the end facet [74]

To verify the effects of this laser-induced stress, the birefringence of the SMF core waveguide was monitored by optically probing a weak single Bragg grating, laser-formed into the fiber core waveguide. The nearly birefringent-free FBG of 0.12 nm bandwidth and 8 dB strength is shown in the reflection spectrum of Fig. 4.19 (unstressed FBG) to broaden and then split into two resolved V and H polarization modes of 120 pm and 200 pm separation following the laser writing of a single stress track and double stress tracks, respectively. Unlike the large long-wavelength shift of the V polarization mode, the H polarization mode approximately retains the same propagation constant. Such wavelength shifts suggest the bright region in Fig. 4.18c to be associated with a strong positive increase in refractive index that is highly asymmetric and mainly aligned with the polarization in the lateral direction as defined between the two stress bars. In contrast, the vertically aligned stressing bars were not found to drive strong refractive index changes or birefringence, as expected by the weak light transmission observed using cross-polarizers in Figs. 4.18e and f. The birefringence induced in both bulk glass waveguides (blue) and fiber core waveguides is shown together in Fig. 4.20 as a function of the separation (S ) between the symmetric stress-inducing tracks and the center wavelength. The waveguides and stress tracks were written with both parallel and perpendicular laser polarizations (EP ark and EP er? ) to preferentially align the nanograting orientation

94

J.R Grenier et al.

Reflection (5 dB/div)

S = 13 µm

Unstressed FBG

Single stress track

H

V Double stress track

1532.6

1533.3

1534.0

1534.7

Wavelength (nm) Fig. 4.19 Unstressed FBG (top blue line), FBG with one stress-inducing track (middle red line), and FBG with two stress-inducing tracks (green bottom line). The tracks are symmetrically positioned on opposite sides of the SMF core waveguide and are written with 13 m separation, 140 nJ pulse energy, and 0.268 mm/s scan speed. The FBG was fabricated with the best conditions identified in Fig. 4.12 and the spectra are offset here for comparison [74]

that could induce the strongest birefringence at each of the indicated laser pulse energies. The strong form birefringence of such nanogratings is evident in the unstressed BGWs fabricated in fused silica with 150 nJ of pulse energy and 100 kHz of repetition rate, yielding a waveguide birefringence of 2:2 104 for parallel writing and 4:1 104 for perpendicular writing as reported for 1 separation in Fig. 4.20. The larger birefringence includes the form birefringence that can be estimated from the difference of 2 104 here and arises when the nanogratings are oriented parallel to the waveguide direction (EP er? ). The introduction of horizontal stressing tracks with separations diminishing to as small as 10 m led to a significant birefringence increase of 4 104 for both types of waveguides and reached a maximum birefringence of 8:3 104 that was associated with the large 891 pm Bragg wavelength splitting observed in the inset spectrum (Fig. 4.20) for the perpendicular writing case. Since the overall birefringence increase is similar for both writing polarizations, one sees the nanograting to only offer a local form birefringence with little reach outside of the stress bars to affect the properties of waveguides nearby. A similar assessment in SMF is shown in Fig. 4.20 for parallel polarization writing of horizontal stress tracks around an SMF core waveguide with three different pulse energies applied under the oil-immersion focusing. Here, a weak FBG was first generated in the fiber core with pulse energy of 5 nJ to 10 nJ as shown in Fig. 4.12 in order to minimize the initial birefringence to approximately

Transmission

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

Birefringence (×10−4)

8

6

420 100 250 100

V

95

H Δl = 891.2pm Δn = 8.31×10−4

nJ kHz nJ kHz

1550

1551 Wavelength (nm)

4

EPer ⊥ in bulk glass

300 nJ 100 kHz

EPar in bulk glass

160 nJ

2 500 kHz EPar in SMF

0 0

10

20

30

40

50

60

70

80

∞

Separation (µm) Fig. 4.20 Measured waveguide birefringence as a function of the stress-inducing track separation with the laser writing of two symmetric modification tracks on opposite sides of the waveguide under test. The results are shown for parallel polarization of the writing laser in SMFs with fabrication conditions of 160 nJ at 500 kHz, and 250 nJ and 420 nJ at 100 kHz for the red, green, and black curves, respectively. The birefringence of waveguides formed in bulk fused silica (equivalent to the coreless fibers) is presented by the blue curves for perpendicular and parallel writing with 300 nJ pulse energy at 100 kHz repetition rate. The dashed and solid lines represent vertical (Fig. 4.18d) and horizontal (Fig. 4.18a) arrangement, respectively, for the stress-inducing tracks in the case of waveguides formed in bulk fused silica glass [74]

2 105 (S D 1 in Fig. 4.20). The SMF birefringence is seen to increase by 3:4 104 , 4:0 104 , and 5:6 104 for the 160 nJ (red data), 250 nJ (green data), and 420 nJ (black data) exposures, respectively. The trends found for the birefringence measurements in fibers are consistent with those found in waveguides formed in bulk fused silica glass under both high NA (Fig. 4.20) and low NA writing conditions [96]. The birefringence induced into bulk glass and SMF core waveguides was also examined with the stress tracks aligned vertically as in Fig. 4.18d. This alignment led to a moderate decrease in birefringence of 1:3 104 to a value of 0:9 104 (dashed blue line) in bulk glass waveguides and a decrease of 2 105 to a value < 4 106 (dashed red line) in SMF, at respective track separations of S D 14 m and S D 20 m as seen in Fig. 4.20. However, this decrease is found to simply reverse the initial birefringence induced while creating the BGW and FBG, respectively, but not going further to reverse the sign of the birefringence. Hence, the minimum recorded birefringence was 4 106 (at our resolution limit) for the SMF case in Fig. 4.20. All the data in Fig. 4.20 were well represented by inverse square functions (solid and dashed lines) of the separation distance (S ).

96

J.R Grenier et al.

EPer⊥

N

1.5

EPer⊥ EPar

1.0

Δl =1.18nm Δn =1.105×10−3

Reflection (2 dB/div)

Birefringence (×10−3)

2.0

0.5

0.0

1544.8

0

2

4

6

8

10

12

1545.7 1546.6 . Wavelength (nm)

14

16

18

Number of stress tracks Fig. 4.21 Waveguide birefringence as a function of the number, N (configuration illustrated in the top left inset), of overwritten stress tracks laid out at a fixed separation of 11 m and fabricated with 160 nJ pulse energy at 500 kHz repetition rate. A logistic function fits the results for parallel (blue circles and blue curve) and perpendicular (green squares and green curve) polarizations of the writing laser. The inset shows an example reflection spectrum of the Bragg resonance observed before (blue solid line –) and after (green dashed line - -) the fabrication of 18 stress tracks at S D 11 m for the parallel writing case. The top right inset illustrates the arrangement of an ensemble of 19 laser modification tracks fabricated with the perpendicular polarization of the writing laser and evenly distributed between an 11 m and 8 m separation [74]

The further increase in birefringence has been explored by inscribing multiple stressing tracks and overwriting the stress tracks around the SMF core as well as by introducing form birefringence directly into the core waveguide with strong laser modification of the core. The resulting waveguide birefringence values are plotted in Fig. 4.21. The blue and green curves show the birefringence increasing as a function of N for the same stressing conditions (160 nJ pulse energy and 11 m separation) but with the FBG under test fabricated with 5 nJ for the parallel writing case (blue curve) and 90 nJ for the perpendicular writing case (green curve). The parallel writing case had a negligible starting birefringence at N D 0 while the perpendicular writing case found an initial 0:4 103 birefringence value. This higher value is due to the form birefringence and higher energy used for the FBG fabrication and is comparable with the initial value found for writing with parallel polarization in fused silica as shown in Fig. 4.20. The data in Fig. 4.21 were fitted to logistic-type functions, with the birefringence values reaching a saturation level after 10 overwritten stress tracks. A closeto-saturation birefringence value of 1:11 103 , inferred from the spectrum inset

2.5

1.0

2.0

0.8

1.5

0.6

l/2 1.0

0.4

800 µm l/4

0.5

0.0

1275

1375

1475

1575

97

Birefringence (×10−3)

Length (mm)

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

0.2

1675

0.0

Wavelength (nm) Fig. 4.22 Birefringence as a function of wavelength (right scale, blue circles, and curve) and minimum waveplate length (left scale, half-wave plate in the red curve, and quarter-wave plate in the green curves). The black horizontal dashed line represents an 800 m retarder device fabricated in SMF. The birefringence spectrum was recorded from this device by a cross-polarizer arrangement, identifying a quarter-wave plate at 1324 nm wavelength [74]

in Fig. 4.20, was found for the parallel writing case while a value of 1:3 103 was found for the perpendicular writing case. Using a combination of 19 tracks distributed between 11 m and 8 m separation and perpendicular polarization of the writing laser, it was possible to form a plane of horizontal stress that further enhanced the birefringence. A maximum birefringence of 2:0 103 was found for this case (top right datum in Fig. 4.21), a value more than twice as large as previously reported with a similar writing technique [100]. With the birefringence values demonstrated here, it is possible to design half-wave retarders in the infrared spectral band with only submillimeter fiber lengths [33]. Figure 4.22 shows the spectral dependence of the birefringence (right scale) in SMF modified with ten pairs of overwritten laser tracks with 11 m separation and formed with 160 nJ pulse energy, 0.268 mm/s scan speed, and 500 kHz laser repetition rate. The minimum length required to obtain a quarter-wave or a half-wave plate can be found from L D WP

neff . /

:

(4.8)

Here, neff . / is the wavelength-dependent birefringence and WP represents the wave retardation (WP D 1=2 for a half-wave and WP D 1=4 for a quarterwave plate). In order to design a spectrally broad waveplate, the relative variation

98

J.R Grenier et al.

of birefringence should follow the relative variation of wavelength according to Eq. 4.9. This yields a constant retardance as a function of wavelength for a fixed waveguide length L: d d.neff / : D neff

(4.9)

For the waveguide birefringence spectrum in Fig. 4.22, one finds the minimum length (Eq. 4.8) for creating quarter-wave and half-wave waveguide retarders (left scale) to vary by 50 % across the 1250 nm to 1700 nm spectrum, from a length of 1 mm to 0.5 mm and from 2 mm to 1 mm, respectively. The birefringence was determined by the cross-polarization technique [33] applied to an 800 m long segment of stressed SMF. This segment led to a quarterwave plate operation measured at 1324 nm as shown in Fig. 4.22. This wave retarder has a 10 nm band between 1690 nm and 1700 nm that satisfies the broadband condition of Eq. 4.9 within a tolerance of 0.2 %. Extrapolation of the waveplate length data to longer wavelengths suggests that broader band waveplates are available here. Alternatively, other laser exposure conditions are expected to shift the birefringence dispersion and possibly better meet the waveplate condition of Eq. 4.8 over broader and in different spectral windows.

4.5.3 Summary In summary, this section demonstrated the advantage of using tightly focused femtosecond laser light to locally tune the birefringence of preexisting optical waveguides. By various means of polarization control and multiple track scanning, a stress birefringence of up to 2 103 was induced in SMF. This approach offers flexible in situ tuning of waveguide birefringence as well as the precise integration of quarter- and half-wave plates to specific wavelengths that are attractive in fiber platforms for higher-level integration of polarization-encoded components into short waveguide segments. These in-fiber polarization components could be integrated with the waveguide couplers described in Sect. 4.3 to enable new approaches for creating polarization-sensitive fiber taps, polarimeters, and other polarization elements with applications of power monitoring in fiber lasers, polarization-dependent fiber sensing, and quantum optics circuits.

4.6 Microfluidics in Optical Fiber The Introduction (Sect. 4.1) identified an intense drive to reduce biological and chemical laboratory processes from bulky free-space systems to much more compact and functional LOC devices that are typically limited today to planar

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

99

substrates [45]. The nanogratings generated during femtosecond laser processing of fused silica opened the novel approach of highly selective chemical etching by FLICE [32, 36–39] that is now addressing these new LOC directions. In this section, we examine the further possibility of using FLICE to wrap microfluidic and optical components around the guiding core waveguide of existing fiber-optic technology and create new types of LIF devices. The FLICE approach was applied here to construct examples of 3D microfluidic networks, microholes, reservoirs, and optical resonators within both types of SMF and coreless optical fiber. These components were then integrated by the powerful laser fabrication techniques introduced in this chapter toward demonstrations of fluorescence and refractive index sensing that underpin a novel all-fiber sensing platform.

4.6.1 3D Microfluidic Networks for Lab-in-Fiber To open this new direction of LIF devices, the formation of 3D optofluidic devices in optical fiber was explored by following the benefits of high NA oil-immersion objective lenses previously described in Sect. 4.2 for reduction of spherical aberration and beam-focusing distortion in the fiber. In this way, flexible fabrication of arbitrarily complex 3D microfluidic networks was shown to become possible by laser writing of nanograting modification templates in the fiber. The laser tracks were opened with weak HF etching to create predictable structures at arbitrary locations targeted within the SMF and coreless fiber types. Laser exposure conditions for chemical etching of fibers were adopted from the recipes developed for bulk glass by Ho et al. [43, 102]. However, an optimization of the laser exposure under the much tighter focusing with the oil-immersion lens (1.25 NA) was found to lower the laser exposure requirements to 25–50 % of that typically required with air lenses (0.55 NA) [43, 102]. The laser and exposure tools were identical with those described in Sect. 4.2, centered on 522 nm wavelength light of 200 fs duration and 1 MHz repetition rate. In the following demonstrations, fiber access ports and reservoir structures were exposed to 60 nJ pulse energy while weaker exposure of 20 nJ pulse energy was preferred to generate the smoothest walls desirable for low optical scattering loss at microchannel and optical resonator surfaces. Laser scanning speeds were typically in the range of 0.3 to 2.5 mm/s, with slower speed favored for smoother etched walls. The walls of reservoirs, large channels, and optical resonators were formed by arrays of laser modification lines spaced by 1 m, with polarization chosen to preferentially align perpendicular to the scan direction [36] to create the smoothest wall profile. The laser modification tracks were etched with 5 % aqueous HF solution for 1 hour to fully open into channels. The first LIF concept demonstrated in Fig. 4.23 is the formation of a 3D microfluidic network embedded within coreless fiber. This representative example split a single microchannel into four separate radial arms that may each be independently probed by laser-formed waveguides. Alternatively, straight through or blind access channels shown in Fig. 4.24 were embedded for optical probing by the

100

J.R Grenier et al.

Fig. 4.23 (a) Schematic and (b) optical micrograph of a 3D microfluidic network embedded within optical fiber of 125 m diameter. A single microchannel is split into four separate radial arms that may each be independently probed by laser-formed waveguides (not shown). The channels opened along laser exposure tracks formed with oil-immersion focusing to avoid optical aberrations. This undistorted patterning of nanograting structures offered precise formation of straight and circular channels after HF etching. Reproduced from [102] by permission of The Royal Society of Chemistry. © 2014 The Royal Society of Chemistry. http://dx.doi.org/10. 1039/C4LC00648H

Fig. 4.24 Optical micrographs of access microchannels traversing across coreless fiber of 125 m diameter from (a) top and (b) side views together with (c) a cross-sectional view of a partially traversing blind hole. The non-distorted template structures exploited oil-immersion focusing to form nanogratings that were opened with HF etching. Reproduced from [102] by permission of The Royal Society of Chemistry. © 2014 The Royal Society of Chemistry. http://dx.doi.org/10. 1039/C4LC00648H

core waveguide of SMF for fluorescence or absorption spectroscopy applications. More elaborate 3D optofluidic networks may be envisioned over long lengths of optical fiber to further exploit the benefits of undistorted laser writing with the oilimmersion lens and thereby interconnect optical waveguides with microchannels in straight, circular, or arbitrarily complex shapes. Lab-in-fibers also require the formation of larger open structures such as reservoirs to facilitate efficient fluidic access and exchange from external sources. Microfluidic reservoirs were formed into the fiber cladding by laser writing of overlapping modification tracks in planes that outlined the reservoir boundary.

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

101

a c

b

Fig. 4.25 (a) Cross and (b) top view optical micrographs of microfluidic reservoirs fabricated in optical fiber by laser writing of overlapping modification tracks in planes that outline the reservoir boundary and that were opened with HF etching. (c) AFM surface profile of a reservoir sidewall over 4 4 textmu m2 area indicating a small 12 nm (rms) surface roughness. Reproduced from [102] by permission of The Royal Society of Chemistry. © 2014 The Royal Society of Chemistry. http://dx.doi.org/10.1039/C4LC00648H

Submerging the laser-processed fiber into HF facilitated etching along such planes to release glass blocks into the surrounding HF bath and thus remove large arbitrary shaped volumes [104]. In fiber, a reservoir of dimensions 50 60 125 m3 was fabricated as shown in the micrographs of Figs. 4.25a and b. Reservoirs may arbitrarily be placed into any geometric shape and size and offer flexible means to form refracting surfaces for optical lenses or surfaces for total internal reflection that broadens the opportunities for integrating micro-optical systems into the LIFs. A key objective in this direction is the etching of optically smooth interfaces that will otherwise cause large optical scattering loss [105] when probed by light or increase the Reynolds number to disturb the laminar fluid flow inside the channel [106]. Atomic force microscopy imaging of the reservoir sidewall in Fig. 4.25a over a 4 4 m2 area is shown in Fig. 4.25c to reveal a small 12 nm (rms) surface roughness that corresponds to /130 local flatness for the telecommunication band. Such an optically smooth surface was anticipated from an assembly of nanograting planes over many laser pulses that were preferentially aligned perpendicularly to the writing laser’s polarization [37]. Selective control over the writing laser exposure and polarization therefore permits formation of smooth 3D microfluidic networks of various sizes [43, 102] that can further be advantageously applied to flexible 3D shaping and positioning of lenses, reflectors, resonators, and other optical components within fiber. Such micro-optical components are not otherwise available inside fused silica from traditional laser ablation or other processing techniques.

102

J.R Grenier et al.

a

b

Before Etching (SMF) Access Port Template

c

After Etching (SMF) Access Port SMF

SMF

Microcavity Template SMF Core

After Etching (Coreless) Access Coreless Port Fiber SMF

Microcavity SMF Core

Laser-Formed Waveguide Spice Plane Microcavity

Fig. 4.26 (a) Schematic of an optical resonator and access port template buried within SMF fiber before HF etching using 2D arrays of overlapping laser tracks. (b) Corresponding schematic after HF etching. (c) A similar optical resonator embedded within coreless fiber and integrated with laser-formed waveguides aligned to the optical axes of spliced SMF core waveguides

4.6.2 Optical Resonators in Optical Fiber The formation of optically smooth surfaces to shape microcavity structures inside the fiber opened the novel possibility of creating micro-optical resonators for interrogation by the core waveguide. Nanograting templates defining an optical resonator were formed by laser-scanning 2D arrays of overlapping laser tracks that connected with overlapping access channels, whose accumulative modification volume was susceptible to HF etching. Schematics of an optical resonator design formed by laser writing inside SMF is shown in Fig. 4.26 before (a) and after (b) HF etching. Optical resonators may also be embedded within coreless fiber as shown in Fig. 4.26c, where probing waveguides were laser-written to positions centered to align with the optical core waveguide when spliced to SMF. This approach offered facile integration of LIF coreless devices with light sources, spectral analyzers, and other optical devices. The optical micrograph of Fig. 4.27a shows an optical resonator embedded in SMF. However, a higher magnification image in Fig. 4.27b revealed an undesired concave etching of the channel sidewalls near the SMF core waveguide that induced strong lensing and diffraction losses across the channel. This undesired over-etching was attributed to the presence of germanium within the SMF core waveguide that has a smaller Ge-O dissociation energy of 660.3 kJ/mol relative to a 799.6 kJ/mol [11] Si-O dissociation energy, rendering germania to be more reactive to HF than silica in the chemical reactions GeO2 C 4HF > 2H 3O C CGeF 62 and S iO2C4HF > 2H 3O CCS iF 62 [107,108], respectively. Hence, laser writing of both waveguides and resonators into coreless fiber was favored for generating optically smooth resonators without undesired waveguide etching. Figure 4.27c, d, e show various optical micrographs of a 5 m wide optical resonator traversing

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

a

f

b

SMF

Etched Core

Microcavity

0 Transmission −2.5 −10

SMF Core

103

40 nm

Reflection

10 μm

dB −15 c

125 μm Coreless Fiber

d

e Coreless Fiber

Microcavity −20

Microcavity

25 μm

5 μm Top View

Side View

−25 1520 1540 1560 1580 1600

Wavelength (nm)

Fig. 4.27 (a) Optical micrograph of a 10 m wide optical resonator formed with a laser and HF etching to intersect the SMF core waveguide and (b) higher magnification view showing undesirable over-etching into the core waveguide. (c) Side view optical micrograph image with front illumination of a 5 m wide optical resonator formed in coreless fiber. (d) The probing laser-formed waveguides imaged under back illumination of the same resonator rotated by 90ı . (e) Magnified optical micrograph of the same resonator with front illumination. (f) Measured transmission (blue) and reflection (red) spectra of a similar air-filled 29 m wide resonator with expected Fabry-Perot interference fringes of 0.5 dB and 14 dB strength, respectively, and 40 nm FSR. c, d, e, and f are reproduced from [102] by permission of The Royal Society of Chemistry. © 2014 The Royal Society of Chemistry. http://dx.doi.org/10.1039/C4LC00648H

across coreless fiber between laser-formed waveguides. The waveguides terminated 5 m before the cavity sidewalls to ensure no chemical etching into the waveguide zone. Figure 4.27f shows the measured transmission and reflection spectra recorded from a similar 29 m wide air-filled microcavity that revealed the expected FabryPerot interference fringes with a 40 nm FSR. The fringe contrasts of 0.5 dB and 14 dB for transmission and reflection spectra, respectively, agree with theoretical values expected after accounting for diffraction losses across the resonator gap. This integrated device therefore demonstrates the principle to seamlessly position, size, and shape optical reflectors, beam splitters, lenses, and more advanced 3D optical components inside optical fiber with potentially low or near-theoretical insertion losses.

104

a

J.R Grenier et al.

b

SMF Fluorophore

−71

Source

dBm

−73 −75 −77

Substrate

To OSA

Source Fluorescence 510 530 550 570 590 Wavelength (nm)

Fig. 4.28 (a) Schematic of a laser-formed microchannel traversing across SMF and filled with a Rhodamine B solution. Fluorescence at 570 nm wavelength was excited by a light source centered at 535 nm wavelength that propagated along the SMF core waveguide and was recorded together with fluorescence in the (b) transmission spectrum. b is reproduced from [102] by permission of The Royal Society of Chemistry. © 2014 The Royal Society of Chemistry. http://dx.doi.org/10. 1039/C4LC00648H

4.6.3 Fluorescence and Refractive Index Sensors The potential LIF applications that can exploit the novel laser fabrication capabilities presented here are numerous and extensive and reach beyond temperature, strain, pressure, acoustic, and chemical sensing. In a first example, absorption and fluorescence sensors are demonstrated by writing a single microchannel across the core waveguide of SMF as previously shown in Fig. 4.24. The schematic of this device in Fig. 4.28a relied on capillary force to draw a solution of Rhodamine B fluorescent dye into the laser-formed channel where absorption or fluorescence could be recorded with a light source propagating along the SMF core waveguide. The spectrum in Fig. 4.28b shows an example of both the source and fluorescence light, centered at 535 nm and 570 nm wavelengths, respectively, being collected in the forward propagation direction of the channel-embedded SMF. Much improved signal to noise contrast is expected in back reflection or with a large NA collection lens focused on the channel-waveguide interaction zone. The demonstration of optical resonators in Fig. 4.27c, d, e opens the significant opportunity of refractive index sensing of fluids directly within optical fiber. As an example, a Fabry-Perot cavity embedded within coreless fiber may be used to sense the refractive index, n, of the fluid contained within the cavity by solving for n in D

2 : 2nL C

(4.10)

Here, is the Fabry-Perot’s FSR, is the center wavelength of the nearest Fabry-Perot transmission peak, and L is the Fabry-Perot’s cavity length. In order to completely fill the cavity with fluid, the rectangular-shaped interferometer design schematically shown in Fig. 4.26c was modified to reduce strong capillary forces at the 90ı corners [109]. Uninhibited fluid flow was found by tapering the access ports

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

a

105

b

Waveguide Optical Axis Fabry-Perot Cavity Coreless Fiber

Taper Access Port

Refractive Index (RIU)

1.40

L = 27.2 μm

1.35

ISopropanol Acetone

1.30 1.25 1.20 1.15 1.10

Methanol Air

1.05 1.00 32

34 36 38 40 42 44 Free Spectral Range (nm)

Fig. 4.29 (a) Optical micrographs of a Fabry-Perot resonator with L D 27:2 m optical length and 45ı tapered access ports. (b) Plot of refractive index values measured for various alcohols and air against the recorded FSR of the resonator cavity for D 1:575 m wavelength together with the calculated refractive index (dashed curve). Reproduced from [102] by permission of The Royal Society of Chemistry. © 2014 The Royal Society of Chemistry. http://dx.doi.org/10.1039/ C4LC00648H

to a 45ı angle to connect smoothly with a 27:2 m long Fabry-Perot resonator as shown in Fig. 4.29a. Figure 4.29b plots the results of refractive index measurements of the resonator filled with air, methanol, acetone, and isopropanol, obtained from Eq. 4.10 for L D 27:2 m and D 1:575 m. The values are plotted against the measured FSR and agree with the refractive index values expected near this telecommunication wavelength [110]. Consideration of the present 0.5 nm resolution of the Fabry-Perot resonance in reflection together with a maximum 43 nm/RIU sensitivity calculated by differentiating Eq. 4.10 with respect to n leads one to find a minimum refractive index resolution of 0.01 for the present device. Alternatively, a better value of minimum detectable refractive index change of 3 104 is available by directly measuring the wavelength shift for a single resonance peak that follows a calculated 1:58 m=RIU sensitivity near the 1:575 m wavelength. Such detection level is attractive for refractive index sensing in a compact in-fiber platform that benefits from low-cost packaging to connect with optical sources and detectors.

4.6.4 Summary This section provided several demonstrations of 3D femtosecond laser writing of waveguides and open structures inside SMF and coreless optical fibers. The formation of overlapping laser modification tracks and subsequent HF etching provided facile means to position, size, and shape various optically smooth microfluidic and optical components that may now be probed by the core waveguide of SMF or

106

J.R Grenier et al.

further integrated with laser-formed optical devices previously described throughout Sect. 4.3 to Sect. 4.5 of this chapter. Representative examples of 3D microfluidic networks in Fig. 4.23, intersecting microholes in Fig. 4.24, microfluidic reservoirs in Fig. 4.25, optical resonators in Fig. 4.27, fluorescence detectors in Fig. 4.28, and refractometers in Fig. 4.29 collectively verified that femtosecond laser writing can be a powerful tool for LIF development. The new directions provide for combination of 3D microfluidic networks and optical resonators with optical waveguides to form novel optical sensing systems conveniently inside optical fiber. Such new LIF concepts will be important for various academic, acoustic, aerospace, automotive, biological, chemical, civil, industrial, and medical applications.

4.7 Summary and Future Outlook The many examples presented in this chapter show how femtosecond laser writing offers a new opportunity for the dense 3D integration of optical devices inside optical fibers. This integration approach overcomes the many challenges and costs of otherwise connecting and packing optical fibers with discrete bulk optics. The chapter first addressed the challenge of aberration-free writing of optical circuits to accurate positions .˙1 m/ inside the cylindrical fiber core and cladding by introducing a high numerical aperture oil-immersion writing technique (Sect. 4.2). In this way, femtosecond laser-formed X-couplers, S-bend couplers, and directional couplers were shown to provide efficient optical connection between the SMF core and the laser-formed cladding waveguides (Sect. 4.3) that underpinned the development of cladding photonics. One may consider moderately efficient (32 %) and low loss (0.2 dB) directional couplers that are available over a narrow spectral band (73 nm) or trade for broadband coupling .> 350 nm/ in X-couplers and S-bend couplers with efficiencies up to 76 % and 33 %, respectively, at the cost of higher losses (1–1.7 dB). The polarization-dependent coupling encountered in the directional couplers was harnessed to fabricate in-fiber polarization-selective taps in SMF and polarization beam splitters in coreless fibers, which were introduced as an alternative platform for symmetric coupling between the laser-written structures. These couplers together with cladding waveguides and BGW devices were combined to form a Mach-Zehnder interferometer in SMF and a temperaturecompensated fiber-optic 3D shape sensor in coreless fiber (Sect. 4.4.3). The overall compactness and high integration of such devices opens opportunities for structural and industrial sensing applications as well as for integration in biomedical and catheter devices. Femtosecond laser writing of stressing tracks was found (Sect. 4.5) to induce a controllable waveguide birefringence up to a maximum value of 2 103 , thereby opening a new means of integrating quarter-wave and half-wave plates in short fiber segments. This birefringence tuning, together with the polarizationdependent couplers presented in Sect. 4.3, defines a solid grounding where more

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

107

complex integrated, in-fiber polarimeters and polarization-sensitive optical circuits can be constructed for polarization phase-shift keying in optical communication and applications in quantum optics. Femtosecond laser irradiation with chemical etching was extended into the fiber to form 3D microfluidic networks, components, reservoirs, and micro-optical resonators with optically smooth sidewall roughness in flexible geometries that were efficiently probed by laser-formed waveguides. A fluorescence detector and optofluidic refractive index sensor were demonstrated (Sect. 4.6), thereby opening the prospects for more advanced lab-in-fiber concepts and complex laboratory-level diagnostics attractive as a compact and flexible optical fiber platform for academic, aerospace, chemical, and biomedical applications. As femtosecond lasers are becoming more reliable, lower cost, and more powerful, their prospects for manufacturing more advanced products continue to strengthen in a broad range of applications. The remarkable advantage of the 3D fabrication of optical and optofluidic microsystems is especially promising on which femtosecond lasers are well poised to greatly enhance the functionality of optical fibers, one of the most widely used optical platforms, and pave the way for powerful new research tools, commercial products, and biomedical devices.

References 1. Corning. There’s Strength in Numbers. http://www.corning.com/news_center/features/ billion/index.aspx/. Accessed September 1, 2013 2. J.I. Peterson, G.G. Vurek, Science 224(4645), 123 (1984) 3. B.S. Kawasaki, K.O. Hill, R.G. Lamont, Opt. Lett. 6(7), 327 (1981) 4. K.O. Hill, Y. Fujii, D.C. Johnson, B.S. Kawasaki, Appl. Phys. Lett. 32(10), 647 (1978) 5. R. Kashyap, Fiber Bragg Gratings (Academic Press, New York, 1999) 6. A. Kersey, M. Davis, H. Patrick, M. Leblanc, K. Koo, C. Askins, M. Putnam, E. Friebele, J. Lightwave Technol. 15(8), 1442 (1997) 7. M. Consales, A. Ricciardi, A. Crescitelli, E. Esposito, A. Cutolo, A. Cusano, ACS Nano 6(4), 3163 (2012) 8. J. Ma, A. Kos, W.J. Bock, X. Li, H. Nguyen, Z.Y. Wang, A. Cusano, J. Lightwave Technol. 30(8), 1127 (2012) 9. A. Chryssis, S. Lee, S. Lee, S. Saini, M. Dagenais, IEEE Photon. Technol. Lett. 17(6), 1253 (2005) 10. S. Pevec, D. Donlagic, Opt. Exp. 19(16), 15641 (2011) 11. Y. Gong, Y. Rao, Y. Guo, Z. Ran, Y. Wu, IEEE Photon. Technol. Lett. 21, 1725 (2009) 12. A. Vengsarkar, P. Lemaire, J. Judkins, V. Bhatia, T. Erdogan, J. Sipe, J. Lightwave Technol. 14(1), 58 (1996) 13. Y. Wang, D.N. Wang, M. Yang, W. Hong, P. Lu, Opt. Lett. 34(21), 3328 (2009) 14. Y. Liu, S. Qu, Y. Li, Opt. Lett. 38(3), 335 (2013) 15. D. Qian, E. Ip, M.F. Huang, M.J. Li, A. Dogariu, S. Zhang, Y. Shao, Y.K. Huang, Y. Zhang, X. Cheng, Y. Tian, P. Ji, A. Collier, Y. Geng, J. Linares, C. Montero, V. Moreno, X. Prieto, T. Wang, in Frontiers in Optics 2012/Laser Science XXVIII (Optical Society of America, USA, 2012), p. FW6C.3 16. G.M.H. Flockhart, W.N. MacPherson, J.S. Barton, J.D.C. Jones, L. Zhang, I. Bennion, Opt. Lett. 28(6), 387 (2003)

108

J.R Grenier et al.

17. R.R. Gattass, E. Mazur, Nat. Photonics 2(4), 219 (2008) 18. R. Osellame, G. Cerullo, R. Ramponi, Femtosecond Laser Micromachining, Topics in Applied Physics, vol. 123 (Springer, NewYork, 2012) 19. J.C. Diels, W. Rudolph, P.F. Liao, P. Kelley, Ultrashort Laser Pulse Phenomena: Fundamentals, Techniques, and Applications on a Femtosecond Time Scale, Optics and Photonics (Academic Press, New York, 1996) 20. S. Küper, M. Stuke, Appl. Phys. B 44(4), 199 (1987) 21. C. Momma, B.N. Chichkov, S. Nolte, F. von Alvensleben, A. Tünnermann, H. Welling, B. Wellegehausen, Opt. Commun. 129(1–2), 134 (1996) 22. C.B. Schaffer, A. Brodeur, N. Nishimura, E. Mazur, in Proc. SPIE 3616, 182 (1999) 23. A. Mermillod-Blondin, C. Mauclair, A. Rosenfeld, J. Bonse, I.V. Hertel, E. Audouard, R. Stoian, Appl. Phys. Lett. 93(2), 021921 (2008) 24. K.M. Davis, K. Miura, N. Sugimoto, K. Hirao, Opt. Lett. 21(21), 1729 (1996) 25. Y. Cheng, K. Sugioka, M. Masuda, K. Shihoyama, K. Toyoda, K. Midorikawa, Opt. Exp. 11(15), 1809 (2003) 26. H. Zhang, S.M. Eaton, P.R. Herman, Opt. Lett. 32(17), 2559 (2007) 27. S. Eaton, W. Chen, L. Zhang, H. Zhang, R. Iyer, J. Aitchison, P. Herman, IEEE Photonics Technol. Lett. 18(20), 2174 (2006) 28. K. Minoshima, A. Kowalevicz, E. Ippen, J. Fujimoto, Opt. Exp. 10(15), 645 (2002) 29. R. Osellame, S. Taccheo, M. Marangoni, R. Ramponi, P. Laporta, D. Polli, S.D. Silvestri, G. Cerullo, J. Opt. Soc. Am. B: Opt. Phys. 20(7), 1559 (2003) 30. W. Watanabe, Y. Note, K. Itoh, Opt. Lett. 30(21), 2888 (2005) 31. J. Burghoff, C. Grebing, S. Nolte, A. Tunnermann, Appl. Phys. Lett. 89(8), 081108 (2006) 32. Y. Shimotsuma, P. Kazansky, J. Oiu, K. Hirao, Phys. Rev. Lett. 91, 247405 (2003) 33. L.A. Fernandes, J.R. Grenier, P.R. Herman, J.S. Aitchison, P.V.S. Marques, Opt. Exp. 19(19), 18294 (2011) 34. W. Cai, A.R. Libertun, R. Piestun, Opt. Exp. 14(9), 3785 (2006) 35. L. Ramirez, M. Heinrich, S. Richter, F. Dreisow, R. Keil, A.V. Korovin, U. Peschel, S. Nolte, A. Tünnermann, Appl. Phys. A 100(1), 1 (2010) 36. R. Taylor, C. Hnatovsky, E. Simova, D. Rayner, V. Bhardwaj, P. Corkum, Opt. Lett. 28, 1043 (2003) 37. C. Hnatovsky, R. Taylor, E. Simova, V. Bhardwaj, D. Rayner, P. Corkum, Opt. Lett. 30, 1867 (2005) 38. C. Hnatovsky, R. Taylor, E. Simova, P. Rajeev, D. Rayner, V. Bhardwaj, P. Corkum, Appl. Phys. A 84, 47 (2006) 39. W. Yang, E. Bricchi, P.G. Kazansky, J. Bovatsek, A.Y. Arai, Opt. Exp. 14(21), 10117 (2006) 40. R. Osellame, V. Maselli, R. Vazquez, R. Ramponi, G. Cerullo, Appl. Phys. Lett. 90(23), 231118 (2007) 41. A. Marcinkeviˇcius, S. Juodkazis, M. Watanabe, M. Miwa, S. Matsuo, H. Misawa, J. Nishii, Opt. Lett. 26(5), 277 (2001) 42. Y. Bellouard, A. Said, M. Dugan, P. Bado, Opt. Exp. 12(10), 2120 (2004) 43. S. Ho, P.R. Herman, J. Aitchison, Appl. Phys. A 106, 5 (2012) 44. Y. Cheng, K. Sugioka, K. Midorikawa, M. Masuda, K. Toyoda, M. Kawachi, K. Shihoyama, Opt. Lett. 28(13), 1144 (2003) 45. G.M. Whitesides, Nature 442, 368 (2006) 46. R. Osellame, H. Hoekstra, G. Cerullo, M. Pollnau, Laser Photon. Rev. 5(3), 442 (2011) 47. B.B. Xu, Y.L. Zhang, H. Xia, W.F. Dong, H. Ding, H.B. Sun, Lab Chip 13, 1677 (2013) 48. K. Zhou, Y. Lai, X. Chen, K. Sugden, L. Zhang, I. Bennion, Opt. Exp. 15(24), 15848 (2007) 49. H. Fu, K. Zhou, P. Saffari, C. Mou, L. Zhang, S. He, I. Bennion, IEEE Photon. Technol. Lett. 20(19), 1609 (2008) 50. K. Zhou, L. Zhang, X. Chen, V. Mezentsev, I. Bennion, Int. J. Smart Nano Mater. 1(4), 237 (2010) 51. K. Zhou, Z. Yan, L. Zhang, I. Bennion, Opt. Exp. 19(12), 11769 (2011)

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

109

52. J. Thomas, E. Wikszak, T. Clausnitzer, U. Fuchs, U. Zeitner, S. Nolte, A. Tünnermann, Appl. Phys. A 86(2), 153 (2007) 53. A. Martinez, M. Dubov, I. Khrushchev, I. Bennion, Electron. Lett. 40(19), 1170 (2004) 54. G.D. Marshall, R.J. Williams, N. Jovanovic, M.J. Steel, M.J. Withford, Opt. Exp. 18(19), 19844 (2010) 55. J.R. Grenier, L.A. Fernandes, P.V. Marques, J.S. Aitchison, P.R. Herman, CLEO:2011-Laser Appl. Photonic Appl. 2, CMZ1 (2011) 56. L. Shah, A.Y. Arai, S.M. Eaton, P.R. Herman, Opt. Exp. 13(6), 1999 (2005) 57. S.M. Eaton, M.L. Ng, R. Osellame, P.R. Herman, J. Non-Cryst. Solids 357(13), 2387 (2011) 58. J.R. Grenier, L.A. Fernandes, J.S. Aitchison, P.V.S. Marques, P.R. Herman, Opt. Lett. 37(12), 2289 (2012) 59. K. Dolgaleva, A. Malacarne, P. Tannouri, L.A. Fernandes, J.R. Grenier, J.S. Aitchison, J. Azaña, R. Morandotti, P.R. Herman, P.V.S. Marques, Opt. Lett. 36(22), 4416 (2011) 60. J.R. Grenier, L.A. Fernandes, P.R. Herman, Opt. Exp. 21(4), 4493 (2013) 61. F.R. Adikan, C.B. Gawith, P.G. Smith, I.J. Sparrow, G.D. Emmerson, C. Riziotis, H. Ahmad, Appl. Opt. 45(24), 6113 (2006) 62. K. Minoshima, A.M. Kowalevicz, I. Hartl, E.P. Ippen, J.G. Fujimoto, Opt. Lett. 26(19), 1516 (2001) 63. F. Dürr, H. Renner, J. Lightwave Technol. 23(2), 876 (2005) 64. J.R. Grenier, L.A. Fernandes, P.R. Herman, Opt. Exp. (2013). Submitted for publication 65. A.M. Streltsov, N.F. Borrelli, Opt. Lett. 26(1), 42 (2001) 66. K. Suzuki, V. Sharma, J.G. Fujimoto, E.P. Ippen, Y. Nasu, Opt. Exp. 14(6), 2335 (2006) 67. W.J. Chen, S.M. Eaton, H. Zhang, P.R. Herman, Opt. Exp. 16(15), 11470 (2008) 68. A. Yariv, IEEE J. Quantum Electron. 9(9), 919 (1973) 69. H. Haus, W. Huang, S. Kawakami, N. Whitaker, J. Lightwave Technol. 5(1), 16 (1987) 70. L.A. Fernandes, J.R. Grenier, P.R. Herman, J.S. Aitchison, P.V. Marques, Opt. Exp. 19(13), 11992 (2011) 71. J. Thomas, N. Jovanovic, R.G. Becker, G.D. Marshall, M.J. Withford, A. Tünnermann, S. Nolte, M.J. Steel, Opt. Exp. 19(1), 325 (2011) 72. J.U. Thomas, N. Jovanovic, R.G. Krämer, G.D. Marshall, M.J. Withford, A. Tünnermann, S. Nolte, M.J. Steel, Opt. Exp. 20(19), 21434 (2012) 73. V.R. Bhardwaj, P.B. Corkum, D.M. Rayner, C. Hnatovsky, E. Simova, R.S. Taylor, Opt. Lett. 29(12), 1312 (2004) 74. L.A. Fernandes, J.R. Grenier, P.V.S. Marques, J.S. Aitchison, P.R. Herman, J. Lightwave Technol. 31(22), 3563 (2013). 75. P. Lu, Q. Chen, Opt. Lett. 36(2), 268 (2011) 76. Y. Wang, M. Yang, D. Wang, S. Liu, P. Lu, J. Opt. Soc. Am. B: Opt. Phys. 27(3), 370 (2010) 77. L. Jiang, J. Yang, S. Wang, B. Li, M. Wang, Opt. Lett. 36(19), 3753 (2011) 78. C.L. Du, Z.L. Ou, J.R. Zheng, Y.Q. Yu, P.G. Yan, J.S. Wang, X. Chen, Adv. Mater. Res. 658, 232 (2013) 79. R.G. Duncan, M.E. Froggatt, S.T. Kreger, R.J. Seeley, D.K. Gifford, A.K. Sang, M.S. Wolfe, in Proceedings of SPIE - The International Society for Optical Engineering, vol. 6530 (2007) 80. A. Fender, W.N. MacPherson, R.R.J. Maier, J.S. Barton, D.S. George, R.I. Howden, G.W. Smith, B.J.S. Jones, S. McCulloch, X. Chen, R. Suo, L. Zhang, I. Bennion, IEEE Sens. J. 8(7), 1292 (2008) 81. K.K. Lee, A. Mariampillai, M. Haque, B.A. Standish, V.X.D. Yang, P.R. Herman, Opt. Exp. (2013). Accepted for publication 82. K.O. Hill, G. Meltz, J. Lightwave Technol. 15(8), 1263 (1997) 83. M.A. Crisfield, Comput. Meth. Appl. Mech. Eng. 81(2), 131 (1990) 84. J. Lauzon, S. Thibault, J. Martin, F. Ouellette, Opt. Lett. 19(23), 2027 (1994) 85. M.S. van der Heiden, K.R. Henken, L.K. Chen, B.G. van den Bosch, R. van den Braber, J. Dankelman, J. van den Dobbelsteen, in SPIE Optical Systems Design, vol. 8550 (SPIE, Barcelona, 2012), pp. 85,500L–85,500L–14

110

J.R Grenier et al.

86. Y.L. Park, S. Elayaperumal, B. Daniel, S.C.R.S.C. Ryu, M.S.M. Shin, J. Savall, R.J. Black, B. Moslehi, M.R. Cutkosky, IEEE/ASME Trans. Mechatron. 15(6), 906 (2010) 87. S. Betti, G. De Marchis, E. Iannone, J. Lightwave Technol. 10(12), 1985 (1992) 88. J.L. O’Brien, A. Furusawa, J. Vuckovic, Nature Photon. 3(12), 687 (2009) 89. M. Lobino, J.L. O’Brien, Nature 469(7328), 43 (2011) 90. Z. Liu, C. Wu, M.L.V. Tse, C. Lu, H.Y. Tam, Opt. Lett. 38(9), 1385 (2013) 91. O. Frazao, C. Jesus, J.M. Baptista, J.L. Santos, P. Roy, IEEE Photon. Technol. Lett. 21(17), 1277 (2009) 92. D. Lesnik, D. Donlagic, Opt. Lett. 38(9), 1494 (2013) 93. R. Goto, R.J. Williams, N. Jovanovic, G.D. Marshall, M.J. Withford, S.D. Jackson, Opt. Lett. 36(10), 1872 (2011) 94. C.C. Willis, E. McKee, P. Böswetter, A. Sincore, J. Thomas, C. Voigtländer, R.G. Krämer, J.D. Bradford, L. Shah, S. Nolte, A. Tünnermann, M. Richardson, Opt. Exp. 21(9), 10467 (2013) 95. T. Geernaert, T. Nasilowski, K. Chah, M. Szpulak, J. Olszewski, G. Statkiewicz, J. Wojcik, K. Poturaj, W. Urbanczyk, M. Becker, et al., IEEE Photon. Technol. Lett. 20(8), 554 (2008) 96. L.A. Fernandes, J.R. Grenier, P.R. Herman, J.S. Aitchison, P.V.S. Marques, Opt. Exp. 20(22), 24103 (2012) 97. L. Sudrie, M. Franco, B. Prade, A. Mysyrowicz, Opt. Commun. 171(4–6), 279 (1999) 98. E. Bricchi, B.G. Klappauf, P.G. Kazansky, Opt. Lett. 29(1), 119 (2004) 99. Y. Shimotsuma, M. Sakakura, P.G. Kazansky, M. Beresna, J. Qiu, K. Miura, K. Hirao, Adv. Mater. 22(36), 4039 (2010) 100. D. Grobnic, S.J. Mihailov, C.W. Smelser, J. Lightwave Technol. 25(8), 1996 (2007) 101. K. Chah, D. Kinet, M. Wuilpart, P. Mégret, C. Caucheteur, Opt. Lett. 38(4), 594 (2013) 102. S. Ho, M. Haque, P.R. Herman, J. Aitchison, Opt. Lett. 37, 1682 (2012) 103. M. Haque, K.K.C. Lee, S. Ho, L.A. Fernandes and P.R. Herman, Lab Chip (2014). doi:10. 1039/C4LC00648H 104. S. Ho, Femtosecond Laser Microfabrication of Optofluidic Lab-on-a-Chip with Selective Chemical Etching. Ph.D. thesis, University of Toronto (2013) 105. F. Toigo, A. Marvin, V. Celli, N. Hill, Phys. Rev. B 15, 5618 (1977) 106. J. Taylor, A. Carrano, S. Kandlikar, Int. J. Thermal Sci. 45, 962 (2006) 107. M. Ohtsu, J. Lightwave Technol. 13, 1200 (1995) 108. C. Tuck, R. Hague, C. Doyle, Meas. Sci. Technol. 17, 2206 (2006) 109. M. Zimmermann, P. Hunziker, E. Delamarche, Mirofluid. Nanofluid. 5, 395 (2008) 110. T. Wei, Y. Han, Y. Li, H. Tsai, H. Xiao, Opt. Exp. 16, 5764 (2008)

Chapter 5

Fabrication of Channel Waveguides in Chalcogenide Glass Films by a Focused Laser Beam K. Shemesh, Yu. Kaganovskii, and M. Rosenbluh

5.1 Introduction Chalcogenide glasses (ChGs), due to their wide infrared transparency, high refractive index, and high Kerr nonlinearity, are of great interest as a waveguide material for micro optics and nonlinear optics [1]. They are also good candidates for many other applications including thermal and medical imaging, biosensing, and telecommunications [2]. Already important in optical storage disks and fibers, they are now being proposed as the basis for solid-state memory technologies. The intrinsic photosensitivity of the ChG materials has been utilized to fine-tune the effective refractive index of ChG waveguides, and thereby the resonant wavelength of micro-ring resonators [3]. ChGs are also emerging as excellent materials to fabricate nonlinear optical devices required for all-optical signal processing. ChGs are characterized by ultrafast broadband nonlinear optical response, high third-order optical nonlinearity (two to three orders of magnitude greater than that of silica), and low linear and nonlinear losses at telecommunications wavelengths [4]. Traditional fabrication techniques, which are used for large-scale production of planar optical devices, involve thermal evaporation and photolithography. For fabrication of channel waveguides in the micrometer range, high-cost fine-line patterning techniques are used currently, such as electron-beam lithography or focused-ion-beam milling [5]. In this paper, we demonstrate a simple optical method for the fabrication of micrometer-width channel waveguides in ChG films that does not require liftoff lithography. The method is based on photo-induced mass transport [6–8]—a phenomenon, which entails the redistribution of material between illuminated and dark areas under illumination of ChGs by light with a frequency at or above the band gap. This phenomenon was used for fabrication of m-size groves in the films, which formed the walls of the channel waveguides, as well as tapers and coupling

K. Shemesh • Yu. Kaganovskii • M. Rosenbluh () Department of Physics, Bar-Ilan University, Ramat-Gan 52900, Israel e-mail: [email protected] G. Marowsky (ed.), Planar Waveguides and other Confined Geometries: Theory, 111 Technology, Production, and Novel Applications, Springer Series in Optical Sciences 189, DOI 10.1007/978-1-4939-1179-0__5, © Springer ScienceCBusiness Media New York 2015

112

K. Shemesh et al.

gratings in the tapers. For our demonstration we use two ChGs: arsenic trisulfide (As2 S3 ) and arsenic selenide As10 Se90 . As2 S3 is one of the most widely studied ChGs and has been used for all-optical devices in various forms—bulk glass, optical fiber, and waveguides. As10 Se90 is known as a material, in which mass transport occurs with a highest rate compared to other arsenic selenide compositions [9]. Previously, it was shown [6, 7] that the mass flow under illumination by above bandgap light depends on the light polarization that allowed excluding effect of temperature at relatively low light intensities. In our case, however, as we use a focused optical laser beam with a waist of 0.7 m, we have a temperature rise due to light absorption in the film, so that the photo-induced mass transport occurs at elevated temperatures. The photo-induced mass transport involves electronic, atomic, and ionic processes. Though the precise links between these processes are not yet fully established, we propose here possible mechanisms and calculate kinetics of the mass redistribution.

5.2 Waveguide Design The basic design of our waveguide is a raised strip with a trapezoidal cross section produced in a 600-nm-thick As2 S3 or As10 S90 amorphous films, with input and output grating couplers (see Fig. 5.1). The ChG film and waveguide are located on a glass substrate. In order to determine the width of the waveguide, which ensures single-mode operation at the telecommunication wavelength 0 D 1.55 m, we simulated propagation of light in raised strips of different widths with the same thickness (600 nm). For the beam propagation simulations, we used RSOFT software tools (http://www. rsoftdesign.com/products.php?sub=Component+Design) that allow both the design and optimization of passive and active photonic devices for optical communications, optoelectronics, and semiconductor manufacturing. The refractive indices of the As2 S3 and As10 Se90 for 0 D 1.55 m are 2.4 and 2.7, respectively. The results of the simulations for As2 S3 are summarized in Figs. 5.2 and 5.3. Figure 5.2 shows single-mode propagation for a waveguide width of 1 m, for which the single mode maintains its shape and is not subject to any expansion or distortion while propagating along the waveguide. Figure 5.3 shows the mode

Fig. 5.1 Scheme of the waveguide design (top view)

5 Fabrication of Channel Waveguides in Chalcogenide Glass Films. . .

a

Computed Transverse Mode Profile (m=0.neff=2.104343)

b

113

Contour Map of Transverse Index Profile at Z=0

Vertical Direction (μm)

1.0

2.4

1

Y (μm)

1

0

Air As2S3

0 Glass substrate

−1

−1 −1

0

0.0

1

−1

0

Horizontal Direction (μm)

0.0

1

X (μm)

Fig. 5.2 Raised strip waveguide cross section: (a) mode analysis for 0.56 1 m2 core, singlemode operation. Colors show relative power inside and near the waveguide; (b) refractive index profile

a

c

1500

Z (μm)

1200

Z (μm)

1500

1500 Z (μm)

d

1200

1200

900

900

900

600

600

600

300

300

300 0

0

0 −2 −1 0 1 X (μm)

−1

−1 0 1 X (μm)

2

b

e

⎪E⎪ 1

1

0 1 X (μm)

⎪E⎪

0.5

0.5 0.0

0 −2.0

500.0 0.0 X (μm)

2.0

1000.0

Z (μm)

0.0 0 −1.6

775.0 0.0 X (μm)

1.6

1550.0

Z (μm)

Fig. 5.3 Mode propagation in a raised strip waveguide, 600 nm thick and variable width. (a, b) Second-order modes are developed when propagating in a 2 m width waveguide. (c) Distortion and expansion of the first-order mode when propagating in a 1.5 m width waveguide. (d, e) Single-mode propagation in a 1 m width waveguide

analysis for this case as well as waveguides of slightly larger widths. Light is directed into waveguide from an optical fiber of about 10 m in diameter using a grating coupler on the ChG surface (Fig. 5.4) and a taper. The grating area is about 10 10 m2 , and the width of the taper base is 10 m. Coupling between an

114

K. Shemesh et al.

Fig. 5.4 Grating coupler scheme

incident mode and a guided mode is possible if the grating satisfies the following Bragg condition for the first-order diffraction maximum [10]: Kin sin in C Kgrating D ˇ:

(5.1)

Here, Kin D 2/ 0 , Kgrating D 2/ƒ, ˇ D 2 neff / 0 , ƒ is the grating period, and neff is the effective refractive index. The propagation constant, ˇ, was calculated numerically, by solving the wave equation under boundary condition of the waveguide cross section (see Ref. 10, Chap. 3). To adjust the lateral diameter of the incident beam ( 10 m) to the submicrometer waveguide width without losses, we have simulated the beam propagation from the grating coupler to the waveguide using the 3D RSOFT program. We found that negligible loss along the tapering region can be attained as long as the taper length is not shorter than 100 m (Fig. 5.5). In our fabrication the coupling grating was recorded by two crossed p-polarized laser beams (see below). The desired grating period, ƒ, depends on the incident angle, in , and can be easily calculated from Eq. (5.1): ƒD

neff

0 : sin in

(5.2)

5.3 Experiments For our experiments we used 400–600-nm-thick As2 S3 and As10 Se90 amorphous films, vacuum deposited (1 105 Torr base pressure) onto a clean glass substrate. The waveguides were fabricated using a focused Ar laser beam (œ D 514 nm) with a focused waist radius w 0.7 m. The scheme of the setup used for fabrication is shown in Fig. 5.6. The laser beam passing through a half-wave plate, polarizer, and

5 Fabrication of Channel Waveguides in Chalcogenide Glass Films. . .

115

0.9 0.8 0.7

Loss

0.6

Taper length

0.5 0.4 0.3 0.2 0.1 0 0

50

100

150

200

Taper length [μm] Fig. 5.5 Calculated dependence of losses on the taper length. With a 100 m taper length the losses are 6 %

z x

y Sample stage

PC

Objective lens Screen Beam splitter Eyepiece Shutter Polarizer

Argon laser, l = 514 nm

Mirror Half-wave plate

Fig. 5.6 Scheme of setup used for waveguide fabrication

beam splitter is focused by an objective lens onto the film surface. After reflection from the surface, the “writing” laser beam goes back through the objective lens and is directed by a beam splitter and eyepiece to a screen which thus shows an image of the focused spot or the microscopic image of the waveguide drawn of the film sur-

116

K. Shemesh et al.

face, depending on the z-position of the sample. The positioning of the film in x-y-zdirections is adjusted by using three computer-controlled motors, thus drawing the necessary configuration of the waveguide, as monitored by the microscopic image. The gratings for coupling of light ( 0 D 1.55 m) between an optical fiber and the waveguide were fabricated by illumination of a selected film area by two crossing p-polarized beams. In As2 S3 the gratings were produced by an Argon laser ( D 514 nm) with the power of 150 mW in each of the beams; in As10 Se90 the gratings were written by a He–Ne laser ( D 633 nm) with a power of 12 mW in each of the crossing beams. A half-wave plate was used to rotate the polarization plane of the laser to the direction of the wave vector of the grating. The beam propagation inside the waveguide was observed by an IR camera with an IR corrected 50 objective lens having 2 cm working distance. IR light near a wavelength of 1.5 m, from a single-mode fiber-coupled tunable diode laser, was directed onto the coupling grating. For ease of unobstructed viewing, this required a relatively large angle of incidence (as well as output angle) in 60o and thus the grating period calculated from Eq. (5.2) for 0 D 1.55 m was ƒ D 1.18 m for As2 S3 and 0.8 m for As10 Se90 . To satisfy these conditions, we established appropriate angles, ˛, between the crossing beams calculated using ƒ D /2 sin(˛/2).

5.4 Results 5.4.1 Optical Spectra Typical optical transmission spectra of the ChG films are shown in Fig. 5.7. Variation of the transmission with wavelength is caused by interference in the film, and interference maxima ( k ) satisfy the condition: 2Hn D k k where H is the film thickness and k is the order of the interference. The transmission spectra allow us to calculate the refractive indices of the materials [11–13], which we have found to be in agreement with the literature.

5.4.2 Formation of Grooves Channel waveguides together with the input and output tapers and coupler areas were fabricated in one step by positioning of the sample stage by stepping motors in the x-y plane by computer control. The waveguide channels are produced between two grooves, which appear on the film surface during the motion of the stage while illuminated by the focused laser spot. The shape of the grooves defines the channel waveguide geometry. Typical AFM images of the grooves obtained in the As2 S3 films at various writing laser powers, P, and speeds are presented in Fig. 5.8. As seen, the width and the

Fig. 5.7 Transmission spectra of as-deposited As2 S3 and As10 Se90 films on a glass substrate. The film thickness (600 nm) was determined by AFM imaging

Transmission [%]

5 Fabrication of Channel Waveguides in Chalcogenide Glass Films. . . 100 90 80 70 60 50 40 30 20 10 0 300

117

As2S3 As10Se90

800

1300

1800

2300

2800

Wavelength [ nm]

Fig. 5.8 Typical AFM images of the grooves produced in As2 S3 films by various laser powers and stage speeds. (a) P D 2 mW, V D 50 m/s; (b) P D 6 mW, V D 50 m/s; (c) P D 8 mW, V D 50 m/s; (d) P D 6 mW, V D 10 m/s. Polarization is normal to the grooves

depth of the grooves increase with laser power and are inversely proportional to the stage speed. The groove becomes discontinuous (Fig. 5.8d) with a speed slower than 10 m/s due to the fact that stepping motors were used for the groove fabrication and at low speeds the dwell time at each step point becomes significantly long. In Fig. 5.9 we show typical profiles of grooves produced in the As2 S3 films under various writing laser powers and stage speeds. The groove shape and size also show a dependence on the direction of the light polarization: the walls of the grooves have larger slope when the electric vector of the linearly polarized light is normal to the forming groove direction (Fig. 5.10).

118

K. Shemesh et al.

Fig. 5.9 Typical profiles of grooves produced in As2 S3 films under various laser powers and stage speeds. (a) V D 50 m/s, powers varying from 2 to 10 mW; (b) P D 6 mW, speeds varying from 10 to 500 m/s. Polarization is normal to the grooves

This observation is important for understanding the mechanism and kinetics of the photo-induced mass transport, as discussed in the next section.

5.4.3 Channel Waveguides, Tapers, and Couplers After optimization of laser power, stage speed, and polarization direction, we were able to write channel waveguides with tapers and couplers. A typical AFM image of the channel between two adjacent grooves and the corresponding profile of the waveguide in As2 S3 film are shown in Fig. 5.11; AFM images of the taper, coupler, and input grating are shown in Fig. 5.12.

5 Fabrication of Channel Waveguides in Chalcogenide Glass Films. . .

119

Fig. 5.10 Typical profiles of grooves produced in As2 S3 films with different directions of polarization and the same power (P D 6 mW) and speed (V D 50 m/s). 1. Polarization parallel to the groove, 2. polarization normal to the groove

a

0.74 μm

Y: 29 μm

0 μm

X: 34 μm

b Z [mm]

0.6 0.4 1.3 μm

0.2 0 0

2

4

6

8

10

12

X [mm] Fig. 5.11 Typical AFM image of the channel waveguide (a) and corresponding cross section (b)

Figure 5.13 demonstrates coupling of light to the waveguide produced in As10 Se90 ChG film. To observe light input and output, we fabricated a relatively short waveguide (200 m length) with a taper of 100 m and coupler of

120

K. Shemesh et al.

Fig. 5.12 AFM images of taper (a), coupler (b), grating (c) in As2 S3 film, and waveguide in As10 Se90 film (d)

30 30 m2 . In the IR camera image, one can see the waveguide illuminated by visible light (Fig. 5.13a), by both visible and IR (Fig. 5.13b), and by IR only (Fig. 5.13c). One can see coupling of IR light (right) and an output light spot (left).

5.5 Discussion To explain results of our experiments, we have to discuss the physical mechanisms involved in the waveguide fabrication process. We concentrate on two main mechanisms: photo-induced mass transfer and mass transfer induced by temperature gradients around a moving focused writing beam.

5 Fabrication of Channel Waveguides in Chalcogenide Glass Films. . .

121

Fig. 5.13 Waveguide in As10 Se90 film seen in IR camera: (a) illumination by visible light; (b) illumination by both visible and IR light ( 0 D 1.55 m); (c) illumination by IR light only. One can see coupling IR light (right) and an output light spot (left)

5.5.1 Photo-Induced Mass Transfer Our analysis shows that the main mechanism of the mass redistribution in the ChG film is photo-induced mass transfer. As was previously shown [6], photoinduced mass transfer in As2 S3 films is directed from illuminated to dark areas. Redistribution of the film material under illumination by a focused beam leads to the formation of a rather deep pit at the center of the beam and ridges surrounding it. It is important to note that this mass transfer is not induced by thermal effects caused by light absorption, but is purely a light-induced mass transfer. As clear proof of this, it is found that the direction of the ridge formation depends on the direction of light polarization [6]. Formation of dips and ridges indicates that there is a light-induced lateral mass transfer (quasi-viscous flow) parallel to the direction of the E-vector of light. The kinetics of photo-induced mass transfer in ChG films was previously discussed [8, 14] and the rates of photo-induced variations of surface profile were calculated taking into account broken chemical bonds, photo-induced stresses, and capillary forces. We introduced photo-induced diffusion coefficients describing the mass transfer kinetics and demonstrated that the competition between stress-induced flux (towards irradiated regions of the film) and the flux induced by an increase of the bulk energy due to broken bonds (directed from irradiated to dark regions) can result in inversion of the mass transfer direction depending on the light intensity.

122

K. Shemesh et al.

Here, we calculate the shape of the profile formed under a moving focused laser beam due to photo-induced mass transfer. The amorphous As2 S3 films are photoconductive p-type semiconductors with atomic structure consisting mainly of chains with P–C and partly C–C bonds (P denotes pnictogen atom and C, chalcogen). When light with frequency at or above the bandgap interacts with the film, electron-hole pairs are generated in the interaction volume and diffuse in all directions. If a Gaussian writing beam moves along a line in the y-direction, the generation rate per unit volume can be calculated as g0 .x/ D I0 exp x 2 =w2 =Eg H;

(5.4)

where I0 exp(x2 /w2 ) is the incident intensity distribution in the x-direction, Eg is the bandgap of the film material, and H, the film thickness, is assumed small compared to ˛ 1 (˛ is the absorption coefficient), and w is the beam radius. As the electrons and holes have different mobilities, their distribution results in the formation of an internal steady-state electric field, E(x), which accelerates slower carriers and slows down faster carriers. In the As2 S3 films the mobility of holes exceeds the mobility of electrons, and thus the steady-state electric field is directed towards the center of the writing beam. Taking into account forming electric field, one can write the hole and electron currents as jp D Dp

Dp dp p eEI dx kT

jn D Dn

Dn dp Cn eE: dx kT

(5.5)

Here, e is the electron charge, n(x) and p(x) and Dn and Dp are the local concentrations and the diffusion coefficients of electrons and holes, respectively, and E(x) is the lateral electric field. The steady-state distribution corresponds to equality of electron and hole currents (jn D jp ); to satisfy the neutrality condition one can suppose n n0 D p p0 (n0 and p0 are the electron and hole concentrations without irradiation, p0 > n0 in As2 S3 ) and thus dp/dx D dn/dx. Then the steady-state electric field is ED

Dp Dn kT e pDp C nDn

(5.6)

and jp D jn D Damb

dn I dx

Damb D

.n C p/ Dn Dp : nDn C pDp

(5.7)

Here, Damb is the ambipolar diffusion coefficient [15, 16]. The distributions n(x) and p(x) can be found from the equation @n @2 n n D g0 .x/ C Damb 2 ; @t @x

(5.8)

5 Fabrication of Channel Waveguides in Chalcogenide Glass Films. . .

123

where we can put @n/@t D 0 considering a steady-state distribution. The boundary conditions are n(1) D 0, dn/dxjx D 0 D 0. The steady-state solution of Eq. (5.8) is 1=4 p 1 I0 R exp R2 =L2 n.x/ D n0 C 4 Eg LH R R x x e x=L 1 erf C C C e x=L 1 erf : (5.9) R 2L R 2L Here, L D (Damb )1/2 is the diffusion length of the carriers, is the lifetime of electrons and holes before recombination. The hole distribution can be also found from Eq. (5.9) as p(x) D p0 C n(x) n0 . After generation and redistribution, electrons and holes are localized around P and C atoms forming relatively stable configurations—valence alternation pairs (VAP), called also self-trapped excitons (STE), which can be considered as radiation C defects. Four main types of STE were found [17] to be relatively stable: P 2 –C3 , C C C C1 –C3 , P2 –P4 , or C1 –P4 (subscript shows number of bonds and superscript notes the sign of charge). Formation of these defects is accompanied by deformation and breakage of bonds and can accelerate atomic jumps compared to their thermal diffusion without irradiation [18]. This results in significant increase in the diffusion coefficients of both chalcogens and pnictides. The calculations of the forming profiles were carried out under the following assumptions: (i) The main mechanism of the mass transport is volume diffusion. This was shown [19] in experiments on flattening of surface relief gratings under homogeneous illumination by light with frequency above the bandgap. (ii) Mobile species have an effective charge, e, positive or negative, since electrons and holes are localized near defects. Both P and C atoms can be charged either C positively (such as PC 4 , C3 ) or negatively (P2 , C1 ) depending on localization of electrons or holes around them. Recent calculations [20] show that diffusion coefficients of positively charged P and C atoms are about two orders of magnitude smaller compared to those negatively charged (P 2 , C1 ), so that one C C can neglect diffusion of P4 , C3 atoms. The drift of P2 and C1 atoms does not change electroneutrality because electrons and holes diffuse much faster than the charged species and ensure the overall neutrality of the film. (iii) Diffusion coefficients of the charged species are proportional to the local density of free volumes, whose concentration depends mainly on the local concentration of radiation defects, n(x) and p(x). (iv) Lateral diffusion flux is defined as a drift of the charged species in the gradient of chemical potential, , caused by lateral electric field E, by light-induced deformation of bonds due to formation of STE, and by variation of the surface profile

K. Shemesh et al.

Fig. 5.14 Groove profile calculated under the assumption that it is produced by a light-induced mass transfer mechanism

h (nm)

124 300 200 100 0 -100 -4 -200 -300 -400 -500 -600

-3

-2

-1

0

1

2

3

4

Distance (μm)

J D

D nrI r D eE C " rn C rK kT

(5.10)

where D D cD P C (1 c)DC , c is the atomic fractures of P atoms in the ChG compound, D and D are diffusion coefficients of P P C 2 and C1 atoms with the localized electrons, " is the additional energy per atom caused by formation of radiation defects, K is the local curvature of the surface profile, and is the average atomic volume.

The normal rate of variation of the surface profile is Vz D H dJ =dx:

(5.11)

The height of the profile, h(x), was calculated as h.x/ D Vz t:

(5.12)

Here, t is the exposure time (t w/V) that equals 14 ms for w D 0.7 m and V D 50 m/s. In Fig. 5.14 we present the groove profile h(x) calculated using Maple program simulation for our experimental conditions. As a fitting parameter, we used an effective diffusion coefficients Dm corresponding to maximum carrier concentrations nm (at x D 0). As one can see, the calculated profile is very similar to that presented in Fig. 5.11 with Dm D 2.2 109 cm2 /s.

5.5.2 Temperature Rise and Thermodiffusion Mass Transfer The full theoretical analysis of the physical phenomena which cause mass transfer under focused laser light also requires knowledge of the temperature distribution in the film. This problem has been previously investigated under various approximations as applied to thin-film micromachining [21, 22] and ablative laser recording of

5 Fabrication of Channel Waveguides in Chalcogenide Glass Films. . .

125

micron size holes for optical disk storage. In these calculations, a film of thickness h and heat diffusivity f was considered on a semi-infinite transparent substrate (along the z axis) with heat diffusivity s . As in our case f s D , and the film thickness, H, is of the order of the beam waist, w, we can assume that the light energy is absorbed in the volume w2 H and is dissipated inside the substrate due to radial heat flow from a hemisphere with the radius w. We can neglect the heat conductivity of the air compared to the glass. In this case, for estimates of temperature rise, we can use a steady-state temperature distribution, T .r/ D

.Tm Troom / w ; r

(5.13)

which is formed during a characteristic time t* w2 / D [23]. Here, Tm D T(w) is the maximal temperature, Troom is the room temperature, Tm Troom is the temperature rise, D D c is the heat diffusivity, and c is the heat capacity per unit volume. With w D 0.7 m, D D 3 107 m2 /s we have t* D 1.6 s which is much shorter than the exposure time under the moving focused beam in our experiments (ti D w/V D 14 ms), and thus we can neglect the beam speed. From the heat balance ˇ d T .r/ ˇˇ Tm Troom ; D 2w2 ıP ˛PH D 2w dr ˇrDw w 2

(5.14)

we obtain Tm Troom

˛PH : 2w

(5.15)

Here, ’ is the absorption coefficient, ıP is the laser power absorbed by the film, and P is the laser power (without reflection). This result coincides with the more detailed and complicated analysis made by Lax [24] for a Gaussian beam illuminating a semi-infinite absorbing medium if ˛H D 1/2 , i.e., all of the beam power is absorbed. In our experiments, as it follows from the optical spectra (Fig. 5.7), transmission of the As2 S3 film at 514 nm is 60 % which corresponds to ˛H D 0.29. With P D 6 mW and D 1.14 J/mKs we obtain Tm Troom 300 K, i.e., Tm 600 K. This means that the maximum temperature exceeds by about 130 K the glass transition temperature Tg for As2 S3 (Tg D 471 K [25]). According to experimental data [26], the kinematic viscosity, , of As2 S3 glass above Tg follows an exponential law D 0 exp(W/kT) with the activation energy W D 1.12 eV and pre-exponent 0 D 3.98 106 St. The dynamic viscosity D calculated from these data for 600 K is 3.2 103 Pa s ( D 3.19 g/cm3 is the density of As2 S3 ). According to Eq. (5.15), the temperature near the groove decreases to Tg value at a distance

126

K. Shemesh et al.

d

Tm Troom w: Tg Troom

(5.16)

With w D 0.7 m we obtain d 1.8 m. The temperature gradient in the direction normal to the forming groove can initiate lateral motion of a liquid layer from hot to cold regions. The dynamics of lateral motion of a thin liquid layer in a temperature gradient was estimated [27] for bulk Si wafer, in which a liquid layer was formed on the surface under pulsed laser irradiation. It was shown that in the approximation of a long laser pulse when the time scale of the laser pulse, tp , is large compared to the time scale for the diffusion of fluid momentum through the thickness of the melt, i.e., tp H2 / k (H is the melt depth, and k the kinematic viscosity), the radial component of liquid velocity can be written in the form Vr D

1 d d T H: d T dr

(5.17)

As can be seen, the radial velocity is proportional to the radial temperature gradient, the thickness of the liquid layer, and the temperature coefficient of the surface tension; it is inversely proportional to the dynamic viscosity . Substituting D 3.2 103 Pa s, d /dT 2 104 J/m2 K [28], dT/dr (Tm – Tg )/d D 6 107 K/m (average value), and H 0.6 m, we obtain Vr 200 m/s, i.e., Vr is of the order of the stage velocity, V. This means that under the driving force caused by the temperature gradient, the film material can move to the cold regions forming grooves under the illuminated spot and mounds near the grooves (as can be seen in Figs. 5.9 and 5.10). According to [21], the normal component of the velocity, Vz , can be estimated as a function of r using a formula Vz .r/ D

H2 d 2r dr

d r : dr

(5.18)

Here, d /dr D (d /dT)(dT/dr), d /dT is a constant independent of T. Taking into account the temperature distribution [Eq. (5.13)], we have estimated maximum Vz value (under illuminated spot) and obtained Vzm

H 2 d Tm Troom : 2 d T d2

(5.19)

Substitution in Eq. (5.19) D 3.2 103 Pa s, d /dT 2 104 J/m2 K, and H 0.6 m results in Vzm 20 m/s. During time of interaction t w/V of the moving beam with the film, the depth of the groove is z Vzm t D 280 nm (with w D 0.7 m and V D 50 m/s). This estimate shows that there is a noticeable contribution of the thermo-induced mass transport into kinetics of the groove formation.

5 Fabrication of Channel Waveguides in Chalcogenide Glass Films. . .

127

Similar calculations for As10 Se90 films are more complicated because the transmission of the 600-nm-thick As10 Se90 film at 514 nm is 1.1 %, i.e., ˛H 4.5. With a power P D 3 mW this results Tm Troom 2,500 K, and in the calculations one should take into account possible evaporation (ablation) of the material. In addition, we didn’t find in the literature any data about viscosity and other characteristics at such high temperatures. The shapes of the grooves however look similar to those for As2 S3 films (see Fig. 5.12d).

5.6 Concluding Remarks We have demonstrated a simple optical method for fabrication of single-mode channel waveguides in ChG films. All elements of the waveguides (couplers, tapers, and channels) can be easily fabricated using illumination by a focused visible laser beam (without wet or plasma etching) and two-beam illumination of selected areas to produce gratings used for coupling. We have also proposed physical mechanisms for the phenomena: photo-induced mass transfer and mass transfer caused by temperature gradients appearing near fabricated grooves due to light absorption. We have calculated the kinetics of the photo-induced mass transfer and found good agreement between experimental and calculated shapes of groove profiles. We note that under intense illumination of As2 S3 films during the waveguide fabrication, surface scattering becomes stronger due to increasing surface roughness and some additional experiments are necessary to optimize the waveguide fabrication process in order to minimize the contribution of scattering to the device losses. One of the ways to decrease the loss can be a thermal treatment of asdeposited As2 S3 films before waveguide fabrication. As was recently reported [29] thermal annealing improves the homogeneity of as-deposited film and reduces the propagation loss of As2 S3 waveguides. As10 Se90 films are much more stable under illumination and no additional roughness appears under laser processing. Acknowledgments This work was supported by the Israel Science Foundation (Grant # 894/10).

References 1. A. Greer, N. Mathur, Nature 437, 1246 (2005) 2. P. Lucas, J. Phys. Condens. Matter 18, 5629 (2006) 3. N. Carlie, J.D. Musgraves, B. Zdyrko, I. Luzinov, J. Hu, V. Singh, A. Agarwal, L.C. Kimerling, A. Canciamilla, F. Morichetti, A. Melloni, K. Richardson, Opt. Express 18, 26728 (2010) 4. R.G. DeCorby, N. Ponnampalam, M.M. Pai, H.T. Nguyen, P.K. Dwivedi, T.J. Clement, C.J. Haugen, J.N. McMullin, S.O. Kasap, IEEE J. Sel. Top. Quant. Electron. 11, 539 (2005)

128

K. Shemesh et al.

5. J. Hu, N. Carlie, N. Feng, L. Petit, A. Agarwal, K. Richardson, L. Kimerling, Opt. Lett. 33, 2500 (2008) 6. A. Saliminia, T.V. Galstian, A. Villeneuve, Phys. Rev. Lett. 85, 4112 (2000) 7. M.L. Trunov, P.M. Lytvyn, P.M. Nagy, O.M. Dyachyns’ka, Appl. Phys. Lett. 96, 111908 (2010) 8. Y. Kaganovskii, D.L. Beke, S. Kökényesi, Appl. Phys. Lett. 97, 061906 (2010) 9. M.L. Trunov, P.M. Nagy, V. Takats, P.M. Lytvyn, S. Kokenyesi, E. Kalman, J. Non-Cryst. Solids 355, 1993 (2009) 10. A. Yariv, P. Yeh, Photonics: Optical Electronics in Modern Communications, 6th edn. (Oxford University Press, New York, Oxford, 2007) 11. N.J. Harrick, Appl. Optics 10, 2344 (1971) 12. R. Swanepoel, J. Phys. E Sci. Instrum. 16, 1214 (1983) 13. J.A. Pradeep, P. Agarwal, J. Appl. Phys. 108, 043515 (2010) 14. Y. Kaganovskii, D.L. Beke, S. Charnovych, S. Kökényesi, M.L. Trunov, J. Appl. Phys. 110, 063502 (2011) 15. W. Roosbroeck, Phys. Rev. B 91, 282 (1953) 16. C. Thomas, I. Joachimsthaler, R. Heiderhoff, L.J. Balk, J. Phys. D Appl. Phys. 37, 2785 (2004) 17. S.R. Elliott, J. Non-Cryst. Solids 81, 71 (1986) 18. H. Fritzsche, Semiconductors 32, 850 (1998) 19. Y. Kaganovskii, M.L. Trunov, D.L. Beke, S. Kökényesi, Mater. Lett. 66, 159 (2011) 20. M.L. Trunov, C. Cserhati, P.M. Lytvyn, Y. Kaganovskii, S. Kökényesi, J. Phys. D Appl. Phys. 46, 245303 (2013) 21. U.C. Paek, A. Kestenbaum, J. Appl. Phys. 44, 2260 (1973) 22. S.Y. Suh, D.L. Anderson, Appl. Optics 23, 3965 (1984) 23. H.S. Carslaw, J.C. Jaeger, Conduction of Heat in Solids (Oxford University Press, New York, 1954) 24. M. Lax, J. Appl. Phys. 48, 3919 (1977) 25. K. Tanaka, K. Shimakawa, Amorphous Chalcogenide Semiconductors and Related Materials (Springer, New York, 2011) 26. G. Chaussemy, J. Fornazero, J.-M. Mackowski, J. Non-Cryst. Solids 58, 219 (1983) 27. T. Schwarz-Selinger, D.G. Cahill, S.-C. Chen, S.-J. Moon, C.P. Grigoropoulos, Phys. Rev. B 64, 155323 (2001) 28. V. Kolevzon, J. Exp. Theor. Phys. 87, 1105 (1998) 29. D.-Y. Choi, S. Madden, D. Bulla, R. Wang, A. Rode, B. Luther-Davies, J. Appl. Phys. 107, 053106 (2010)

Chapter 6

Laser Processed Photonic Devices Jerome Lapointe and Raman Kashyap

6.1 Introduction The last century was that of electronics; it is now one of photonics. As Richard Feynman (Nobel Prize, 1965) suggested in 1959, “Smaller, Faster, Cheaper” would lead the world, and in many ways he has proven to be correct. Over the past decades, photonics devices and integrated optics have been among the most revolutionary areas of research and advances. Although integrated optics devices are well advanced these days, there is still much to do and most of these components are still expensive to manufacture for mass deployment. In fact, most of these require clean room facilities, as well as several expensive manufacturing steps such as phase mask fabrication or photolithography. This chapter aims at explaining a potential solution to fast manufacturing of cheap integrated optics by laser writing. The interactions between lasers and transparent materials, including nonlinear absorption and the origin of refractive index modification, are initially explained. Furthermore, an entire section is dedicated to waveguide fabrication using lasers. Some analyzing techniques and tools are also presented. However, the chapter focuses on two important photonic materials: glass and lithium niobate. Nevertheless, all demonstrations and explanations can be generalized to most linear and nonlinear transparent materials, which will be showcased throughout the chapter.

J. Lapointe Fabulas Laboratory, Department of Engineering Physics, Polytechnique Montreal, Montreal, QC, Canada H3C 3A7 e-mail: [email protected] R. Kashyap () Fabulas Laboratory, Department of Electrical Engineering, Polytechnique Montreal, Montreal, QC, Canada H3C 3A7 Fabulas Laboratory, Department of Engineering Physics, Polytechnique Montreal, Montreal, QC, Canada H3C 3A7 e-mail: [email protected] G. Marowsky (ed.), Planar Waveguides and other Confined Geometries: Theory, 129 Technology, Production, and Novel Applications, Springer Series in Optical Sciences 189, DOI 10.1007/978-1-4939-1179-0__6, © Springer ScienceCBusiness Media New York 2015

130

J. Lapointe and R. Kashyap

Finally, fabrication of photonic devices using laser ablation is also addressed in the last section, as an alternative technique for making specialist prototyping devices.

6.2 Nonlinear Energy Absorption of fs Laser Pulses When a femtosecond laser pulse is incident on a transparent material with an energy gap Eg larger than the energy of the photon emitted by the laser, there is no possibility for linear absorption. However, if the intensity is sufficiently high, absorption can occur via nonlinear effects such as multiphoton ionization and tunnel or avalanche ionization.

6.2.1 Multiphoton Ionization The ionization of an electron by multiple photons requires the simultaneous absorption of m photons of energy hv, where m is the smallest possible integer for which the total energy is sufficient to ionize an electron (mh > Eg , as shown in Fig. 6.1). Many photons are required to excite a single electron into the conduction band, because of the transparent materials’ large bandgap such as in LN.

6.2.2 Tunnel Ionization Tunnel ionization occurs when a laser impulse creates an intense electric field that reduces the Coulomb potential energy barrier, therefore allowing an electron to jump from the valence band to the conduction band. An important deformation of the material band structure promotes this ionization because of the intensity of the generated electric field. Under very high intensities, the aforementioned multiphoton and tunnel ionizations compete with each other, with the former gaining the upper hand in most interactions between fs lasers and dielectrics [1–4].

Fig. 6.1 Multiphoton ionization principle

6 Laser Processed Photonic Devices

131

Fig. 6.2 Avalanche ionization principle. Variation (solid arrows) and transfer (dashed arrows) of electrons energy

6.2.3 Avalanche Ionization This nonlinear ionization occurs when an electron, free at the bottom of the conduction band and exposed to an intense photon field, is accelerated and acquires substantial kinetic energy. When the total amount of energy surpasses the sum of the conduction band’s minimal gap energy, an electron can ionize another electron at the valence band. Both can now be accelerated in the electric field, henceforth causing an avalanche where the free electron density in the conduction band increases exponentially (see Fig. 6.2). When this density reaches a certain threshold, the dielectric becomes locally absorbent. With the intensity of fs laser pulses, avalanche ionization is negligible in comparison to multiphoton and tunnel effect ionizations. However, this ionization effect is the only option for ionization when the laser intensity is too low for the two other effects described above. As such, avalanche ionization is preferred when materials present impurities and dislocations. Depending on the type of defect present in a crystal, the significance of the avalanche effect can be increased, as the electrons could be at intermediate levels [3–5].

6.3 High and Low Repetition Rate Writing Regimes Nonlinear absorption in transparent materials occurs at intensities in the vicinity of 1013 W/cm2 , which for an impulse of 100 fs corresponds to energy densities of about a J/cm2 [5]. Such energy densities can be attained with the help of lasers, namely that of the Ti:Sapphire, with impulses of Js to tens of nJ (depending on the focus diameter, also called beam waist) and by varying the laser scan speed or repetition rate. The repetition rate of a laser is the number of pulses per second emitted by the laser. There are two distinct repetition rate regimes for fs laser writing: high and low. These regimes are characterized by the critical repetition rate at which the impulsion period is different than the time required for the diffusion of heat outside the focal volume. The critical repetition rates required range from kHz to MHz depending on the material’s thermal diffusivity.

132

J. Lapointe and R. Kashyap

This is precisely the reason why it is very difficult to write a waveguide by changing the refractive index at the focal point using a continuous wave (CW) laser such as with a CO2 laser. The laser can reach energies needed to be nonlinearly absorbed but energy accumulation is too high, which in turn results in internal cavitation or direct material ablation. However, CW lasers can be used to fabricate buried waveguide using photosensitivity of the material [6]. The latter is outside the scope of this chapter; however, waveguides also may be formed in thin films by ablation [7–12], as discussed in Sect. 6.11.

6.4 Two Types of Induced Index Modification To date, two concepts for index modification have been used for waveguide fabrication. Both can be adequately described within the framework of induced lattice defects [13]. In type I, which occurs at lower energies, heat accumulation at the focus induces a fast state transformation from the crystalline to the amorphous state. This results in stress that can increase the refractive index locally. The waveguide is therefore produced in the focal region of the laser [14]. This type of index modification produces good quality waveguides [15] but disappears at temperatures of over 150 ı C in a matter of hours [13, 14]. In type II, laser interactions result in a decrease in the refractive index. The waveguide is therefore produced in the region adjacent to the interaction volume. A simple method to produce these types of waveguides is to write multiple parallel lines; the guiding thus occurs between these lines [13, 16]. For this type of waveguide, the index modification occurs because of the photorefractive effect, which is naturally present in LN [17]. The effect consists of inducing a noninstantaneous and nonlocal refractive index variation in the crystal with laser illumination. This variation is due to the combination of multiple effects created by impurities that can be optically ionized. For example, in lithium niobate the most photoreactive impurities are Fe, Cu, and Mn. The beam ionizes these impurities, which can then move inwards in the crystal via charge transport mechanisms such as conduction band diffusion, with photovoltaic current and forces generated by the external field [18]. In LN, this photo-induced transport is principally linked to photovoltaic currents. These currents carry charges from illuminated areas to darker regions, which increases density, therefore increasing the index as well. Recently, waveguide writing inside an LN fiber using this principle combined with a vortex beam has proven successful [19].

6 Laser Processed Photonic Devices

133

6.5 Basic Steps for Fabricating Waveguides in Transparent Material Using a fs Pulse Laser and Analyzing Methods Fabricating waveguides using a femtosecond pulse laser is quick and simple. A laser beam with a power of 1 W (average), a focusing lens, and a translation stage are the three basic components required (shown in Fig. 6.3). Several variables can be controlled for laser beam, such as power, polarization, beam diameter, beam focus shape, etc., in order to produce an automated highquality waveguide writing system. Figure 6.4 shows the setup used at our FABULAS Laboratory located at Polytechnique Montreal, in Montreal, Canada. The laboratory includes ten different lasers that can be switched towards the sample. The most used laser for waveguide writing, the one seen on the picture, is a Pharos Altos at 1,030 nm (power 8 W, repetition rate from 1 to 600 kHz, pulse width from 50 to 300 fs). The setup includes a beam expander, shutter, half-wave plate, a beam splitter, and a power meter with feedback to automatically and precisely control the laser power. Before the focusing lens, apparatus, such as quarter-wave plates, can be added (or removed quickly using magnetic kinematic stages) to control the polarization of the laser beam. Finally, a high-precision, two-axis, horizontal motorized stage moves the sample and the vertical axis controls the lens position in order to minimize vibrations transmitted to the sample. The setup is mounted on a heavy granite block installed on a pneumatic optical table to further reduce vibrations. The whole setup is inside a HEPA filter system under a slight positive pressure to minimize dust accumulation. An extractor removes debris, should this be necessary.

6.5.1 Laser Beam Alignment, Polarization, and Shaping of the Laser Focus A perfect focusing shape is crucial to fabricate high-quality waveguides repeatably. First, the laser beam must have a symmetrical Gaussian shape, which is usually the case with commercial lasers. One can measure the beam profile using a CCD

Fig. 6.3 Waveguide fabrication

134

J. Lapointe and R. Kashyap

Fig. 6.4 The FABULAS laser fabrication system. 1. Femtosecond laser. 2. Beam expander. 3. Motorized half-wave plate. 4. Beam splitter acting as a polarizer. 5. Feedback power meter. 6. Shutter. 7. Quarter-wave plate. 8. Focusing lens installed on a motorized vertical stage. 9. Vacuum sample holder installed on a motorized horizontal 2-axis stage. The white lines show the beam path

camera or the knife-edge technique. Second, the beam must be right in the center and parallel to the axis of the focusing lens. This alignment can be long and arduous.

6 Laser Processed Photonic Devices

135

Fig. 6.5 (a) Beam evolution near the focus not using a slit, (b) energy distribution in YZ plane not using a slit, (c) beam evolution near focus using a slit, (d) energy distribution in YZ plane using a slit, and (e) schematic of a waveguide writing setup using cylindrical lenses. Adapted from [22, 23]

Note that in complex systems in which different lasers with different wavelengths are used, the mirrors must be changed every time and a good alignment method is essential. The polarization of the laser beam also affects the waveguide. Using a halfwave plate, one can choose the polarization to be parallel or perpendicular to the waveguide direction. A polarization perpendicular to the waveguide direction will produce a highly polarization-dependent waveguide while one parallel to the waveguide direction will produce a polarization-independent waveguide for linear propagation. As one of the advantages of using a laser to fabricate waveguides is to make 3D waveguides, the best way to make uniform waveguides independent to the direction of writing is to choose circular polarization with a quarter-wave plate. Unfortunately, at low repetition rates, even if we have a perfect beam with a perfectly symmetric shape of the spot at the focus as shown in Fig. 6.5a, the waveguide will not be symmetric. In fact, as shown in Fig. 6.5b, the waveguide size perpendicular to the laser beam along the y-axis will be about the size of the beam waist, as there is no energy outside of this area. Otherwise, parallel to the laser beam (z-axis), the waveguide size will be larger, as seen in the equation for the confocal parameter b D 2 ¨0 2 /œ. It was noticed, as shown on Fig. 6.6, that the number of scans influences the waveguides to become more symmetric. This phenomenon may be explained by the fact that multi-scans reduce the probability of irregularities that occur when performing a single scan. Nevertheless, several methods can be used to overcome this nonsymmetrical issue efficiently. Firstly, without the use of other devices, one can simply make the waveguide cross-section shape required by using several scans in which each scan is displaced slightly from the previous one [20]. This method,

136

J. Lapointe and R. Kashyap

Fig. 6.6 Microscope images of the end view (sample facet) of the waveguides, showing the tendency of waveguides to be symmetric by increasing the number of scans. Each column is for a scan speed noted at the top. The number of scan is noted at the bottom left corner of each picture

although efficient, multiplies the time it takes to fabricate waveguides and can generate complications when one wants to fabricate 3D waveguides or other complex devices. A second way is to use cylindrical lenses, which generate an elliptic beam just before the focusing lens, as shown in Fig. 6.5 [21, 22]. In addition, a quick and very effective solution is to introduce a slit of width about 500 m just before the focusing lens [23, 24]. After focusing, the beam shape generated by these two last solutions can be seen in Fig. 6.5c, d. Again, these two solutions are very good for straight waveguides but need to be motorized for 3D writing as the slit or the axes of the cylindrical lenses must remain parallel to the waveguide. This proves to be rather complex. At high repetition rates, this nonsymmetrical issue disappears, thanks to the isotropic heat diffusion out of the focal volume [25–27]. In fact, a circular symmetry of the waveguide cross section is achievable due to heat accumulation, which makes the waveguide larger than the focal point. Typically, the waveguide diameter increases with the repetition rate of the laser and can be up to ten times the focal diameter 2¨0 of the laser, 2¨0 D 4œF= D;

(6.1)

where œ is the wavelength of the laser, F is the focal length, and D is the beam diameter before the lens, as shown in Fig. 6.7.

6 Laser Processed Photonic Devices

137

Fig. 6.7 Laser-focusing parameters

The choice of the lens is therefore extremely important. The numerical aperture (NA) of the lens must be chosen and understood properly, as NA D n sin ™ D n D=2F

(6.2)

2¨0 D 2œn= NA

(6.3)

where n D 1 is the refractive index (if immersion oil is not used) of air. A beam expander can be used to match the lens diameter and then obtain the full NA of the lens. If the beam is larger than the lens, the power below the lens must be verified. When one wants to reproduce an experiment, the beam size must be considered. For example, in Table 6.1, Minoshima used a 100 magnification lens which has an NA typically above 1, but because of the use of a smaller beam diameter, this NA becomes 0.6 [26].

6.5.2 Analyzing Methods The physical properties and propagation efficiency are essential characteristics to be analyzed in order to understand guiding failures and to improve a waveguide. In this section, we explain some of the basic waveguide characterization methods. Note that several other specific characteristics can be also analyzed as far as waveguides are concerned. For example, Raman scatterings can provide information on deformation and strain in a waveguide [28].

Study (et al.) Davis (1996) [34] Davis (1996) [34] Hirao (1998) [44] Schaffer (2001) [25] Minoshima (2001) [26] Streltsov (2002) [4] Will (2002) [125] Cerullo (2002) [21] Osellame 2004 [126] Eaton (2005) [127] Ams (2005) [23]

œlaser (nm) 810

1

790

120

1

Phosphate

800

375

300

150

120

30

Borosilicate 1,045 1,000

1,040 166

1

800

Fused silica Er:Ybdoped

Er:Ybdoped

80,000

Borosilicate 400

100

25,000

80

120

200

4,000

120

200

470

Average power (mW) 470

1,500

520 1.5

520

448

0.04

15

0.1

–

Few J Few

270

0.025

Few J Few

10

20

0.01

80

125

0.02

0.1

1

1

1

1

1

1

1

1

10

10

Scan speed # of (mm/s) scans 0.1 1

160

2

20

5

Gerd Marowsky Editor

Planar Waveguides and other Confined Geometries Theory, Technology, Production, and Novel Applications

Springer Series in Optical Sciences Volume 189 Founded by H. K. V. Lotsch Editor-in-Chief: W. T. Rhodes Editorial Board: Ali Adibi, Atlanta Toshimitsu Asakura, Sapporo Theodor W. Hänsch, Garching Ferenc Krausz, Garching Bo A. J. Monemar, Linköping Herbert Venghaus, Berlin Horst Weber, Berlin Harald Weinfurter, München

More information about this series at http://www.springer.com/series/624

Springer Series in Optical Sciences The Springer Series in Optical Sciences, under the leadership of Editor-in-Chief William T. Rhodes, Georgia Institute of Technology, USA, provides an expanding selection of research monographs in all major areas of optics: lasers and quantum optics, ultrafast phenomena, optical spectroscopy techniques, optoelectronics, quantum information, information optics, applied laser technology, industrial applications, and other topics of contemporary interest. With this broad coverage of topics, the series is of use to all research scientists and engineers who need up-to-date reference books. The editors encourage prospective authors to correspond with them in advance of submitting a manuscript. Submission of manuscripts should be made to the Editor-in-Chief or one of the Editors. See also www.springer.com/series/624 Editor-in-Chief William T. Rhodes School of Electrical and Computer Engineering Georgia Institute of Technology Atlanta, GA 30332-0250, USA e-mail: [email protected] Editorial Board Ali Adibi School of Electrical and Computer Engineering Georgia Institute of Technology Atlanta, GA 30332-0250, USA e-mail: [email protected] Toshimitsu Asakura Faculty of Engineering Hokkai-Gakuen University 1-1, Minami-26, Nishi 11, Chuo-ku Sapporo, Hokkaido 064-0926, Japan e-mail: [email protected] Theodor W. Hänsch Max-Planck-Institut für Quantenoptik Hans-Kopfermann-Straße 1 85748 Garching, Germany e-mail: [email protected] Ferenc Krausz Ludwig-Maximilians-Universität München Lehrstuhl für Experimentelle Physik Am Coulombwall 1 85748 Garching, Germany and Max-Planck-Institut für Quantenoptik Hans-Kopfermann-Straße 1 85748 Garching, Germany e-mail: [email protected]

Bo A. J. Monemar Department of Physics and Measurement Technology Materials Science Division Linköping University 58183 Linköping, Sweden e-mail: [email protected] Herbert Venghaus Fraunhofer Institut für Nachrichtentechnik Heinrich-Hertz-Institut Einsteinufer 37 10587 Berlin, Germany e-mail: [email protected] Horst Weber Optisches Institut Technische Universität Berlin Straße des 17. Juni 135 10623 Berlin, Germany e-mail: [email protected] Harald Weinfurter Sektion Physik Ludwig-Maximilians-Universität München Schellingstraße 4/III 80799 München, Germany e-mail: [email protected]

Gerd Marowsky Editor

Planar Waveguides and other Confined Geometries Theory, Technology, Production, and Novel Applications

123

Editor Gerd Marowsky Laser-Laboratorium Göttingen e.V. Göttingen, Germany

ISSN 0342-4111 ISSN 1556-1534 (electronic) ISBN 978-1-4939-1178-3 ISBN 978-1-4939-1179-0 (eBook) DOI 10.1007/978-1-4939-1179-0 Springer New York Heidelberg Dordrecht London Library of Congress Control Number: 2014948197 © Springer Science+Business Media New York 2015 This work is subject to copyright. All rights are reserved by the Publisher, whether the whole or part of the material is concerned, specifically the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microfilms or in any other physical way, and transmission or information storage and retrieval, electronic adaptation, computer software, or by similar or dissimilar methodology now known or hereafter developed. Exempted from this legal reservation are brief excerpts in connection with reviews or scholarly analysis or material supplied specifically for the purpose of being entered and executed on a computer system, for exclusive use by the purchaser of the work. Duplication of this publication or parts thereof is permitted only under the provisions of the Copyright Law of the Publisher’s location, in its current version, and permission for use must always be obtained from Springer. Permissions for use may be obtained through RightsLink at the Copyright Clearance Center. Violations are liable to prosecution under the respective Copyright Law. The use of general descriptive names, registered names, trademarks, service marks, etc. in this publication does not imply, even in the absence of a specific statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. While the advice and information in this book are believed to be true and accurate at the date of publication, neither the authors nor the editors nor the publisher can accept any legal responsibility for any errors or omissions that may be made. The publisher makes no warranty, express or implied, with respect to the material contained herein. Printed on acid-free paper Springer is part of Springer Science+Business Media (www.springer.com)

Preface

The aim of this book is to provide an actual collection of highlights in the technology, production, and novel applications of waveguides and other confined geometries, in particular optical fibers. It is well known that waveguide phenomena are nowadays a textbook subject and some energy is needed to prove that waveguide problems are still of great scientific and commercial interest. Any textbook approach should go back to the books by Theodor Tamir,1 who always considered waveguiding as the heart of any integrated optics. It is very interesting to study the details of his first book on this subject in as early as 1975. There he dated the beginning of integrated optics to the late 1960s and mentioned as primary applications signal processing and optical communications. It is striking to note that he did not mention at this time any analytical applications (lab-on-chip) or sensors. However, he already did mention the possible chances of novel optical phenomena opened by the concentration of high intensity fields in thin films and effects due to attendant enhancement of nonlinear and/or active properties of such films. It should be emphasized that at least two contributions in this book deal with nonlinear phenomena in waveguiding structures and potential applications. Contributions came from Europe, Canada, and Israel. The manuscripts have been arranged as follows: • Theoretical considerations for semi-infinite planar waveguides. Unusual, novel ways of efficient frequency conversion in structured fibers and nanoplasmonic waveguides • Five contributions on laser writing of waveguiding structures in various geometries and materials • Channel formation in cluster targets as an example of self-organization of waveguiding structures

1

Still available is the second corrected and updated edition of the book “Integrated Optics,” T. Tamir editor, Springer-Verlag, Berlin, Heidelberg, New York, 1979. v

vi

Preface

• An example of a novel application of Bragg grating technology using optical fibers for 3D shape sensing The contributions are beyond the normal textbook style, representing cuttingedge research results. A short preview/summary of some of the selected contributions is given below: In Chap. 1 of this book radiation emerging from an open-ended waveguide is studied in theory. The idealized case of a planar waveguide open to an infinite half space is considered. An iterative scheme is constructed in analogy to the exact solution of reflection from a step-potential in one-dimensional quantum mechanics and Fresnel reflection of electromagnetic radiation from a half space. For the planar waveguide, the first step in the iterative scheme is evaluated. This yields an approximation to the radiation pattern emerging from the waveguide, as well as the amplitude of the wave reflected back into the waveguide. Another selected example, Chap. 2, considers second-harmonic generation in a circular cylindrical waveguide with embedded periodically arranged tubelets of high nonlinear susceptibility. The configuration is similar to usual quasi-phasematched arrangements, but places the nonlinear polarization sheet at intensity peaks of the guided fundamental wave. This leads (yet only in theory) under optimized conditions to high conversion efficiencies and hence pump depletion has to be considered in the framework of mode-coupling theory. A major advance on femtosecond laser structuring inside optical fibers in Chap. 4 presents powerful new directions for inscribing optical, microfluidic, and mechanical structure devices in the fiber cladding that efficiently interconnect with the fiber core waveguide. This all-fiber platform circumvents tedious packaging and assembly process steps to enable highly functional photonic microsystems and labin-fiber devices to form into a compact and flexible optical fiber system that greatly enhances the value of today’s widely deployed fiber cables. The modification of optical properties of dielectrics has led to the fabrication of waveguides in a variety of glasses and crystals as shown in Chap. 6. UV photosensitivity of germanium-doped glass led to a new technology of fiber Bragg gratings; now femtosecond lasers have allowed yet another aspect of laser-material interaction to be exploited, bordering in the twilight zone between optical damage and plasma formation. This not fully understood process has also led to the production of 3D waveguides and holds the promise of easing the process of waveguide fabrication in all sorts of transparent media, provided the optical loss can be tamed. At the other end of the spectrum, the brute force of carbon dioxide lasers has also been used to cut glass to form delicate, yet complex, low-loss optical devices for fast prototyping and integration. These technologies are reviewed by examining the induction of refractive index changes and waveguides in several different materials. An unusual case of waveguide generation is discussed in Chap. 9: channel formation due to focusing of high-power laser radiation in a self-generated rare gas plasma. The discovery of a stable highly nonlinear mechanism that can compress power to a density exceeding thermonuclear values led to a new era of power

Preface

vii

compression. The associated steps, increasing by a factor of 1010 in power density, mark different stages of technological breakthroughs. Chapter 10 discusses a novel method for direct femtosecond laser-based writing of Bragg gratings and micro-waveguides not only inside the core but also in the cladding of a standard telecom fiber. This enables an optical 3D shape monitoring system using just a single one-core optical fiber. For a 1.5 m long fiber, the tip position can be tracked with an accuracy of less than 1 mm for the x,y,z-coordinates. Applications of this new technology range from medical tracking systems to longterm inspection of boreholes and drilling wells in the oil and gas industry. Göttingen, Germany March 2014

Gerd Marowsky

Acknowledgments

The editor wishes to thank Jaydev Jethwa (Max Planck Institute for Biophysical Chemistry), Charles K. Rhodes (University of Illinois at Chicago), and Anke Düker (Laser-Laboratorium Göttingen) for critical reading of part of the manuscripts and many practical hints and fruitful discussions. Valuable coordination and constant technical assistance of Dirk Born, Jutta Steckel, and Tatjana Kasten (all from LaserLaboratory Göttingen) is gratefully acknowledged. The editor owes particular thanks to Ho Ying Fan from Springer USA in New York for his very engaged and continuous interest in timely finalization of the book-project. The editor took the liberty to make appropriate changes in some of the manuscripts for better readability of the book.

ix

Contents

1

2

Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide .. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . B.U. Felderhof Optimizing Second-Harmonic Generation in a Circular Cylindrical Waveguide with Embedded Periodically Arranged Tubelets of Nonlinear Susceptibility . . . . . .. . . . . . . . . . . . . . . . . . . . B.U. Felderhof, G. Marowsky, and J. Troe

3

Nanoplasmonic Metal –Insulator –Metal Waveguides . . . . . . . . . . . . . . . . . Moshik Cohen, Reuven Shavit, and Zeev Zalevsky

4

Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber Cladding . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . Jason R. Grenier, Moez Haque, Luís A. Fernandes, Kenneth K.C. Lee, and Peter R. Herman

1

21 45

67

5

Fabrication of Channel Waveguides in Chalcogenide Glass Films by a Focused Laser Beam . . . . . . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . 111 K. Shemesh, Yu. Kaganovskii, and M. Rosenbluh

6

Laser Processed Photonic Devices . . . . . . . . . . . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . 129 Jerome Lapointe and Raman Kashyap

7

Advanced Coupling Technologies for Planar and Strip Waveguides .. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . 169 Thomas Fricke-Begemann and Jürgen Ihlemann

8

Nonlinear Light Propagation in Laser-Written Waveguide Arrays ... . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . 185 Matthias Heinrich, Stefan Nolte, and Alexander Szameit

xi

xii

9

Contents

Stable Power Compression with Efficient Relativistic UV Channel Formation in Cluster Targets . . . . . . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . 207 Alex B. Borisov and Charles K. Rhodes

10 Fiber-Optical 3D Shape Sensing . . . . . . . . . . . . . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . 227 Christian Waltermann, Jan Koch, Martin Angelmahr, Jörg Burgmeier, Markus Thiel, and Wolfgang Schade 11 Polarized Fiber Lasers and Amplifiers . . . . . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . 251 Oliver Fitzau Index . . . . . . . . .. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . 265

Chapter 1

Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide B.U. Felderhof

PACS numbers: 41.20.Jb, 42.25.Bs, 42.79.Gn, 43.20.+g

1.1 Introduction In a classic paper Levine and Schwinger [1] studied the radiation of sound from an unflanged circular pipe. Later they extended their theory to electromagnetic radiation [2]. Their work constituted the first major advance in the theory of diffraction after Sommerfeld’s exact solution of the problem of plane wave diffraction by an ideally conducting half plane [3]. In the theory of diffraction of sound, microwaves, or light, the radiation is assumed to propagate in uniform space with reflection by rigid objects or idealized boundaries. For a lucid introduction to the theory of diffraction we refer to Sommerfeld’s lecture notes [4]. The early theory of diffraction was reviewed by Bouwkamp [5]. Later developments are discussed by Born and Wolf [6]. A brief review of the principles and applications of open-ended waveguides with idealized walls was presented by Gardiol [7]. The invention of the dielectric waveguide by Hondros and Debye [8] has led to the development of optical fibers and the subsequent advances in telecommunication. In the theoretical determination of running wave solutions to Maxwell’s equations in a spatially inhomogeneous medium the radiation is assumed to propagate in a guiding structure of infinite length. The problem of emergence of radiation from a semi-infinite waveguide into a half-space is of obvious technical interest. In the case of sound the analysis is based on the exact solution of Levine and Schwinger [1,9–12]. For a dielectric waveguide the observation of the emerging radiation can be used as a tool to study the nature of the driving incident wave [13].

B.U. Felderhof () Institut für Theorie der Statistischen Physik, RWTH Aachen University, Templergraben 55, 52056 Aachen, Germany e-mail: [email protected] G. Marowsky (ed.), Planar Waveguides and other Confined Geometries: Theory, Technology, Production, and Novel Applications, Springer Series in Optical Sciences 189, DOI 10.1007/978-1-4939-1179-0__1, © Springer ScienceCBusiness Media New York 2015

1

2

B.U. Felderhof

It is advantageous to simplify the theoretical analysis by the use of planar symmetry. The theory of Levine and Schwinger was extended to planar geometry by Heins [14,15]. In the following we study radiation emerging from a semi-infinite planar dielectric waveguide. As an intermediate step the wave function in the exit plane must be calculated. In this case the integral equation technique of Schwinger [16] cannot be implemented, because of the complicated nature of the integral kernel. We evaluate the emitted radiation and the coefficients of reflection back into the waveguide approximately in a first step of an iterative scheme. We show in two appendices that the iterative scheme converges to the exact solution in the related problems of reflection by a step potential in one-dimensional quantum mechanics and of Fresnel reflection of an electromagnetic plane wave by a half-space. For the planar dielectric waveguide it does not seem practically possible to go beyond the first step of the iterative scheme. In a numerical example we study a planar waveguide consisting of a slab of uniform dielectric constant, bounded on both sides by a medium with a smaller dielectric constant [17–19]. In the case studied the first step of the iterative scheme leads to a modification of the wave function at the exit plane which is relatively small in comparison with the incident wave. Hence we may expect that the calculation provides a reasonable approximation to the exact solution.

1.2 Planar Open End Geometry We employ Cartesian coordinates .x; y; z/ and consider a planar waveguide in the half-space z < 0 with stratified dielectric constant ".x/ and uniform magnetic permeability 1 . In the half-space z > 0 the dielectric constant is uniform with value "0 and the magnetic permeability is 1 . We consider solutions of Maxwell’s equations which do not depend on the coordinate y and depend on time t through a factor exp.i !t/. Waves traveling to the right in the left half-space will be partly reflected at the plane z D 0 and partly transmitted into the right halfspace. The solutions of Maxwell’s equations may be decomposed according to two polarizations. For TE polarization the components Ex ; Ez , and Hy vanish, and the equations may be combined into the single equation @2 Ey @2 Ey C C "1 ! 2 Ey D 0 2 @x @z2

.TE/:

(1.1)

We have used SI units. For TM polarization the components Ey ; Hx , and Hz vanish, and the equations may be combined into the single equation @2 Hy @2 Hy 1 d " @Hy C "1 ! 2 Hy D 0 C 2 2 @x @z " dx @x

.TM/:

(1.2)

1 Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide

3

Fig. 1.1 Geometry of the planar waveguide

x ⑀1

d

⑀2

0

⑀' z

⑀2 ⑀1

d

⑀'

y

We assume that the profile ".x/ is symmetric, ".x/ D ".x/, and has a simple form with ".x/ increasing monotonically for x < 0 from value "1 to a maximum value "2 at x D 0. An example of the geometry under consideration is shown in Fig. 1.1. In the example the dielectric constant in the left half-space equals a constant "2 for d < x < d and a constant "1 < "2 for x < d and x > d . For definiteness we consider only TM polarization. It is convenient to denote the magnetic field component Hy .x; z/ for z < 0 as u.x; z/ and for z > 0 as v.x; z/. The continuity conditions at z D 0 are u.x; 0/ D v.x; 0C/;

ˇ ˇ 1 @v.x; z/ ˇˇ 1 @u.x; z/ ˇˇ D 0 : ".x/ @z ˇzD0 " @z ˇzD0C

(1.3)

We consider a solution u0n .x; z/ of Eq. (1.2) given by a guided mode solution u0n .x; z/ D

n .x/ exp.ipn z/;

(1.4)

where n .x/ is the guided mode wave function and pn the guided mode wavenumber. We assume pn > 0, so that the wave u0n .x; z/ exp.i !t/ is traveling to the right. The complete solution takes the form un .x; z/ D u0n .x; z/ C u1n .x; z/;

vn .x; z/;

(1.5)

where u1n .x; z/ and vn .x; z/ must be determined such that the continuity conditions Eq. (1.3) are satisfied. The function u1n .x; z/ describes the reflected wave, and vn .x; z/ describes the wave radiated into the right-hand half-space. Since the right-hand half-space is uniform the solution vn .x; z/ takes a simple form and can be expressed as Z 1 p Fn .q/ exp.i qx C i "0 1 ! 2 q 2 z/ dq: (1.6) vn .x; z/ D 1

p p The contribution from the interval "0 1 j!j < q < p"0 1 j!j corresponds to waves traveling to the right; the contribution from jqj > "0 1 j!j corresponds to evanescent waves.

4

B.U. Felderhof

Similarly the solution u1n .x; z/ in the left half-space can be expressed as nX m 1

u1n .x; z/ D

Z Rmn

m .x/ exp.ipm z/

1

C

Rn .q/ .q; x/ exp.i

p

"1 1 ! 2 q 2 z/ dq;

0

mD0

(1.7)

where the sum corresponds to guided waves traveling to the left, with nm the number of such guided modes possible at the given frequency !, and the integral corresponds to waves radiating towards the left. We require that the mode solutions are normalized such that [20] Z Z

1

1 1 1

m .x/ n .x/

".x/

Z dx D ımn ;

1

m .x/

.q; x/ dx D 0; ".x/

1

.q; x/ .q 0 ; x/ dx D ı.q q 0 /: ".x/

(1.8)

The guided mode solutions f m .x/g can be taken to be real. Orthogonality follows from Eq. (1.2). We show in the next section how the functions u1n .x; z/ and vn .x; z/ may in principle be evaluated from an iterative scheme. The coefficients fRmn g and the amplitude function Rn .q/ also follow from the scheme.

1.3 Iterative Scheme The iterative scheme is based on successive approximations to the scattering solution. Thus we write the exact solution as infinite sums un .x; z/ D

1 X

vn .x; z/ D

/ u.j n .x; z/;

j D0

1 X

/ v.j n .x; z/;

(1.9)

j D0

.j C1/

.j C1/

.x; z/; vn .x; z/ determined from the previous with the terms un .j / .j / .0/ un .x; z/; vn .x; z/. In zeroth approximation we identify un .x; z/ with the incident wave, u.0/ n .x; z/ D

n .x/ exp.ipn z/:

(1.10)

.0/

The corresponding vn .x; z/ will be determined by continuity at the exit plane z D 0. .0/ From Eq. (1.10) we have un .x; 0/ D n .x/. This has the Fourier transform n .q/ D

1 2

Z

1 1

n .x/ exp.i qx/

dx:

(1.11)

1 Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide

5

Using continuity of the wave function at z D 0 and the expression Eq. (1.6) we find correspondingly Z v.0/ n .x; z/ D

1 1

n .q/ exp.i qx C i

p "0 1 ! 2 q 2 z/ dq;

(1.12)

.0/

so that in zeroth approximation Fn .q/ D n .q/. Clearly the zeroth approximation does not satisfy the second continuity equation in Eq. (1.3), and we must take care of this in the next approximation. For the difference of terms in Eq. (1.3) we find n.0/ .x/ D

i pn ".x/

n .x/ C

i "0

Z

p "0 1 ! 2 q 2 n .q/ exp.i qx/ dq:

1

1

(1.13)

.0/

By symmetry n .x/ is symmetric in x for n even and antisymmetric in x for n odd. .1/ The next approximation un .x; z/ can be found by comparison with the solution of the problem where the profile ".x/ extends over all space and radiation is generated by a source ".x/.x/ı.z/ with a Sommerfeld radiation condition, so that radiation is emitted to the right for z > 0 and to the left for z < 0. This antenna solution can be expressed as Z uA .x; z/ D

1

K.x; x 0 ; z/.x 0 / dx 0 ;

(1.14)

1

with kernel K.x; x 0 ; z/. The latter can be calculated from the Fourier decomposition 1 ı.z/ D 2

Z

1

e ipz dp;

(1.15)

1

in terms of the integral K.x; x 0 ; z/ D

1 2

Z

1

G.x; x 0 ; p/ e ipz dp;

(1.16)

1

with the prescription that the path of integration in the complex p plane runs just above the negative real axis and just below the positive real axis. The Green function G.x; x 0 ; p/ can be found from the solution of the one-dimensional wave equation, d 2 G 1 d " dG C ."1 ! 2 p 2 /G D ".x/ı.x x 0 /: dx 2 " dx dx

(1.17)

The solution takes the form [20] G.x; x 0 ; p/ D

p

".x/

f2 .x< ; p/f3 .x> ; p/ p 0 ".x /; .f2 ; f3 ; p/

(1.18)

6

B.U. Felderhof

where x< .x> / is the smaller (larger) of x and x 0 and the remaining quantities will be specified in the next section. The Green function satisfies the symmetry properties G.x; x 0 ; p/ D G.x; x 0 ; p/;

G.x; x 0 ; p/ D G.x; x 0 ; p/;

(1.19)

and the reciprocity relation G.x; x 0 ; p/ D G.x 0 ; x; p/:

(1.20)

Consequently the kernel K.x; x 0 ; z/ has the properties K.x; x 0 ; z/ D K.x; x 0 ; z/;

K.x; x 0 ; z/ D K.x; x 0 ; z/;

(1.21)

as well as K.x; x 0 ; z/ D K.x 0 ; x; z/:

(1.22)

.1/

The function un .x; z/ is now identified as Z u.1/ n .x; z/ D

1 1

K.x; x 0 ; z/n.0/ .x 0 / dx 0 :

(1.23)

The minus sign is needed to provide near cancellation of the source density between .0/ .1/ the zeroth and first order solutions, n .x/ C n .x/ 0. We find the first order .1/ function Fn .q/ by Fourier transform from the value at z D 0 in the form Fn.1/ .q/

1 D 2

Z

1

1

i qx u.1/ dx: n .x; 0/e

(1.24)

.1/

The corresponding function vn .x; z/ is found from Eq. (1.6). The first order source .1/ density n .x/ is found to be n.1/ .x/

ˇ Z 1p .1/ 1 @un .x; z/ ˇˇ i D C "0 1 ! 2 q 2 Fn.1/ .q/ exp.i qx/ dq: ˇ ".x/ @z "0 1 zD0 (1.25) .1/

In principle the first order function un .x; 0/ in the exit plane z D 0 may be regarded as the result of a linear operator R.1/ acting on the state n .x/ given by the incident wave. The iterated solution then corresponds to the action with the operator R D R.1/ .I R.1/ /1 , where I is the identity operator. In order j of the .j / geometric series corresponding to the operator R the wave functions u1n .x; z/ and .j / vn .x; z/ in the left and right half-space can be found by completing the function .j / .j / u1n .x; 0/ D v1n .x; 0/ in the exit plane by left and right running waves, respectively.

1 Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide

7

Assuming that the scheme has been extended to all orders we obtain the solutions .0/ u1n .x; z/ D un .x; z/ un .x; z/ and vn .x; z/ given by Eq. (1.9). By construction at .j / .j / each step un .x; 0/ D vn .x; 0/. In the limit we must have 1 X

n.j / .x/ D 0;

(1.26)

j D0

so that the continuity conditions Eq. (1.3) are exactly satisfied. In Appendix 1 we show how the iterative scheme reproduces the exact solution for reflection from a step potential in one-dimensional quantum mechanics. In Appendix 2 we show the same for Fresnel reflection. In the integral in Eq. (1.23) it is convenient to perform the integral over p first, .0/ since n .x 0 / does not depend on p. The pole at pm , arising from a zero of the denominator in Eq. (1.18), yields the first order reflection coefficient [20] Z 1 i .1/ .0/ Rmn D (1.27) m .x/n .x/ dx: 2pm 1 The second term in Eq. (1.2) corresponds to the remainder of the integral, after .1/ subtraction of the simple pole contributions. The function Rn .q/ will be discussed .1/ in the next section. In the calculation of Fn .q/ from Eq. (1.24) we find Fn.1/ .q/ D

nX m 1

.1/ Rmn m .q/ C ıFn.1/ .q/;

(1.28)

mD0 .1/

where ıFn .q/ is the contribution from the remainder of the integral over p, after subtraction of the simple pole contributions. Formally, in the complete solution Eq. (1.2), the reflection coefficients Rmn and the amplitude function Rn .q/ are found as Rmn D .

m ; u1n .0//;

Rn .q/ D . .q/; u1n .0//:

(1.29)

with the scalar product as given by Eq. (1.8). The first step of the iterative scheme yields .1/ D. Rmn

.1/ m ; un .0//;

Rn.1/ .q/ D . .q/; u.1/ n .0//:

(1.30)

The continuum states .q/ can be discretized in the usual way, so that the expressions in Eq. (1.30) can be regarded as elements of a matrix R.1/ . As indicated above, the iterative scheme corresponds to a geometric series, so that the reflection coefficients in Eq. (1.29) can be found as elements of the matrix R D .I R.1/ /1 I; where I is the identity matrix.

(1.31)

8

B.U. Felderhof

Finally the function Fn .q/ can be found from the corresponding state un .0/ as in Eq. (1.24). The function Fn .q/ can be related to the radiation scattered into the right half-space. The scattering angle is related to the component q by p sin D q= "0 1 ! 2 :

(1.32)

Defining the scattering cross section n ./ by n ./ sin d D jFn .q/j2 qdq;

(1.33)

we find the relation n ./ D

p p "0 1 ! 2 "0 1 ! 2 q 2 jFn .q/j2 :

(1.34)

In lowest approximation the cross section is proportional to the absolute square of the Fourier transform of the guided mode n .x/. To higher order the cross section is affected by the reflection into other modes.

1.4 Continuous Spectrum .1/

The calculation of the function Rn .q/ corresponding to the contribution from the continuous spectrum requires a separate discussion. The wave equation (1.17) is related to a quantum mechanical Schrödinger equation for a particle in a potential. The bound states of the Schrödinger problem correspond to the guided modes, and the scattering states correspond to a continuous spectrum of radiation modes. The eigenstates of the Hamilton operator of the Schrödinger problem satisfy a completeness relation which can be usefully employed in the waveguide problem. Explicitly the homogeneous one-dimensional Schrödinger equation correspondp ing to Eq. (1.17) via the relation .x/ D ".x/f .x/ reads [20] d 2f V .x/f D p 2 f; dx 2

(1.35)

where the function V .x/ is given by V .x/ D "1 ! 2 C

p d2 1 " 2p : dx "

(1.36)

By comparison with the quantum mechanical Schrödinger equation we see that U.x/ D N1 C V .x/;

(1.37)

where N1 D "1 1 ! 2 may be identified as the potential. The bound state energies correspond to fN1 pn2 g.

1 Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide

9

It is convenient to assume that the dielectric profile ".x/ equals "1 for x < x1 and x > x1 , so that the potential U.x/ vanishes for jxj > x1 . We define three independent solutions of the Schrödinger equation (1.35) with specified behavior for jxj > x1 . The behavior of the function f1 .x; p/ is specified as f1 .x; p/ D e i q1 x ; f1 .x; p/ D W11 e

for x < x1 ;

i q1 x

C W21 e i q1 x ;

with wavenumber q1 D

for x > x1 ;

p N1 p 2 :

(1.38)

(1.39)

The behavior of the function f2 .x; p/ is specified as f2 .x; p/ D e i q1 x ;

for x < x1 ;

f2 .x; p/ D W12 e i q1 x C W22 e i q1 x ;

for x > x1 :

(1.40)

Similarly, the behavior of the function f3 .x; p/ is specified as f3 .x; p/ D W22 e i q1 x C W12 e i q1 x ; f3 .x; p/ D e

i q1 x

;

for x < x1 ;

for x > x1 :

(1.41)

The coefficients W12 and W22 are elements of the transfer matrix of the planar structure, WD

W11 W12 W21 W22

1 D 0 T

T T 0 RR0 R0 R 1

:

(1.42)

Because of the assumed symmetry of the dielectric profile we have in the present case R0 D R and T 0 D T , so that W21 D W12 . Moreover W11 W22 C W122 D 1:

(1.43)

The functions f2 .x; p/ and f3 .x; p/ were used in the calculation of the Green function in Eq. (1.18). The denominator in that expression is the Wronskian of f2 ; f3 given by .f2 ; f3 / D 2i q1 W22 .p; !/:

(1.44)

From the solution of the inhomogeneous Schrödinger equation it follows that the completeness relation of the normal mode solutions may be expressed as [21] p p Z 1 nX m 1 0 f2 .x; N1 q 2 /f2 .x 0 ; N1 q 2 / 1 n .x/ n .x / p C p dq D ı.xx 0 /: 0/ 2 ; !/j2 2 ".x/".x jW . N q 1 22 1 nD0 (1.45)

10

B.U. Felderhof

Correspondingly the Green function may be decomposed as G.x; x 0 ; p/ D

nX m 1 nD0

n .x/ n .x pn2 p 2

0

/

1 p C ".x/".x 0 / 2

Z

p N1 q 2 /f2 .x 0 ; N1 q 2 / p dq: .N1 q 2 p 2 / jW22 . N1 q 2 ; !/j2 (1.46)

1

f2 .x;

1

p

Hence we find for the antenna kernel K.x; x 0 ; z/ from Eq. (1.16) by use of the integration prescription 0

K.x; x ; z/ D

nX m 1 nD0

i 2pn

i p ".x/".x 0 / 4

Z

1 0

n .x/ n .x

0

/ e ipn jzj

p p f2 .x; N1 q 2 /f2 .x 0 ; N1 q 2 / i pN1 q 2 jzj e dq: p p N1 q 2 jW22 . N1 q 2 ; !/j2 (1.47)

The first order left-hand wave function is therefore found from Eq. (1.23) as u.1/ n .x; z/ D

nX m 1 mD0

i . 2pm

.0/ m ; "n / m .x/

e ipm z

p p Z 1 .0/ . "f2 . N1 q 2 /; "n / i p 0 p C ".x/".x / p 4 N1 q 2 jW22 . N1 q 2 ; !/j2 0 p p 2 f2 .x; N1 q 2 /e i N1 q z dq; (1.48) with scalar product as given by Eq. (1.8). The wave function is the sum of guided modes running to the left and of radiation into the left-hand half-space. The first term agrees with the reflection coefficient given by Eq. (1.27). By symmetry the .0/ matrix element . m ; "n / vanishes unless m and n are both even or both odd. The .1/ integral provides an alternative expression for the remainder ıun .x; z/. From Eq. (1.45) we may identify p p 1 .q; x/ D p p ".x/f2 .x; N1 q 2 /: 2jW22 . N1 q 2 ; !/j

(1.49)

.1/

With this definition the function Rn .q/ is given by p p .0/ . "f2 . N1 q 2 /; "n / i .1/ p p Rn .q/ D p 2 2 N1 q 2 jW22 . N1 q 2 ; !/j i D p . .q/; "n.0/ /: 2 N1 q 2

(1.50)

1 Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide

11

The second line has the same structure as Eq. (1.27). Although the decomposition .1/ in Eq. (1.48) is of theoretical interest, the calculation of the function un .x; z/ is performed more conveniently as indicated in Eq. (1.23), with the integral over p performed first.

1.5 Numerical Example We demonstrate the effectiveness of the scheme on a numerical example. We consider a flat dielectric profile defined by ".x/ D "2 for d < x < d and ".x/ D "1 for jxj > d with values "2 D 2:25"0 and "1 D 2:13"0 . In the right half-space we put "0 D "0 , and we put 1 D 0 everywhere. The geometry is shown in Fig. 1.1. By symmetry the guided modes in infinite space are either symmetric or antisymmetric in x. The explicit expressions for the mode wave functions can be found by the transfer matrix method [20]. At each of the two discontinuities the coefficients of the plane waves exp.i qi x/ and exp.i qi x/ are transformed into coefficients of the plane waves exp.i qj x/ and exp.i qj x/ by a matrix involving Fresnel coefficients given by tij D

2"j qi ; "i qj C "j qi

rij D

"j qi "i qj ; "i qj C "j qi

.i; j / D .1; 2/;

(1.51)

with wavenumbers qj D

q

kj2 p 2 ;

kj D

p "j 1 !:

(1.52)

The wavenumbers pn .!/ of the guided modes are found as zeros of the transfer matrix element W22 .p; !/, which takes the explicit form "2 q 2 C "22 q12 W22 .p; !/ D e 2i q1 d cos 2q2 d i 1 2 sin 2q2 d : 2"1 "2 q1 q2

(1.53)

The guided mode wave functions f n .x/g, their Fourier transforms fn .q/g, and the Green function G.x; x 0 ; p/ can be found in explicit form. In Fig. 1.2 we show the ratio of wavenumbers pn .k/=k as a function of kd for the first few guided modes, p with k D !=c, where c D 1= "0 0 is the velocity of light in vacuum. We choose the frequency corresponding to kd D 12. In that case there are two symmetric modes, denoted as TM0 and TM2, and one antisymmetric mode, denoted as TM1. We assume the incident wave to be symmetric in x. Then it is not necessary to consider the antisymmetric mode. In Fig. 1.3 we show the corresponding normalized wave functions 0 .x/ and 2 .x/. In Fig. 1.4 we show their Fourier transforms 0 .q/ and 2 .q/. The wavenumbers at kd D 12 are

12

B.U. Felderhof

1.5

n=0

pn(k)/k

1.49

n=1

n=2

1.48 1.47 1.46 0

5

10

15 kd

20

25

30

Fig. 1.2 Plot of the reduced wavenumber pn .k/=k of the lowest order guided waves for n D 0; 1; 2, as functions of kd for values of the dielectric constant given in the text

1.5

2(x)

1

0(x),

Fig. 1.3 Plot of the wave functions 0 .x/ and 2 .x/ of the guided modes with n D 0 (no nodes) and n D 2 (two nodes) as functions of x=d

0.5 0 −0.5 −1 −1.5 −3

−2

−1

0 x/d

1

2

3

p0 D 17:955=d and p2 D 17:624=d . The edge of the continuum is given by k1 d D 17:513, and the corresponding value for "2 is k2 d D 18. .0/ In Fig. 1.5 we show the source density in .x/ of the zeroth approximation for n D 0; 2 as a function of x, as given by Eq. (1.13). The coefficients of the simple pole contributions can be calculated from Eq. (1.27). We find numerically for the .1/ discrete part Rd of the matrix R.1/ .1/ Rd

.1/

D

.1/

R00 R02 .1/ .1/ R20 R22

!

D

0:2477 0:0004 : 0:0013 0:2312

(1.54)

For the first correction to the emitted radiation we need to calculate the function .1/ un .x; 0/. The kernel K.x; x 0 ; 0/ in Eq. (1.23) can be evaluated numerically. On account of the symmetry in ˙p it is sufficient to calculate twice the integral along the positive real p axis, with path of integration just below the axis. In the numerical integration over p in Eq. (1.16) the simple poles at fpm g cause problems.

1 Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide

13

0.3 f0(q),f2(q)

0.2 0.1 0 −0.1 −0.2 −0.3 −10

−5

0 qd

5

10

Fig. 1.4 Plot of the Fourier transform 0 .q/ and 2 .q/ of the wave functions of the guided modes with n D 0 (solid curve) and n D 2 (dashed curve) as functions of qd

6 4 −ir0(0)(x), −ir2(0)(x)

Fig. 1.5 Plot of the source .0/ densities i0 .x/ and .0/ i2 .x/, as given by Eq. (1.13), as functions of x=d

2 0 −2 −4 −2

−1

0

1

2

x/d

In order to avoid the simple poles we therefore integrate instead along a contour consisting of the line from 0 to k1 just below the axis, a semicircle in the lower half of the complex p plane centered at .k1 C k2 /=2 and of radius .k2 k1 /=2, and the line just below the real axis from k2 to C1. In Fig. 1.6 we plot as an example the real part of K.x; 0; 0/ as a function of x. The plot of the imaginary part is similar. .1/ In Fig. 1.7 we show the imaginary part of the function u0 .x; 0/, as calculated from Eq. (1.23). This is nearly identical with the contribution from the simple poles at p0 and p2 , which is also shown in Fig. 1.7. In Fig. 1.8 we show the real part of .1/ the function u0 .x; 0/. Here the simple poles do not contribute. The magnitude of .1/ the wave function at the origin u0 .0; 0/ D 0:149 0:005i may be compared with .0/ that of the zeroth approximation u0 .0; 0/ D 1:346. This shows that the first order correction is an order of magnitude smaller than the zeroth order approximation. .0/ .1/ Consequently we may expect that the sum u0 .x; 0/ C u0 .x; 0/ provides a close approximation to the exact value.

14

B.U. Felderhof

Fig. 1.6 Plot of the real part of the kernel K.x; 0; 0/, as given by Eq. (1.16), as a function of x=d

0.3

Re K(x,0,0)

0.2 0.1 0 −0.1 −0.2 −0.3 −3

−2

−1

0

1

2

3

x/d 0.35 0.3 −Re u(1) 0 (x,0)

Fig. 1.7 Plot of the real part of the first order wave .1/ function u0 .x; 0/ at the exit plane as a function of x=d (solid curve), compared with the contribution of the two guided waves .1/ .1/ R00 u0 .x/ C R20 u2 .x/ (dashed curve)

0.25 0.2 0.15 0.1 0.05 0

−2

−1

.0/

0 x/d

1

2

.1/

In Fig. 1.9 we show the absolute value jF0 .q/ C F0 .q/j of the Fourier trans.0/ .1/ form of the sum u0 .x; 0/ C u0 .x; 0/ and compare with the zeroth approximation .0/ jF0 .q/j D j0 .q/j. By use of Eq. (1.34) the absolute square of the transform yields the angular distribution of radiation emitted into the right-hand half-space.

1.6 Discussion In the above we have employed an iterative scheme inspired by the exact solution of two fundamental scattering problems, reflection by a step potential in onedimensional quantum mechanics, shown in Appendix 1, and Fresnel reflection of electromagnetic radiation by a half-space, shown in Appendix 2. For the planar dielectric waveguide we have implemented only the first step of the iterative scheme. In the numerical example shown in Sect. 1.5 even this first step leads to interesting results. The method is sufficiently successful that it encourages application in other situations.

1 Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide

15

0.015

(1)

−Im u0 (x,0)

0.0125 0.01 0.0075 0.005 0.0025 0 −2

−1

0 x/d

1

2

.1/

Fig. 1.8 Plot of the imaginary part of the first order wave function u0 .x; 0/ at the exit plane as a function of x=d

0.35 0.3 F0(q)

0.25 0.2 0.15 0.1 0.05 0

0

2

4

6

8

10

qd .0/

.1/

Fig. 1.9 Plot of the absolute value of the Fourier transform jF0 .q/ C F0 .q/j of the sum of zero order and first order wave function at the exit plane (solid curve), compared with the Fourier .0/ transform jF0 .q/j (dashed curve)

In particular it will be of interest to apply the method to a circular cylindrical dielectric waveguide or optical fiber. The mathematics of the method carries over straightforwardly to this more complicated geometry, with the plane wave behavior in the transverse direction replaced by Bessel functions. Due to symmetry the problem for both planar and cylindrical geometry can be reduced to an equation for a scalar wave function, so that the theory is similar to that for sound propagation. This suggests that an interesting comparison can be made with a lattice Boltzmann simulation. For a rigid circular pipe such a simulation has already been performed by da Silva and Scavone [22], with interesting results. A finite element method has been applied to a rigid open-ended duct of more general cross section [23].

16

B.U. Felderhof

Appendix 1 In this Appendix we show how the iterative scheme reproduces the exact solution of the time-independent one-dimensional Schrödinger equation with a step potential. We consider the equation

d 2u C V .z/u D p 2 u; d z2

(1.55)

with potential V .z/ D 0 for z < 0 and V .z/ D V for z > 0. In proper units p 2 is the energy. We denote the solution for z > 0 as v.z/. For a wave incident from the left the exact solution reads 0

u.z/ D e ipz C Be ipz ;

v.z/ D C e ip z ;

(1.56)

p where p 0 D p 2 V and the reflection coefficient B and transmission coefficient C are given by p p0 ; p C p0

BD

C D

2p : p C p0

(1.57)

The wave function and its derivative are continuous at z D 0. We apply the iterative scheme and put to zeroth order 0

u.0/ .z/ D e ipz ;

v.0/ .z/ D e ip z :

(1.58)

The antenna solution uA .z/ solves the equation d 2 uA C p 2 uA D ı.z/ d z2

(1.59)

for all z. It is given by uA .z/ D K.z/;

K.z/ D

1 ipjzj e : 2ip

(1.60)

To zeroth order the source is .0/ D

ˇ ˇ d u.0/ ˇˇ d v.0/ ˇˇ C D i.p p 0 /: d z ˇzD0 d z ˇzD0

(1.61)

We put the first order solution equal to u.1/ .z/ D K.z/.0/ D

p p 0 ipz ; e 2p

v.1/ .z/ D

p p 0 ip0 z e : 2p

(1.62)

1 Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide

17

Note the minus sign in K.z/.0/ . The value at the exit z D 0 is sufficient to calculate the coefficients B and C from the geometric series BD

1 X p p0 j j D1

2p

C D

;

1 X p p0 j 2p

j D0

:

(1.63)

By continuation one finds for the wave function at order j for j 1 u

.j /

.z/ D

p p0 2p

j e

ipz

;

v

.j /

.z/ D

p p0 2p

j

0

e ip z :

(1.64)

Hence for j 1 the source at order j is

.j /

p p0 D i.p C p / 2p 0

j ;

.j 1/

(1.65)

so that the sum over all j vanishes, 1 X

.j / D 0;

(1.66)

j D0

as it should. Alternatively one can write directly from Eq. (1.62) u1 .z/ D

.p p 0 /=.2p/ p p 0 ipz ipz e D e ; 1 .p p 0 /=.2p/ p C p0

v1 .z/ D

p p 0 ip0 z e : p C p0 (1.67)

Adding this to u.0/ .z/; v.0/ .z/ one reproduces Eq. (1.56).

Appendix 2 In this Appendix we show how the iterative scheme reproduces the exact solution for Fresnel reflection from a half-space. We consider infinite space with dielectric constant " for z < 0 and "0 for z > 0. The magnetic permeability equals 1 everywhere. We consider waves independent of y and TM polarization. Then the magnetic field component Hy .x; z/ satisfies the scalar equation (1.2). We put Hy .x; z/ D u.x; z/ for z < 0 and Hy .x; z/ D v.x; z/ for z > 0. The continuity conditions at z D 0 are ˇ ˇ 1 @u.x; z/ ˇˇ 1 @v.x; z/ ˇˇ u.x; 0/ D v.x; 0C/; D 0 : (1.68) " @z ˇzD0 " @z ˇzD0C

18

B.U. Felderhof

For a plane wave incident from the left the exact solution reads u.x; z/ D e i qx e ipz C Be ipz ;

0

v.x; z/ D C e i qxCip z ;

(1.69)

p p 0 N1 q 2 ; p 0 D N1 q 2 , and reflection coefficient B and with p D transmission coefficient C given by BD

"0 p "p 0 ; "0 p C "p 0

C D

2"0 p : "0 p C "p 0

(1.70)

We apply the iterative scheme and put to zeroth order u.0/ .x; z/ D e i qxCipz ;

0

v.0/ .x; z/ D e i qxCip z :

(1.71)

The antenna solution uA .x; z/ solves the equation @2 uA @2 uA C C "1 k 2 uA D ".x/ı.z/ @x 2 @z2

(1.72)

for all .x; z/. For .x/ D q e i qx it is given by uA .x; z/ D e i qx K.z/q ;

K.z/ D

" ipjzj e : 2ip

(1.73)

To zeroth order the source q is q.0/

De

i qx

ˇ ˇ 1 @u.0/ ˇˇ p p0 1 @v.0/ ˇˇ 0 : D i C " @z ˇzD0 "0 @z ˇzD0 " "

(1.74)

We put the first order solution equal to u.1/ .x; z/ D e i qx K.z/q.0/ D v.1/ .x; z/ D

"0 p "p 0 i qxipz ; e 2"0 p

"0 p "p 0 i qxCip0 z e : 2"0 p

(1.75)

.0/

Note the minus sign in e i qx K.z/q . The value at the exit z D 0 is sufficient to calculate the coefficients B and C from the geometric series BD

1 0 X " p "p 0 j j D1

2"0 p

;

C D

1 0 X " p "p 0 j j D0

2"0 p

By continuation one finds for the wave function at order j for j 1

:

(1.76)

1 Radiation from a Semi-infinite Unflanged Planar Dielectric Waveguide

u.j /.x; z/ D

"0 p "p 0 2"0 p

j

v.j / .x; z/ D

e i qxipz ;

"0 p "p 0 2"0 p

19

j

0

e i qxCip z : (1.77)

Hence for j 1 the source at order j is q.j / D i

p0 p C 0 " "

"0 p "p 0 2"0 p

j ;

.j 1/

(1.78)

so that the sum over all j vanishes, 1 X

q.j / D 0;

(1.79)

j D0

as it should. Alternatively one can write directly from Eq. (1.75) u1 .x; z/ D

."0 p "p 0 /=.2"0 p/ "0 p "p 0 i qxipz i qxipz e D e ; 1 ."0 p "p 0 /=.2"0 p/ "0 p C "p 0

v1 .x; z/ D

"0 p "p 0 i qxCip0 z e : "0 p C "p 0

(1.80)

Adding this to u.0/ .x; z/; v.0/ .x; z/ one reproduces Eq. (1.69). We note that the zeroth and first order source densities are related by q.1/ D Mq.0/ ;

M D

"0 p C "p 0 : 2"0 p

(1.81)

Hence we find B D 1 M 1 ;

C D 1 C B:

(1.82)

This suggests that more generally the complete solution of the scattering problem may be found from the relation between the zeroth and first order source densities.

References 1. 2. 3. 4. 5. 6. 7.

H. Levine, J. Schwinger, Phys. Rev. 73, 383 (1948) H. Levine, J. Schwinger, Commun. Pure Appl. Math. 3, 355 (1950) A. Sommerfeld, Math. Ann. 47, 317 (1896) A. Sommerfeld, Optics (Akademische Verlagsgesellschaft, Leipzig, 1964) H. Bouwkamp, Rep. Prog. Phys. 17, 35 (1954) M. Born, E. Wolf, Principles of Optics (Pergamon Press, Oxford, 1975) F.E. Gardiol, in Advances in Electronics and Electron Physics, vol. 63, ed. by P.W. Hawkes (Academic, London, 1985), p. 139

20

B.U. Felderhof

8. D. Hondros, P. Debye, Ann. d. Phys. 32, 465 (1910) 9. G.F. Homicz, J.A. Lordi, J. Sound Vib. 41, 283 (1975) 10. P. Joseph, C.L. Morfey, J. Acoust. Soc. Am. 105, 2590 (1999) 11. M.S. Howe, Hydrodynamics and Sound (Cambridge University Press, Cambridge, 2007) 12. S.W. Rienstra, A. Hirschberg, An Introduction to Acoustics 2014, www.win.tue.nl/~sjoerdr/ papers/boek.pdf 13. D.M.S. Soh, J. Nilsson, S. Baek, C. Codemard, Y. Jeong, V. Philippov, J. Opt. Soc. Am. A21, 1241 (2004) 14. A.E. Heins, Q. Appl. Math. 6, 157 (1948) 15. P.C. Clemmow, Proc. R. Soc. A 205, 286 (1951) 16. F.E. Borgnis, C.H. Papas, Electromagnetic Waveguides and Resonators (Springer, Berlin, 1958) 17. D. Marcuse, Theory of Dielectric Optical Waveguides (Academic, New York, 1974) 18. H. Kogelnik, in Integrated Optics, Topics Appl. Phys. 7, ed. by T. Tamir (Springer, Berlin, 1979) 19. P. Lorrain, D.R. Corson, F. Lorrain, Electromagnetic Fields and Waves (Freeman, New York, 1988) 20. A. Bratz, B.U. Felderhof, G. Marowsky, Appl. Phys. B 50, 393 (1990) 21. R.G. Newton, Scattering Theory of Waves and Particles (McGraw-Hill, New York, 1966) 22. A.R. da Silva, G.P. Scavone, J. Phys. A 40, 397 (2007) 23. W. Duan, R. Kirby, J. Acoust. Soc. Am. 131, 3638 (2012)

Chapter 2

Optimizing Second-Harmonic Generation in a Circular Cylindrical Waveguide with Embedded Periodically Arranged Tubelets of Nonlinear Susceptibility B.U. Felderhof, G. Marowsky, and J. Troe

2.1 Introduction An efficient method of generating second-harmonic radiation (SHG) can find use in a variety of technical applications. Confined geometry—such as in fibers or film waveguides—allows concentration of the fundamental radiation at the position of the material with nonlinear susceptibility. In earlier work [1] we have investigated SHG in a planar geometry and studied the dependence on the position of nonlinear material with respect to the planar device that guides the fundamental radiation. SHG was enhanced by a judicious use of periodicity of the nonlinear material in the direction of propagation of the fundamental wave. In this paper we consider instead confinement of radiation in a circular waveguide or optical fiber. This geometry has the advantage of confinement in both transverse dimensions, thus avoiding diffraction and the corresponding dispersion of the fundamental beam in a transverse direction. The following calculations show that the circular geometry is preferable to the planar one, even when in the latter case the beam has infinite width, so that diffraction no longer plays a role. In the following we analyze SHG in a circular waveguide for an idealized situation of high symmetry. The nonlinear material—representing an idealized polarization sheet [2]—is assumed to be arranged in a periodic array of cylindrical tubelets centered around the axis of the waveguide. The period in the axial direction can be optimized by use of a Bragg condition involving the wavenumbers of both

B.U. Felderhof () Institut für Theorie der Statistischen Physik, RWTH Aachen University Templergraben 55, 52056 Aachen, Germany e-mail: [email protected] G. Marowsky • J. Troe Laser-Laboratorium Göttingen e.V. Hans-Adolf-Krebs-Weg 1, 37077 Göttingen, Germany e-mail: [email protected] G. Marowsky (ed.), Planar Waveguides and other Confined Geometries: Theory, Technology, Production, and Novel Applications, Springer Series in Optical Sciences 189, DOI 10.1007/978-1-4939-1179-0__2, © Springer ScienceCBusiness Media New York 2015

21

22

B.U. Felderhof et al.

the fundamental and the doubled frequency. In addition one can optimize the axial width of the tubelets and their transverse radius. By integration over the radius the calculation can be extended to cover the case of tubelets of finite thickness, or of an array of solid cylindrical pieces. Admittedly, the idealized situation under consideration may be difficult to realize experimentally. The intention of our model calculation is to elucidate the principles, and to serve as a guide for the analysis of more realistic but less symmetric situations. Due to the high symmetry of the model situation we can limit attention to a small number of modes. This advantage is lost in more realistic situations. The paper is organized as follows: First we perform a calculation in analogy to that for planar geometry [1] for a finite length L of nonlinear material distributed in N tubelets, where N is much larger than unity. For optimum phase matching the intensity of the generated SHG grows in proportion to L2 . In the circular waveguide the efficiency is sufficiently high so that it is necessary to consider depletion of the fundamental. On a large length scale the effect of depletion may be studied by use of mode-coupling theory. The situation is mathematically analogous to that of SHG in anisotropic crystals, so that the mode-coupling theory of Armstrong et al. [3] can be used. Apparently this was not realized by Zhao et al. [4], who formulated mode-coupling equations on the much smaller length scale of the period of the array. Second-harmonic generation in poled optical fibers using gratings optically written by mode interference was studied experimentally by Fermann et al. [5]. Analogous experiments in thermally poled twin-hole glass fibers were performed by Mizunami et al. [6, 7]. Pump depletion in a waveguide filled with periodically poled lithium niobate was observed by Parameswaran et al. [8] to be in good agreement with theory.

2.2 Circular Waveguide Theory We consider a circular waveguide of radius b filled with material which is uniform in the axial direction z and with electric and magnetic permeability, which depend only on the radial direction r. We use cylindrical coordinates .r; '; z/. The dielectric profile ".r; !/ and magnetic profile .r; !/ depend also on frequency !. We assume that for the frequencies of interest " and are real. Also we assume that " and tend to constants "i ; i for small r and to constants "f ; f for r ! b. In later application we consider in particular a two-layer situation with "; D "2 ; 2 for 0 < r < d and "; D "1 ; 1 for d < r < b. We consider plane wave solutions of Maxwell’s equations which depend on z and t through a factor exp.ipz i !t/ and which do not depend on the azimuthal angle '. Maxwell’s equations for the electric and magnetic field amplitudes then read in SI units [9–11]

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

drHr d "rEr C ip"rEz D 0; C iprHz D 0; dr dr E' H' dH' dE' C D i !Hz ; C D i !"Ez ; dr r dr r dHz dEz ipEr D i !H' ; ipHr D i !"E' ; dr dr pE' D !Hr ; pH' D !"Er :

23

(2.1)

The solutions of these equations may be decomposed according to two polarizations. For TE-polarization the components Er ; Ez , and H' vanish, and the equations may be combined into the single equation d 2 E' 1 r d.=r/ dE' 1 d 2 C "! 2 E' D p 2 E' dr 2 dr dr r dr r

.TE/: (2.2)

For TM-polarization the components Hr ; Hz , and E' vanish, and the equations may be combined into the single equation d 2 H' r d."=r/ dH' 1 1 d" 2 C "! H' D p 2 H' dr 2 " dr dr "r dr r 2

.TM/: (2.3)

We consider first TE-polarization. We assume that for 0 < r < ri the permeabilities "; equal "i ; i and that for r > rf they equal "f ; f . We write the solution of Eq. (2.2) in these two regions: E' .r/ D J1 .qi r/

for r < ri ;

E' .r/ D Af J1 .qf r/ C Bf Y1 .qf r/

for r > rf ;

with Bessel-functions J1 .qr/; Y1 .qr/ and wavenumbers q qj D "j j ! 2 p 2 :

(2.4)

(2.5)

The coefficients Af and Bf are related by the boundary conditions at r D b. The p wavenumbers fqi ; qf g are real only up to a maximum value of p given by "j j ! in either case and are pure imaginary beyond this value. For such wavenumbers we rewrite the second equation in (2.4) as E' .r/ D AI1 . f r/ C BK1 . f r/

for r > rf ; (2.6) p with modified Bessel-functions I1 . r/ and K1 . r/ and D p 2 "! 2 . The p guided mode solutions occur at discrete values fpj g of p larger than "f f !. We assume that the radius b is sufficiently large that the waveguide condition can be approximated by A.p; !/ D 0:

(2.7)

24

B.U. Felderhof et al.

At fixed ! the roots of this equation determine the discrete values fpj g for which a guided mode solution exists. We call A.p; !/ the dispersion function. The explicit expressions for the coefficients A.p; !/ and B.p; !/ in the analogous case of TM-polarization will be given in Eq. (2.54). The one-dimensional wave equation (2.2) can be transformed to a form resembling the one-dimensional time-independent Schrödinger equation by use of the transformation r f .r/: (2.8) E' .r/ D r By substitution we find that Eq. (2.2) is transformed to d 2f V .r/f D p 2 f; dr 2

(2.9)

where the function V .r/ is given by r V .r/ D "! 2 C

d2 r dr 2

r

1 d log.r/ r C : r dr

(2.10)

It is of interest to derive an expression for the norm of the eigensolutions. Differentiating Eq. (2.9) with respect to p 2 one derives the identity @ @f @f @f @ f D f 2: 2 (2.11) @r @r @p 2 @p @r Applying this identity to guided mode solutions normalized as in Eq. (2.4) we find by integration over r and use of the waveguide condition (2.7) ˇ Z b 1 @A.p; !/ ˇˇ r E 2 E'j .r/ dr D B.pj ; !/ : (2.12) Nj D 2f pj @p ˇpj 0 .r/ We shall show in the next section that the norm is related to the intensity of the mode. It follows from Eq. (2.3) that for TM-polarization exactly the same relations hold if we replace E' by H' , " by , and by ". Where necessary the symbols corresponding to the two types of solution will be distinguished by a superscript E or M.

2.3 Excitation of Guided Modes In this section we describe how the eigenmodes may be excited by an oscillating dipole density. We begin by relating the norm of an eigenmode, given by Eq. (2.12), to the physical intensity. The energy current density averaged over a time period 2=! is given by the Poynting vector S D

1 Re.E H /: 2

(2.13)

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

25

The z-component of this expression may be decomposed into Sz D SzE C SzM ;

(2.14)

with the separate terms for TE- and TM-polarizations SzE D

p jE' j2 ; 2!

SzM D

p jH' j2 : 2!"

(2.15)

We define the total intensity by the integrals Z

Z

b

I E D 2 0

SzE .r/r dr;

b

I M D 2 0

SzM .r/r dr:

(2.16)

The intensity does not depend on z. For a single eigenmode of either TE- or TM-type the expressions (2.15) become E Szj D

pjE 2!

jE'j j2 ;

M Szj D

pjM 2!"

jH'j j2 :

(2.17)

By comparison with Eq. (2.12) we find that for a single eigenmode excited with amplitude aj the intensity is related to the norm of the mode by Ij D

pj Nj jaj j2 : !

(2.18)

This expression is formally the same for both polarizations. Using orthogonality of the eigenmodes [9–11] we find that for a linear superposition of guided modes, all oscillating at the same frequency !, the total intensity is given by I D

X .IjE C IjM /;

(2.19)

j

which again does not depend on z. Next we investigate how radiation is emitted by an antenna embedded in the waveguide. We consider a surface polarization [12–14] P S .z/ of finite extent in the z-direction, independent of ', located at radius r D r0 , and oscillating at frequency !. The corresponding charge and current densities are .r/ D

@PzS @ ı.r r0 / PzS ı.r r0 /; @z @r j .r/ D i !P S .z/ı.r r0 /;

(2.20)

26

B.U. Felderhof et al.

which must be added as source terms to Maxwell’s equations. The charge and current densities are related by the continuity equation i ! C r j D 0. A Fourier analysis of the surface polarization yields Z

S PO .p/e ipz dp:

P S .z/ D

(2.21)

From Maxwell’s equations we now find instead of Eq. (2.2) d 2 EO ' 1 O r d.=r/ d EO ' 1 d 2 2 C "! p 2 E' dr 2 dr dr r dr r D ! 2 PO'S ı.r r0 /:

(2.22)

Similarly instead of Eq. (2.3) d 2 HO ' 1 O r .d "=r/ d HO ' 1 d" 2 2 C "! H' D p dr 2 " dr dr "r dr r 2 d 1 d" OS Pz ı.r r0 / !p POrS ı.r r0 /: ı.r r0 / i ! POzS dr " dr

(2.23)

The solution of these equations may be found with the aid of the Green’s functions G E .r; r0 / and G M .r; r0 / defined by the equation d 2G V .r/G D p 2 G C ı.r r0 /: dr 2

(2.24)

The Green’s function may be expressed as G.r; r0 / D

f1 .r< /f2 .r> / ; .f1 ; f2 /

(2.25)

where r< .r> / is the smaller (larger) of r and r0 , in terms of the two fundamental solutions f1 ; f2 defined by r f1E .r/

D r

f2E .r/ D

r J1 .qi r/; i r K1 . f r/; f

r

r J1 .qi r/; for r < ri ; "i r r f2M .r/ D K1 . f r/; for r > rf ; (2.26) "f

f1M .r/

D

with the Wronskian ˇ ˇ ˇ f1 f2 ˇ ˇ .f1 ; f2 / D ˇ 0 0 ˇˇ: f1 f2

(2.27)

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

27

The Wronskian takes the value .f1E ; f2E / D

1 E A .p; !/; f

.f1M ; f2M / D

1 M A .p; !/: "f

(2.28)

The solution of Eq. (2.22) is given by EO ' .p; r/ D ! 2 Œ.r/=r 1=2 G E .r; r0 /Œ.r0 /r0 1=2 PO'S :

(2.29)

The solution of Eq. (2.23) is given by HO ' .p; r/ D i !Œ".r/=r 1=2

@G M .r;r0 / @r0

C

1 d ln ".r0 / M 2 dr0 G .r; r0 /

C 2r10 G M .r; r0 / Œ".r0 /=r0 1=2 POzS !pŒ".r/=r 1=2 G M .r; r0 /Œ".r0 /=r0 1=2 POrS : (2.30) For a surface polarization P S .z/ with arbitrary variation in the z-direction the fields E' .r; z/ and H' .r; z/ are now obtained by Fourier superposition. Thus we find Z Z E' .r; z/ D EO ' .p; r/e ipz dp; H' .r; z/ D HO ' .p; r/e ipz dp; (2.31) S where EO ' .p; r/ and HO ' .p; r/ are given by Eqs. (2.29) and (2.30) in terms of PO .p/. The Wronskian, given by Eq. (2.28), vanishes at the eigenvalues fpjE g and fpjM g. For large z the contribution from the corresponding poles dominates the integrals in Eq. (2.31). This allows us to evaluate the amplitude of the various guided modes excited by the oscillating surface polarization.

2.4 Emitted Radiation In this section we analyze the radiation emitted by a circular cylindrical antenna, as introduced in the preceding section, in more detail. We are interested in the radiation channeled into the waveguide and detected at large positive z. At sufficiently large distance from the antenna, i.e., after the decay of transients corresponding to evanescent wave solutions, the behavior of the fields is dominated by pole contributions to the integrals, corresponding to roots of the waveguide condition (2.7). The contributions may be found by contour integration in Eq. (2.31) with the poles at positive fpj g shifted slightly upwards into the complex plane and those at fpj g shifted slightly downwards. We note that it follows from Eq. (2.6) that for values fpj g for which the waveguide condition is satisfied f1 .pj ; r/ D B.pj ; !/f2 .pj ; r/:

(2.32)

28

B.U. Felderhof et al.

Thus we find for large positive z, far from the source P S .z/, X E E E a1j E' .r; z/ j .r/ exp.ipj z/;

(2.33)

j

where we employ the notation E j .r/

D

p .r/=rf1jE .r/:

(2.34)

The amplitudes are given by E OS E j .r0 /P' .pj /;

E a1j D i ! 2 .pjE NjE /1 r0

(2.35)

where we have used Eq. (2.12). From Eq. (2.33) we may evaluate the intensity defined in Eq. (2.16). Because of the orthogonality of the different modes [9–11] there are no cross terms, and we find by use of Eq. (2.18) X X IjE D 3 ! 3 .pjE NjE /1 r02 Œ jE .r0 / 2 jPO'S .pjE /j2 : (2.36) IE D j

j

Similarly we find for large positive z X M a1j H' .r; z/

M M j .r/ exp.ipj z/;

(2.37)

j

with the notation M j .r/

D

p ".r/=rf1jM .r/:

(2.38)

The amplitudes are given by M D !.pjM NjM /1 Rj .r0 /POrS .pjM / C Zj .r0 /POzS .pjM / ; a1j

(2.39)

with the abbreviations Rj .r/ D Zj .r/ D

ir M p ".r/ j @ r

M j .r/

".r/

@r

M j .r/;

1 C r

M j .r/

:

(2.40)

This yields for the intensity IM D

X

IjM

j

D 3!

X j

ˇ2 ˇ .pjM NjM /1 ˇRj .r0 /POrS .pjM / C Zj .r0 /POzS .pjM /ˇ : (2.41)

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

29

The expressions (2.36) and (2.41) have a fairly simple structure. The efficiency with which a surface polarization P S .z/ excites the guided modes is determined by its Fourier component at the wavenumber pj , as well as by its radial location r0 via the eigenfunction j .r0 /, which appears quadratically with its proper normalization Nj .

2.5 Phase Matching In this section we discuss the principle of second-harmonic generation by use of a phase-matched adsorbate embedded in a circular cylindrical waveguide. We shall assume that the adsorbate either is located as a thin layer directly outside the core or is embedded in the core. We consider a surface polarization P S .z/ located at radius r0 and induced by an incident fundamental wave. The polarization acts as an antenna emitting waves at the second-harmonic frequency. Thus we put P S .r0 ; z/ D .2/ .z/ W E 10 .r0 ; z/E 10 .r0 ; z/;

(2.42)

where E 10 .r0 ; z/ is the incident fundamental field at the location of the adsorbate. If the fundamental field oscillates at frequency !, then the surface polarization oscillates at frequency 2!, and this must be taken into account in the expressions of the preceding sections. We assume that the adsorbate is so weak that it does not disturb the fundamental wave. This is expressed by the subscript zero in (2.42). The fundamental wave is a linear combination of guided modes with z-dependence exp.ipj z/ with wavenumber pj .!/. We shall assume that the susceptibility .2/ depends on z via the density of adsorbed molecules. If the adsorbate has a periodicity in the z-direction with period a characterized by the wavenumber K D 2=a, then we may expect resonance when the phasematching condition pj .2!/ D 2pk .!/ C nK;

n D 0; ˙1; ˙2; : : :

(2.43)

is satisfied. More specifically it is natural to aim at satisfying the condition p0 .2!/ D 2p0 .!/ ˙ K;

(2.44)

for the lowest mode j D 0. We shall call this the Bragg condition. We consider in particular a grating of period a consisting of N adsorbate tubelets of width w < a. An example of the grating and waveguide is shown in Figs. 2.1 and 2.2. The susceptibility function is given by .z/ D .2/ gN .z/;

(2.45)

30

B.U. Felderhof et al.

Fig. 2.1 Axial cross section of the waveguide and adsorbate structure. The figure should be rotated about the z axis to get the three-dimensional picture

r d 0 d

⑀1 ⑀2 ⑀2

z

⑀1

Fig. 2.2 Three-dimensional picture of the waveguide and adsorbate structure

with the Bragg function gN .z/ D

N 1 X

1 .w; z na w/; 2 nD0

(2.46)

where .w; z/ D 1

for D0

w w : 2

(2.47)

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

31

The prefactor .2/ in (2.45) is a third rank tensor independent of z. We shall assume that .2/ has the characteristics of a layer isotropic about the surface normal in the radial direction. We also assume that there exists a mirror plane containing the radial normal to exclude chirality. From these assumptions it follows that .2/ has only three independent components (for details see [14–17]). The Fourier-component O S .p/ is proportional to P Z 1 1 GO N .p 2pk .!// D gN .z/e 2ipk .!/zipz d z 2 1 D

exp.i sk w/ 1 1 exp .iN sk a/ ; 2 i sk 1 exp.i sk a/

(2.48)

where we have introduced the variable sk D 2pk .!/ p:

(2.49)

For real p the absolute square of the second factor in Eq. (2.48) is given by ˇ ˇ 2 ˇ 1 e iN sa ˇ2 ˇ D sin .N sa=2/ ; ˇ (2.50) FN .sa/ D ˇ 1 e i sa ˇ sin2 .sa=2/ which takes the values N 2 at sa D 2n, where n D 0; ˙1; ˙2; : : :. Since we wish O S .p/ to be maximum at p0 .2!/ we choose the lattice distance a such that P a D 2j2p0 .!/ p0 .2!/j1

(2.51)

corresponding to n D 1 or n D 1. In this way we satisfy the Bragg condition (2.44). The width of the function in Eq. (2.50) at s D ˙2=a is of order 1=Na. Hence the area of the peak is proportional to N . The larger N , the more precisely the condition (2.51) must be satisfied. An error a in the value of a implies an error p D 2a=a2 in p-space. If we require this to be at most 1=Na, then N cannot be larger than a=2a. Ideally one would use a tunable laser and adjust the frequency ! such that the condition (2.51) is precisely satisfied. With that choice the absolute square of the first factor in Eq. (2.48) is maximal at w D 12 a.

2.6 Second-Harmonic Generation In this section we investigate the effect of geometry on the efficiency for secondharmonic generation. We consider the core of the waveguide to be a cylinder of radius d with dielectric constant "2 surrounded by an outer mantle with uniform dielectric constant "1 < "2 . The grating of adsorbed molecules is located at radius r0 , either inside or outside the core (r0 < d or r0 > d ). We put the magnetic permeability equal to 0 everywhere and consider guided mode solutions of TM type. We study the dependence of the efficiency for second-harmonic generation on the radius r0 .

32

B.U. Felderhof et al.

The discontinuity of the dielectric constant at r D d corresponds to jump conditions for the tangential component H' .r/. The first condition is that H' .r/ is continuous at r D d . The wave equation (2.3) may be rewritten as ".r/

H' 1 dH' d C C "! 2 H' D p 2 H' : dr ".r/ dr r".r/

(2.52)

Hence the second condition is that .dH' =dr C H' =r/=" is continuous at the interface. In analogy to Eqs. (2.4) and (2.6) we write the solution as H' .r/ D J1 .q2 r/;

for 0 < r < d;

D A I1 . 1 r/ C B M K1 . 1 r/; M

for d < r < b;

(2.53)

p p where q2 D "2 0 ! 2 p 2 and 1 D p 2 "1 0 ! 2 . From the two continuity equations we find for the coefficients AM and B M "1 q2 dJ0 .q2 d /K1 . 1 d / C 1 dJ1 .q2 d /K0 . 1 d /; "2 "1 B M .p; !/ D q2 dJ0 .q2 d /I1 . 1 d / C 1 dJ1 .q2 d /I0 . 1 d /: "2 AM .p; !/ D

(2.54)

Putting AM .p; !/ D 0 for fixed ! one finds the wavenumbers pjM .k/ of the guided modes. The guided mode solutions take the form M j .r/

D J1 .q2j r/;

for 0 < r < d;

D B M .pjM ; !/K1 . 1j r/;

for d < r < b:

(2.55)

From Eq. (2.12) one finds for their norm Z NjM

b

D 0

r Œ ".r/

M 2 j .r/

ˇ 1 @AM .p; !/ ˇˇ M dr D B .pj ; !/ ˇ M: @p 2"1 pjM pj

(2.56)

The electrical field has components Er .r/ D

p H' ; !"

Ez .r/ D

H' i dH' C : !" dr r

(2.57)

We assume that the fundamental is present as a single mode oscillating at frequency M ! with amplitude a1k .!/. Hence the electrical field vector is E .!I r; z/ D

M .!/ M a1k p !".r/ k

M k .r/e r

Ci

d

M k .r/

dr

C

M k .r/ r

e z exp.ipkM z/: (2.58)

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

33

We assume an isotropic tensor .2/ with mirror symmetry. The induced surface polarization is P SM .2!; z/ D gN .z/

2

M .!/ a1k !".!; r0 /

X k .!; r0 / exp.2ipkM z/;

(2.59)

with Bragg factor given by Eq. (2.46) and vector X k .!; r0 / given by X k .!; r/ D 1 pkM

2 M k .!; r/

2

C2i3 pkM .2/

M k .!; r/

.2/

d

M k .r/

d

dr

M k .r/

dr .2/

C

C

2 M k .r/

er

r M k .r/ ez; r

(2.60)

.2/

where 1 D rrr ; 2 D rzz , and 3 D zrz D zzr are the relevant components of the nonlinear susceptibility tensor .2/ . We assume that the layer of second-order susceptibility is locally flat, so that the subscript r corresponds to the locally normal component and z to the locally tangential component. For a representation of the tensor in the local Cartesian frame see Roders et al. [17]. The emitted secondharmonic radiation is TM-polarized. The intensity of the emitted second-harmonic radiation is given by Eq. (2.41), with the right-hand side taken at frequency 2! instead of !. We find by use of Eq. (2.18)

IjM .2!/ D

1 2 jGO N .pjM .2!/ 2pkM .!//j2 M !".!; r0 /4 pj .2!/NjM .2!/pkM .!/2 NkM .!/2 ˇ ˇ2 2 ˇRj .2!; r0 /Xkr .!; r0 / C Zj .2!; r0 /Xkz .!; r0 /ˇ IkM .!/ :

(2.61)

The conversion coefficient is defined by M M MM j k D Ij .2!/=Ik .!/:

(2.62)

We write the conversion coefficient in the form MM jk D

2 O jGN .pjM .2!/ 2pkM .!//j2 Aj k .r0 /IkM .!/; c

(2.63)

with coefficient Aj k .r0 / D

ˇ ˇ ˇRj .2!; r0 /Xkr .!; r0 / C Zj .2!; r0 /Xkz .!; r0 /ˇ2 k".!; r0 /4 pjM .2!/NjM .2!/pkM .!/2 NkM .!/2

;

(2.64)

and write the latter as Aj k .r0 / D

1 X "30 d 6

C .j jkI r0 / ;

(2.65)

34

B.U. Felderhof et al.

1.5 p2(k)/k,p1(k)/k,p0(k)/k

Fig. 2.3 Plot of the wavenumber p0 .k/ of the lowest order guided wave (solid curve), of the wavenumber p1 .k/ of the first-order guided wave (long dashes), of the wavenumber p2 .k/ of the second-order guided wave (short dashes), as functions of kd for values of the dielectric constant given in the text

1.49 1.48 1.47 1.46 10

20

30

40

50

kd

with dimensionless coefficients C .j jkI r0 /. The factors Rj and Zj are given by Eq. (2.40), and Xr and Xz are given by Eq. (2.60). The coupling coefficients C .j jk/ depend on the radius r0 and the geometry of the waveguide. The efficiency of second-harmonic generation for the chosen geometry is characterized by the Bragg prefactor jGO N j2 and the coefficients C .j jkI r0 /. We consider the width d to be fixed, and vary the frequency !. The input laser is tuned in a narrow frequency range, so that dispersion of the dielectric constant near ! and 2! may be neglected. We put "2 .!/ D 2:25"0, "2 .2!/ D 2:28"0 , in combination with "1 .!/ D 2:13"0 and "1 .2!/ D 2:17"0 . In Fig. 2.3 we plot the reduced wavenumbers p0 .k/=k; p1 .k/=k, and p2 .k/=k at the fundamental p frequency as functionspof kd . The ratios fpn .k/=kg are larger than "1 ="0 D 1:4595 and less than "2 ="0 D 1:5. The corresponding plots at the secondharmonic frequency are very similar. In Fig. 2.4 we plot the coefficient C11 .0j0I r0/ at kd =24 as a function of the fraction r0 =d . In Figs. 2.5 and 2.6 we present similar plots for the coefficients .2/ C22 .0j0I r0/ and C33 .0j0I r0/. The plot in Fig. 2.4 for susceptibility 1 D rrr shows the largest rate of conversion. It is of interest to compare the optimal situation with that for a planar waveguide. We have found earlier that for a planar waveguide consisting of a slab of dielectric constant "2 of thickness 2d surrounded by a medium of dielectric constant "1 second-harmonic generation is optimal for a thin polarization layer midway between the two interfaces (in Ref. 1 this was called geometry III). For the planar waveguide the conversion coefficient took the form X 4 2

MM j kP D GNj kP Bj k JkM .!/; (2.66) !

with Bragg factor GNj kP D jGO N .pjM .2!/ 2pkM .!//j2 :

(2.67)

Here the wavenumbers p must be calculated for the guided modes of the planar waveguide, so that the lattice distance a and the Bragg factor GNj kP differ from

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

35

4000 3000 C11(0 0)

2000 1000 0

0

0.2

0.4

0.6 r0/d

0.8

1

Fig. 2.4 Plot of the coupling coefficient C11 .0j0I r0 / for kd D 24 as a function of r0 =d . The coefficient characterizes the efficiency of conversion, as given by Eqs. (2.63) and (2.65), of the lowest order guided wave with largest wavenumber p0 .k/ at the fundamental frequency ! D kc to the mode with largest wavenumber p0 .2k/ at the second-harmonic frequency 2! D 2kc. The radius of the tubelet of nonlinear susceptibility is r0 , and d is the radius of the core of the waveguide. The subscripts 11 indicate the contribution which is quadratic in the component .2/ 1 D rrr of the second-order susceptibility tensor

0.2 0.15 C22(0 0) 0.1 0.05 0

0

0.2

0.4

0.6 r0/d

0.8

1

Fig. 2.5 Plot of the coupling coefficient C22 .0j0I r0 / for kd D 24 as a function of r0 =d . The coefficient characterizes the efficiency of conversion, as given by Eqs. (2.63) and (2.65), of the lowest order guided wave with largest wavenumber p0 .k/ at the fundamental frequency ! D kc to the mode with largest wavenumber p0 .2k/ at the second-harmonic frequency 2! D 2kc. The radius of the tubelet of nonlinear susceptibility is r0 , and d is the radius of the core of the waveguide. The subscripts 22 indicate the contribution which is quadratic in the component .2/ 2 D rzz of the second-order susceptibility tensor

the lattice distance and corresponding factor GNj kC for a cylindrical waveguide appearing in Eq. (2.63). The intensity JkM .!/ is defined from the integral of the Poynting vector along the transverse coordinate. In order to compare the two geometries we put IkM .!/ D d 2 S C ;

JkM .!/ D 2d S P ;

(2.68)

36

B.U. Felderhof et al.

0.175 0.15 0.125 0.1 C33(0 0) 0.075 0.05 0.025 0

0

0.2

0.4

0.6

0.8

1

r0/d Fig. 2.6 Plot of the coupling coefficient C33 .0j0I r0 / for kd D 24 as a function of r0 =d . The coefficient characterizes the efficiency of conversion, as given by Eqs. (2.63) and (2.65), of the lowest order guided wave with largest wavenumber p0 .k/ at the fundamental frequency ! D kc to the mode with largest wavenumber p0 .2k/ at the second-harmonic frequency 2! D 2kc. The radius of the tubelet of nonlinear susceptibility is r0 , and d is the radius of the core of the waveguide. The subscripts 33 indicate the contribution which is quadratic in the component .2/ 1 D zzr of the second-order susceptibility tensor

and write the conversion coefficient (2.63) for the cylindrical waveguide in the form MM j kC D

2 2 GNj kC Aj kC .r0 /d 2 S C ; c

(2.69)

where GNj kC is the Bragg factor defined as in Eq. (2.67). The conversion coefficient for the planar waveguide is written similarly as MM j kP D

2 2 GNj kP Aj kP d 2 S P : c

(2.70)

4 X Bj k : kd

(2.71)

By comparison with Eq. (2.66) Aj kP D

We consider kd D 24, as in the experiment of Parameswaran et al. [8], with wavelength of the fundamental D 2=k D 1550 nm and d 6m, and use the same dielectric constants as above. Then we find for the cylindrical waveguide p0 .!/d D 35:837 and p0 .2!/d D 72:388, and for the planar waveguide p0 .!/d D 35:972 and p0 .2!/d D 72:463. The lattice distance a, given by Eq. (2.51), in the two cases takes the value aC D 8:79 d;

aP D 12:12 d:

(2.72)

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

37

5000 4000 C11(0 0) 3000 2000 1000 0 7.5

10

12.5

15

17.5 kd

20

22.5

25

Fig. 2.7 Plot of the coupling coefficient C11 .0j0/ for the circular waveguide as a function of kd (solid curve). For each value of kd , the optimal radius r0 has been chosen. For comparison we also plot the coupling coefficient C11 .0j0/ for the planar waveguide as a function of kd (dashed curve). The notation is explained in the caption to Fig. 2.4

Correspondingly we find for the coupling factors in Eqs. (2.69) and (2.70) for 2 D 3 D 0 A00C .rm / D 4275 j1 j2 =."30 d 6 /;

A00P D 32:47 j1 j2 =."30 d 6 /:

(2.73)

for the value rm D 0:593 d corresponding to the maximum in Fig. 2.4. The prefactors in Eq. (2.73) are the values of the coupling coefficients C11C .0j0/ D 4275 and C11P .0j0/ D 32:47. In Fig. 2.7 we show the coupling coefficient C11C .0j0/ as a function of kd . At each value of kd the optimal radius r0 has been chosen. For comparison we show also the coupling coefficient C11P .0j0/ as a function of kd for the planar waveguide. This shows a decrease with increasing frequency of the fundamental. Clearly the circular waveguide geometry is to be preferred for most frequencies . For large N the Bragg factors G in Eqs. (2.69) and (2.70) vary rapidly with frequency. It makes sense to compare the two geometries at their peak values for second-harmonic generation. Hence we put the factor FN in Eq. (2.50) equal to N 2 in both cases. Then the Bragg factors differ only by the first factor in Eq. (2.48). Taking w D a=2 in both cases we get for the two Bragg factors at the peak value GN 00C D 0:198 N 2 ;

GN 00P D 0:377 N 2 :

(2.74)

The prefactors for the two geometries in the conversion coefficients (2.68) and (2.69) take similar values. The circular geometry may have an advantage over the planar geometry in the efficiency of input of the fundamental wave. In the above numerical example we find for the circular waveguide with susceptibility 1 D 1013 esu the conversion factor in SI units 5 2 M MM 00C D 2:7 10 L I .!/;

(2.75)

38

B.U. Felderhof et al.

Table 2.1 Selected conversion efficiencies (for details, cf. text) SHG-experiment

P .2!/=P .!/ in %

Reference

Surface-SHG simple reflection

1012

KDP-crystal in transmission

1:72 104

Planar waveguide

1 104

G.T. Boyd, Y. R. Shen, T.W. Hänsch Second-harmonic generation from sub-monolayer molecular adsorbates using a CW diode laser Seventh International Conference Laser Spectroscopy VII Maui, HI, USA, 24–28 June 1985 A. Yariv Quantum Electronics Third Edition, Wiley, New York, 1988 Chapter 16.7: Second-Harmonic Generation with Gaussian Beams, pp. 402 A. Bratz, B. U. Felderhof, G. Marowsky Second-harmonic generation in planar waveguides Appl. Phys. B 50, 393–404 (1990) This work

optimized geometry III

Quasi-phase-matched SHG in a fiber under optimized conditions

2.7

where L D Na is the length of material with nonlinear susceptibility 1 . For an 2 input power of the fundamental I M .!/ D 100 mW this becomes MM 00C D 2:7L with L in cm. By definition the conversion factor is less than unity. This implies that for a length 1 cm we must take depletion into account. In Table 2.1 we have summarized some relevant conversion data from reliable literature sources. The table shows that SHG conversion varies by many orders of magnitude, depending on the experiment. The conversion efficiency 1012 % concerns the famous Maui surface experiment of Boyd, Shen, and Hänsch, demonstrating surface SHG of a sub-monolayer of pyridine adsorbed on a silver electrode. The other SHG conversion data concern KDP, an optimized planar waveguide geometry of Bratz et al. [1], and the proposed configuration of Fig. 2.2 in this work. Due to strong spatial confinement and Bragg interference the conversion efficiency is strongly enhanced and pump depletion has to be considered even for device lengths as short as 1 cm. Therefore the device length was taken to be 0.1 cm to avoid depletion and make the data comparable. It should be noted that for the KDP-case SHG was considered with Gaussian beams; hence the efficiency increases only linearly with crystal thickness.

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

39

2.7 Depletion For a sufficiently long stretch of nonlinear susceptibility depletion of the fundamental must be taken into account. We consider a stretch with M periods of nonlinear susceptibility .2/ , where M is a large multiple of N . It is assumed that N is sufficiently small that the preceding theory, with neglect of depletion, may be applied. In the experiment of Parameswaran et al. [8] with a planar waveguide the number of periods is about M D 4000. The period a is assumed to be adjusted to the frequency of the fundamental by use of Eq. (2.51). Due to the Bragg factor, conversion is then limited to the lowest mode with wavenumber p0 .2!/. We assume first that the input laser is tuned to the peak value, so that the Bragg factor is proportional to N 2 , as in Eq. (2.74). On a large length scale the intensity of the fundamental I0M .!I z/ decreases with distance along the waveguide, and the intensity of the second harmonic I0M .2!I z/ increases. For brevity we denote I1 .z/ D I0M .!I z/ and I2 .z/ D I0M .2!I z/. We define corresponding slowly varying wave amplitudes A1 .z/ and A2 .z/ by [3] I1 .z/ D p1 A1 .z/2 I1 .0/;

I2 .z/ D

1 p2 A2 .z/2 I1 .0/; 2

(2.76)

with the abbreviations p1 D p0 .!/;

p2 D p0 .2!/:

(2.77)

The amplitudes A1 .z/ and A2 .z/ are assumed to satisfy the mode-coupling equations dA1 D A1 A2 ; dz p1 dA2 D 2 A21 ; dz p2

(2.78)

where the coefficient can be evaluated from the preceding theory for the behavior at small z. The mode-coupling equations imply the conservation law I1 .z/ C I2 .z/ D I1 .0/:

(2.79)

The equations have the solution s 1 A1 .z/ D p sech z; p1 with

A2 .z/ D

2 tanh z; p2

(2.80)

s D p1

2 ; p2

(2.81)

40

B.U. Felderhof et al.

so that correspondingly I1 .z/ D I1 .0/sech2 z;

I2 .z/ D I1 .0/ tanh2 z:

(2.82)

Comparison with Eq. (2.62) yields 2 D 8

a2 2 i w=a je 1j2 A00 I1 .0/; c

(2.83)

with coupling factor A00 given by Eq. (2.65). The decay length 1= decreases with increasing intensity of the incident laser light. We note the identity

dA1 dz

2 C 2 A21 .p1 A21 1/ D 0:

(2.84)

This shows that the solution may be interpreted as the motion of a particle in a quartic potential at zero energy, or as the interface profile between two phases of a fluid [18]. The identity is equivalent with the conservation law (2.79). If the input laser is not tuned to the peak value we must use complex amplitudes A1 .z/; A2 .z/ and generalize the mode-coupling equations to [3, 19] dA1 D A1 A2 e i p z ; dz p1 dA2 D 2 A21 e i p z ; dz p2

(2.85)

with phase mismatch p D p2 2p1 nK:

(2.86)

With the normalization B1 D

p p1 A1 ;

B2 D

1p p2 A2 2

(2.87)

the mode-coupling equations can be expressed as dB1 D B1 B2 e i p z ; dz 1 dB2 D B12 e i p z ; dz 2

(2.88)

with coefficient p D 2:

(2.89)

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

41

With the complex notation B1 D b1 e i'1 ;

B2 D i b2 e i'2 ;

(2.90)

the mode-coupling equations (2.88) can be cast in the standard form with real variables [3] db1 D b1 b2 sin ; dz 1 db2 D b12 sin ; dz 2

d'1 D b2 cos ; dz 1 b2 d'2 D 1 cos ; dz 2 b2

(2.91)

with phase difference D p z C '2 2'1 :

(2.92)

The mode-coupling equations imply the energy conservation law, which may be expressed as b12 .z/ C 2b22 .z/ D 1:

(2.93)

With a final change of variables p v D b2 2;

u D b1 ;

D z

(2.94)

the equations become du D uv sin ; d dv D u2 sin ; d d d D s C cot ln.u2 v/; d d

s D

p :

(2.95)

These equations have the two conservation laws u2 C v2 D 1;

u2 v cos C

p 2 p 2 v DC v; 2 2 0

(2.96)

where the constant is determined by the initial values at z D 0 according to D u0 v20 cos 0 . In our case D 0, since v0 D 0. The equations can be solved in terms of the elliptic integral D

1 2

Z

v2

q 0

1 x.1 x/2 14 s 2 x 2

dx:

(2.97)

42

B.U. Felderhof et al.

0.6 0.5 0.4 v2 0.3 0.2 0.1 0.0 −20

−10

0

10

20

Δs Fig. 2.8 Plot of the reduced second-harmonic intensity v2 at fixed length L D 1= as a function of the reduced detuning parameter s D p= , where p is the phase mismatch. The notation is explained in Sect. 2.7

Explicitly D

p p F .arcsin.v= /j 2 /;

D 8=.8 C s 2 C

p s 4 C 16s 2 /; (2.98)

where F .'j 2 / is the elliptic integral of the first kind [20]. In particular F .'j1/ D 2 arctanh.tan.'=2// leads to v D tanh in agreement with Eq. (2.82). The expression Eq. (2.98) can be inverted to v./ D

p p sn.= ; /;

(2.99)

p with Jacobian elliptic function sn.= ; /. In Fig. 2.8 we plot the reduced second2 harmonic intensity v for fixed length D 1 as a function of the detuning parameter s. The plot shows a spectral line with sidewings. For fixed detuning parameter s the second-harmonic intensity varies periodically as a function of distance . Note that in the present theory the mode-coupling equations are assumed to hold on a length scale much larger than the period of the grating. This is in contrast to the theory of Zhao et al. [4], who assume mode-coupling equations on the scale of the period. The present formulation allows understanding of the effect of depletion in the framework of the well-known theory developed by Armstrong et al. [3] for second-harmonic generation in anisotropic crystals. Finally we note that it follows from Eq. (2.82) that for optimal phase matching the stretch of nonlinear susceptibility L1=2 over which the second-harmonic intensity I2 is one half of the input fundamental intensity I1 .0/ is given by L1=2 D

0:881 1 1 arctanh p D : 2

(2.100)

2 Optimizing Second Harmonic Generation in a Circular Cylindrical. . .

43

For the numerical example used in Eq. (2.75) we have 2 D 2:7 105 I1 .0/, so that L1=2 D

5:36 1013 cm; p 1 I1 .0/

(2.101)

p with 1 in esu and I1 .0/ in mW. The prefactor follows from 5:36 D 0:881= 0:027. Thus the half-length varies inversely with the second-order susceptibility and the square root of the input fundamental intensity. In Eq. (2.101) it is assumed that the radius of the tubelet r0 has the optimal value shown in Fig. 2.4.

2.8 Discussion We have presented a model calculation of second-harmonic generation in a circular cylindrical waveguide or optical fiber for a situation where the nonlinear material is isotropic and distributed in a radially symmetric manner. Though the geometry is not easy to realize experimentally, the calculation shows the essential features of the mechanism. A comparison with an earlier calculation for a planar waveguide [1] shows that the confinement in cylindrical geometry has distinct advantages. The work of Parameswaran et al. [8] shows that second-harmonic generation in cylindrical geometry can be realized experimentally and is quite effective. The conversion efficiency is sufficiently high that depletion of the fundamental must be taken into account. We have shown that depletion can be described in terms of the mode-coupling formalism developed by Armstrong et al. [3] for secondharmonic generation in anisotropic crystals.

References 1. A. Bratz, B.U. Felderhof, G. Marowsky, Appl. Phys. B 50, 393 (1990) 2. B.U. Felderhof, G. Marowsky, Appl. Phys. B 43, 161 (1987) 3. J.A. Armstrong, N. Bloembergen, J. Ducuing, P. S. Pershan, Phys. Rev. 127, 1918 (1962); reprinted in N. Bloembergen Nonlinear Optics (Addison-Wesley, Redwood City, 1992) 4. L.-M. Zhao, G.-K. Yue, Y.-S. Zhou, EPL 99, 34002 (2012) 5. M.E. Fermann, L. Li, M.C. Farries, L.J. Poyntz-Wright, L. Dong, Optics Lett. 14, 748 (1989) 6. T. Mizunami, T. Tsukuda, Y. Noi, K. Horimoto, Proc. Soc. Photo-Opt. Instrum. Eng. 5350, 115 (2004) 7. T. Mizunami, Y. Sadakane, Y. Tatsumoto, Thin Solid Films 516, 5890 (2008) 8. K.R. Parameswaran, J.R. Kurz, R.V. Roussev, M.M. Fejer, Optics Lett. 27, 43 (2002) 9. D. Marcuse, Theory of Dielectric Optical Waveguides (Academic, New York, 1974) 10. H. Kogelnik, in Integrated Optics, Topics Appllied Physics 7, ed. by T. Tamir (Springer, Berlin, 1979), p. 13 11. H.A. Haus Waves and Fields in Optoelectronics (Prentice Hall, Englewood Cliffs, 1974) 12. B.U. Felderhof, G. Marowsky, Appl. Phys. B 43, 161 (1991). 13. V. Mizrahi, J.E. Sipe, J. Opt. Soc. Am. B 5, 660 (1988)

44

B.U. Felderhof et al.

14. J.M. Chen, J. R. Bower, C. S. Wang, C. H. Lee, Opt. Commun. 9, 132 (1973) 15. C.K. Chen, T.F. Heinz, D. Ricard, Y.R. Shen, Phys. Rev. Lett. 46, 1010 (1981) 16. B. Dick, Chem. Phys. 96, 199 (1985) 17. O. Roders, O. Befort, G. Marowsky, D. Möbius, A. Bratz, Appl. Phys. B 59, 537 (1994) 18. N.G. van Kampen, Phys. Rev. A 135, 362 (1964) 19. H. Paul, Nichtlineare Optik II (Akademie-Verlag, Berlin, 1973) 20. M. Abramowitz, I.A. Stegun, Handbook of Mathematical Functions (Dover, New York, 1970)

Chapter 3

Nanoplasmonic Metal–Insulator–Metal Waveguides Moshik Cohen, Reuven Shavit, and Zeev Zalevsky

3.1 Introduction With the rapidly growing demand for higher data processing rates, silicon-based electronic devices approach fundamental speed and bandwidth limitations, which is an increasingly serious problem that impedes further progress in numerous fields of modern science and technology. These limitations arise from interconnect delays and from increased power dissipation of transistors as their gate lengths approach single-nanometer scale [1–4]. Possible solution for these setbacks may lay in photonics devices, as photons provide considerably superior information bandwidth and improved thermal properties compared with electrons [5, 6]. Although semiconductor-based optical devices were previously introduced [7–10], largescale integration of photonic circuitry has been fundamentally limited by their large, diffraction-limited size and by the poor optical response of silicon at optical frequencies. Recently, it has been suggested that surface plasmon nanophotonics may overcome these limitation [11–14]. Newly introduced plasmonic nanoantennas [12, 15–17], waveguides [18–21], and devices [18, 22–24] unlock an enormous potential for exciting new applications based on SPPs. Predominantly, nanometric

M. Cohen () Faculty of Engineering, Bar-Ilan University, Ramat-Gan 52900, Israel Department of Electrical and Computer Engineering, Ben-Gurion University of the Negev, Beer-Sheva 84105, Israel e-mail: [email protected] R. Shavit Department of Electrical and Computer Engineering, Ben-Gurion University of the Negev, Beer-Sheva 84105, Israel e-mail: [email protected] Z. Zalevsky Faculty of Engineering, Bar-Ilan University, Ramat-Gan 52900, Israel Bar-Ilan Institute for Nanotechnology and Advanced Materials, Ramat-Gan 52900, Israel e-mail: [email protected] G. Marowsky (ed.), Planar Waveguides and other Confined Geometries: Theory, Technology, Production, and Novel Applications, Springer Series in Optical Sciences 189, DOI 10.1007/978-1-4939-1179-0__3, © Springer ScienceCBusiness Media New York 2015

45

46

M. Cohen et al.

all-optical logic devices that use plasmonics as data carriers are of prime importance for future information processing and photonic computing technologies. Still, although plasmonic-based logic devices were recently introduced [10, 25], logic devices which operate directly on SPPs in deep nanoscale have not been reported. In Sect. 3.1, we design, fabricate, and characterize a novel, silicon-based alloptical nanoplasmonic exclusive or (XOR) gate. The device achieves smallest reported dimensions for plasmonic logic gate and therefore achieves significantly low losses and small delay times. The logic operation is obtained by interference of SPPs through ultrathin Ag film with measured lateral dimensions of 4 20 nm, achieving the smallest reported dimensions for all-optical logic gate. Additional logic and Boolean functionalities can be realized by engineering the interferometer dimensions. We propose a special excitation and waveguiding scheme which facilitates the launch of nanometric SPPs from laser illumination and rout them toward the gate. High-resolution (HR) atomic force microscopy (AFM) system with He–Ne laser at wavelength of 633 nm is used to excite and trace the nanoplasmonic waves along the structure and particularly at the device’s area. We theoretically and experimentally show full logic XOR functionality of the reported gate, with device operating at broad frequency range which enables multi-tera-bits per second (Tbit s1 ) data processing rates. In Sect. 3.2 we show that Kelvin probe force microscopy (KPFM) can image and characterize SPPs achieving molecular-scale resolution. Since SPPs are bound to the surface and confined to deep subwavelength scales, high-resolution imaging of nanoplasmonic modes using conventional optical microscopy is nearly impossible [26–29]. Subdiffraction optical imaging of surface plasmons can be achieved using near-field techniques, as scanning near-field optical microscope (SNOM) and its modifications that use metal tips [30–36]. In SNOM, a subwavelength optical aperture samples the average optical signal intensity as a function of position. However, spatial resolution and collection efficiency are both limited by the aperture size and by the distance between a sample and the tip. This is mainly because SNOM samples only the decaying or evanescent part of the optical signal outside the nanoscale object [37]. To date the smallest commercially available SNOM tips achieve aperture diameters of 50–100 nm ([CSL STYLE ERROR: reference with no printed form.]). Plasmonic imaging with nanometric spatial resolution can also be achieved using electron energy loss spectroscopy (EELS) [38–40], with time-resolved measurements that are also demonstrated using laser-excited photocathodes in electric microscopy [41, 42]. KPFM, also known as surface potential microscopy, is a variant of AFM which was first introduced in 1991 [43]. KPFM enables to measure the work function difference between a scanning tip and a surface with submolecular resolution and submilivolt sensitivity [44–49]. When a scanning probe tip is electrically connected to a conductive sample, a contact potential difference (CPD) will arise due to the different work functions of the tip and the sample. KPFM measures local variations in the CPD by applying a voltage between the sample and the tapping AFM tip so that the electric field caused by the CPD and the resulting force on the tip are compensated. For a certain tip position, the compensating voltage represents the local contact potential difference (LCPD) and can be determined either with a feedback loop or by measuring the

3 Nanoplasmonic Metal–Insulator–Metal Waveguides

47

voltage dependence frequency shift [43, 46, 50–52]. Recently, we used KPFM and space–time Fourier analysis to characterize SPP modes with resolution of 10 nm [53, 54]. Here, we show that KPFM can image and characterize surface plasmon polaritons with resolution at the single-nanometer scale. A theoretical model is proposed to define the relation between CPD and SPPs and provide an in-depth understanding of the imaging mechanism. We characterize plasmonic nanoantenna and waveguiding structures achieving resolution of only 2 nm. Additionally, we observe that the sign of the CPD can be used to obtain information on the electric field’s directionality, toward full-vector characterization of SPPs.

3.2 Nanoplasmonic Logic Circuitry Based on Multilayer Gap Waveguides The proposed system is comprised of two metal–insulator–metal (MIM) SPP waveguides connected to the dipole nanoantennas at one end and to the logic device in their other end. Figure 3.1a illustrates the operational concept of the proposed nanoplasmonic system. Each nanoantenna is illuminated by a laser and converts the incident light to propagating SPPs along the corresponding waveguide. The modes are guided to the device, where they undergo all-optical logic operation. The XOR

Fig. 3.1 Nanoplasmonic interferometer-based XOR gate integrated with SPP excitation and waveguiding system. (a) Schematic illustration of the reported nanoplasmonic system. Micronscale optical excitation is converted to nanoscale plasmonic waves by the resonant dipole nanoantennas, confined and guided via plasmonic MIM waveguides toward the plasmonic XOR device, which performs the logic operation. The inset shows a 3D illustration of the nanoplasmonic interferometer which is used to realize XOR logic functionality. s D 20 nm, the thickness of the internal metallic layer is • D 4 nm, and LI D 300 nm represents the overall interferometer length. (b) SEM image of the fabricated nanoplasmonic system

48

M. Cohen et al.

logic device consists of two MIM waveguides separated by a 4 nm (• D 4 nm)-thick metallic layer. The MIM waveguides comprising the nanoplasmonic interferometer are integrated with identical dielectric cores of two independent MIM plasmonic waveguides. In the other perimeter of the system, the waveguides are connected to resonant dipole nanoantennas to achieve efficient excitation of propagating SPPs from laser illumination. To fabricate nanoplasmonic devices, 20 nm Ag layer was sputtered on top of chemically cleaned wafers, via ion sputtering at vacuum levels of less than 9e-7 Torr without cooling. The structures were patterned using gallium focused ion beam (Ga FIB) with 7 nm ion beam spot size. The acceleration voltage was set to 5 KV and currents as low as 0.69 nA were applied. Figure 3.1b shows scanning electron microscopy (SEM) image of the fabricated nanometric interferometer, integrated with the plasmonic system. The silver structures are shown in bright colors, and the gray background represents the SOI substrate. We respectively mark the inputs and outputs of the device as “I1 ”, “I2 ”, and “Out”. The overall area occupied by the nanoplasmonic gate with the excitation system is 1 1 m, which is more than 200 times smaller compared with the system reported in [25]. The average surface roughness measured on the internal faces of the system is 2 nm, obtained by experimental optimization of the lithography process. The theoretical operation principle of the nanoplasmonic interferometer may be explained using the coupled-mode theory [55], which suggests that a structure built out of two identical slab waveguides with a subwavelength separation transfers light between the two waveguides with a constant phase shift of /2. The spatial periodicity of the power transfer between the two MIM waveguides depends on the magnitude of the wave number k D 2 /œSPP , where œSPP is the wavelength of the propagating plasmonic mode within the waveguide. In optical frequencies, the refractive index of metals can be expressed as n D ni C jnj , where the real part ni governs the phase of a signal and the imaginary part nj origins absorption. From the refractive index, we extract the relative permittivity by " D "0 C j"00 "0 D n2i n2j I

"00 D 2ni nj

(3.1)

where "0 and "00 are the real and imaginary part of ", respectively. The thickness of the silver metallic layer is numerically designed to accomplish relative phase shift of between the plasmonic modes, which is required to realize XOR operation [56]. The MIM waveguides comprising the interferometer are integrated with identical dielectric cores of two independent MIM plasmonic waveguides. In the other perimeter of the system, the waveguides are connected to resonant dipole nanoantennas to achieve efficient excitation of propagating SPPs from laser illumination. It was recently observed that excitation of MIM SPP waveguides using dipole nanoantennas achieves coupling efficiencies which are orders of magnitude

3 Nanoplasmonic Metal–Insulator–Metal Waveguides

49

higher compared with direct illumination of bare waveguide [57]. To achieve maximum excitation efficiency, we maximize the intensity of the electric field in the dipole gap and simultaneously minimize the impedance mismatch between the dipole and the waveguide by geometry optimization. These requirements are met by maximization of the net power flowing through the waveguide cross section, which also ensures flow of propagating SPPs toward the device. The net power flow is given by “ W D

n! o n dS Re P !

(3.2)

! where P is the Poynting vector for the propagating SPPs and ! n is a vector in the direction of wave propagation. The dimensions of the nanoantennas are optimized to achieve maximum W in the MIM waveguides. The numerical analysis and optimization of the structures were carried out using finite element method (FEM) commercial SW package HFSS V14 [58]. Figure 3.2a shows the 3D electromagnetic model for analysis and optimization of the system. The model is comprised of Ag plasmonic nanostructures deposited on SOI substrate, with the materials properties obtained from [53, 54]. Each nanoantenna is illuminated by a laser at a wavelength of 1.55 m, linearly polarized in the dipole direction and with parameterized incident angle. Each laser beam is focused to a radius of 1 m, centered at the origin of the corresponding nanoantenna. Selectively dense meshing at a maximum of 1 nm cell size was assigned at the metallic regions to precisely capture the plasmonic logic operation obtained by the device. The model was terminated by PML absorbing boundaries, matched to the material at the boundary of each computational domain. Convergence criterion was set to less than 1 % energy variation between three successive iterations of adaptive mesh refinement. The results are presented at the optical frequency, i.e., 194.55 THz. Figure 3.2c shows the numerically calculated electric field magnitude for XOR(“1”, “1”) D “0” logic operation, in which both nanoantennas are illuminated. The optical laser radiation is efficiently coupled to SPP modes that propagate through MIM waveguides toward the nanoplasmonic XOR device. Zoom in-to the area of the device shows destructive plasmon interference, which results in logic zero (“0”) at the output of the device, as emphasized in the inset. Figure 3.2d illustrates XOR(“1”, “0”) D “1” logic operation, with zoom in-to the area of the device shown in the inset shows the high field value which corresponds to logic “1”. For this case, a portion of the propagating SPPs is reflected from the device’s input and coupled to the other waveguide. The intensity of the undesired reflected field is 20 dB lower compared with that of the plasmon in the excited waveguide, i.e., S12 D 20 dB. Full modulation, i.e., 30 dB extinction ratio at the device’s output, is achieved after less than 300 nm of interference length (LI < 300 nm, as defined in Fig. 3.1a). This indicates a high-speed phase accumulation through tunneling of the plasmonic modes, until relative phase shift of between the waveguides is accomplished. Figure 3.2e, f shows the electric

50

M. Cohen et al.

a

b

c

d

f

e 4.00

3.50

I1

3.00

3.00

I1

2.50

Electric Field [V/m]

Electric Field [V/m]

3.50

Out

2.00 1.50 1.00 0.50

Out

2.50 2.00 1.50 1.00 0.50

0.00 0.00

0.25

0.50

0.75

1.00 D [mm]

1.25

1.50

1.75

2.00

0.00 0.00

0.25

0.50

0.75

1.00

1.25

1.50

1.75

2.00

D [mm]

Fig. 3.2 Theoretical analysis and design of the nanoplasmonic XOR gate and excitation system. (a) 3D EM model for the analysis and optimization of the nanoplasmonic device. (b) 2D description of the model. The graphs in Fig. 3.2e, f are plotted on the dashed line defined here. (c) 3D numerical calculation results of the system performance for XOR(“1”, “1”) D “0”; the device’s region is shown in the inset. (d) 3D numerical calculation results of the system performance for XOR(“1”, “0”) D “1”; the device’s region is shown in the inset. (e) Electric field magnitude along the system, for the case of XOR(“1”, “1”). The field is presented along the dashed line defined in Fig. 3.2b. The fields are plotted for three different phases of the laser excitation as the red, brown, and blue patterns that correspond to the excitation phases of 450, 500, and 550, respectively. (f) Electric field magnitude for XOR(“1”, “0”), plotted along the same geometry and for the same laser excitation phases as in Fig. 3.2e

3 Nanoplasmonic Metal–Insulator–Metal Waveguides

51

Fig. 3.3 Extinction ratio and power transfer analysis. (a) Extinction ratio as a function of the device’s length. (b) Electric fields in the device’s region for XOR(“1”, “1”) for • D 20 nm (upper image) and for • D 5 nm (lower image)

field magnitude at the center of the MIM waveguide and the device for XOR(“1”, “1”) D “0” and XOR(“1”, “1”) D “1”, respectively. The field is plotted along the dashed line defined in Fig. 3.2b, for three different phases of the illuminating lasers. Figure 3.2e shows the destructive interference results in logic “0” for the case of two active lasers. In Fig. 3.2f we observe similar electric field profiles at the input (located at D D 1.6 m) and output (located at D D 1.9 m) of the device, for logic level “1”, which is an essential property for the realization of logic gates. The black graph in Fig. 3.3a shows the extinction ratio versus the interference length, as the blue and red curves are XOR(“1”, “0”) and XOR(“1”, “1”), respectively. It is observed that the extinction ratio has two peaks, at L D 130 nm and L D 280 nm, corresponding to the peaks appearing in XOR(“1”, “0”). Extinction ratio of 35 dB is obtained for L D 280 nm; this high value is achieved due to strong destructive interference in XOR(“1”, “1”) response. The dependence of the power transfer as a function of the separation width was rigorously changing for values of • varying from 3 to 20 nm (• D S). Figure 3.3b shows the fields in the XOR device’s area for • D 20 nm and for • D 5 nm. We observe very low coupling between the waveguides for • D 20 nm, yielding luck in destructive interference. For • D 5 nm the coupling between the waveguides is higher, which results in destructive interference, and XOR(“1”, “1”) D “0” is accomplished. However, the observed “0” logic level achieved for • D 5 nm is significantly higher than the “0” logic level in the optimal design (• D 5 nm). The higher level of “0” results in degradation in the extinction ratio to a maximum of 12 dB, compared with 35 dB obtained in the optimal design. We use the surface electric potential measurement in frequency-modulated scanning Kelvin probe microscopy (FMSKPM) for experimental characterization of the reported nanoplasmonic structures. Surface potential microscopy measures the CPD, between the scanning tip and the characterized device. Generally, CPD is highly material dependent and related to the work functions of pure material and to additional surface dipole moments [59]. The contributions of bulk and surface plasmons to the work functions of materials [60–64] as well as to the van der Waals force [65, 66] were previously

52

M. Cohen et al.

Fig. 3.4 Performance characterization of the nanoplasmonic logic XOR gate, integrated with the excitation and waveguiding system. (a) 2D measurement of XOR(“1”, “1”) D “0” logic functionality. (b) HR SEM image of the fabricated structure for characterization of XOR(“1”, “1”) D “0” logic functionality. (c) 2D measurement of XOR(“0”, “1”) D “1” logic functionality. (d) HR SEM image of the fabricated structure for characterization of XOR(“0”, “1”) D “1” logic functionality

reported. Our AFM system includes He–Ne laser at wavelength of 633 nm which illuminates the entire sample to excite propagating SPPs from the nanoantenna gaps toward the XOR device. Figure 3.4a presents a 2D image of the surface electric potential on the sample for XOR(I1 D “1”, I2 D “1”) D “0” experiment, obtained for the structure shown in Fig. 3.4b. High field values are measured at both I1 and I2 , i.e., “1”. The XOR device realizes destructive interference between the SPPs at I1 and I2 , which results in low field values at the device’s output, i.e., “0”, as shown in Fig. 3.3b. Additional “hot spots” appear on the sample outside the plasmonic system. These “hot spots” represent localized surface plasmons excited by the interaction of the laser light and residual Ag nanoparticles, which remained on the sample after the lithography process. We note that even though the laser

3 Nanoplasmonic Metal–Insulator–Metal Waveguides

53

Fig. 3.5 Measured electric potential along the nanoplasmonic XOR device. (a) The blue line represents the measured field for XOR(I1 D ‘1’, I2 D “0”) D “1”. The black line represents the measured electric potential for XOR(I1 D ‘1’, I2 D ‘1’) D “0”. Dashed points correspond to discrete measured values. The length of the XOR gate is defined by the interference length for which 10 dB extinction ratio is observed, i.e., 150 nm. (b) The line along which the fields are presented for the two experimental setups

illuminates the whole structure, the dominant effect which governs the device operation is caused by propagating SPPs from the nanoantennas. Therefore we neglect effects caused by localized plasmons as well as by direct illumination of the device [67]. The ultrasmall size of the introduced nanoplasmonic structures poses strong limitation on the capability to precisely confine the laser beam to separately excite each nanoantenna. Therefore, we fabricated the identical device integrated with a single nanoantenna and MIM waveguide, as shown in Fig. 3.4d. Figure 3.4c shows the experimental results of XOR(I1 D “0”, I2 D “1”) D “1”, obtained by the characterization of the structure depicted in Fig. 3.4d. We observe low (“0”) field values at I1 and high field values (“1”) at I2 . For this combination of inputs, the device yields high field values at the output “Out”, as emphasized in Fig. 3.4d, resulting it XOR(“0”, “1”) D “1”. The reported nanoplasmonic gate implements Boolean XOR function on the propagating SPPs at inputs “I1 ”and “I2 ”. Hence, signal level of “1” at the device’s output “Out” results if only one of the inputs to the gate is at logic level “1”. Otherwise, logic “0” shall be measured at “Out”.

54

M. Cohen et al. Table 3.1 Experimental results at the output of the plasmonic logic XOR gate I1 0 0 1 1

I2 0 1 0 1

Out D XOR(I1 , I2 ) 0 1 1 0

Logic level of “1” at the inputs I1 and I2 is observed only when the corresponding nanoantenna is illuminated. A 10 dB extinction ratio between the logic levels at the device’s output “Out” is obtained at the device’s length of 150 nm, increasing up to 30 dB for the device’s length of 280 nm

Figure 3.5a shows the measured surface electric potential along the device for XOR(I1 D “1”, I2 D “1”) and XOR(I1 D “0”, I2 D “1”). The fields are presented from the inputs to the gate (L D 0) to the boundary of the physical device (L D 300 nm), as a function of the distance, L. The quanta are presented along a dashed line as described in Fig. 3.4b. We define an electric potential at the output of > 16 [mV] as the “1” or ‘ON’ state and potential < 6 [mV] as “0” or “OFF” state. For the case of XOR(I1 D “1”, I2 D “1”), destructive interference between the plasmonic modes along the device leads to rapid attenuation of the signal which results in “0” logic level at the output, as shown in the black graph of Fig. 3.5a. For the case of XOR(I1 D “0”, I2 D “1”) the field maintains high level through the device, achieving “1” at the output, as shown in the blue graph of Fig. 3.5a. The average surface roughness measured at the internal faces of the waveguides is 2 nm, with measured average periodicity of 10 nm. These values are much smaller than the wavelength of the propagating SPP, thus introducing small additional loss mechanism. These losses have little effect on the XOR performance, as the SPPs are attenuated for both XOR(“1”, “0”) and XOR(“1”, “1”) scenarios, thus having negligible effect on the extinction ratio. The experimental results are summarized in Table 3.1, which is in perfect agreement with the true table of a XOR device. Extinction ratio of 10 dB between the logic levels at the device’s output is accomplished after of only 150 nm, increasing up to 30 dB for the device’s length of 280 nm. The extremely small size of the device is achieved due to the introduced interferometry structure. Tunneling of the SPP modes through the nanometric separation layer leads to rapid phase accumulation, until relative phase shift of between the waveguides is accomplished. This architecture achieves the required phase accumulation much faster and after smaller interference length compared with the linear interference mechanism used in [25], where the phase accumulation is based on propagation length. As a result, the XOR device reported in this paper is more than three orders of magnitude smaller than the one reported in [25]. As micron-scale plasmonic devices [10, 25] suffer from high propagation loss, longer delay times, and huge size mismatch with CMOS electronics, the current concept can be the first nanoplasmonic architectural solution for all of these setbacks.

3 Nanoplasmonic Metal–Insulator–Metal Waveguides

a

55

b

62.50

Potential [dBmV]

50.00 37.50 25.00

13dB

12.50 0.00 -12.50 0.00

100.00

200.00

300.00

400.00

500.00 550.00

-1

Re {kx} [nm ]

Fig. 3.6 Spatial Fourier analysis of the measured surface electric potential on the sample. (a) The red curve shows the spatial FFT performed on the field along the XOR device, defined as “Line 1” in Fig. 3.5b. The blue curve presents spatial FFT analysis of the field outside the XOR device, performed on “Line 2” in Fig. 3.5b. (b) Definition of the lines on which we performed spatial FFT

We provide further experimental evidence for the existence of propagating SPPs along the device by observing the spatial frequency content of the measured fields on the sample. Since the gate exhibits imperfect impedance matching at its boundaries, partial standing waves are excited along the system. These standing waves are characterized by stationary spatial behavior, which is identical to the spatial frequency of the propagating SPPs and therefore can be detected via surface potential measurement in FM KPFM. To examine the spatial frequency content of the fields along the XOR gate, we performed spatial fast Fourier transform (FFT) on the surface electric potential measured along the sample. Figure 3.6a presents the spatial FFT results for two different measurements of the surface electric potential on the sample. The lines on which the FFT was calculated are detailed in Fig. 3.6b. The blue curve shows the spatial FFT of the surface potential along a line, which is outside the device (Line 1 in Fig. 3.6b), as the red curve is the spatial FFT of the surface potential along the center of the device (Line 2 in Fig. 3.6b). For both measurements shown in Fig. 3.6a the dominant field component appears at low spatial frequencies, a result which is in good agreement with the general electrostatic character of the measured potential and is due to the standing waves in the structure. However, we observe a strong spatial frequency component in the field along the device, at Re fkSPP g D 125 m1 . The amplitude of this component is 13 dB higher than the corresponding component in the measurement described by the blue curve. This result confirms the existence of propagating SPPs with wave vector of Re fkSPP g D 125 m1 inside the device, which is in excellent agreement with Dione [19] and Chen [68]. This further substantiates our theoretical analysis and experiments.

56

M. Cohen et al.

3.3 Molecular-Scale Imaging of Modes in Nanoplasmonic Slot Waveguides with Scanning Kelvin Probe Microscopy In this section we introduce for the first time, the imaging of surface plasmon polaritons with KPFM. Although traditionally considered as electrostatic measurement, we show that KPFM can characterize near fields at optical frequencies within single-nanometer scale. The experimental results are supported by 3D numerical calculations as well as analytical model. Figure 3.7 illustrates the process of SPP characterization with scanning KPFM. The origin of nanoplasmonic sensing with KPFM lies in the fact that KPFM measures the CPD between the scanning probe tip and the surface [46, 69]. The CPD is closely related with the charge distribution on the surface as well as with the surface plasmon polaritons [70–76]. When nanometallic structures are illuminated with optical radiation, coherent oscillations of free electrons are excited on the surface. These highly confined optically induced charge density waves preserve the frequency of incident photons and strongly affect the work function in the vicinity of the device. Optically excited variations in the work function of CdSe nanowires [77] and 2D array of subwavelength apertures [78] were recently characterized by electric force microscopy and KPFM. According to the Lorentz model, the motion of electrons in metals is governed by a second-order partial differential equation: 2 @ x @x 2 m C x D eE C (3.3) @t 2 @t

Fig. 3.7 Illustration of nanoplasmonic characterization with KPFM. Dipole nanoantenna is connected to MIM waveguide with nanometric gap width. The device is illuminated by a laser and the excited plasmons change the CPD between the tip and the surface, which is measured by KPFM with molecular-scale resolution

3 Nanoplasmonic Metal–Insulator–Metal Waveguides

57

Here m and e are the electron mass and charge, respectively; x is the electron displacement from the nucleus, D 1/ is the damping rate, is the spring constant, and E is the electric field. Assuming time harmonic behavior for the electric field and displacement, neglecting in the free electron region yields the Drude polarizability: P D Nex D

1 Ne 2 E .x; t/ m ¨2 C i ¨

(3.4)

where ! D 2f is the optical angular frequency of the electric field. The inplane relative permittivity ("k "r C i"i ) can be extracted from (3.4), using " D 1 C P/E.The real and imaginary parts of "k are attributed to intraband and interband transitions, respectively. Extended Drude model which considers the restoration force () is a preferred analytical description at the bound electron region. This model achieves excellent agreement for Au within 500–1,000 nm wavelength range [79]. Further improvement to the extended Drude model can be obtained by adding terms which carefully p describe the critical points (CP) [80, 81]. Near the plasma frequency, ! !p D Ne 2 =m"0, the relative permittivity is very small ("(! p ) ! 0). Hence, E(x, t) becomes a pure depolarization field with quanta of these charge oscillations referred to as plasmons. Using the relation between polarization and charge density Pol D r P, the surface electric potential is calculated by integrating the charge density function over the computational surface: “ V .r/ D

P ol .r/ ds 0 4"0 jr r 0 j

(3.5)

The charge density function may also be obtained by solving the Fock equations using an exchange potential operator [82, 83], a more accurate solution but computationally expensive when obtained numerically. The experimental setup used in this work is depicted in Fig. 3.8a. The sample is illuminated from above by a He–Ne laser at wavelength of 633 nm (! D 2.98 1015 r/s) linearly polarized in parallel with the dipole orientation. Since ¨ 1013 , the in-plane relative permittivity can be written as "k D "B ! 2p /! 2 C i! 3p /! 2 , with "B as the contribution of bound electrons and ! p as the plasma frequency. In our measurements topography and KPFM images are recorded sequentially using the lift mode technique to minimize cross talk between the measurements [84]. To this end, we first acquire the surface topography of a single line in tapping mode and then retrace this topography over the same line at a set lift height from the surface to measure the KPFM signal. To map the work function of the sample, we apply both AC voltage (VAC ) and DC voltage (VDC ) to the AFM tip. VAC generates oscillating electrical forces between the AFM tip and sample surface, and VDC nullifies the oscillating electrical forces that originated from CPD between the tip and sample surface. In our study, the tip–sample distance (H) significantly influences the resolution and sensitivity of the measurements. For small values of H, the KPFM image is dominated by short-range forces ( H6 ) like

58

M. Cohen et al.

Fig. 3.8 Schematic description of our KPFM experimental process and fabricated devices. (a) Schematic of the measurement principle. First the topography is acquired in tapping mode, and then the tip elevates to a set lift height, H, to create the CPD map. (b) Description of the analyzed nanoplasmonic devices. Dipole nanoantenna with arm length “LA” and gap “g” are connected to MIM waveguide of length LW. The thickness and width of all metal strips are 12 nm

van der Waals and capillary interactions. However, for larger values of H, long-range electrostatic and magnetic interactions ( H2 ) govern the results. Therefore, it is critical to optimize the lift height for high-quality imaging. To demonstrate unambiguously that we can measure and image plasmonic waves with molecular resolution, we chose to investigate hybrid devices of dipole nanoantennas integrated with MIM plasmonic waveguides, as shown in Fig. 3.8b. These devices are of prime importance for a large variety of applications and have several advantages for our study. First, the combination of nanoantenna and plasmonic waveguide enables to image both localized SPs and propagating SPPs. Localized SPs are optically excited at the nanoantenna and are coupled to propagating modes along the waveguide. Furthermore, by comparing CPD images with calculated vector fields, we show that KPFM measurements provide information on the directionality of the optical fields. The devices were fabricated by electron beam lithography (EBL), ion beam sputtering (Ag, 10 nm), and lift-off. Figure 3.9a presents a SEM image of the analyzed device, with geometrical dimensions of LW D 750 nm, LA D 100 nm, and g D 12 nm. The image was recorded at beam current of 0.4 nA and low accelerating voltage of 5 kV. Figure 3.9b shows an AFM topography image of the device in 3D, obtained using Si tip with 2 nm diameter. Subsequently, KPFM characterization of the same device was performed in lift mode while the device is illuminated by a He–Ne laser. The KPFM measurements were performed for tip–sample distances ranging from 10 to 250 nm. We observe that for small values of H, short-range interactions strongly affect the KPFM image. For larger tip–sample distances, the results are governed by the long-range interactions. The range of distances for which we obtained the best resolution was between 30 and 50 nm. Figure 3.9c shows the KPFM image recorded for tip–sample distance of H D 35 nm, which exhibits clear nanometric resolution. We observe two dipolar-like modes on the

3 Nanoplasmonic Metal–Insulator–Metal Waveguides

59

Fig. 3.9 SEM, AFM, KPFM, and numerical analysis of MIM nanoplasmonic device. (a) Highresolution SEM image of the fabricated and analyzed device. (b) 3D AFM topography image of the device. The image was recorded with Si super sharp tip with 2 nm aperture. (c) CPD image of the device under optical illumination with He–Ne laser at frequency of 474 THz, recorded with the same tip as (a). KPFM signal scale bar, 1.7–C1.7 V. (d) 3D numerical calculation (FEM) results of the analyzed device under optical illumination of He–Ne laser, similar to the experimental setup used to obtain the results in (c). Scale bar, 50 nm

antenna segments, with strong fields at the antenna ends and at the gap, as expected for a dipole plasmonic nanoantenna in the visible [53, 54]. The localized fields at the nanoantenna gap extend along the MIM waveguide, periodically changing their polarity. The modal behavior of the propagating SPPs along the waveguide is clearly observed in the KPFM image (Fig. 3.9c). Four periods of modes appear along the waveguide, represented by four spots with similar spatial dimensionality. The shapes of the waveguide as well as the field decay into its metallic arms are very well captured. This provides direct experimental evidence of a propagating surface plasmon polariton wave, obtained for the first time for SPPs confined to 12 10 nm mode area. Strong localized fields are observed also on the exterior metal–insulator interfaces of the waveguides, as predicted by the theory of SPPs ([CSL STYLE ERROR: reference with no printed form.]).

60

M. Cohen et al.

We observe that the measured KPFM fields on the ends of the nanoantenna are inversely polarized, with the field on the left edge as positive C1.5 V and the field on the right edge as negative –1.5 V. This important property of the KPFM signal is directly related with the direction of the optical field, as will be further discussed herein. This behavior is reproduced in 3D numerical calculation results, which were obtained using FEM commercial SW package HFSS V15 [53, 54]; see Fig. 3.9d. The calculated vector electric field along the sample is plotted at frequency of 474 THz (wavelength of 633 nm), with the arrows representing the direction of the field. KPFM signal of C1.5 V is measured at the left end of the nanoantenna (see Fig. 3.9c) that corresponds to the optical field direction of b z (see Fig. 3.9d). Consistently, a signal of 1.5 V is measured at the right end of the nanoantenna (see Fig. 3.9c) that corresponds to the optical field direction of Cb z (see Fig. 3.9d). These results contribute valuable information on the polarization of the electrical field, which cannot be obtained with standard SNOM which measures the average field’s magnitude. The high correlation between the calculated electric field and KPFM maps is a direct evidence that KPFM can measure fields at optical frequencies. Now, we show that KPFM can characterize SPPs with 2 nm spatial resolution, by resolving the propagation properties of MIM waveguide with gap (g) difference of 2 nm. Figure 3.10a presents the configuration of the analyzed devices. Figure 3.10b shows the calculated electric field at frequency of 474 THz (œ D 633 nm) for devices with LW D 900 nm, g D 10, 20, 30, and 60 nm. We observe inverse relation between the wavelength of the propagating SPPs, œSPP , and the gap width. As the gap width decreases, the plasmons are confined in both dimensions and vice versa; a confinement which increases the propagation loss. This nonlinear dispersion behavior is evidenced by the difference number of SPP periods that propagate within the waveguide. For g D 10 nm, seven periods of SPP modes are contained inside the waveguide, as for g D 60 nm only four periods are observed (see Fig. 3.10b). The calculated electric field along the center of the waveguide (dashed line in Fig. 3.10a) is shown in Fig. 3.10c, which further demonstrate the change in œSPP as the gap width increases. Figure 3.10d shows the KPFM signal map for g D 30 nm and the tip–sample distance of H D 35 nm, selected for maximum resolution. This image has similar characteristics to Fig. 3.9c with two main differences. First, only three periods of SPPs are contained within the waveguide (compared with four periods in Fig. 3.9c), this is due to the increase in gap width from 12 to 30 nm, a result which is in very good agreement with our calculations (Fig. 3.10b). Second, lower field intensities are observed at the gap and on both nanoantenna ends, mainly caused by impedance mismatch between the dipole and the waveguide and by geometrical shift from resonance. The exact spatial frequency of the propagating SPPs is detected by analyzing the frequency content of the KPFM measurements along the waveguide via spatial FFT. The black graph in Fig. 3.10e presents the results of spatial FFT performed on the KPFM signal inside the waveguide (marked by Line 1 in Fig. 3.10d), with the blue curve corresponding to the spatial FFT performed outside the device (Line 2). Both measurements shown

3 Nanoplasmonic Metal–Insulator–Metal Waveguides

61

Fig. 3.10 (a) Spatial frequency analysis of the nanoplasmonic devices using KPFM, spatial FFT, and numerical calculations. (b) Numerical analysis of the nanoplasmonic devices with g D 10 nm, 20, 30, and 60 nm, under optical illumination. Decrease in the spatial frequency (higher œSPP ) is observed when g is increased. (c) Calculated electric field at 474 THz plotted along the center of the MIM waveguides (dashed line in (a)) corresponding to the 3D results in (b). (d) CPD image of the device under optical illumination with He–Ne laser at frequency of 474 THz, recorded with Si super sharp tip at H D 35 nm. KPFM signal scale bar, 1.2–C1.2 V. (e) Spatial FFT results of the KPFM signal inside the waveguide (black graph, calculated along Line 1 in (d)) and outside the waveguide (Line 2 in (d)). Scale bars, 100 nm in (a) and 50 nm in (d)

in Fig. 3.10e have dominant field component at low frequencies, a result which is in good agreement with the general electrostatic character of KPFM and can be referred to the standing waves in the structure. However, we observe a strong spatial frequency component in the field along the device, œSPP D 248 nm. The amplitude of this component is 15 dB higher than the corresponding component in the measurement described by the blue curve, providing solid evidence for the existence of propagating SPPs inside the waveguide. We used this method to characterize the propagation properties in a series of fabricated nanoplasmonic devices with gap width varying between 10 and 30 nm in steps of only 2 nm (i.e., g D 10, 12, : : : ,30 nm), LA D 100 nm, and LW D 3,000 nm. For each KPFM measurement, we found œSPP by performing spatial FFT and measuring the plasmon wavelength at the peak of the curve (see Fig. 3.10e).

62

M. Cohen et al.

Fig. 3.11 SPP characterization with 2 nm resolution and experimental results for the device with an 8 nm gap width. (a) œSPP as a function of the gap width, g, obtained experimentally (black dots) and theoretically (continuous blue curve). (b) Topography image of the device with g D 8 nm, obtained with our AFM using supersharp Si tip. (c) KPFM image of the device in (b). Scale bars, 100 nm. KPFM signal scale bar, 1.3–C1.3 V

We use long waveguides (LW œSPP ) in order to minimize the standing waves in the device and improve the resolution. Figure 3.11a shows the experimentally obtained dispersion curve (blue graph), with the calculation results presented in the black curve. We observe different experimentally obtained plasmon propagation wavelength (œSPP ) for waveguides with gap difference of 2 nm, which confirm that KPFM can resolve SPPs with 2 nm resolution, currently limited by the aperture dimensions of the scanning probe. The maximum deviation between the calculated and experimental dispersion curves is • D 2.5 nm, less than 1 % from the mean œSPP . Figure 3.11b shows the fabrication result of a similar device with a gap width of g D 8 nm, with the KPFM measurement of this device presented in Fig. 3.11c. We see that for a gap width of 8 nm and smaller the waveguide does not support propagating SPP modes. Instead, the localized SPPs at the antenna gap decay exponentially, similar to a single interface plasmonic waveguide. This can be explained by the very small gap width, which prevents mode hybridation from the two metal–air interfaces of the waveguide. This behavior is attributed also to the metal roughness (1 nm in each face, overall 2 nm) which size is now 25 % of the gap width.

3.4 Summary This chapter provides a deep insight into highly confined MIM plasmonic waveguides, including two sections with novel contributions. In the first section we propose as well as validate theoretically and experimentally for the first time the capability to compress all-optical logic devices into volumes smaller than œ3 /15,500. By employing extremely confined SPPs as information carriers in optical frequencies, the reported nanoplasmonic binary XOR gate exhibits the speed and bandwidth performances of photonics, with dimensions of integrated electronics.

3 Nanoplasmonic Metal–Insulator–Metal Waveguides

63

Extinction ratio of 10 dB is measured at the output for the device’s length of 150 nm, rising up to 30 dB for the device’s length of only 280 nm. The introduced interferometry architecture can be used to realize a variety of plasmonic logic in deep nanoscale. In the second section, we used AFM and KPFM to image MIM nanoplasmonic devices with smallest reported gap dimensions of 8 nm, providing first ever experimental evidence for propagating SPP modes in these dimensions. We have shown that KPFM can achieve SPP imaging resolution of 2 nm and provide 2D images which are in good agreement with theoretical calculations obtained at optical frequencies. Our findings and results advance the scientific frontier and establish MIM geometry and SPPs as future nanoscale technologies for a huge variety of applications: applications ranging from nanoscale optical microscopy and spectroscopy, integrated optical nanocircuitry, optoelectronics engineering to ultrasensitive sensing and quantum nanoplasmonics.

References 1. M.L. Brongersma, V.M. Shalaev, The case for plasmonics. Science 328, 440–441 (2010). doi:10.1126/science.1186905 2. J.A. Dionne, L.A. Sweatlock, M.T. Sheldon et al., Silicon-based plasmonics for on-chip photonics. IEEE J. Sel. Top. Quant. Electron. 16, 295–306 (2010). doi:10.1109/JSTQE.2009.2034983 3. E. Ozbay, Plasmonics: merging photonics and electronics at nanoscale dimensions. Science 311, 189–193 (2006). doi:10.1126/science.1114849 4. J.A. Schuller, E.S. Barnard, W. Cai et al., Plasmonics for extreme light concentration and manipulation. Nat. Mater. 9, 193–204 (2010). doi:10.1038/nmat2630 5. N. Engheta, Circuits with light at nanoscales: optical nanocircuits inspired by metamaterials. Science 317, 1698–1702 (2007). doi:10.1126/science.1133268 6. R. Kirchain, L. Kimerling, A roadmap for nanophotonics. Nat. Photonics 1, 303–305 (2007). doi:10.1038/nphoton.2007.84 7. V.R. Almeida, C.A. Barrios, R.R. Panepucci, M. Lipson, All-optical control of light on a silicon chip. Nature 431, 1081–1084 (2004). doi:10.1038/nature02921 8. L. Bi, J. Hu, P. Jiang et al., On-chip optical isolation in monolithically integrated non-reciprocal optical resonators. Nat. Photonics 5, 758–762 (2011). doi:10.1038/nphoton.2011.270 9. C. Koos, P. Vorreau, T. Vallaitis et al., All-optical high-speed signal processing with silicon–organic hybrid slot waveguides. Nat. Photonics 3, 216–219 (2009). doi:10.1038/nphoton.2009.25 10. H. Wei, Z. Wang, X. Tian et al., Cascaded logic gates in nanophotonic plasmon networks. Nat. Comm. 2, 387 (2011). doi:10.1038/ncomms1388 11. A.G. Curto, G. Volpe, T.H. Taminiau et al., Unidirectional emission of a quantum dot coupled to a nanoantenna. Science 329, 930–933 (2010). doi:10.1126/science.1191922 12. A. Kinkhabwala, Z. Yu, S. Fan et al., Large single-molecule fluorescence enhancements produced by a bowtie nanoantenna. Nat. Photonics 3, 654–657 (2009). doi:10.1038/nphoton.2009.187 13. S. Lal, S. Link, N.J. Halas, Nano-optics from sensing to waveguiding. Nat. Photonics 1, 641–648 (2007). doi:10.1038/nphoton.2007.223 14. M. Schnell, A. García-Etxarri, A.J. Huber et al., Controlling the near-field oscillations of loaded plasmonic nanoantennas. Nat. Photonics 3, 287–291 (2009). doi:10.1038/nphoton.2009.46

64

M. Cohen et al.

15. T. Kosako, Y. Kadoya, H.F. Hofmann, Directional control of light by a nano-optical Yagi–Uda antenna. Nat. Photonics 4, 312–315 (2010). doi:10.1038/nphoton.2010.34 16. T. Pakizeh, M. Käll, Unidirectional ultracompact optical nanoantennas. Nano Lett. 9, 2343–2349 (2009). doi:10.1021/nl900786u 17. T. Shegai, S. Chen, V.D. Miljkovi´c et al., A bimetallic nanoantenna for directional colour routing. Nat. Comm. 2, 481 (2011). doi:10.1038/ncomms1490 18. S.I. Bozhevolnyi, V.S. Volkov, E. Devaux et al., Channel plasmon subwavelength waveguide components including interferometers and ring resonators. Nature 440, 508–511 (2006). doi:10.1038/nature04594 19. J.A. Dionne, L.A. Sweatlock, H.A. Atwater, A. Polman, Plasmon slot waveguides: towards chip-scale propagation with subwavelength-scale localization. Phys. Rev. B 73, 035407 (2006). doi:10.1103/PhysRevB.73.035407 20. J.R. Krenn, Nanoparticle waveguides: watching energy transfer. Nat. Mater. 2, 210–211 (2003). doi:10.1038/nmat865 21. R.F. Oulton, V.J. Sorger, D.A. Genov et al., A hybrid plasmonic waveguide for subwavelength confinement and long-range propagation. Nat. Photonics 2, 496–500 (2008). doi:10.1038/nphoton.2008.131 22. P. Berini, I.D. Leon, Surface plasmon-polariton amplifiers and lasers. Nat. Photonics 6, 16–24 (2012). doi:10.1038/nphoton.2011.285 23. H. Yan, X. Li, B. Chandra et al., Tunable infrared plasmonic devices using graphene/insulator stacks. Nat. Nanotech. 7, 330–334 (2012). doi:10.1038/nnano.2012.59 24. N.I. Zheludev, Photonic–plasmonic devices: a 7-nm light pen makes its mark. Nat. Nanotech. 5, 10–11 (2010). doi:10.1038/nnano.2009.460 25. Y. Fu, X. Hu, C. Lu et al., All-optical logic gates based on nanoscale plasmonic slot waveguides. Nano Lett. 12, 5784–5790 (2012). doi:10.1021/nl303095s 26. E. Abbe, Beiträge zur theorie des mikroskops und der mikroskopischen Wahrnehmung. Arch. ür Mikrosk. Anat. 9, 413–418 (1873). doi:10.1007/BF02956173 27. W. Heisenberg, Über den anschaulichen Inhalt der quantentheoretischen Kinematik und Mechanik. Z. Für Phys. 43, 172–198 (1927). doi:10.1007/BF01397280 28. A. Sommerfeld, Ueber die Fortpflanzung elektrodynamischer Wellen längs eines Drahtes. Ann. Phys. 303, 233–290 (1899). doi:10.1002/andp.18993030202 29. E. Abbe, Beiträge zur Theorie des Mikroskops und der mikroskopischen Wahrnehmung. Arch. Für Mikrosk. Anat. 9, 413–418 (1873). doi:10.1007/BF02956173 30. E. Betzig, A. Lewis, A. Harootunian et al., Near field scanning optical microscopy (NSOM). Biophys. J. 49, 269–279 (1986). doi:10.1016/S0006-3495(86)83640-2 31. J. Chen, M. Badioli, P. Alonso-González et al., Optical nano-imaging of gate-tunable graphene plasmons. Nature 487, 77–81 (2012). doi:10.1038/nature11254 32. R. Esteban, R. Vogelgesang, J. Dorfmüller et al., Direct near-field optical imaging of higher order plasmonic resonances. Nano Lett. 8, 3155–3159 (2008). doi:10.1021/nl801396r 33. Z. Fei, A.S. Rodin, G.O. Andreev et al., Gate-tuning of graphene plasmons revealed by infrared nano-imaging. Nature 487, 82–85 (2012). doi:10.1038/nature11253 34. R. Hillenbrand, T. Taubner, F. Keilmann, Phonon-enhanced light–matter interaction at the nanometre scale. Nature 418, 159–162 (2002). doi:10.1038/nature00899 35. Y. Inouye, S. Kawata, Near-field scanning optical microscope with a metallic probe tip. Opt. Lett. 19, 159–161 (1994). doi:10.1364/OL.19.000159 36. M. Schnell, P. Alonso-González, L. Arzubiaga et al., Nanofocusing of mid-infrared energy with tapered transmission lines. Nat. Photonics 5, 283–287 (2011). doi:10.1038/nphoton.2011.33 37. P.E. Batson, Plasmonic modes revealed. Science 335, 47–48 (2012). doi:10.1126/science.1215588 38. H. Duan, A.I. Fernández-Domínguez, M. Bosman et al., Nanoplasmonics: classical down to the nanometer scale. Nano Lett. 12, 1683–1689 (2012). doi:10.1021/nl3001309 39. V. Iberi, N. Mirsaleh-Kohan, J.P. Camden, understanding plasmonic properties in metallic nanostructures by correlating photonic and electronic excitations. J. Phys. Chem. Lett. 4, 1070–1078 (2013). doi:10.1021/jz302140h

3 Nanoplasmonic Metal–Insulator–Metal Waveguides

65

40. J.A. Scholl, A. García-Etxarri, A.L. Koh, J.A. Dionne, Observation of quantum tunneling between two plasmonic nanoparticles. Nano Lett. 13, 564–569 (2013). doi:10.1021/nl304078v 41. J.S. Kim, T. LaGrange, B.W. Reed et al., Imaging of transient structures using nanosecond in situ TEM. Science 321, 1472–1475 (2008). doi:10.1126/science.1161517 42. A.H. Zewail, Four-dimensional electron microscopy. Science 328, 187–193 (2010). doi:10.1126/science.1166135 43. M. Nonnenmacher, M.P. O’Boyle, H.K. Wickramasinghe, Kelvin probe force microscopy. Appl. Phys. Lett. 58, 2921–2923 (1991). doi:10.1063/1.105227 44. P. Grutter, Scanning probe microscopy: seeing the charge within. Nat. Nanotech. 7, 210–211 (2012). doi:10.1038/nnano.2012.43 45. H. Hoppe, T. Glatzel, M. Niggemann et al., Kelvin Probe force microscopy study on conjugated polymer/fullerene bulk heterojunction organic solar cells. Nano Lett. 5, 269–274 (2005). doi:10.1021/nl048176c 46. H.O. Jacobs, H.F. Knapp, A. Stemmer, Practical aspects of Kelvin probe force microscopy. Rev. Sci. Instr. 70, 1756 (1999). doi:10.1063/1.1149664 47. F. Mohn, L. Gross, N. Moll, G. Meyer, Imaging the charge distribution within a single molecule. Nat. Nanotech. 7, 227–231 (2012). doi:10.1038/nnano.2012.20 48. E.J. Spadafora, R. Demadrille, B. Ratier, B. Grévin, Imaging the carrier photogeneration in nanoscale phase segregated organic heterojunctions by kelvin probe force microscopy. Nano Lett. 10, 3337–3342 (2010). doi:10.1021/nl101001d 49. L. Yan, C. Punckt, I.A. Aksay et al., Local voltage drop in a single functionalized graphene sheet characterized by kelvin probe force microscopy. Nano Lett. 11, 3543–3549 (2011). doi:10.1021/nl201070c 50. S.A. Burke, J.M. LeDue, Y. Miyahara et al., Determination of the local contact potential difference of PTCDA on NaCl: a comparison of techniques. Nanotechnology 20, 264012 (2009). doi:10.1088/0957-4484/20/26/264012 51. L. Nony, A.S. Foster, F. Bocquet, C. Loppacher, Understanding the atomic-scale contrast in Kelvin probe force microscopy. Phys. Rev. Lett. 103, 036802. arXiv:09074015 (2009). doi:10.1103/PhysRevLett.103.036802 52. S. Sadewasser, P. Jelinek, C.-K. Fang et al., New insights on atomic-resolution frequencymodulation kelvin-probe force-microscopy imaging of semiconductors. Phys. Rev. Lett. 103, 266103 (2009). doi:10.1103/PhysRevLett.103.266103 53. M. Cohen, Z. Zalevsky, R. Shavit, Towards integrated nanoplasmonic logic circuitry. Nanoscale 5, 5442–5449 (2013). doi:10.1039/C3NR00830D 54. M. Cohen, Z. Zalevsky, R. Shavit, Towards integrated nanoplasmonic logic circuitry. Nanoscale (2013). doi:10.1039/C3NR00830D 55. A. Yariv, Coupled-mode theory for guided-wave optics. IEEE J. Quant. Electron. 9, 919–933 (1973). doi:10.1109/JQE.1973.1077767 56. O. Limon, Z. Zalevsky, Nanophotonic interferometer realizing all-optical exclusive or gate on a silicon chip. Opt. Eng. 48, 064601–064601 (2009). doi:10.1117/1.3156021 57. A. Andryieuski, R. Malureanu, G. Biagi et al., Compact dipole nanoantenna coupler to plasmonic slot waveguide. Opt. Lett. 37, 1124–1126 (2012). doi:10.1364/OL.37.001124 58. V.G. Kravets, G. Zoriniants, C.P. Burrows et al., Composite Au nanostructures for fluorescence studies in visible light. Nano Lett. 10, 874–879 (2010). doi:10.1021/nl903498h 59. M. Nonnenmacher, M. O’Boyle, H.K. Wickramasinghe, Surface investigations with a Kelvin probe force microscope. Ultramicroscopy 42–44(Part 1), 268–273 (1992). doi:10.1016/03043991(92)90278-R 60. I. Brodie, Uncertainty, topography, and work function. Phys. Rev. B 51, 13660–13668 (1995). doi:10.1103/PhysRevB.51.13660 61. F.J. García de Abajo, The role of surface plasmons in ion-induced kinetic electron emission. Nucl. Instr. Meth. Phys. Res. Sect. B Beam Interact. Mater. Atoms 98, 445–449 (1995). doi:10.1016/0168-583X(95)00164-6 62. F.A. Gutierrez, J. Díaz-Valdés, H. Jouin, Bulk-plasmon contribution to the work function of metals. J. Phys. Condens. Matter 19, 326221 (2007). doi:10.1088/0953-8984/19/32/326221

66

M. Cohen et al.

63. R. Mehrotra, J. Mahanty, Free electron contribution to the workfunction of metals. J. Phys. C Solid State Phys. 11, 2061–2064 (1978). doi:10.1088/0022-3719/11/10/016 64. M. Schmeits, A. Lucas, Physical adsorption and surface plasmons. Surf. Sci. 64, 176–196 (1977). doi:10.1016/0039-6028(77)90265-5 65. E. Gerlach, Equivalence of van der Waals forces between Solids and the surface-plasmon interaction. Phys. Rev. B 4, 393–396 (1971). doi:10.1103/PhysRevB.4.393 66. N.R. Hill, M. Haller, V. Celli, Van der Waals forces and molecular diffraction from metal surfaces, with application to Ag(111). Chem. Phys. 73, 363–375 (1982). doi:10.1016/03010104(82)85175-6 67. J. Wen, S. Romanov, U. Peschel, Excitation of plasmonic gap waveguides by nanoantennas. Opt. Express 17, 5925–5932 (2009). doi:10.1364/OE.17.005925 68. J. Chen, G.A. Smolyakov, S.R. Brueck, K.J. Malloy, Surface plasmon modes of finite, planar, metal-insulator-metal plasmonic waveguides. Opt. Express 16, 14902–14909 (2008). doi:10.1364/OE.16.014902 69. W. Melitz, J. Shen, A.C. Kummel, S. Lee, Kelvin probe force microscopy and its application. Surf. Sci. Rep. 66, 1–27 (2011). doi:10.1016/j.surfrep.2010.10.001 70. C. Barth, C.R. Henry, Surface double layer on (001) surfaces of alkali halide crystals: a scanning force microscopy study. Phys. Rev. Lett. 98, 136804 (2007). doi:10.1103/PhysRevLett.98.136804 71. A.J. Bennett, Influence of the electron charge distribution on surface-plasmon dispersion. Phys. Rev. B 1, 203–207 (1970). doi:10.1103/PhysRevB.1.203 72. W. Ekardt, Work function of small metal particles: self-consistent spherical jellium-background model. Phys. Rev. B 29, 1558–1564 (1984). doi:10.1103/PhysRevB.29.1558 73. L. Gross, F. Mohn, P. Liljeroth et al., Measuring the charge state of an adatom with noncontact atomic force microscopy. Science 324, 1428–1431 (2009). doi:10.1126/science.1172273 74. T. König, G.H. Simon, H.-P. Rust et al., Measuring the charge state of point defects on MgO/Ag(001). J. Am. Chem. Soc. 131, 17544–17545 (2009). doi:10.1021/ja908049n 75. T. Leoni, O. Guillermet, H. Walch et al., Controlling the charge state of a single redox molecular switch. Phys. Rev. Lett. 106, 216103 (2011). doi:10.1103/PhysRevLett.106.216103 76. C. Sommerhalter, T.W. Matthes, T. Glatzel et al., High-sensitivity quantitative Kelvin probe microscopy by noncontact ultra-high-vacuum atomic force microscopy. Appl. Phys. Lett. 75, 286–288 (1999). doi:10.1063/1.124357 77. S. Schäfer, Z. Wang, R. Zierold et al., Laser-induced charge separation in CdSe nanowires. Nano Lett. 11, 2672–2677 (2011). doi:10.1021/nl200770h 78. J.A. Hutchison, A. Liscio, T. Schwartz et al., Tuning the work-function via strong coupling. Adv. Mater. 25, 2481–2485 (2013). doi:10.1002/adma.201203682 79. A. Vial, A.-S. Grimault, D. Macías et al., Improved analytical fit of gold dispersion: application to the modeling of extinction spectra with a finite-difference time-domain method. Phys. Rev. B 71, 085416 (2005). doi:10.1103/PhysRevB.71.085416 80. P.G. Etchegoin, E.C. Le Ru, M. Meyer, An analytic model for the optical properties of gold. J. Chem. Phys. 125, 164705 (2006). doi:10.1063/1.2360270 81. A. Vial, T. Laroche, Description of dispersion properties of metals by means of the critical points model and application to the study of resonant structures using the FDTD method. J. Phys. Appl. Phys. 40, 7152 (2007). doi:10.1088/0022-3727/40/22/043 82. J. Bardeen, Theory of the work function. II. The surface double layer. Phys. Rev. 49, 653–663 (1936). doi:10.1103/PhysRev.49.653 83. J.C. Slater, H.M. Krutter, The Thomas-Fermi method for metals. Phys. Rev. 47, 559–568 (1935). doi:10.1103/PhysRev.47.559 84. H.O. Jacobs, H.F. Knapp, S. Müller, A. Stemmer, Surface potential mapping: a qualitative material contrast in SPM. Ultramicroscopy 69, 39–49 (1997). doi:10.1016/S03043991(97)00027-2

Chapter 4

Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber Cladding Jason R. Grenier, Moez Haque, Luís A. Fernandes, Kenneth K.C. Lee, and Peter R. Herman

4.1 Introduction Over the past forty years, single-mode optical fibers have been used to guide encoded light signals over long distances at fast speeds, high modulation rates (100 GB/s to TB/s), and exceptionally low transmission loss (0.2 dB/km). Today, there is more than 1.8 billion kilometers [1] of fiber deployed around the globe, much of which forms the backbone of today’s Internet. Optical fibers also appear in many other useful forms that include large-core multimode, multicore, coreless, and photonic crystal fibers, finding broad application from the doped fibers that underpin high-power fiber lasers to the facile biomedical tools [2] used for in vivo diagnostic, endoscopic, and surgical procedures. A major challenge in optical fiber technology is creating optical, interconnecting, microfluidic, and sensing devices that can penetrate through the thick cladding layer and reach into the core waveguide. One traditional approach has been to pull on bundled fibers as they are heated and tapered to make fused-fiber directional couplers [3]. A less invasive procedure was discovered by Hill and coworkers in 1978 that imprinted Bragg-grating structures directly within the core waveguide under UV laser exposure [4]. Such in-core fiber Bragg gratings (FBGs) manipulate the spectral response of the waveguide to serve as, for example, wavelength division multiplexing (WDM) filters or dispersion compensators in telecommunication networks, mirrors in fiber lasers, and static or dynamic sensing elements for strain, temperature, and refractive index detection in other applications [5, 6]. However, these and other related methods are directed mainly at the core waveguide at the center of the fiber, where light guiding is typically confined to less than 1% of the total cross-sectional fiber area for the case of single-mode

J.R. Grenier () • M. Haque • L.A. Fernandes • K.K.C. Lee • P.R. Herman Department of Electrical and Computer Engineering, University of Toronto, Institute for Optical Sciences, 10 Kings College Rd., Toronto, Ontario, M5S 3G4, Canada e-mail: [email protected]; [email protected] G. Marowsky (ed.), Planar Waveguides and other Confined Geometries: Theory, Technology, Production, and Novel Applications, Springer Series in Optical Sciences 189, DOI 10.1007/978-1-4939-1179-0__4, © Springer ScienceCBusiness Media New York 2015

67

68

J.R Grenier et al.

a

b

SMF Core

ide

FBG

u eg

v

fs

wa

Fig. 4.1 Femtosecond laser writing of a (a) directional coupler in bulk glass and (b) Bragg grating in a fiber core waveguide

optical fibers. There exists a large and relatively unexplored volume in which to consider cladding devices that promise to add significantly more functionality and improve the value of the optical fiber. Several advances are emerging in the direction of fiber cladding devices, including the surface functionalization of cladding surfaces for label-free chemical, biological, and acoustic sensing [7, 8], acid thinning of fibers for evanescent [9] and interferometric sensing [10, 11], laser writing of long period waveguide gratings to couple and sense from fiber cladding modes [12], and laser drilling of microholes to the core waveguide for sensing [13, 14]. An alternate direction for increasing the performance of optical fiber is the formation of multicore waveguides within a single fiber. Such fibers recently enabled a record 1.05 Petabits/s communication rate [15] while the writing of FBGs into the individual waveguide cores served to define a novel temperature-independent two-axis bend sensor [16]. Here, the core waveguides are independent and isolated from each other and pose significant packaging challenges for efficient light coupling at the fiber facets. To further expand the opportunity for fiber cladding photonic and sensing devices, a threedimensional (3D) internal fabrication technology that can form optical devices and interconnections around and between the waveguides and also embed microfluidic and other microelectromechanical system (MEMS) structures to interact with the guided light is highly desirable. A major opportunity for creating higher-performance fiber cladding devices comes from the rapidly expanding field of ultrashort pulsed laser processing of transparent materials. Such lasers have opened a new realm of opportunities for 3D writing of compact micro-optical systems directly inside the bulk of transparent materials [17, 18] as depicted in Fig. 4.1a. Here, nonlinear optical absorption precisely confines laser interactions within a small focal volume where optical breakdown, multiphoton and/or tunnel ionization, electron avalanche, nonequilibrium heating, dense plasma formation, and micro-explosion evolve on record short-time and small-size scales [19–22]. This highly nonlinear physics regime briefly generates extreme temperatures that, under the right condition,

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

69

can mitigate significant shock- or thermally induced collateral damage [23]. Hence, this physics can be favorably manipulated to fabricate 3D optical devices such as: buried optical waveguides [24], volume gratings [25], Bragg-grating waveguides (BGWs) [26], directional couplers [27, 28], waveguide lasers [29], mode converters [30], and second-harmonic waveguide sources [31] in bulk glasses. One unusual aspect of femtosecond laser interactions in fused silica is the formation of nanogratings [32] that underlie significant new opportunities for creating birefringent optical waveguides [33], polarization-selective diffractive optical elements [34], and buried optical waveplates [35]. The nanogratings further open the way for preferential etching [36–39] to enable 3D fabrication of buried microfluidics with submicron resolution by the method known as femtosecond laser irradiation with chemical etching (FLICE). An etching contrast ratio of up to 280:1 between laser-processed and unmodified volumes in fused silica was demonstrated with a range of 2.5–20 % hydrofluoric acid (HF) solutions [38, 40–42]. The 3D FLICE technique enables unprecedented flexibility in fabricating 3D lab-on-chips (LOCs) in fused silica with optically smooth 10 nm (rms) surface roughness [43] and compares well with the 0.8 nm (rms) surface roughness found without nanograting formation in Foturan® photosensitive glass after post-baking and post-annealing steps [44]. FLICE therefore provides a major opportunity to continue reducing biological and chemical laboratory processes from bulky freespace systems toward dense packaging beyond the current planar LOC geometries as reviewed by Whitesides [45] and new 3D design approaches for highly advanced and packaged optofluidic microsystems as reviewed by Osellame et al. [46] and Xu et al. [47]. The pure fused silica cladding found in most types of standard, multicore, and photonic crystal fiber presents an ideal material platform on which to bring microfluidic and structural components into even more compact size scales. By wrapping microfluidic and optical components around the guiding core waveguide of existing fiber-optic technology, one envisions a new concept for lab-in-fiber (LIF) devices. The fused silica cladding is highly favorable for biocompatibility and resistance to chemical erosion and therefore presents a promising LIF platform. LIF offers superior packaging advantages over LOCs by (1) harnessing the mechanical flexibility and robustness of optical fiber, (2) naturally facilitating intimate optical interrogation of microfluidic and micro-reactor components, and (3) providing a convenient platform for interconnecting with light sources, diagnostics, and fiber interreactors. Lab-in-fiber concepts are only recently emerging for creating multifunctional sensing and actuating devices to probe micro- and nanoscale volumes in optical fiber. Bennion and coworkers [48–51] were first to apply FLICE in glass fiber, taking advantage of the 3D direct laser writing to template and then open up cladding microfluidic networks. Although the rough FLICE surfaces led to significant optical insertion loss, much smoother channel walls of 10 nm (rms) roughness were recently demonstrated in bulk glass [43]. Hence, the 3D direct laser writing and FLICE

70

J.R Grenier et al.

techniques are examined here toward new prospects for creating LIF and smart catheter devices that can efficiently exchange information and combine sensing data for broad opportunity in telecom and local area networks, security and defense systems, medical diagnostic and surgical procedures, and low-cost health-care products. This chapter examines the emerging domain of laser microstructuring and inscribing of optical fibers to embed and integrate highly functional optical, microfluidic, and microelectromechanical devices that interconnect efficiently with the fiber core. In background research, one can find numerous examples of laser processing into the core of optical fiber, such as the writing of FBGs by UV lasers [4] or femtosecond lasers with phase mask [52] or point-by-point [53, 54] methods (Fig. 4.1b). However, the direct laser writing into the fiber cladding has remained elusive due to strong beam distortion caused by the spherical and astigmatic optical aberration at the small fiber diameter, typically 125 m for telecommunication fiber. The approach adopted here for undistorted 3D processing inside optical fiber was met with a 1.25 numerical aperture (NA) oil-immersion lens [55], the topic of Sect. 4.2. This distortion-free writing enabled the formation of numerous fiber cladding devices on which we have sought to improve the functionality of optical fibers. This technique promises to overcome many of the challenges and high costs otherwise seen in connecting and packaging optical fiber with discrete bulk devices. The first devices presented here are aimed at the challenge of coupling light out of the core waveguide of a single-mode fiber (SMF) into laser-written cladding waveguides. Section 4.3 presents the spectral coupling characteristics of laserwritten X-couplers, S-bend couplers, and directional couplers. Coreless optical fiber is further introduced as an alternative platform for harnessing symmetric coupling between laser-written core and cladding waveguides. The polarization properties of the couplers are further examined and directions defined for designing polarization-selective optical taps and polarization beam splitters that exploit a laserinduced waveguide birefringence. Section 4.4 begins with the optical properties of the laser-written waveguides and introduces the following examples of photonic cladding devices: BGW filters comparing formation in the fiber core waveguide and the cladding, an in-fiber Mach-Zehnder interferometer (MZI), and a distributed position-shape-temperature sensor. Section 4.5 shows how laser-written stressing tracks can induce waveguide birefringence into the fiber core and enable submillimeter in-fiber wave retarders. Lastly, the concept of 3D writing of microfluidic networks, reservoirs, and micro-optical resonators with optically smooth sidewall roughness into single-mode and coreless fibers is presented in Sect. 4.6. The facile integration of the open structures with laser-formed waveguides culminates with the demonstration of an in-fiber optofluidic Fabry-Perot refractive index sensor. This chapter therefore describes a new laser processing technology and the outlook for creating 3D optical and optofluidic microsystems inside a compact and flexible optical fiber platform that promise highly functional LIF devices for complex laboratory-level diagnostics.

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

71

4.2 Laser Structuring of Optical Fibers The underlying methodologies for writing optical circuits inside optical fibers are described in this section for the specific case of Corning SMF-28® fiber, selected because of its widespread deployment as the backbone of optical communication networks, as well as its low cost and small optical loss. However, one fundamental challenge with writing optical circuits in SMF is the lower coupling efficiency ( 5 m gap from the glass surface. Further, the orientation of the laser polarization was a useful control parameter on multiple purposes to orient the nanograting alignment preferentially. For example, one could reduce both the waveguide loss and the waveguide birefringence when the laser polarization was parallel and the nanogratings were perpendicular to the waveguide axis. Alternatively, dramatically faster chemical etching rates were found [38] when the laser polarization was perpendicular to the modification track, facilitating rapid acid flow along nanogratings aligned parallel with the track. The concept of using an AOM to create laser burst trains of femtosecond pulses that form segmented waveguides in bulk fused silica glass was previously reported in [18, 26]. Here, the waveguide consists of an array of partially overlapping refractive index voxels that offer a strong first-order Bragg resonance at wavelength

B D 2neff ƒ, where neff is the effective index (1.445) of the waveguide mode and ƒ is the grating period. In the telecommunication band, a Bragg wavelength of B D 1550 nm follows from a grating period of 536 nm, controlled by the ratio of the scan speed (0.268 mm/s) to the AOM modulation frequency (500 Hz). The grating period can be arbitrarily varied on each voxel by the DAQ card (Fig. 4.2) to introduce phase shifts and apodization for the flexible tailoring of BGW spectrum [58, 59]. BGWs were formed in the fused silica cladding of SMF and in the coreless fiber with oil-immersion focusing (Fig. 4.2 inset) under various exposure conditions such as 130 nJ pulse energy, 0.268 mm/s scan speed, and 60 % duty cycle at 500 kHz repetition rate or 71 nJ pulse energy, 0.1 mm/s scan speed, and 60 % duty cycle at 1 MHz repetition rate. Bragg gratings were also written into the preexisting core waveguide of SMF [55, 60] at lower exposures in the range of 10 nJ to 120 nJ, 0.268 mm/s scan speed, and 500 kHz repetition rate. A lower exposure here is the result of the stronger ultrafast laser interaction in the Ge-doped core waveguide volume. A practical objective in writing optical circuits in coreless fiber is facilitating an efficient optical connection with standard fibers or optical systems. A simple assembly and packing approach that we examined here is the fusion splicing of the waveguide-embedded coreless fiber to SMF. In one approach, fusion splicing was completed after the laser writing step. However, the high temperature generated during the arc discharge erased a long 374 m segment of the waveguide in the

74

J.R Grenier et al.

Fig. 4.4 Optical micrographs of coreless optical fiber (left) with a core waveguide inscribed by a femtosecond laser (a) before and (b) after fusion splicing to an SMF (right). The fusion splice is seen to have erased a 374 µm segment of the laser-formed waveguide in (a), leading to a large insertion loss (10 dB) in contrast with low loss (1 dB) in the case of (b)

coreless fiber as shown in Fig. 4.4a, leading to an 10 dB insertion loss with SMF. Alternatively, a much improved insertion loss of 1 dB was found when the coreless fiber was first fusion spliced to SMF and followed with waveguide writing in the coreless fiber to meet the SMF core waveguide as shown in Fig. 4.4b. Hence, this latter approach is more preferable while also offering the advantage of real-time monitoring as optical circuits form and connect with the SMF. The transmission and reflection spectra of the laser-formed waveguides and embedded devices were recorded by probing the device under test via end-coupled SMF or free-space lens launching of various infrared light sources (Thorlabs: ASE-FL7002, 1520 nm to 1610 nm; Agilent: 83437A, 1200 nm to 1700 nm; Photonetics: Tunics-BT, 1520 nm to 1600 nm; and AFC BBS1310, 1275 nm to 1345 nm). Reflection spectra were recorded with an optical fiber circulator. Index-matching oil was applied at all glass-fiber interfaces to reduce the Fresnel reflections and FabryPerot effects. All spectra were normalized relative to a direct fiber-to-fiber transmission and recorded with an optical spectrum analyzer (OSA: Ando AQ6317B, with 0.01 nm resolution) or a spectrometer (Ibsen Photonics: I-MON 512E) suited for real-time measurement during the laser writing. The polarization properties of the laser-formed devices were probed by free-space launching of infrared light through a broadband polarizer (Thorlabs: LPNIR) and a 10 (0.16 NA) lens to excite either horizontally or vertically linearly polarized eigenmodes defined as having electric fields aligned parallel or perpendicular to the sample surface, respectively. The intensity profiles of the propagating modes were captured by imaging the end fiber facet onto a phosphor-coated CCD camera (Spiricon: SP-1550M) with a 60 (0.65 NA) lens.

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

75

The laser writing and device characterization methods described in this section are now applied to build the photonic and optofluidic cladding components described in the following sections.

4.3 Optical Couplers for Fiber Cladding Photonics This section addresses the major challenge of coupling light into and out of the light-guiding structures that are to be written in the cladding of optical fibers. Three approaches of coupling light from an SMF core waveguide into femtosecond laserformed waveguides are investigated by using X-couplers, S-bend couplers, and directional couplers as depicted in Fig. 4.5a, b, c. In each case, the coupling waveguide was formed to intersect with (X, S-bend) or run parallel near (directional) the centered core waveguide and then curved at 30 mm bend radius to meet tangentially with a straight spur cladding waveguide that is parallel to the core waveguide. A 15 mm long BGW was formed along the spur to create a back reflection for probing of the coupler efficiency and also for determining the polarization axis and birefringence of the waveguide. In this way, polarization-selective taps in SMF and polarization beam splitters in coreless fiber were designed and fabricated.

4.3.1 X-Couplers in Single-Mode Fiber X-couplers, also known as cross couplers, are formed by two waveguides that intersect at a given crossing angle (). X-couplers are widely found in commercial planar lightwave circuits made by lithographic patterning. Direct laser writing of

Fig. 4.5 Femtosecond (fs) laser writing of waveguides by focusing through index-matching oil to form an (a) X-coupler, (b) S-bend coupler, and (c) directional coupler in an SMF [64]

76

J.R Grenier et al.

1.0 SMF core

Transmission

0.8 0.6 q =20⬚ 8.3 µm

Core

0.4

fs waveguide 0.2 fs waveguide 0.0

0

10

20

30

40

50

70

90

Angle(⬚) Fig. 4.6 Normalized optical transmission in the through-port (SMF core waveguide; blue squares) and cross-port (fs waveguide; green triangles) as a function of the crossing angle for a X-coupler. The fitted (dashed) lines follow the analytical model of DRurr and Renner [63]. Inset, optical micrograph of a femtosecond laser-formed waveguide crossing an SMF core waveguide at 20ı crossing angle [64]

X-couplers has also been studied to explore more flexible writing options. For example, broadband X-couplers with up to 95 % tapping efficiency and 1 dB loss have been demonstrated in silica-on-silicon with UV direct writing [61] while 50% coupling has been shown in bulk soda lime glass (Corning 0215) with femtosecond laser writing [62]. Such couplers have the advantage of coupling light in short interaction lengths of tens of microns, which is attractive in the limited space of optical fibers. A major challenge of forming X-couplers in SMF is the accurate alignment required to position the crossing waveguide to intercept the center of the core waveguide. As an example, the inset image in Fig. 4.6 shows a femtosecond laserformed waveguide crossing an SMF core waveguide at a 20ı crossing angle, where a statistical alignment error of ˙1 m was estimated. Real-time recording of the optical transmission at 1550 nm wavelength during writing of the X-coupler provided the through-port transmission of the SMF core waveguide (blue squares) as plotted in Fig. 4.6 for 0ı to 90ı coupling angles. A minimum transmission value of 2.9 % is shown at a crossing angle of 2:2ı . Both core and spur waveguides were more fully assessed for X-couplers in the high coupling region with crossing angles of 1:3ı to 3:1ı , bend radius of 30 mm, and offset distance of 45 m from the fiber core. After accounting for a loss of 3.2 dB, attributed to the curved waveguide and straight BGW sections, the optical transmission inferred to couple into the crossport (green triangles) was also plotted in Fig. 4.6 and found to yield a maximum 76 % for a crossing angle of 1:9ı . With 6 % power remaining in the core waveguide,

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

77

1.0

Transmission

fs waveguide 0.8

8.3 µm Core

0.6

SMF Core

0.4 0.2 0.0

fs waveguide 30

40

50

60

70

80

90

100

Bend Radius (mm) Fig. 4.7 Normalized optical transmission in the through-port SMF core waveguide (blue squares) and fs laser cross-port waveguide (green triangles) as a function of the bend radius for an S-bend coupler. Inset, optical micrograph (compressed by a factor of 4 in the horizontal direction) of a femtosecond laser-formed waveguide curving out of the SMF core with a 30 mm bend radius [64]

the X-coupler yielded an 18 % loss that was attributed to optical scattering at the crossing point of the waveguides. Vertical and horizontal linearly polarized spectra (1250 nm to 1650 nm) were recorded for several X-couplers and revealed less than 10 % variation in the coupling ratio over a 400 nm band and with no appreciable polarization dependence.

4.3.2 S-Bend Couplers in Single-Mode Fiber In an alternative approach to couple light out of an SMF core waveguide, a femtosecond laser-formed waveguide was inscribed by starting in the core and curving outwards to a distance of 45 m into the cladding following along two reversing circular arcs that terminated into a straight 15 mm long BGW segment as shown in Fig. 4.5b. The inset in Fig. 4.7 shows an optical micrograph (compressed by a factor of 4 in the horizontal direction) of a femtosecond laser-formed waveguide curving out of the SMF core with a 30 mm bend radius. To vary the degree of light coupling, the bend radius of the arcs was varied from 30 mm to 100 mm, yielding the normalized power splitting shown in Fig. 4.7 for the through-port SMF core waveguide (blue squares) and femtosecond waveguide crossing waveguide port (green triangles). The propagation loss incurred in the curved waveguide and straight BGW sections was removed here, thus revealing a maximum coupling of 33% for a bend radius of 30 mm. This value falls monotonically with longer bend radius to < 2 % coupling at 100 mm bend radius. In this data range, the observed

78

J.R Grenier et al.

1.00 0.98

IL = 5%

Transmission

0.96

Beat length = 13.5 mm

0.94 0.92 0.90 0.88 0.86 0

5

10

15

20

Length (mm) Fig. 4.8 Real-time recording of the normalized optical transmission of 1550 nm light through an SMF core waveguide (blue line) as a femtosecond laser formed a parallel waveguide 10 m away from the core to form an asymmetric directional coupler [64]

net loss of 20–33 % was attributed to optical scattering at the intersection point of the waveguides. As in the case of the X-couplers, the S-bend couplers showed less than 10% variation in the coupling ratio over a 400 nm band (1250 nm to 1650 nm) and with no appreciable polarization dependence.

4.3.3 Direction Couplers in Single-Mode Fiber Directional couplers transfer optical power via evanescent fields between two or more waveguides positioned in close proximity to each other and are widely used in planar lightwave circuits. Directional couplers are readily fabricated by fusing two twisted glass fibers but require femtosecond lasers to write 22 [28, 65], 3 3 [66] symmetric, and broadband asymmetric [67] directional couplers in bulk glass. Directional couplers have the advantage of complete energy transfer over coupler lengths predicted by rigorous coupled mode theory [68, 69]; however, they are highly wavelength and polarization-dependent. Asymmetric directional couplers in SMF are presented here by femtosecond laser writing of waveguides parallel with and offset by 10 m to 12 m from the core waveguide and formed by exposure of 130 nJ pulse energy and 0.268 mm/s scan speed. Figure 4.8 shows the normalized optical transmission measured at 1550 nm in the SMF core waveguide (blue line) as a function of the coupler length, recorded

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

79

in real time over length increasing from 0 to 20.5 mm. The beating of two harmonic functions seen here consists of a fast oscillating component of the usual evanescent coupling and a slower component owing to waveguide birefringence that induces polarization-dependent coupling ratios of rH and rV . The coupling ratio could be well represented for the asymmetric directional coupler by the expression 2 . /sin2 rH;V . / D H;V

H;V . / L ; H;V . /

(4.1)

where the subscripts, H and V, represent the horizontal and vertical linearly polarized eigenmodes, respectively, is the coupling coefficient, L is the coupling length, and . / is the amplitude dephasing term, given by v u H;V . / D u t

1C

1 ˇH;V . / 2 H;V . /

2 :

(4.2)

. /

as For the present case of asymmetric couplers, it is convenient to define H;V H;V . / the effective coupling coefficient. The transmission through the core waveguide in the first complete beat cycle between 6.94 mm and 20.4 mm length in Fig. 4.8 could be well represented by the equation T.L/ D 1

rH C rV 2

;

(4.3)

yielding effective coupling coefficients of 1.53 rad/mm and 1.30 rad/mm for the vertical and horizontal polarization eigenmodes, respectively. The difference in these values produced a beat length of 13.5 mm as labeled in Fig. 4.8 when the differential coupling phases .. V H /L/ accumulated a -phase. The respective amplitude values of V2 D 0:08 and H2 D 0:09 for the vertical and horizontal polarizations align with the 9 % coupling value inferred from the first half cycle transmission (86 %) after accounting for the 5 % insertion loss (IL) resulting from the abrupt starting point of the laser-formed waveguide. In order to minimize device loss, one may consider the design of directional couplers having the shorter lengths ( 350 nm > 350 nm < 73 nm < 175 nm

Negligible Negligible Strong Strong

1.2 1–1.7 0.2 0.04

Based on a coupling length of 0.099 mm; Based on a zero length coupler

In this section, coupling of light from the core waveguide of SMF was demonstrated with X-, S-bend, and directional couplers whose characteristics are summarized and compared in Table 4.1. Despite the asymmetric waveguides (ˇ ¤ 0), coupling ratios from 0 to 76 % were demonstrated. While directional couplers based on evanescent fields had the lowest losses introduced by the coupler (0.2 dB), their wavelength dependence, defined here as the wavelength range over which less than 5 % variation in the coupling ratio was observed, was more limited relative to the higher-loss (1–1.7 dB) broadband .> 350 nm/ S-bend and X-couplers. The design of directional couplers can be further tailored by the waveguide separation to increase or decrease the coupling strength. In this way, weak polarization or non-polarization taps may be designed with large waveguide separation (> 10 m) while shorter separation (i.e., 9 m) increases the overall coupling strength as stronger evanescent coupling ( V;H ) improves the magnitude of the amplitude dephasing term as seen in Eq. 4.2. However, the overall efficiency

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

83

of directional couplers in this weak coupling regime is restricted by the ˇ-mismatch, which can be addressed alternatively by using X- (Sect. 4.3.1) or S-bend (Sect. 4.3.2) couplers. The coupler losses summarized in Table 4.1 only represent the losses introduced by the coupler itself and do not include the propagation loss (Sect. 4.2) encountered in guiding the light in the fiber cladding. S-bend and X-couplers provided polarization-independent coupling while the strong polarization-dependent coupling offered by the directional couplers provided new directions for designing in-fiber polarization-selective taps and polarization beam splitters. In summary, the challenge of coupling light between the SMF core and light-guiding cladding structures has been met with multiple coupler types, whose loss and spectral and polarization coupling characteristics were analyzed.

4.4 Femtosecond Laser-Formed Cladding Photonic Devices Waveguides are the fundamental component for routing light signals in optical circuits in which couplers and gratings offer powerful ways to multiplex signals and tailor their spectral responses. This section discusses the properties of femtosecond laser-written waveguides and BGW devices as formed inside single-mode and coreless optical fibers. An in-line MZI in SMF and a 3D distributed position-shapetemperature sensor in coreless fiber are presented as examples of the powerful integration approaches that are now available given the new coupling techniques presented in Sect. 4.3.

4.4.1 Waveguides and Bragg-Grating Waveguides in the Core and Cladding of Optical Fibers The femtosecond laser oil-immersion writing technique described in Sect. 4.2 was used to extend single-mode waveguide writing from bulk glass to the cladding of SMF and coreless optical fibers, providing waveguides with propagation loss as low as 0.5 dB/cm. The AOM modulation techniques introduced in Sect. 4.2 provided the burst trains of femtosecond laser pulses on which low- and high-strength, first-order gratings were formed both in the core waveguide and cladding waveguides of SMF and coreless fibers. While several laser approaches, including femtosecond direct laser writing, have been developed for writing Bragg gratings into the preexisting germanium-doped SMF core [52–54], their integration into the cladding of optical fibers opens new opportunities for cladding photonic devices that we explore in this section. The spectral response of strong BGWs is first examined for various writing positions in SMF and coreless fiber using nearly identical exposures (120 nJ to

84

J.R Grenier et al.

a

b

c

d

Fig. 4.11 Linearly polarized transmission spectra of 25 mm long BGWs fabricated in (a) the core of an SMF with 130 nJ pulse energy, (b) the cladding of an SMF with 120 nJ, and (c) the center of a coreless fiber with 130 nJ. Insets, optical micrographs of BGW end facets (writing laser from the top) with expanded views of the waveguide zone (image diameter is 12 m). (d) Vertical (V) and horizontal (H) linearly polarized and unpolarized (U) transmission spectra for the BGW in (c) [60]

130 nJ). Transmission spectra are shown in Fig. 4.11a, b, c for the respective cases of positioning the BGW near-center of the preexisting core of SMF, off-center (r D 30 m) in the cladding of an SMF, and centered in the coreless optical fiber. The inset optical micrographs shown in Fig. 4.11a,b,c are of the waveguide end facets with magnified views revealing a dual modification zone of positive increase in refractive index of a larger diameter .3:6 m/ white zone under a smaller diameter zone .2:1 m/ of negative refractive index change that appears dark. The spectra of Fig. 4.11 all show a strong and narrow Bragg resonance ( 3dB D 0:3 nm) near B D 1550 nm with propagation losses varying from 1 dB/cm to 1.9 dB/cm. However, there was a significant difference between the strength of coupling and number of permitted cladding modes. When the BGWs were centered in the core waveguide of the SMF (Fig. 4.11a) and the center of the coreless fiber (Fig. 4.11c), a very open spectrum formed that was dominated by strong coupling to the discrete LP0n cladding modes that matched well with the stick spectra as shown in the SMF case (Fig. 4.11a), calculated in [60]. Moderately strong coupling was also observed in both fiber types to a higher-order azimuthal cladding mode (LP1n ) that arose from imperfect centering of the BGW as reported by [71,72]. Also contributing to the coupling is the asymmetric refractive index profile as seen in

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

1.450 SMF core n =1.44922

1.449

Effective Index

Fig. 4.12 Effective index at 1550 nm wavelength of FBG (black circles) and BGW (black squares) as a function of the laser pulse energy. Horizontal lines indicate the refractive index of the SMF core (green dashed line), fused silica fiber cladding (blue dashed line), and the effective index of the unmodified SMF mode (red dashed line) [74]

85

FBG

1.448 1.447

SMF neff =1.44630

1.446 1.445 1.444

BGW Silica n =1.44402

0

20

40

60

80 100 120 140 160 180

Pulse Energy (nJ)

the higher-resolution optical micrographs inset of Fig. 4.11a, b, c. Coupling to an increasing density of azimuthal cladding modes progressed systematically as the BGW position was increasingly displaced from the center axis, eventually leading to broadening and weaker coupling until the weak (7.3 dB loss) near-continuum in Fig. 4.11b was observed for the 30 m offset. Figure 4.11d shows transmission spectra for vertical (V) and horizontal (H) linear polarization and unpolarized (U) light coupled into the BGW formed in the center of a coreless fiber (Fig. 4.11c). A waveguide birefringence of 1:03 104 was inferred from the spectral shifting of the V and H Bragg resonances that was more than 2 higher than values previously reported with weaker focusing [33]. This higher birefringence is a result of higher asymmetric stresses [73] induced by the 1.25 NA oil-immersion lens. Such large birefringence was harnessed to form polarization beam splitters in coreless fiber (Sect. 4.3.4) and previously in bulk glass [70]. Further tuning of the waveguide birefringence by femtosecond laser-written stressing tracks is discussed in Sect. 4.5. The effective refractive index is a key waveguide parameter required in the design of optical circuits. The effective index value of neff D 1:44630 is defined in Fig. 4.12 for 1550 nm wavelength against the indicated cladding (1.44402) and core (1.44922) refractive index values. The effective refractive index of BGWs formed in the SMF core and cladding was inferred from the measured Bragg wavelength for a range of laser pulse energies applied between 5 nJ and 170 nJ and is plotted in Fig. 4.12 for 1550 nm wavelength along with the SMF cladding (1.44402), core (1.44922), and effective (1.44630) refractive index values. The threshold exposure of 5 nJ pulse energy for forming a grating into the preexisting SMF core waveguide was significantly lower than the 70 nJ pulse energy required to form both the waveguide and the grating structure in the fused silica fiber cladding. Above these threshold values, the laser pulse energy provided a means of tuning the effective refractive index and hence the propagation constants (ˇ) of

86

J.R Grenier et al.

a

b

−5

FSR = 32 nm

L

BGW SMF Core

Transmission (dB)

fs waveguide −10 −15 −20

1300

1350

1400

1450

1500

1550

1600

Wavelength (nm)

Fig. 4.13 (a) Femtosecond laser-formed MZI in an SMF and (b) the resulting transmission spectrum probed with vertical linearly polarized light [64]

the waveguides. Such tunability is useful in the design of directional couplers where the maximum coupling efficiency depends on the propagation constant mismatch (ˇ) as shown in Eq. 4.2.

4.4.2 Mach-Zehnder Interferometer Device Mach-Zehnder interferometers are an important optical component that find application as sensors or as wavelength-dependent filters and wavelength division multiplexers in telecommunications. Femtosecond laser-written MZIs have previously been demonstrated in bulk glass [28] with a 10 m path length difference. In the limited volume of fiber cladding, a large path difference has not been previously demonstrated with the formation of a second waveguide arm, and MZIs were limited to designs based on tapered fibers [75], microcavities [76, 77], and long period gratings [78]. The fabrication of a fiber-integrated MZI is presented here as an example of a more functional photonic in-fiber device. The demonstration is made possible by combining the coupler presented in Sect. 4.3 with the cladding waveguides in Sect. 4.4.1. The MZI design consists of two broadband S-bend couplers (Sect. 4.3.2) with 30 mm bend radius to couple light between the SMF core waveguide and a laser-formed cladding waveguide offset by 40 m from the SMF core as depicted in Fig. 4.13a. A 15 mm length BGW ( B D 1316 nm) was also fabricated in the core of SMF with 20 nJ pulse energy in order to monitor the V and H polarization axes once the fiber had been removed from the fabrication setup. The total length of the cladding waveguide arm was L2 D 38:382 mm, consisting of a 34 mm long straight section and two 2.191 mm long S-bend couplers. Although this design only offers 1 m longer physical path length over the core waveguide section (L1 D 38:381 mm), the large difference in the effective index of the SMF core

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

87

waveguide (neff1 D 1:44630) and the laser-formed cladding waveguide (neff2 D 1:4446 ˙ 0:0003), as seen in Fig. 4.12, is significant in creating a large optical path difference estimated at L2 neff2 L1 neff1 D 1 m) without requiring any large displacement of the cladding waveguide arm. The measured transmission spectrum (Fig. 4.13b) was recorded with vertical linearly polarized light and clearly shows interferometric fringes with a maximum contrast of 16.5 dB at 1445 nm. The S-bend couplers were designed to couple as much light into the cladding waveguide to compensate for their higher propagation loss. The measured free spectral range (FSR) of 32 nm at 1550 nm wavelength agrees with FSR D

2 ; L2 neff2 L1 neff1 C

(4.6)

yielding a value of 33.9 nm that falls within the experimental uncertainty of the cladding BGW effective index (1:4446 ˙ 0:0003) from Fig. 4.12. The FSR can be tuned most strongly with the MZI device length (L), while a smaller degree of tuning is available with coiling the waveguide around the cladding as well as by varying the effective index of the cladding waveguide with the laser exposure.

4.4.3 Bragg-Grating Waveguide Shape Sensor Fiber-optic sensing is broadly applied today with the sensing region typically confined to the core waveguide of an SMF. For the case of laser-inscribed Bragg gratings, optical sensing relies on a shift of the Bragg resonant wavelength that in the case of strain gauging typically requires secure bonding or embedding of the fiber within a host structure in order to strain the grating along the central neutral axis of the fiber. For more flexible applications such as in shape or position sensing and accelerometers, the grating-embedded waveguide should be displaced away from the neutral axis of a bending structure, for example, as demonstrated in multicore optical fibers (MCFs) [79, 80] and further discussed in Chap. 10. However, the coupling of light into each radially distributed waveguide core to interrogate all the Bragg gratings simultaneously remains a challenge with such MCF-based sensors. In this section, we examine femtosecond laser direct writing of optical circuits in a coreless optical fiber that is fusion spliced to an SMF to provide a unique solution for simultaneous FBG interrogation through a single waveguide core of the SMF. This combination of multiple 3D optical components is shown to offer distributed shape, position, and temperature sensing. Figure 4.14a shows a schematic of a fiber-optic shape sensor that is being fabricated with a femtosecond laser focused by an oil-immersion lens as previously described in Sect. 4.2. The laser exposure conditions of 1 MHz repetition rate, 71 nJ pulse energy, 0.1 mm/s scan speed, and 60 % duty cycle were used to form the BGW sensor segments. Prior to laser structuring, the coreless fiber was fusion spliced to the SMF to avoid thermal erasing of laser-written structures as discussed in Sect. 4.2.

88

J.R Grenier et al.

Fig. 4.14 (a) Schematic of a 3D distributed shape and thermal sensor written in coreless fiber by a femtosecond laser focused with an oil-immersion lens. The embedded Bragg-grating sensors are labeled 1 to 9 . Optical micrographs of the fiber cross section (125 m diameter) at (b) the coupling and (c) sensor regions, showing the arrangement of the internal laser-written waveguides [81]

The sensor consisted of three parallel waveguides, one 1 3 directional coupler, two waveguides with S-bends, and nine BGWs, all written in a single exposure step inside the coreless fiber. A nearly equal power splitting at 1310 nm wavelength was obtained with a 500 m long directional coupler by using a waveguide separation of 9 m in a right-angled isosceles triangle arrangement as shown in Fig. 4.14b. The two off-center waveguides were drawn out by S-bends (40 mm radius) to the 40 m radial positions as shown in the cross-sectional image of Fig. 4.14c. Following the S-bends, the three waveguides were formed into straight and parallel paths to define the distributed sensing region, over which three 1 cm long BGWs were written along each waveguide at 2 cm center-to-center separations, forming three groups of axially colocated BGW triplets as illustrated in Fig. 4.14a. Each BGW was tuned to a different Bragg resonance scaled from 1 D 1280 nm to 9 D 1320 nm in 5 nm increments. This short to long wavelength ordering positioned the spectrum of cladding-mode-coupled light from an upstream BGW outside of the Bragg resonance of a downstream BGW [53]. The fiber shape could be inferred from the shifts in Bragg wavelength of all nine BGWs as monitored with a spectrometer (Ibsen Photonics: I-MON 512E) through the single waveguide port of the SMF shown in Fig. 4.14a. The Bragg wavelength shift was first calibrated against strain and temperature according to the conventional FBG response, which relates the Bragg wavelength shift, , to strain, , and thermal variation, T , according to [82] 1 D .1 pe / C .˛ C /T;

n

(4.7)

where pe is the effective strain-optic constant, ˛ is the thermal expansion coefficient, n is the refractive index, and is the thermo-optic coefficient. A strain sensitivity and

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

89

Fig. 4.15 (a) Four superimposed photographs of the fiber sensor bent in various shapes showing scattered light from the laser-formed waveguides in the coreless fiber while end-fired with a red diode laser from the SMF. (b) Fiber profiles calculated from Bragg resonance shift of nine BGWs are shown in dashed lines superimposed onto the fiber shapes of (a). Green lines indicate the BGW triplet locations [81]

thermal response of the sensor was determined to be = D 1:06 ˙ 0:06 pm= and =T D 9:1 ˙ 0:6 pm/ı C, respectively, which is consistent with the response values of 1:2 pm= and 10.0 pm/ı C, respectively, found in traditional FBGs at longer 1550 nm wavelength [82]. An example of fiber shape sensing at uniform room temperature is presented in Fig. 4.15 by the four cases of nonuniform fiber bending. Red diode laser light was launched into the fiber in order to record the scattered light optical images that were superimposed in Fig. 4.15a with the four different images of fiber shape. For each sensor shape, the nine Bragg wavelength shifts were used in Eq. (4.7) to infer the bending radius and azimuthal bending plane at the three BGW axial positions. These values were decomposed into bend radii on orthogonal planes and followed with a cubic spline interpolation to calculate a continuously varying curvature and azimuth along the length of the fiber. The shape and position of the fiber was finally determined by the finite element method of corotational analysis, which discretized the fiber into curved rigid beam elements that were aligned tangentially at each node [83]. The fiber shapes calculated in this way for each of the fibers imaged in Fig. 4.15a are shown in Fig. 4.15b as dashed lines that closely align with the BGW locations highlighted in green. Hence, the fiber shape sensing could precisely follow the lateral BGW displacements up to 26 mm and bending radii as small as 77 mm. Figure 4.16 shows two examples of the calculated fiber shape (top) together with the reflection spectrum (bottom) recorded at different instants of dynamically changing conditions of fiber bending at room temperature (Fig. 4.16a) and nonuniform heating (Fig. 4.16b). The red lines in the reflection spectrum mark the unstrained and room-temperature Bragg wavelengths for the BGWs in each sensing arm (i.e., center and side) further labeled by a different color. As expected, fiber bending induces large wavelength shifts of up to 560 pm in the off-center BGWs relative to the non-shifting center BGWs, corresponding to a minimum bend radius of 75 mm. The present fiber sensor was designed such that the center waveguide is minimally sensitive to any bend-induced strain and therefore can be used to sense

90

J.R Grenier et al.

Fig. 4.16 Fiber shape and temperature profile (top) calculated from the Bragg resonance shift of nine BGWs in corresponding reflection spectrum (bottom), where the red lines indicate the Bragg wavelengths of unstrained gratings at room temperature. Fiber bending with (a) uniform and (b) graded temperature along the fiber length [81]

temperature and to compensate Bragg wavelength shifts in the off-center BGWs due to thermal variations. Figure 4.16b presents simultaneous sensing of fiber shape and temperature for nonuniform bending and heating of the fiber sensor with a hot iron. Temperature over a range of 24 to 100 ıC was determined from the wavelength shift of the center BGWs and extended by linear interpolation to profile the region between axially colocated BGW triplets. Assuming uniform temperature in the fiber’s cross section, the observed wavelength shifts of the center and sidearm BGWs adjusted for temperature to isolate values for the fiber strain and thus offer the real-time measure of the temperature gradient seen along the fiber in false color together with the fiber sensor shape. The BGW spectra line shape could also be broadened into a spectral chirp when heated at a point smaller than the 1 cm long BGW length and give more precise information of thermal gradients along the grating [84]. The successful demonstration of the temperature-compensated fiber-optic 3D shape sensor was predicated on the 3D writing of a balanced 1 3 waveguide coupler from which distributed BGW sensor signals could all be efficiently relayed into a single fusion spliced SMF. This approach offered advantages in facile and flexible fabrication in comparison with shape sensors based on multiple-fiber assemblies [85,86] or in an MCF [79,80]. In combination, the MZI and BGW sensor examples presented here demonstrate the utility of femtosecond laser writing for creating fiber cladding photonics that can be conveniently probing from a single core waveguide such as provided in SMF. The overall compact size and high temperature

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

91

tolerance of the present devices are further attractive for structural, industrial, reactor, and pipeline applications as well as for integration into biomedical and catheter devices. Much more advanced and functional cladding photonic circuits may now be considered for design and application.

4.5 Birefringence Tuning in Fibers Optical fibers are typically desired without having any polarization sensitivity and are therefore manufactured with very small birefringence of 107 for telecommunication and optical sensing applications. However, polarization-sensitive devices are required in new applications such as phase-shift keying for optical communication [87], quantum optics [88,89], strain, pressure, and temperature sensing [90,91], twist and torsion sensing [92], and single polarization fiber lasers [93, 94]. To this end, polarization-maintaining fibers are also widely available with high birefringence values ranging from 104 in commercial fibers to 103 in microstructured optical fibers [95] and up to 102 in photonic crystal fibers [90]. Such polarizationdependent optical systems also require quarter-wave and half-wave plates, Faraday rotators, and other polarization elements to be integrated and packaged into the optical fiber systems. Laser processing is attractive as a more flexible method to replace such lumped elements and directly embed polarization devices such as polarizers, waveplates [33], polarization splitters [70], and high birefringent stresses [74, 96] directly within the optical fiber or circuit. In this section, we examine how laser processing can bypass the cumbersome lumped-element fiber packaging step and facilitate the integration and miniaturization of polarization components directly within optical fiber technology. The presented results report on the control of waveguide birefringence in both the core waveguide of the SMF and in laser-formed waveguides by writing laser-stressing tracks under various geometries, polarization direction, laser pulse energy, and degree of track overwriting. The high birefringence values promise to create more compact submillimeter polarization devices.

4.5.1 Stress-Induced Birefringence Laser writing of waveguides is well known to cause local asymmetric stresses [73, 96] that manifest in a waveguide birefringence of 104 as shown in Fig. 4.11 (Sect. 4.4). This intrinsic waveguide birefringence was also found to include a strong component of form birefringence owing to the laser formation of nanogratings in fused silica glasses [39, 97–99]. One can harness these stress and nanograting effects and manipulate the waveguide birefringence by writing laser modification tracks in close proximity to preexisting waveguides. In this way, the waveguide birefringence can be flexibly tuned to lower birefringence to values of 106 [96]

92

J.R Grenier et al.

Fig. 4.17 Femtosecond laser stress tracks written around a FBG inscribed in the SMF core waveguide. The electric field amplitude vectors, EV and EH , represent the vertical and horizontal orientations of the waveguide polarization eigenmodes. The center-to-center track separation (S) is noted between the fiber waveguide core and the stress-inducing modification tracks. An optical micrograph of the cross section of a finalized device is shown in the bottom right corner [74]

or increase birefringence to values of 8 104 [96, 100, 101] with adjacent pairs of laser modification tracks, or as high as 2:0 103 with multiple overwritten tracks [74]. The schematic shown in Fig. 4.17 shows the high numerical aperture (HNA) oil-immersion writing geometry, as introduced in Sect. 4.2, together with the stressinducing laser tracks being fabricated around the core waveguide of the SMF. The polarization eigenmodes in the center waveguide (y-direction) are defined as EV for vertical and EH for horizontal in the z-axis and x-axis directions, respectively.

4.5.2 Birefringence Tuning An example of the morphology, laser-formed waveguides surrounded by horizontally and vertically positioned stress-inducing tracks is shown in the end-view optical micrographs of Fig. 4.18a and d, respectively. To better assess the center waveguide birefringence, the same waveguides were back-illuminated and viewed through two crossed polarizers aligned vertical (Fig. 4.18b), horizontal (Fig. 4.18e), and diagonal (Fig. 4.18c and f) as indicated by the green crosses. The highest birefringence is inferred from the brightest light patterns, which appeared for the horizontally arranged stressing tracks in Fig. 4.18c. The long horizontal bright strip indicated the presence of long-range ( 10 m) stresses that reached symmetrically from the stress-inducing tracks to overlap at the center waveguide under test.

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

93

Fig. 4.18 Optical micrographs of the facets of waveguides fabricated in fused silica and surrounded horizontally (a–c) and vertically (d–f) by symmetric pairs of stress-inducing tracks. The green crosses indicate the direction of polarizers used to record the cross-polarization image for (b), (c), (e), and (f). A typical optical mode profile of 1560 nm guided light in (d) is shown to scale with guiding lines marking the mode position over the laser-modified structure seen in the end facet [74]

To verify the effects of this laser-induced stress, the birefringence of the SMF core waveguide was monitored by optically probing a weak single Bragg grating, laser-formed into the fiber core waveguide. The nearly birefringent-free FBG of 0.12 nm bandwidth and 8 dB strength is shown in the reflection spectrum of Fig. 4.19 (unstressed FBG) to broaden and then split into two resolved V and H polarization modes of 120 pm and 200 pm separation following the laser writing of a single stress track and double stress tracks, respectively. Unlike the large long-wavelength shift of the V polarization mode, the H polarization mode approximately retains the same propagation constant. Such wavelength shifts suggest the bright region in Fig. 4.18c to be associated with a strong positive increase in refractive index that is highly asymmetric and mainly aligned with the polarization in the lateral direction as defined between the two stress bars. In contrast, the vertically aligned stressing bars were not found to drive strong refractive index changes or birefringence, as expected by the weak light transmission observed using cross-polarizers in Figs. 4.18e and f. The birefringence induced in both bulk glass waveguides (blue) and fiber core waveguides is shown together in Fig. 4.20 as a function of the separation (S ) between the symmetric stress-inducing tracks and the center wavelength. The waveguides and stress tracks were written with both parallel and perpendicular laser polarizations (EP ark and EP er? ) to preferentially align the nanograting orientation

94

J.R Grenier et al.

Reflection (5 dB/div)

S = 13 µm

Unstressed FBG

Single stress track

H

V Double stress track

1532.6

1533.3

1534.0

1534.7

Wavelength (nm) Fig. 4.19 Unstressed FBG (top blue line), FBG with one stress-inducing track (middle red line), and FBG with two stress-inducing tracks (green bottom line). The tracks are symmetrically positioned on opposite sides of the SMF core waveguide and are written with 13 m separation, 140 nJ pulse energy, and 0.268 mm/s scan speed. The FBG was fabricated with the best conditions identified in Fig. 4.12 and the spectra are offset here for comparison [74]

that could induce the strongest birefringence at each of the indicated laser pulse energies. The strong form birefringence of such nanogratings is evident in the unstressed BGWs fabricated in fused silica with 150 nJ of pulse energy and 100 kHz of repetition rate, yielding a waveguide birefringence of 2:2 104 for parallel writing and 4:1 104 for perpendicular writing as reported for 1 separation in Fig. 4.20. The larger birefringence includes the form birefringence that can be estimated from the difference of 2 104 here and arises when the nanogratings are oriented parallel to the waveguide direction (EP er? ). The introduction of horizontal stressing tracks with separations diminishing to as small as 10 m led to a significant birefringence increase of 4 104 for both types of waveguides and reached a maximum birefringence of 8:3 104 that was associated with the large 891 pm Bragg wavelength splitting observed in the inset spectrum (Fig. 4.20) for the perpendicular writing case. Since the overall birefringence increase is similar for both writing polarizations, one sees the nanograting to only offer a local form birefringence with little reach outside of the stress bars to affect the properties of waveguides nearby. A similar assessment in SMF is shown in Fig. 4.20 for parallel polarization writing of horizontal stress tracks around an SMF core waveguide with three different pulse energies applied under the oil-immersion focusing. Here, a weak FBG was first generated in the fiber core with pulse energy of 5 nJ to 10 nJ as shown in Fig. 4.12 in order to minimize the initial birefringence to approximately

Transmission

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

Birefringence (×10−4)

8

6

420 100 250 100

V

95

H Δl = 891.2pm Δn = 8.31×10−4

nJ kHz nJ kHz

1550

1551 Wavelength (nm)

4

EPer ⊥ in bulk glass

300 nJ 100 kHz

EPar in bulk glass

160 nJ

2 500 kHz EPar in SMF

0 0

10

20

30

40

50

60

70

80

∞

Separation (µm) Fig. 4.20 Measured waveguide birefringence as a function of the stress-inducing track separation with the laser writing of two symmetric modification tracks on opposite sides of the waveguide under test. The results are shown for parallel polarization of the writing laser in SMFs with fabrication conditions of 160 nJ at 500 kHz, and 250 nJ and 420 nJ at 100 kHz for the red, green, and black curves, respectively. The birefringence of waveguides formed in bulk fused silica (equivalent to the coreless fibers) is presented by the blue curves for perpendicular and parallel writing with 300 nJ pulse energy at 100 kHz repetition rate. The dashed and solid lines represent vertical (Fig. 4.18d) and horizontal (Fig. 4.18a) arrangement, respectively, for the stress-inducing tracks in the case of waveguides formed in bulk fused silica glass [74]

2 105 (S D 1 in Fig. 4.20). The SMF birefringence is seen to increase by 3:4 104 , 4:0 104 , and 5:6 104 for the 160 nJ (red data), 250 nJ (green data), and 420 nJ (black data) exposures, respectively. The trends found for the birefringence measurements in fibers are consistent with those found in waveguides formed in bulk fused silica glass under both high NA (Fig. 4.20) and low NA writing conditions [96]. The birefringence induced into bulk glass and SMF core waveguides was also examined with the stress tracks aligned vertically as in Fig. 4.18d. This alignment led to a moderate decrease in birefringence of 1:3 104 to a value of 0:9 104 (dashed blue line) in bulk glass waveguides and a decrease of 2 105 to a value < 4 106 (dashed red line) in SMF, at respective track separations of S D 14 m and S D 20 m as seen in Fig. 4.20. However, this decrease is found to simply reverse the initial birefringence induced while creating the BGW and FBG, respectively, but not going further to reverse the sign of the birefringence. Hence, the minimum recorded birefringence was 4 106 (at our resolution limit) for the SMF case in Fig. 4.20. All the data in Fig. 4.20 were well represented by inverse square functions (solid and dashed lines) of the separation distance (S ).

96

J.R Grenier et al.

EPer⊥

N

1.5

EPer⊥ EPar

1.0

Δl =1.18nm Δn =1.105×10−3

Reflection (2 dB/div)

Birefringence (×10−3)

2.0

0.5

0.0

1544.8

0

2

4

6

8

10

12

1545.7 1546.6 . Wavelength (nm)

14

16

18

Number of stress tracks Fig. 4.21 Waveguide birefringence as a function of the number, N (configuration illustrated in the top left inset), of overwritten stress tracks laid out at a fixed separation of 11 m and fabricated with 160 nJ pulse energy at 500 kHz repetition rate. A logistic function fits the results for parallel (blue circles and blue curve) and perpendicular (green squares and green curve) polarizations of the writing laser. The inset shows an example reflection spectrum of the Bragg resonance observed before (blue solid line –) and after (green dashed line - -) the fabrication of 18 stress tracks at S D 11 m for the parallel writing case. The top right inset illustrates the arrangement of an ensemble of 19 laser modification tracks fabricated with the perpendicular polarization of the writing laser and evenly distributed between an 11 m and 8 m separation [74]

The further increase in birefringence has been explored by inscribing multiple stressing tracks and overwriting the stress tracks around the SMF core as well as by introducing form birefringence directly into the core waveguide with strong laser modification of the core. The resulting waveguide birefringence values are plotted in Fig. 4.21. The blue and green curves show the birefringence increasing as a function of N for the same stressing conditions (160 nJ pulse energy and 11 m separation) but with the FBG under test fabricated with 5 nJ for the parallel writing case (blue curve) and 90 nJ for the perpendicular writing case (green curve). The parallel writing case had a negligible starting birefringence at N D 0 while the perpendicular writing case found an initial 0:4 103 birefringence value. This higher value is due to the form birefringence and higher energy used for the FBG fabrication and is comparable with the initial value found for writing with parallel polarization in fused silica as shown in Fig. 4.20. The data in Fig. 4.21 were fitted to logistic-type functions, with the birefringence values reaching a saturation level after 10 overwritten stress tracks. A closeto-saturation birefringence value of 1:11 103 , inferred from the spectrum inset

2.5

1.0

2.0

0.8

1.5

0.6

l/2 1.0

0.4

800 µm l/4

0.5

0.0

1275

1375

1475

1575

97

Birefringence (×10−3)

Length (mm)

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

0.2

1675

0.0

Wavelength (nm) Fig. 4.22 Birefringence as a function of wavelength (right scale, blue circles, and curve) and minimum waveplate length (left scale, half-wave plate in the red curve, and quarter-wave plate in the green curves). The black horizontal dashed line represents an 800 m retarder device fabricated in SMF. The birefringence spectrum was recorded from this device by a cross-polarizer arrangement, identifying a quarter-wave plate at 1324 nm wavelength [74]

in Fig. 4.20, was found for the parallel writing case while a value of 1:3 103 was found for the perpendicular writing case. Using a combination of 19 tracks distributed between 11 m and 8 m separation and perpendicular polarization of the writing laser, it was possible to form a plane of horizontal stress that further enhanced the birefringence. A maximum birefringence of 2:0 103 was found for this case (top right datum in Fig. 4.21), a value more than twice as large as previously reported with a similar writing technique [100]. With the birefringence values demonstrated here, it is possible to design half-wave retarders in the infrared spectral band with only submillimeter fiber lengths [33]. Figure 4.22 shows the spectral dependence of the birefringence (right scale) in SMF modified with ten pairs of overwritten laser tracks with 11 m separation and formed with 160 nJ pulse energy, 0.268 mm/s scan speed, and 500 kHz laser repetition rate. The minimum length required to obtain a quarter-wave or a half-wave plate can be found from L D WP

neff . /

:

(4.8)

Here, neff . / is the wavelength-dependent birefringence and WP represents the wave retardation (WP D 1=2 for a half-wave and WP D 1=4 for a quarterwave plate). In order to design a spectrally broad waveplate, the relative variation

98

J.R Grenier et al.

of birefringence should follow the relative variation of wavelength according to Eq. 4.9. This yields a constant retardance as a function of wavelength for a fixed waveguide length L: d d.neff / : D neff

(4.9)

For the waveguide birefringence spectrum in Fig. 4.22, one finds the minimum length (Eq. 4.8) for creating quarter-wave and half-wave waveguide retarders (left scale) to vary by 50 % across the 1250 nm to 1700 nm spectrum, from a length of 1 mm to 0.5 mm and from 2 mm to 1 mm, respectively. The birefringence was determined by the cross-polarization technique [33] applied to an 800 m long segment of stressed SMF. This segment led to a quarterwave plate operation measured at 1324 nm as shown in Fig. 4.22. This wave retarder has a 10 nm band between 1690 nm and 1700 nm that satisfies the broadband condition of Eq. 4.9 within a tolerance of 0.2 %. Extrapolation of the waveplate length data to longer wavelengths suggests that broader band waveplates are available here. Alternatively, other laser exposure conditions are expected to shift the birefringence dispersion and possibly better meet the waveplate condition of Eq. 4.8 over broader and in different spectral windows.

4.5.3 Summary In summary, this section demonstrated the advantage of using tightly focused femtosecond laser light to locally tune the birefringence of preexisting optical waveguides. By various means of polarization control and multiple track scanning, a stress birefringence of up to 2 103 was induced in SMF. This approach offers flexible in situ tuning of waveguide birefringence as well as the precise integration of quarter- and half-wave plates to specific wavelengths that are attractive in fiber platforms for higher-level integration of polarization-encoded components into short waveguide segments. These in-fiber polarization components could be integrated with the waveguide couplers described in Sect. 4.3 to enable new approaches for creating polarization-sensitive fiber taps, polarimeters, and other polarization elements with applications of power monitoring in fiber lasers, polarization-dependent fiber sensing, and quantum optics circuits.

4.6 Microfluidics in Optical Fiber The Introduction (Sect. 4.1) identified an intense drive to reduce biological and chemical laboratory processes from bulky free-space systems to much more compact and functional LOC devices that are typically limited today to planar

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

99

substrates [45]. The nanogratings generated during femtosecond laser processing of fused silica opened the novel approach of highly selective chemical etching by FLICE [32, 36–39] that is now addressing these new LOC directions. In this section, we examine the further possibility of using FLICE to wrap microfluidic and optical components around the guiding core waveguide of existing fiber-optic technology and create new types of LIF devices. The FLICE approach was applied here to construct examples of 3D microfluidic networks, microholes, reservoirs, and optical resonators within both types of SMF and coreless optical fiber. These components were then integrated by the powerful laser fabrication techniques introduced in this chapter toward demonstrations of fluorescence and refractive index sensing that underpin a novel all-fiber sensing platform.

4.6.1 3D Microfluidic Networks for Lab-in-Fiber To open this new direction of LIF devices, the formation of 3D optofluidic devices in optical fiber was explored by following the benefits of high NA oil-immersion objective lenses previously described in Sect. 4.2 for reduction of spherical aberration and beam-focusing distortion in the fiber. In this way, flexible fabrication of arbitrarily complex 3D microfluidic networks was shown to become possible by laser writing of nanograting modification templates in the fiber. The laser tracks were opened with weak HF etching to create predictable structures at arbitrary locations targeted within the SMF and coreless fiber types. Laser exposure conditions for chemical etching of fibers were adopted from the recipes developed for bulk glass by Ho et al. [43, 102]. However, an optimization of the laser exposure under the much tighter focusing with the oil-immersion lens (1.25 NA) was found to lower the laser exposure requirements to 25–50 % of that typically required with air lenses (0.55 NA) [43, 102]. The laser and exposure tools were identical with those described in Sect. 4.2, centered on 522 nm wavelength light of 200 fs duration and 1 MHz repetition rate. In the following demonstrations, fiber access ports and reservoir structures were exposed to 60 nJ pulse energy while weaker exposure of 20 nJ pulse energy was preferred to generate the smoothest walls desirable for low optical scattering loss at microchannel and optical resonator surfaces. Laser scanning speeds were typically in the range of 0.3 to 2.5 mm/s, with slower speed favored for smoother etched walls. The walls of reservoirs, large channels, and optical resonators were formed by arrays of laser modification lines spaced by 1 m, with polarization chosen to preferentially align perpendicular to the scan direction [36] to create the smoothest wall profile. The laser modification tracks were etched with 5 % aqueous HF solution for 1 hour to fully open into channels. The first LIF concept demonstrated in Fig. 4.23 is the formation of a 3D microfluidic network embedded within coreless fiber. This representative example split a single microchannel into four separate radial arms that may each be independently probed by laser-formed waveguides. Alternatively, straight through or blind access channels shown in Fig. 4.24 were embedded for optical probing by the

100

J.R Grenier et al.

Fig. 4.23 (a) Schematic and (b) optical micrograph of a 3D microfluidic network embedded within optical fiber of 125 m diameter. A single microchannel is split into four separate radial arms that may each be independently probed by laser-formed waveguides (not shown). The channels opened along laser exposure tracks formed with oil-immersion focusing to avoid optical aberrations. This undistorted patterning of nanograting structures offered precise formation of straight and circular channels after HF etching. Reproduced from [102] by permission of The Royal Society of Chemistry. © 2014 The Royal Society of Chemistry. http://dx.doi.org/10. 1039/C4LC00648H

Fig. 4.24 Optical micrographs of access microchannels traversing across coreless fiber of 125 m diameter from (a) top and (b) side views together with (c) a cross-sectional view of a partially traversing blind hole. The non-distorted template structures exploited oil-immersion focusing to form nanogratings that were opened with HF etching. Reproduced from [102] by permission of The Royal Society of Chemistry. © 2014 The Royal Society of Chemistry. http://dx.doi.org/10. 1039/C4LC00648H

core waveguide of SMF for fluorescence or absorption spectroscopy applications. More elaborate 3D optofluidic networks may be envisioned over long lengths of optical fiber to further exploit the benefits of undistorted laser writing with the oilimmersion lens and thereby interconnect optical waveguides with microchannels in straight, circular, or arbitrarily complex shapes. Lab-in-fibers also require the formation of larger open structures such as reservoirs to facilitate efficient fluidic access and exchange from external sources. Microfluidic reservoirs were formed into the fiber cladding by laser writing of overlapping modification tracks in planes that outlined the reservoir boundary.

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

101

a c

b

Fig. 4.25 (a) Cross and (b) top view optical micrographs of microfluidic reservoirs fabricated in optical fiber by laser writing of overlapping modification tracks in planes that outline the reservoir boundary and that were opened with HF etching. (c) AFM surface profile of a reservoir sidewall over 4 4 textmu m2 area indicating a small 12 nm (rms) surface roughness. Reproduced from [102] by permission of The Royal Society of Chemistry. © 2014 The Royal Society of Chemistry. http://dx.doi.org/10.1039/C4LC00648H

Submerging the laser-processed fiber into HF facilitated etching along such planes to release glass blocks into the surrounding HF bath and thus remove large arbitrary shaped volumes [104]. In fiber, a reservoir of dimensions 50 60 125 m3 was fabricated as shown in the micrographs of Figs. 4.25a and b. Reservoirs may arbitrarily be placed into any geometric shape and size and offer flexible means to form refracting surfaces for optical lenses or surfaces for total internal reflection that broadens the opportunities for integrating micro-optical systems into the LIFs. A key objective in this direction is the etching of optically smooth interfaces that will otherwise cause large optical scattering loss [105] when probed by light or increase the Reynolds number to disturb the laminar fluid flow inside the channel [106]. Atomic force microscopy imaging of the reservoir sidewall in Fig. 4.25a over a 4 4 m2 area is shown in Fig. 4.25c to reveal a small 12 nm (rms) surface roughness that corresponds to /130 local flatness for the telecommunication band. Such an optically smooth surface was anticipated from an assembly of nanograting planes over many laser pulses that were preferentially aligned perpendicularly to the writing laser’s polarization [37]. Selective control over the writing laser exposure and polarization therefore permits formation of smooth 3D microfluidic networks of various sizes [43, 102] that can further be advantageously applied to flexible 3D shaping and positioning of lenses, reflectors, resonators, and other optical components within fiber. Such micro-optical components are not otherwise available inside fused silica from traditional laser ablation or other processing techniques.

102

J.R Grenier et al.

a

b

Before Etching (SMF) Access Port Template

c

After Etching (SMF) Access Port SMF

SMF

Microcavity Template SMF Core

After Etching (Coreless) Access Coreless Port Fiber SMF

Microcavity SMF Core

Laser-Formed Waveguide Spice Plane Microcavity

Fig. 4.26 (a) Schematic of an optical resonator and access port template buried within SMF fiber before HF etching using 2D arrays of overlapping laser tracks. (b) Corresponding schematic after HF etching. (c) A similar optical resonator embedded within coreless fiber and integrated with laser-formed waveguides aligned to the optical axes of spliced SMF core waveguides

4.6.2 Optical Resonators in Optical Fiber The formation of optically smooth surfaces to shape microcavity structures inside the fiber opened the novel possibility of creating micro-optical resonators for interrogation by the core waveguide. Nanograting templates defining an optical resonator were formed by laser-scanning 2D arrays of overlapping laser tracks that connected with overlapping access channels, whose accumulative modification volume was susceptible to HF etching. Schematics of an optical resonator design formed by laser writing inside SMF is shown in Fig. 4.26 before (a) and after (b) HF etching. Optical resonators may also be embedded within coreless fiber as shown in Fig. 4.26c, where probing waveguides were laser-written to positions centered to align with the optical core waveguide when spliced to SMF. This approach offered facile integration of LIF coreless devices with light sources, spectral analyzers, and other optical devices. The optical micrograph of Fig. 4.27a shows an optical resonator embedded in SMF. However, a higher magnification image in Fig. 4.27b revealed an undesired concave etching of the channel sidewalls near the SMF core waveguide that induced strong lensing and diffraction losses across the channel. This undesired over-etching was attributed to the presence of germanium within the SMF core waveguide that has a smaller Ge-O dissociation energy of 660.3 kJ/mol relative to a 799.6 kJ/mol [11] Si-O dissociation energy, rendering germania to be more reactive to HF than silica in the chemical reactions GeO2 C 4HF > 2H 3O C CGeF 62 and S iO2C4HF > 2H 3O CCS iF 62 [107,108], respectively. Hence, laser writing of both waveguides and resonators into coreless fiber was favored for generating optically smooth resonators without undesired waveguide etching. Figure 4.27c, d, e show various optical micrographs of a 5 m wide optical resonator traversing

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

a

f

b

SMF

Etched Core

Microcavity

0 Transmission −2.5 −10

SMF Core

103

40 nm

Reflection

10 μm

dB −15 c

125 μm Coreless Fiber

d

e Coreless Fiber

Microcavity −20

Microcavity

25 μm

5 μm Top View

Side View

−25 1520 1540 1560 1580 1600

Wavelength (nm)

Fig. 4.27 (a) Optical micrograph of a 10 m wide optical resonator formed with a laser and HF etching to intersect the SMF core waveguide and (b) higher magnification view showing undesirable over-etching into the core waveguide. (c) Side view optical micrograph image with front illumination of a 5 m wide optical resonator formed in coreless fiber. (d) The probing laser-formed waveguides imaged under back illumination of the same resonator rotated by 90ı . (e) Magnified optical micrograph of the same resonator with front illumination. (f) Measured transmission (blue) and reflection (red) spectra of a similar air-filled 29 m wide resonator with expected Fabry-Perot interference fringes of 0.5 dB and 14 dB strength, respectively, and 40 nm FSR. c, d, e, and f are reproduced from [102] by permission of The Royal Society of Chemistry. © 2014 The Royal Society of Chemistry. http://dx.doi.org/10.1039/C4LC00648H

across coreless fiber between laser-formed waveguides. The waveguides terminated 5 m before the cavity sidewalls to ensure no chemical etching into the waveguide zone. Figure 4.27f shows the measured transmission and reflection spectra recorded from a similar 29 m wide air-filled microcavity that revealed the expected FabryPerot interference fringes with a 40 nm FSR. The fringe contrasts of 0.5 dB and 14 dB for transmission and reflection spectra, respectively, agree with theoretical values expected after accounting for diffraction losses across the resonator gap. This integrated device therefore demonstrates the principle to seamlessly position, size, and shape optical reflectors, beam splitters, lenses, and more advanced 3D optical components inside optical fiber with potentially low or near-theoretical insertion losses.

104

a

J.R Grenier et al.

b

SMF Fluorophore

−71

Source

dBm

−73 −75 −77

Substrate

To OSA

Source Fluorescence 510 530 550 570 590 Wavelength (nm)

Fig. 4.28 (a) Schematic of a laser-formed microchannel traversing across SMF and filled with a Rhodamine B solution. Fluorescence at 570 nm wavelength was excited by a light source centered at 535 nm wavelength that propagated along the SMF core waveguide and was recorded together with fluorescence in the (b) transmission spectrum. b is reproduced from [102] by permission of The Royal Society of Chemistry. © 2014 The Royal Society of Chemistry. http://dx.doi.org/10. 1039/C4LC00648H

4.6.3 Fluorescence and Refractive Index Sensors The potential LIF applications that can exploit the novel laser fabrication capabilities presented here are numerous and extensive and reach beyond temperature, strain, pressure, acoustic, and chemical sensing. In a first example, absorption and fluorescence sensors are demonstrated by writing a single microchannel across the core waveguide of SMF as previously shown in Fig. 4.24. The schematic of this device in Fig. 4.28a relied on capillary force to draw a solution of Rhodamine B fluorescent dye into the laser-formed channel where absorption or fluorescence could be recorded with a light source propagating along the SMF core waveguide. The spectrum in Fig. 4.28b shows an example of both the source and fluorescence light, centered at 535 nm and 570 nm wavelengths, respectively, being collected in the forward propagation direction of the channel-embedded SMF. Much improved signal to noise contrast is expected in back reflection or with a large NA collection lens focused on the channel-waveguide interaction zone. The demonstration of optical resonators in Fig. 4.27c, d, e opens the significant opportunity of refractive index sensing of fluids directly within optical fiber. As an example, a Fabry-Perot cavity embedded within coreless fiber may be used to sense the refractive index, n, of the fluid contained within the cavity by solving for n in D

2 : 2nL C

(4.10)

Here, is the Fabry-Perot’s FSR, is the center wavelength of the nearest Fabry-Perot transmission peak, and L is the Fabry-Perot’s cavity length. In order to completely fill the cavity with fluid, the rectangular-shaped interferometer design schematically shown in Fig. 4.26c was modified to reduce strong capillary forces at the 90ı corners [109]. Uninhibited fluid flow was found by tapering the access ports

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

a

105

b

Waveguide Optical Axis Fabry-Perot Cavity Coreless Fiber

Taper Access Port

Refractive Index (RIU)

1.40

L = 27.2 μm

1.35

ISopropanol Acetone

1.30 1.25 1.20 1.15 1.10

Methanol Air

1.05 1.00 32

34 36 38 40 42 44 Free Spectral Range (nm)

Fig. 4.29 (a) Optical micrographs of a Fabry-Perot resonator with L D 27:2 m optical length and 45ı tapered access ports. (b) Plot of refractive index values measured for various alcohols and air against the recorded FSR of the resonator cavity for D 1:575 m wavelength together with the calculated refractive index (dashed curve). Reproduced from [102] by permission of The Royal Society of Chemistry. © 2014 The Royal Society of Chemistry. http://dx.doi.org/10.1039/ C4LC00648H

to a 45ı angle to connect smoothly with a 27:2 m long Fabry-Perot resonator as shown in Fig. 4.29a. Figure 4.29b plots the results of refractive index measurements of the resonator filled with air, methanol, acetone, and isopropanol, obtained from Eq. 4.10 for L D 27:2 m and D 1:575 m. The values are plotted against the measured FSR and agree with the refractive index values expected near this telecommunication wavelength [110]. Consideration of the present 0.5 nm resolution of the Fabry-Perot resonance in reflection together with a maximum 43 nm/RIU sensitivity calculated by differentiating Eq. 4.10 with respect to n leads one to find a minimum refractive index resolution of 0.01 for the present device. Alternatively, a better value of minimum detectable refractive index change of 3 104 is available by directly measuring the wavelength shift for a single resonance peak that follows a calculated 1:58 m=RIU sensitivity near the 1:575 m wavelength. Such detection level is attractive for refractive index sensing in a compact in-fiber platform that benefits from low-cost packaging to connect with optical sources and detectors.

4.6.4 Summary This section provided several demonstrations of 3D femtosecond laser writing of waveguides and open structures inside SMF and coreless optical fibers. The formation of overlapping laser modification tracks and subsequent HF etching provided facile means to position, size, and shape various optically smooth microfluidic and optical components that may now be probed by the core waveguide of SMF or

106

J.R Grenier et al.

further integrated with laser-formed optical devices previously described throughout Sect. 4.3 to Sect. 4.5 of this chapter. Representative examples of 3D microfluidic networks in Fig. 4.23, intersecting microholes in Fig. 4.24, microfluidic reservoirs in Fig. 4.25, optical resonators in Fig. 4.27, fluorescence detectors in Fig. 4.28, and refractometers in Fig. 4.29 collectively verified that femtosecond laser writing can be a powerful tool for LIF development. The new directions provide for combination of 3D microfluidic networks and optical resonators with optical waveguides to form novel optical sensing systems conveniently inside optical fiber. Such new LIF concepts will be important for various academic, acoustic, aerospace, automotive, biological, chemical, civil, industrial, and medical applications.

4.7 Summary and Future Outlook The many examples presented in this chapter show how femtosecond laser writing offers a new opportunity for the dense 3D integration of optical devices inside optical fibers. This integration approach overcomes the many challenges and costs of otherwise connecting and packing optical fibers with discrete bulk optics. The chapter first addressed the challenge of aberration-free writing of optical circuits to accurate positions .˙1 m/ inside the cylindrical fiber core and cladding by introducing a high numerical aperture oil-immersion writing technique (Sect. 4.2). In this way, femtosecond laser-formed X-couplers, S-bend couplers, and directional couplers were shown to provide efficient optical connection between the SMF core and the laser-formed cladding waveguides (Sect. 4.3) that underpinned the development of cladding photonics. One may consider moderately efficient (32 %) and low loss (0.2 dB) directional couplers that are available over a narrow spectral band (73 nm) or trade for broadband coupling .> 350 nm/ in X-couplers and S-bend couplers with efficiencies up to 76 % and 33 %, respectively, at the cost of higher losses (1–1.7 dB). The polarization-dependent coupling encountered in the directional couplers was harnessed to fabricate in-fiber polarization-selective taps in SMF and polarization beam splitters in coreless fibers, which were introduced as an alternative platform for symmetric coupling between the laser-written structures. These couplers together with cladding waveguides and BGW devices were combined to form a Mach-Zehnder interferometer in SMF and a temperaturecompensated fiber-optic 3D shape sensor in coreless fiber (Sect. 4.4.3). The overall compactness and high integration of such devices opens opportunities for structural and industrial sensing applications as well as for integration in biomedical and catheter devices. Femtosecond laser writing of stressing tracks was found (Sect. 4.5) to induce a controllable waveguide birefringence up to a maximum value of 2 103 , thereby opening a new means of integrating quarter-wave and half-wave plates in short fiber segments. This birefringence tuning, together with the polarizationdependent couplers presented in Sect. 4.3, defines a solid grounding where more

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

107

complex integrated, in-fiber polarimeters and polarization-sensitive optical circuits can be constructed for polarization phase-shift keying in optical communication and applications in quantum optics. Femtosecond laser irradiation with chemical etching was extended into the fiber to form 3D microfluidic networks, components, reservoirs, and micro-optical resonators with optically smooth sidewall roughness in flexible geometries that were efficiently probed by laser-formed waveguides. A fluorescence detector and optofluidic refractive index sensor were demonstrated (Sect. 4.6), thereby opening the prospects for more advanced lab-in-fiber concepts and complex laboratory-level diagnostics attractive as a compact and flexible optical fiber platform for academic, aerospace, chemical, and biomedical applications. As femtosecond lasers are becoming more reliable, lower cost, and more powerful, their prospects for manufacturing more advanced products continue to strengthen in a broad range of applications. The remarkable advantage of the 3D fabrication of optical and optofluidic microsystems is especially promising on which femtosecond lasers are well poised to greatly enhance the functionality of optical fibers, one of the most widely used optical platforms, and pave the way for powerful new research tools, commercial products, and biomedical devices.

References 1. Corning. There’s Strength in Numbers. http://www.corning.com/news_center/features/ billion/index.aspx/. Accessed September 1, 2013 2. J.I. Peterson, G.G. Vurek, Science 224(4645), 123 (1984) 3. B.S. Kawasaki, K.O. Hill, R.G. Lamont, Opt. Lett. 6(7), 327 (1981) 4. K.O. Hill, Y. Fujii, D.C. Johnson, B.S. Kawasaki, Appl. Phys. Lett. 32(10), 647 (1978) 5. R. Kashyap, Fiber Bragg Gratings (Academic Press, New York, 1999) 6. A. Kersey, M. Davis, H. Patrick, M. Leblanc, K. Koo, C. Askins, M. Putnam, E. Friebele, J. Lightwave Technol. 15(8), 1442 (1997) 7. M. Consales, A. Ricciardi, A. Crescitelli, E. Esposito, A. Cutolo, A. Cusano, ACS Nano 6(4), 3163 (2012) 8. J. Ma, A. Kos, W.J. Bock, X. Li, H. Nguyen, Z.Y. Wang, A. Cusano, J. Lightwave Technol. 30(8), 1127 (2012) 9. A. Chryssis, S. Lee, S. Lee, S. Saini, M. Dagenais, IEEE Photon. Technol. Lett. 17(6), 1253 (2005) 10. S. Pevec, D. Donlagic, Opt. Exp. 19(16), 15641 (2011) 11. Y. Gong, Y. Rao, Y. Guo, Z. Ran, Y. Wu, IEEE Photon. Technol. Lett. 21, 1725 (2009) 12. A. Vengsarkar, P. Lemaire, J. Judkins, V. Bhatia, T. Erdogan, J. Sipe, J. Lightwave Technol. 14(1), 58 (1996) 13. Y. Wang, D.N. Wang, M. Yang, W. Hong, P. Lu, Opt. Lett. 34(21), 3328 (2009) 14. Y. Liu, S. Qu, Y. Li, Opt. Lett. 38(3), 335 (2013) 15. D. Qian, E. Ip, M.F. Huang, M.J. Li, A. Dogariu, S. Zhang, Y. Shao, Y.K. Huang, Y. Zhang, X. Cheng, Y. Tian, P. Ji, A. Collier, Y. Geng, J. Linares, C. Montero, V. Moreno, X. Prieto, T. Wang, in Frontiers in Optics 2012/Laser Science XXVIII (Optical Society of America, USA, 2012), p. FW6C.3 16. G.M.H. Flockhart, W.N. MacPherson, J.S. Barton, J.D.C. Jones, L. Zhang, I. Bennion, Opt. Lett. 28(6), 387 (2003)

108

J.R Grenier et al.

17. R.R. Gattass, E. Mazur, Nat. Photonics 2(4), 219 (2008) 18. R. Osellame, G. Cerullo, R. Ramponi, Femtosecond Laser Micromachining, Topics in Applied Physics, vol. 123 (Springer, NewYork, 2012) 19. J.C. Diels, W. Rudolph, P.F. Liao, P. Kelley, Ultrashort Laser Pulse Phenomena: Fundamentals, Techniques, and Applications on a Femtosecond Time Scale, Optics and Photonics (Academic Press, New York, 1996) 20. S. Küper, M. Stuke, Appl. Phys. B 44(4), 199 (1987) 21. C. Momma, B.N. Chichkov, S. Nolte, F. von Alvensleben, A. Tünnermann, H. Welling, B. Wellegehausen, Opt. Commun. 129(1–2), 134 (1996) 22. C.B. Schaffer, A. Brodeur, N. Nishimura, E. Mazur, in Proc. SPIE 3616, 182 (1999) 23. A. Mermillod-Blondin, C. Mauclair, A. Rosenfeld, J. Bonse, I.V. Hertel, E. Audouard, R. Stoian, Appl. Phys. Lett. 93(2), 021921 (2008) 24. K.M. Davis, K. Miura, N. Sugimoto, K. Hirao, Opt. Lett. 21(21), 1729 (1996) 25. Y. Cheng, K. Sugioka, M. Masuda, K. Shihoyama, K. Toyoda, K. Midorikawa, Opt. Exp. 11(15), 1809 (2003) 26. H. Zhang, S.M. Eaton, P.R. Herman, Opt. Lett. 32(17), 2559 (2007) 27. S. Eaton, W. Chen, L. Zhang, H. Zhang, R. Iyer, J. Aitchison, P. Herman, IEEE Photonics Technol. Lett. 18(20), 2174 (2006) 28. K. Minoshima, A. Kowalevicz, E. Ippen, J. Fujimoto, Opt. Exp. 10(15), 645 (2002) 29. R. Osellame, S. Taccheo, M. Marangoni, R. Ramponi, P. Laporta, D. Polli, S.D. Silvestri, G. Cerullo, J. Opt. Soc. Am. B: Opt. Phys. 20(7), 1559 (2003) 30. W. Watanabe, Y. Note, K. Itoh, Opt. Lett. 30(21), 2888 (2005) 31. J. Burghoff, C. Grebing, S. Nolte, A. Tunnermann, Appl. Phys. Lett. 89(8), 081108 (2006) 32. Y. Shimotsuma, P. Kazansky, J. Oiu, K. Hirao, Phys. Rev. Lett. 91, 247405 (2003) 33. L.A. Fernandes, J.R. Grenier, P.R. Herman, J.S. Aitchison, P.V.S. Marques, Opt. Exp. 19(19), 18294 (2011) 34. W. Cai, A.R. Libertun, R. Piestun, Opt. Exp. 14(9), 3785 (2006) 35. L. Ramirez, M. Heinrich, S. Richter, F. Dreisow, R. Keil, A.V. Korovin, U. Peschel, S. Nolte, A. Tünnermann, Appl. Phys. A 100(1), 1 (2010) 36. R. Taylor, C. Hnatovsky, E. Simova, D. Rayner, V. Bhardwaj, P. Corkum, Opt. Lett. 28, 1043 (2003) 37. C. Hnatovsky, R. Taylor, E. Simova, V. Bhardwaj, D. Rayner, P. Corkum, Opt. Lett. 30, 1867 (2005) 38. C. Hnatovsky, R. Taylor, E. Simova, P. Rajeev, D. Rayner, V. Bhardwaj, P. Corkum, Appl. Phys. A 84, 47 (2006) 39. W. Yang, E. Bricchi, P.G. Kazansky, J. Bovatsek, A.Y. Arai, Opt. Exp. 14(21), 10117 (2006) 40. R. Osellame, V. Maselli, R. Vazquez, R. Ramponi, G. Cerullo, Appl. Phys. Lett. 90(23), 231118 (2007) 41. A. Marcinkeviˇcius, S. Juodkazis, M. Watanabe, M. Miwa, S. Matsuo, H. Misawa, J. Nishii, Opt. Lett. 26(5), 277 (2001) 42. Y. Bellouard, A. Said, M. Dugan, P. Bado, Opt. Exp. 12(10), 2120 (2004) 43. S. Ho, P.R. Herman, J. Aitchison, Appl. Phys. A 106, 5 (2012) 44. Y. Cheng, K. Sugioka, K. Midorikawa, M. Masuda, K. Toyoda, M. Kawachi, K. Shihoyama, Opt. Lett. 28(13), 1144 (2003) 45. G.M. Whitesides, Nature 442, 368 (2006) 46. R. Osellame, H. Hoekstra, G. Cerullo, M. Pollnau, Laser Photon. Rev. 5(3), 442 (2011) 47. B.B. Xu, Y.L. Zhang, H. Xia, W.F. Dong, H. Ding, H.B. Sun, Lab Chip 13, 1677 (2013) 48. K. Zhou, Y. Lai, X. Chen, K. Sugden, L. Zhang, I. Bennion, Opt. Exp. 15(24), 15848 (2007) 49. H. Fu, K. Zhou, P. Saffari, C. Mou, L. Zhang, S. He, I. Bennion, IEEE Photon. Technol. Lett. 20(19), 1609 (2008) 50. K. Zhou, L. Zhang, X. Chen, V. Mezentsev, I. Bennion, Int. J. Smart Nano Mater. 1(4), 237 (2010) 51. K. Zhou, Z. Yan, L. Zhang, I. Bennion, Opt. Exp. 19(12), 11769 (2011)

4 Femtosecond Laser Inscription of Photonic and Optofluidic Devices in Fiber. . .

109

52. J. Thomas, E. Wikszak, T. Clausnitzer, U. Fuchs, U. Zeitner, S. Nolte, A. Tünnermann, Appl. Phys. A 86(2), 153 (2007) 53. A. Martinez, M. Dubov, I. Khrushchev, I. Bennion, Electron. Lett. 40(19), 1170 (2004) 54. G.D. Marshall, R.J. Williams, N. Jovanovic, M.J. Steel, M.J. Withford, Opt. Exp. 18(19), 19844 (2010) 55. J.R. Grenier, L.A. Fernandes, P.V. Marques, J.S. Aitchison, P.R. Herman, CLEO:2011-Laser Appl. Photonic Appl. 2, CMZ1 (2011) 56. L. Shah, A.Y. Arai, S.M. Eaton, P.R. Herman, Opt. Exp. 13(6), 1999 (2005) 57. S.M. Eaton, M.L. Ng, R. Osellame, P.R. Herman, J. Non-Cryst. Solids 357(13), 2387 (2011) 58. J.R. Grenier, L.A. Fernandes, J.S. Aitchison, P.V.S. Marques, P.R. Herman, Opt. Lett. 37(12), 2289 (2012) 59. K. Dolgaleva, A. Malacarne, P. Tannouri, L.A. Fernandes, J.R. Grenier, J.S. Aitchison, J. Azaña, R. Morandotti, P.R. Herman, P.V.S. Marques, Opt. Lett. 36(22), 4416 (2011) 60. J.R. Grenier, L.A. Fernandes, P.R. Herman, Opt. Exp. 21(4), 4493 (2013) 61. F.R. Adikan, C.B. Gawith, P.G. Smith, I.J. Sparrow, G.D. Emmerson, C. Riziotis, H. Ahmad, Appl. Opt. 45(24), 6113 (2006) 62. K. Minoshima, A.M. Kowalevicz, I. Hartl, E.P. Ippen, J.G. Fujimoto, Opt. Lett. 26(19), 1516 (2001) 63. F. Dürr, H. Renner, J. Lightwave Technol. 23(2), 876 (2005) 64. J.R. Grenier, L.A. Fernandes, P.R. Herman, Opt. Exp. (2013). Submitted for publication 65. A.M. Streltsov, N.F. Borrelli, Opt. Lett. 26(1), 42 (2001) 66. K. Suzuki, V. Sharma, J.G. Fujimoto, E.P. Ippen, Y. Nasu, Opt. Exp. 14(6), 2335 (2006) 67. W.J. Chen, S.M. Eaton, H. Zhang, P.R. Herman, Opt. Exp. 16(15), 11470 (2008) 68. A. Yariv, IEEE J. Quantum Electron. 9(9), 919 (1973) 69. H. Haus, W. Huang, S. Kawakami, N. Whitaker, J. Lightwave Technol. 5(1), 16 (1987) 70. L.A. Fernandes, J.R. Grenier, P.R. Herman, J.S. Aitchison, P.V. Marques, Opt. Exp. 19(13), 11992 (2011) 71. J. Thomas, N. Jovanovic, R.G. Becker, G.D. Marshall, M.J. Withford, A. Tünnermann, S. Nolte, M.J. Steel, Opt. Exp. 19(1), 325 (2011) 72. J.U. Thomas, N. Jovanovic, R.G. Krämer, G.D. Marshall, M.J. Withford, A. Tünnermann, S. Nolte, M.J. Steel, Opt. Exp. 20(19), 21434 (2012) 73. V.R. Bhardwaj, P.B. Corkum, D.M. Rayner, C. Hnatovsky, E. Simova, R.S. Taylor, Opt. Lett. 29(12), 1312 (2004) 74. L.A. Fernandes, J.R. Grenier, P.V.S. Marques, J.S. Aitchison, P.R. Herman, J. Lightwave Technol. 31(22), 3563 (2013). 75. P. Lu, Q. Chen, Opt. Lett. 36(2), 268 (2011) 76. Y. Wang, M. Yang, D. Wang, S. Liu, P. Lu, J. Opt. Soc. Am. B: Opt. Phys. 27(3), 370 (2010) 77. L. Jiang, J. Yang, S. Wang, B. Li, M. Wang, Opt. Lett. 36(19), 3753 (2011) 78. C.L. Du, Z.L. Ou, J.R. Zheng, Y.Q. Yu, P.G. Yan, J.S. Wang, X. Chen, Adv. Mater. Res. 658, 232 (2013) 79. R.G. Duncan, M.E. Froggatt, S.T. Kreger, R.J. Seeley, D.K. Gifford, A.K. Sang, M.S. Wolfe, in Proceedings of SPIE - The International Society for Optical Engineering, vol. 6530 (2007) 80. A. Fender, W.N. MacPherson, R.R.J. Maier, J.S. Barton, D.S. George, R.I. Howden, G.W. Smith, B.J.S. Jones, S. McCulloch, X. Chen, R. Suo, L. Zhang, I. Bennion, IEEE Sens. J. 8(7), 1292 (2008) 81. K.K. Lee, A. Mariampillai, M. Haque, B.A. Standish, V.X.D. Yang, P.R. Herman, Opt. Exp. (2013). Accepted for publication 82. K.O. Hill, G. Meltz, J. Lightwave Technol. 15(8), 1263 (1997) 83. M.A. Crisfield, Comput. Meth. Appl. Mech. Eng. 81(2), 131 (1990) 84. J. Lauzon, S. Thibault, J. Martin, F. Ouellette, Opt. Lett. 19(23), 2027 (1994) 85. M.S. van der Heiden, K.R. Henken, L.K. Chen, B.G. van den Bosch, R. van den Braber, J. Dankelman, J. van den Dobbelsteen, in SPIE Optical Systems Design, vol. 8550 (SPIE, Barcelona, 2012), pp. 85,500L–85,500L–14

110

J.R Grenier et al.

86. Y.L. Park, S. Elayaperumal, B. Daniel, S.C.R.S.C. Ryu, M.S.M. Shin, J. Savall, R.J. Black, B. Moslehi, M.R. Cutkosky, IEEE/ASME Trans. Mechatron. 15(6), 906 (2010) 87. S. Betti, G. De Marchis, E. Iannone, J. Lightwave Technol. 10(12), 1985 (1992) 88. J.L. O’Brien, A. Furusawa, J. Vuckovic, Nature Photon. 3(12), 687 (2009) 89. M. Lobino, J.L. O’Brien, Nature 469(7328), 43 (2011) 90. Z. Liu, C. Wu, M.L.V. Tse, C. Lu, H.Y. Tam, Opt. Lett. 38(9), 1385 (2013) 91. O. Frazao, C. Jesus, J.M. Baptista, J.L. Santos, P. Roy, IEEE Photon. Technol. Lett. 21(17), 1277 (2009) 92. D. Lesnik, D. Donlagic, Opt. Lett. 38(9), 1494 (2013) 93. R. Goto, R.J. Williams, N. Jovanovic, G.D. Marshall, M.J. Withford, S.D. Jackson, Opt. Lett. 36(10), 1872 (2011) 94. C.C. Willis, E. McKee, P. Böswetter, A. Sincore, J. Thomas, C. Voigtländer, R.G. Krämer, J.D. Bradford, L. Shah, S. Nolte, A. Tünnermann, M. Richardson, Opt. Exp. 21(9), 10467 (2013) 95. T. Geernaert, T. Nasilowski, K. Chah, M. Szpulak, J. Olszewski, G. Statkiewicz, J. Wojcik, K. Poturaj, W. Urbanczyk, M. Becker, et al., IEEE Photon. Technol. Lett. 20(8), 554 (2008) 96. L.A. Fernandes, J.R. Grenier, P.R. Herman, J.S. Aitchison, P.V.S. Marques, Opt. Exp. 20(22), 24103 (2012) 97. L. Sudrie, M. Franco, B. Prade, A. Mysyrowicz, Opt. Commun. 171(4–6), 279 (1999) 98. E. Bricchi, B.G. Klappauf, P.G. Kazansky, Opt. Lett. 29(1), 119 (2004) 99. Y. Shimotsuma, M. Sakakura, P.G. Kazansky, M. Beresna, J. Qiu, K. Miura, K. Hirao, Adv. Mater. 22(36), 4039 (2010) 100. D. Grobnic, S.J. Mihailov, C.W. Smelser, J. Lightwave Technol. 25(8), 1996 (2007) 101. K. Chah, D. Kinet, M. Wuilpart, P. Mégret, C. Caucheteur, Opt. Lett. 38(4), 594 (2013) 102. S. Ho, M. Haque, P.R. Herman, J. Aitchison, Opt. Lett. 37, 1682 (2012) 103. M. Haque, K.K.C. Lee, S. Ho, L.A. Fernandes and P.R. Herman, Lab Chip (2014). doi:10. 1039/C4LC00648H 104. S. Ho, Femtosecond Laser Microfabrication of Optofluidic Lab-on-a-Chip with Selective Chemical Etching. Ph.D. thesis, University of Toronto (2013) 105. F. Toigo, A. Marvin, V. Celli, N. Hill, Phys. Rev. B 15, 5618 (1977) 106. J. Taylor, A. Carrano, S. Kandlikar, Int. J. Thermal Sci. 45, 962 (2006) 107. M. Ohtsu, J. Lightwave Technol. 13, 1200 (1995) 108. C. Tuck, R. Hague, C. Doyle, Meas. Sci. Technol. 17, 2206 (2006) 109. M. Zimmermann, P. Hunziker, E. Delamarche, Mirofluid. Nanofluid. 5, 395 (2008) 110. T. Wei, Y. Han, Y. Li, H. Tsai, H. Xiao, Opt. Exp. 16, 5764 (2008)

Chapter 5

Fabrication of Channel Waveguides in Chalcogenide Glass Films by a Focused Laser Beam K. Shemesh, Yu. Kaganovskii, and M. Rosenbluh

5.1 Introduction Chalcogenide glasses (ChGs), due to their wide infrared transparency, high refractive index, and high Kerr nonlinearity, are of great interest as a waveguide material for micro optics and nonlinear optics [1]. They are also good candidates for many other applications including thermal and medical imaging, biosensing, and telecommunications [2]. Already important in optical storage disks and fibers, they are now being proposed as the basis for solid-state memory technologies. The intrinsic photosensitivity of the ChG materials has been utilized to fine-tune the effective refractive index of ChG waveguides, and thereby the resonant wavelength of micro-ring resonators [3]. ChGs are also emerging as excellent materials to fabricate nonlinear optical devices required for all-optical signal processing. ChGs are characterized by ultrafast broadband nonlinear optical response, high third-order optical nonlinearity (two to three orders of magnitude greater than that of silica), and low linear and nonlinear losses at telecommunications wavelengths [4]. Traditional fabrication techniques, which are used for large-scale production of planar optical devices, involve thermal evaporation and photolithography. For fabrication of channel waveguides in the micrometer range, high-cost fine-line patterning techniques are used currently, such as electron-beam lithography or focused-ion-beam milling [5]. In this paper, we demonstrate a simple optical method for the fabrication of micrometer-width channel waveguides in ChG films that does not require liftoff lithography. The method is based on photo-induced mass transport [6–8]—a phenomenon, which entails the redistribution of material between illuminated and dark areas under illumination of ChGs by light with a frequency at or above the band gap. This phenomenon was used for fabrication of m-size groves in the films, which formed the walls of the channel waveguides, as well as tapers and coupling

K. Shemesh • Yu. Kaganovskii • M. Rosenbluh () Department of Physics, Bar-Ilan University, Ramat-Gan 52900, Israel e-mail: [email protected] G. Marowsky (ed.), Planar Waveguides and other Confined Geometries: Theory, 111 Technology, Production, and Novel Applications, Springer Series in Optical Sciences 189, DOI 10.1007/978-1-4939-1179-0__5, © Springer ScienceCBusiness Media New York 2015

112

K. Shemesh et al.

gratings in the tapers. For our demonstration we use two ChGs: arsenic trisulfide (As2 S3 ) and arsenic selenide As10 Se90 . As2 S3 is one of the most widely studied ChGs and has been used for all-optical devices in various forms—bulk glass, optical fiber, and waveguides. As10 Se90 is known as a material, in which mass transport occurs with a highest rate compared to other arsenic selenide compositions [9]. Previously, it was shown [6, 7] that the mass flow under illumination by above bandgap light depends on the light polarization that allowed excluding effect of temperature at relatively low light intensities. In our case, however, as we use a focused optical laser beam with a waist of 0.7 m, we have a temperature rise due to light absorption in the film, so that the photo-induced mass transport occurs at elevated temperatures. The photo-induced mass transport involves electronic, atomic, and ionic processes. Though the precise links between these processes are not yet fully established, we propose here possible mechanisms and calculate kinetics of the mass redistribution.

5.2 Waveguide Design The basic design of our waveguide is a raised strip with a trapezoidal cross section produced in a 600-nm-thick As2 S3 or As10 S90 amorphous films, with input and output grating couplers (see Fig. 5.1). The ChG film and waveguide are located on a glass substrate. In order to determine the width of the waveguide, which ensures single-mode operation at the telecommunication wavelength 0 D 1.55 m, we simulated propagation of light in raised strips of different widths with the same thickness (600 nm). For the beam propagation simulations, we used RSOFT software tools (http://www. rsoftdesign.com/products.php?sub=Component+Design) that allow both the design and optimization of passive and active photonic devices for optical communications, optoelectronics, and semiconductor manufacturing. The refractive indices of the As2 S3 and As10 Se90 for 0 D 1.55 m are 2.4 and 2.7, respectively. The results of the simulations for As2 S3 are summarized in Figs. 5.2 and 5.3. Figure 5.2 shows single-mode propagation for a waveguide width of 1 m, for which the single mode maintains its shape and is not subject to any expansion or distortion while propagating along the waveguide. Figure 5.3 shows the mode

Fig. 5.1 Scheme of the waveguide design (top view)

5 Fabrication of Channel Waveguides in Chalcogenide Glass Films. . .

a

Computed Transverse Mode Profile (m=0.neff=2.104343)

b

113

Contour Map of Transverse Index Profile at Z=0

Vertical Direction (μm)

1.0

2.4

1

Y (μm)

1

0

Air As2S3

0 Glass substrate

−1

−1 −1

0

0.0

1

−1

0

Horizontal Direction (μm)

0.0

1

X (μm)

Fig. 5.2 Raised strip waveguide cross section: (a) mode analysis for 0.56 1 m2 core, singlemode operation. Colors show relative power inside and near the waveguide; (b) refractive index profile

a

c

1500

Z (μm)

1200

Z (μm)

1500

1500 Z (μm)

d

1200

1200

900

900

900

600

600

600

300

300

300 0

0

0 −2 −1 0 1 X (μm)

−1

−1 0 1 X (μm)

2

b

e

⎪E⎪ 1

1

0 1 X (μm)

⎪E⎪

0.5

0.5 0.0

0 −2.0

500.0 0.0 X (μm)

2.0

1000.0

Z (μm)

0.0 0 −1.6

775.0 0.0 X (μm)

1.6

1550.0

Z (μm)

Fig. 5.3 Mode propagation in a raised strip waveguide, 600 nm thick and variable width. (a, b) Second-order modes are developed when propagating in a 2 m width waveguide. (c) Distortion and expansion of the first-order mode when propagating in a 1.5 m width waveguide. (d, e) Single-mode propagation in a 1 m width waveguide

analysis for this case as well as waveguides of slightly larger widths. Light is directed into waveguide from an optical fiber of about 10 m in diameter using a grating coupler on the ChG surface (Fig. 5.4) and a taper. The grating area is about 10 10 m2 , and the width of the taper base is 10 m. Coupling between an

114

K. Shemesh et al.

Fig. 5.4 Grating coupler scheme

incident mode and a guided mode is possible if the grating satisfies the following Bragg condition for the first-order diffraction maximum [10]: Kin sin in C Kgrating D ˇ:

(5.1)

Here, Kin D 2/ 0 , Kgrating D 2/ƒ, ˇ D 2 neff / 0 , ƒ is the grating period, and neff is the effective refractive index. The propagation constant, ˇ, was calculated numerically, by solving the wave equation under boundary condition of the waveguide cross section (see Ref. 10, Chap. 3). To adjust the lateral diameter of the incident beam ( 10 m) to the submicrometer waveguide width without losses, we have simulated the beam propagation from the grating coupler to the waveguide using the 3D RSOFT program. We found that negligible loss along the tapering region can be attained as long as the taper length is not shorter than 100 m (Fig. 5.5). In our fabrication the coupling grating was recorded by two crossed p-polarized laser beams (see below). The desired grating period, ƒ, depends on the incident angle, in , and can be easily calculated from Eq. (5.1): ƒD

neff

0 : sin in

(5.2)

5.3 Experiments For our experiments we used 400–600-nm-thick As2 S3 and As10 Se90 amorphous films, vacuum deposited (1 105 Torr base pressure) onto a clean glass substrate. The waveguides were fabricated using a focused Ar laser beam (œ D 514 nm) with a focused waist radius w 0.7 m. The scheme of the setup used for fabrication is shown in Fig. 5.6. The laser beam passing through a half-wave plate, polarizer, and

5 Fabrication of Channel Waveguides in Chalcogenide Glass Films. . .

115

0.9 0.8 0.7

Loss

0.6

Taper length

0.5 0.4 0.3 0.2 0.1 0 0

50

100

150

200

Taper length [μm] Fig. 5.5 Calculated dependence of losses on the taper length. With a 100 m taper length the losses are 6 %

z x

y Sample stage

PC

Objective lens Screen Beam splitter Eyepiece Shutter Polarizer

Argon laser, l = 514 nm

Mirror Half-wave plate

Fig. 5.6 Scheme of setup used for waveguide fabrication

beam splitter is focused by an objective lens onto the film surface. After reflection from the surface, the “writing” laser beam goes back through the objective lens and is directed by a beam splitter and eyepiece to a screen which thus shows an image of the focused spot or the microscopic image of the waveguide drawn of the film sur-

116

K. Shemesh et al.

face, depending on the z-position of the sample. The positioning of the film in x-y-zdirections is adjusted by using three computer-controlled motors, thus drawing the necessary configuration of the waveguide, as monitored by the microscopic image. The gratings for coupling of light ( 0 D 1.55 m) between an optical fiber and the waveguide were fabricated by illumination of a selected film area by two crossing p-polarized beams. In As2 S3 the gratings were produced by an Argon laser ( D 514 nm) with the power of 150 mW in each of the beams; in As10 Se90 the gratings were written by a He–Ne laser ( D 633 nm) with a power of 12 mW in each of the crossing beams. A half-wave plate was used to rotate the polarization plane of the laser to the direction of the wave vector of the grating. The beam propagation inside the waveguide was observed by an IR camera with an IR corrected 50 objective lens having 2 cm working distance. IR light near a wavelength of 1.5 m, from a single-mode fiber-coupled tunable diode laser, was directed onto the coupling grating. For ease of unobstructed viewing, this required a relatively large angle of incidence (as well as output angle) in 60o and thus the grating period calculated from Eq. (5.2) for 0 D 1.55 m was ƒ D 1.18 m for As2 S3 and 0.8 m for As10 Se90 . To satisfy these conditions, we established appropriate angles, ˛, between the crossing beams calculated using ƒ D /2 sin(˛/2).

5.4 Results 5.4.1 Optical Spectra Typical optical transmission spectra of the ChG films are shown in Fig. 5.7. Variation of the transmission with wavelength is caused by interference in the film, and interference maxima ( k ) satisfy the condition: 2Hn D k k where H is the film thickness and k is the order of the interference. The transmission spectra allow us to calculate the refractive indices of the materials [11–13], which we have found to be in agreement with the literature.

5.4.2 Formation of Grooves Channel waveguides together with the input and output tapers and coupler areas were fabricated in one step by positioning of the sample stage by stepping motors in the x-y plane by computer control. The waveguide channels are produced between two grooves, which appear on the film surface during the motion of the stage while illuminated by the focused laser spot. The shape of the grooves defines the channel waveguide geometry. Typical AFM images of the grooves obtained in the As2 S3 films at various writing laser powers, P, and speeds are presented in Fig. 5.8. As seen, the width and the

Fig. 5.7 Transmission spectra of as-deposited As2 S3 and As10 Se90 films on a glass substrate. The film thickness (600 nm) was determined by AFM imaging

Transmission [%]

5 Fabrication of Channel Waveguides in Chalcogenide Glass Films. . . 100 90 80 70 60 50 40 30 20 10 0 300

117

As2S3 As10Se90

800

1300

1800

2300

2800

Wavelength [ nm]

Fig. 5.8 Typical AFM images of the grooves produced in As2 S3 films by various laser powers and stage speeds. (a) P D 2 mW, V D 50 m/s; (b) P D 6 mW, V D 50 m/s; (c) P D 8 mW, V D 50 m/s; (d) P D 6 mW, V D 10 m/s. Polarization is normal to the grooves

depth of the grooves increase with laser power and are inversely proportional to the stage speed. The groove becomes discontinuous (Fig. 5.8d) with a speed slower than 10 m/s due to the fact that stepping motors were used for the groove fabrication and at low speeds the dwell time at each step point becomes significantly long. In Fig. 5.9 we show typical profiles of grooves produced in the As2 S3 films under various writing laser powers and stage speeds. The groove shape and size also show a dependence on the direction of the light polarization: the walls of the grooves have larger slope when the electric vector of the linearly polarized light is normal to the forming groove direction (Fig. 5.10).

118

K. Shemesh et al.

Fig. 5.9 Typical profiles of grooves produced in As2 S3 films under various laser powers and stage speeds. (a) V D 50 m/s, powers varying from 2 to 10 mW; (b) P D 6 mW, speeds varying from 10 to 500 m/s. Polarization is normal to the grooves

This observation is important for understanding the mechanism and kinetics of the photo-induced mass transport, as discussed in the next section.

5.4.3 Channel Waveguides, Tapers, and Couplers After optimization of laser power, stage speed, and polarization direction, we were able to write channel waveguides with tapers and couplers. A typical AFM image of the channel between two adjacent grooves and the corresponding profile of the waveguide in As2 S3 film are shown in Fig. 5.11; AFM images of the taper, coupler, and input grating are shown in Fig. 5.12.

5 Fabrication of Channel Waveguides in Chalcogenide Glass Films. . .

119

Fig. 5.10 Typical profiles of grooves produced in As2 S3 films with different directions of polarization and the same power (P D 6 mW) and speed (V D 50 m/s). 1. Polarization parallel to the groove, 2. polarization normal to the groove

a

0.74 μm

Y: 29 μm

0 μm

X: 34 μm

b Z [mm]

0.6 0.4 1.3 μm

0.2 0 0

2

4

6

8

10

12

X [mm] Fig. 5.11 Typical AFM image of the channel waveguide (a) and corresponding cross section (b)

Figure 5.13 demonstrates coupling of light to the waveguide produced in As10 Se90 ChG film. To observe light input and output, we fabricated a relatively short waveguide (200 m length) with a taper of 100 m and coupler of

120

K. Shemesh et al.

Fig. 5.12 AFM images of taper (a), coupler (b), grating (c) in As2 S3 film, and waveguide in As10 Se90 film (d)

30 30 m2 . In the IR camera image, one can see the waveguide illuminated by visible light (Fig. 5.13a), by both visible and IR (Fig. 5.13b), and by IR only (Fig. 5.13c). One can see coupling of IR light (right) and an output light spot (left).

5.5 Discussion To explain results of our experiments, we have to discuss the physical mechanisms involved in the waveguide fabrication process. We concentrate on two main mechanisms: photo-induced mass transfer and mass transfer induced by temperature gradients around a moving focused writing beam.

5 Fabrication of Channel Waveguides in Chalcogenide Glass Films. . .

121

Fig. 5.13 Waveguide in As10 Se90 film seen in IR camera: (a) illumination by visible light; (b) illumination by both visible and IR light ( 0 D 1.55 m); (c) illumination by IR light only. One can see coupling IR light (right) and an output light spot (left)

5.5.1 Photo-Induced Mass Transfer Our analysis shows that the main mechanism of the mass redistribution in the ChG film is photo-induced mass transfer. As was previously shown [6], photoinduced mass transfer in As2 S3 films is directed from illuminated to dark areas. Redistribution of the film material under illumination by a focused beam leads to the formation of a rather deep pit at the center of the beam and ridges surrounding it. It is important to note that this mass transfer is not induced by thermal effects caused by light absorption, but is purely a light-induced mass transfer. As clear proof of this, it is found that the direction of the ridge formation depends on the direction of light polarization [6]. Formation of dips and ridges indicates that there is a light-induced lateral mass transfer (quasi-viscous flow) parallel to the direction of the E-vector of light. The kinetics of photo-induced mass transfer in ChG films was previously discussed [8, 14] and the rates of photo-induced variations of surface profile were calculated taking into account broken chemical bonds, photo-induced stresses, and capillary forces. We introduced photo-induced diffusion coefficients describing the mass transfer kinetics and demonstrated that the competition between stress-induced flux (towards irradiated regions of the film) and the flux induced by an increase of the bulk energy due to broken bonds (directed from irradiated to dark regions) can result in inversion of the mass transfer direction depending on the light intensity.

122

K. Shemesh et al.

Here, we calculate the shape of the profile formed under a moving focused laser beam due to photo-induced mass transfer. The amorphous As2 S3 films are photoconductive p-type semiconductors with atomic structure consisting mainly of chains with P–C and partly C–C bonds (P denotes pnictogen atom and C, chalcogen). When light with frequency at or above the bandgap interacts with the film, electron-hole pairs are generated in the interaction volume and diffuse in all directions. If a Gaussian writing beam moves along a line in the y-direction, the generation rate per unit volume can be calculated as g0 .x/ D I0 exp x 2 =w2 =Eg H;

(5.4)

where I0 exp(x2 /w2 ) is the incident intensity distribution in the x-direction, Eg is the bandgap of the film material, and H, the film thickness, is assumed small compared to ˛ 1 (˛ is the absorption coefficient), and w is the beam radius. As the electrons and holes have different mobilities, their distribution results in the formation of an internal steady-state electric field, E(x), which accelerates slower carriers and slows down faster carriers. In the As2 S3 films the mobility of holes exceeds the mobility of electrons, and thus the steady-state electric field is directed towards the center of the writing beam. Taking into account forming electric field, one can write the hole and electron currents as jp D Dp

Dp dp p eEI dx kT

jn D Dn

Dn dp Cn eE: dx kT

(5.5)

Here, e is the electron charge, n(x) and p(x) and Dn and Dp are the local concentrations and the diffusion coefficients of electrons and holes, respectively, and E(x) is the lateral electric field. The steady-state distribution corresponds to equality of electron and hole currents (jn D jp ); to satisfy the neutrality condition one can suppose n n0 D p p0 (n0 and p0 are the electron and hole concentrations without irradiation, p0 > n0 in As2 S3 ) and thus dp/dx D dn/dx. Then the steady-state electric field is ED

Dp Dn kT e pDp C nDn

(5.6)

and jp D jn D Damb

dn I dx

Damb D

.n C p/ Dn Dp : nDn C pDp

(5.7)

Here, Damb is the ambipolar diffusion coefficient [15, 16]. The distributions n(x) and p(x) can be found from the equation @n @2 n n D g0 .x/ C Damb 2 ; @t @x

(5.8)

5 Fabrication of Channel Waveguides in Chalcogenide Glass Films. . .

123

where we can put @n/@t D 0 considering a steady-state distribution. The boundary conditions are n(1) D 0, dn/dxjx D 0 D 0. The steady-state solution of Eq. (5.8) is 1=4 p 1 I0 R exp R2 =L2 n.x/ D n0 C 4 Eg LH R R x x e x=L 1 erf C C C e x=L 1 erf : (5.9) R 2L R 2L Here, L D (Damb )1/2 is the diffusion length of the carriers, is the lifetime of electrons and holes before recombination. The hole distribution can be also found from Eq. (5.9) as p(x) D p0 C n(x) n0 . After generation and redistribution, electrons and holes are localized around P and C atoms forming relatively stable configurations—valence alternation pairs (VAP), called also self-trapped excitons (STE), which can be considered as radiation C defects. Four main types of STE were found [17] to be relatively stable: P 2 –C3 , C C C C1 –C3 , P2 –P4 , or C1 –P4 (subscript shows number of bonds and superscript notes the sign of charge). Formation of these defects is accompanied by deformation and breakage of bonds and can accelerate atomic jumps compared to their thermal diffusion without irradiation [18]. This results in significant increase in the diffusion coefficients of both chalcogens and pnictides. The calculations of the forming profiles were carried out under the following assumptions: (i) The main mechanism of the mass transport is volume diffusion. This was shown [19] in experiments on flattening of surface relief gratings under homogeneous illumination by light with frequency above the bandgap. (ii) Mobile species have an effective charge, e, positive or negative, since electrons and holes are localized near defects. Both P and C atoms can be charged either C positively (such as PC 4 , C3 ) or negatively (P2 , C1 ) depending on localization of electrons or holes around them. Recent calculations [20] show that diffusion coefficients of positively charged P and C atoms are about two orders of magnitude smaller compared to those negatively charged (P 2 , C1 ), so that one C C can neglect diffusion of P4 , C3 atoms. The drift of P2 and C1 atoms does not change electroneutrality because electrons and holes diffuse much faster than the charged species and ensure the overall neutrality of the film. (iii) Diffusion coefficients of the charged species are proportional to the local density of free volumes, whose concentration depends mainly on the local concentration of radiation defects, n(x) and p(x). (iv) Lateral diffusion flux is defined as a drift of the charged species in the gradient of chemical potential, , caused by lateral electric field E, by light-induced deformation of bonds due to formation of STE, and by variation of the surface profile

K. Shemesh et al.

Fig. 5.14 Groove profile calculated under the assumption that it is produced by a light-induced mass transfer mechanism

h (nm)

124 300 200 100 0 -100 -4 -200 -300 -400 -500 -600

-3

-2

-1

0

1

2

3

4

Distance (μm)

J D

D nrI r D eE C " rn C rK kT

(5.10)

where D D cD P C (1 c)DC , c is the atomic fractures of P atoms in the ChG compound, D and D are diffusion coefficients of P P C 2 and C1 atoms with the localized electrons, " is the additional energy per atom caused by formation of radiation defects, K is the local curvature of the surface profile, and is the average atomic volume.

The normal rate of variation of the surface profile is Vz D H dJ =dx:

(5.11)

The height of the profile, h(x), was calculated as h.x/ D Vz t:

(5.12)

Here, t is the exposure time (t w/V) that equals 14 ms for w D 0.7 m and V D 50 m/s. In Fig. 5.14 we present the groove profile h(x) calculated using Maple program simulation for our experimental conditions. As a fitting parameter, we used an effective diffusion coefficients Dm corresponding to maximum carrier concentrations nm (at x D 0). As one can see, the calculated profile is very similar to that presented in Fig. 5.11 with Dm D 2.2 109 cm2 /s.

5.5.2 Temperature Rise and Thermodiffusion Mass Transfer The full theoretical analysis of the physical phenomena which cause mass transfer under focused laser light also requires knowledge of the temperature distribution in the film. This problem has been previously investigated under various approximations as applied to thin-film micromachining [21, 22] and ablative laser recording of

5 Fabrication of Channel Waveguides in Chalcogenide Glass Films. . .

125

micron size holes for optical disk storage. In these calculations, a film of thickness h and heat diffusivity f was considered on a semi-infinite transparent substrate (along the z axis) with heat diffusivity s . As in our case f s D , and the film thickness, H, is of the order of the beam waist, w, we can assume that the light energy is absorbed in the volume w2 H and is dissipated inside the substrate due to radial heat flow from a hemisphere with the radius w. We can neglect the heat conductivity of the air compared to the glass. In this case, for estimates of temperature rise, we can use a steady-state temperature distribution, T .r/ D

.Tm Troom / w ; r

(5.13)

which is formed during a characteristic time t* w2 / D [23]. Here, Tm D T(w) is the maximal temperature, Troom is the room temperature, Tm Troom is the temperature rise, D D c is the heat diffusivity, and c is the heat capacity per unit volume. With w D 0.7 m, D D 3 107 m2 /s we have t* D 1.6 s which is much shorter than the exposure time under the moving focused beam in our experiments (ti D w/V D 14 ms), and thus we can neglect the beam speed. From the heat balance ˇ d T .r/ ˇˇ Tm Troom ; D 2w2 ıP ˛PH D 2w dr ˇrDw w 2

(5.14)

we obtain Tm Troom

˛PH : 2w

(5.15)

Here, ’ is the absorption coefficient, ıP is the laser power absorbed by the film, and P is the laser power (without reflection). This result coincides with the more detailed and complicated analysis made by Lax [24] for a Gaussian beam illuminating a semi-infinite absorbing medium if ˛H D 1/2 , i.e., all of the beam power is absorbed. In our experiments, as it follows from the optical spectra (Fig. 5.7), transmission of the As2 S3 film at 514 nm is 60 % which corresponds to ˛H D 0.29. With P D 6 mW and D 1.14 J/mKs we obtain Tm Troom 300 K, i.e., Tm 600 K. This means that the maximum temperature exceeds by about 130 K the glass transition temperature Tg for As2 S3 (Tg D 471 K [25]). According to experimental data [26], the kinematic viscosity, , of As2 S3 glass above Tg follows an exponential law D 0 exp(W/kT) with the activation energy W D 1.12 eV and pre-exponent 0 D 3.98 106 St. The dynamic viscosity D calculated from these data for 600 K is 3.2 103 Pa s ( D 3.19 g/cm3 is the density of As2 S3 ). According to Eq. (5.15), the temperature near the groove decreases to Tg value at a distance

126

K. Shemesh et al.

d

Tm Troom w: Tg Troom

(5.16)

With w D 0.7 m we obtain d 1.8 m. The temperature gradient in the direction normal to the forming groove can initiate lateral motion of a liquid layer from hot to cold regions. The dynamics of lateral motion of a thin liquid layer in a temperature gradient was estimated [27] for bulk Si wafer, in which a liquid layer was formed on the surface under pulsed laser irradiation. It was shown that in the approximation of a long laser pulse when the time scale of the laser pulse, tp , is large compared to the time scale for the diffusion of fluid momentum through the thickness of the melt, i.e., tp H2 / k (H is the melt depth, and k the kinematic viscosity), the radial component of liquid velocity can be written in the form Vr D

1 d d T H: d T dr

(5.17)

As can be seen, the radial velocity is proportional to the radial temperature gradient, the thickness of the liquid layer, and the temperature coefficient of the surface tension; it is inversely proportional to the dynamic viscosity . Substituting D 3.2 103 Pa s, d /dT 2 104 J/m2 K [28], dT/dr (Tm – Tg )/d D 6 107 K/m (average value), and H 0.6 m, we obtain Vr 200 m/s, i.e., Vr is of the order of the stage velocity, V. This means that under the driving force caused by the temperature gradient, the film material can move to the cold regions forming grooves under the illuminated spot and mounds near the grooves (as can be seen in Figs. 5.9 and 5.10). According to [21], the normal component of the velocity, Vz , can be estimated as a function of r using a formula Vz .r/ D

H2 d 2r dr

d r : dr

(5.18)

Here, d /dr D (d /dT)(dT/dr), d /dT is a constant independent of T. Taking into account the temperature distribution [Eq. (5.13)], we have estimated maximum Vz value (under illuminated spot) and obtained Vzm

H 2 d Tm Troom : 2 d T d2

(5.19)

Substitution in Eq. (5.19) D 3.2 103 Pa s, d /dT 2 104 J/m2 K, and H 0.6 m results in Vzm 20 m/s. During time of interaction t w/V of the moving beam with the film, the depth of the groove is z Vzm t D 280 nm (with w D 0.7 m and V D 50 m/s). This estimate shows that there is a noticeable contribution of the thermo-induced mass transport into kinetics of the groove formation.

5 Fabrication of Channel Waveguides in Chalcogenide Glass Films. . .

127

Similar calculations for As10 Se90 films are more complicated because the transmission of the 600-nm-thick As10 Se90 film at 514 nm is 1.1 %, i.e., ˛H 4.5. With a power P D 3 mW this results Tm Troom 2,500 K, and in the calculations one should take into account possible evaporation (ablation) of the material. In addition, we didn’t find in the literature any data about viscosity and other characteristics at such high temperatures. The shapes of the grooves however look similar to those for As2 S3 films (see Fig. 5.12d).

5.6 Concluding Remarks We have demonstrated a simple optical method for fabrication of single-mode channel waveguides in ChG films. All elements of the waveguides (couplers, tapers, and channels) can be easily fabricated using illumination by a focused visible laser beam (without wet or plasma etching) and two-beam illumination of selected areas to produce gratings used for coupling. We have also proposed physical mechanisms for the phenomena: photo-induced mass transfer and mass transfer caused by temperature gradients appearing near fabricated grooves due to light absorption. We have calculated the kinetics of the photo-induced mass transfer and found good agreement between experimental and calculated shapes of groove profiles. We note that under intense illumination of As2 S3 films during the waveguide fabrication, surface scattering becomes stronger due to increasing surface roughness and some additional experiments are necessary to optimize the waveguide fabrication process in order to minimize the contribution of scattering to the device losses. One of the ways to decrease the loss can be a thermal treatment of asdeposited As2 S3 films before waveguide fabrication. As was recently reported [29] thermal annealing improves the homogeneity of as-deposited film and reduces the propagation loss of As2 S3 waveguides. As10 Se90 films are much more stable under illumination and no additional roughness appears under laser processing. Acknowledgments This work was supported by the Israel Science Foundation (Grant # 894/10).

References 1. A. Greer, N. Mathur, Nature 437, 1246 (2005) 2. P. Lucas, J. Phys. Condens. Matter 18, 5629 (2006) 3. N. Carlie, J.D. Musgraves, B. Zdyrko, I. Luzinov, J. Hu, V. Singh, A. Agarwal, L.C. Kimerling, A. Canciamilla, F. Morichetti, A. Melloni, K. Richardson, Opt. Express 18, 26728 (2010) 4. R.G. DeCorby, N. Ponnampalam, M.M. Pai, H.T. Nguyen, P.K. Dwivedi, T.J. Clement, C.J. Haugen, J.N. McMullin, S.O. Kasap, IEEE J. Sel. Top. Quant. Electron. 11, 539 (2005)

128

K. Shemesh et al.

5. J. Hu, N. Carlie, N. Feng, L. Petit, A. Agarwal, K. Richardson, L. Kimerling, Opt. Lett. 33, 2500 (2008) 6. A. Saliminia, T.V. Galstian, A. Villeneuve, Phys. Rev. Lett. 85, 4112 (2000) 7. M.L. Trunov, P.M. Lytvyn, P.M. Nagy, O.M. Dyachyns’ka, Appl. Phys. Lett. 96, 111908 (2010) 8. Y. Kaganovskii, D.L. Beke, S. Kökényesi, Appl. Phys. Lett. 97, 061906 (2010) 9. M.L. Trunov, P.M. Nagy, V. Takats, P.M. Lytvyn, S. Kokenyesi, E. Kalman, J. Non-Cryst. Solids 355, 1993 (2009) 10. A. Yariv, P. Yeh, Photonics: Optical Electronics in Modern Communications, 6th edn. (Oxford University Press, New York, Oxford, 2007) 11. N.J. Harrick, Appl. Optics 10, 2344 (1971) 12. R. Swanepoel, J. Phys. E Sci. Instrum. 16, 1214 (1983) 13. J.A. Pradeep, P. Agarwal, J. Appl. Phys. 108, 043515 (2010) 14. Y. Kaganovskii, D.L. Beke, S. Charnovych, S. Kökényesi, M.L. Trunov, J. Appl. Phys. 110, 063502 (2011) 15. W. Roosbroeck, Phys. Rev. B 91, 282 (1953) 16. C. Thomas, I. Joachimsthaler, R. Heiderhoff, L.J. Balk, J. Phys. D Appl. Phys. 37, 2785 (2004) 17. S.R. Elliott, J. Non-Cryst. Solids 81, 71 (1986) 18. H. Fritzsche, Semiconductors 32, 850 (1998) 19. Y. Kaganovskii, M.L. Trunov, D.L. Beke, S. Kökényesi, Mater. Lett. 66, 159 (2011) 20. M.L. Trunov, C. Cserhati, P.M. Lytvyn, Y. Kaganovskii, S. Kökényesi, J. Phys. D Appl. Phys. 46, 245303 (2013) 21. U.C. Paek, A. Kestenbaum, J. Appl. Phys. 44, 2260 (1973) 22. S.Y. Suh, D.L. Anderson, Appl. Optics 23, 3965 (1984) 23. H.S. Carslaw, J.C. Jaeger, Conduction of Heat in Solids (Oxford University Press, New York, 1954) 24. M. Lax, J. Appl. Phys. 48, 3919 (1977) 25. K. Tanaka, K. Shimakawa, Amorphous Chalcogenide Semiconductors and Related Materials (Springer, New York, 2011) 26. G. Chaussemy, J. Fornazero, J.-M. Mackowski, J. Non-Cryst. Solids 58, 219 (1983) 27. T. Schwarz-Selinger, D.G. Cahill, S.-C. Chen, S.-J. Moon, C.P. Grigoropoulos, Phys. Rev. B 64, 155323 (2001) 28. V. Kolevzon, J. Exp. Theor. Phys. 87, 1105 (1998) 29. D.-Y. Choi, S. Madden, D. Bulla, R. Wang, A. Rode, B. Luther-Davies, J. Appl. Phys. 107, 053106 (2010)

Chapter 6

Laser Processed Photonic Devices Jerome Lapointe and Raman Kashyap

6.1 Introduction The last century was that of electronics; it is now one of photonics. As Richard Feynman (Nobel Prize, 1965) suggested in 1959, “Smaller, Faster, Cheaper” would lead the world, and in many ways he has proven to be correct. Over the past decades, photonics devices and integrated optics have been among the most revolutionary areas of research and advances. Although integrated optics devices are well advanced these days, there is still much to do and most of these components are still expensive to manufacture for mass deployment. In fact, most of these require clean room facilities, as well as several expensive manufacturing steps such as phase mask fabrication or photolithography. This chapter aims at explaining a potential solution to fast manufacturing of cheap integrated optics by laser writing. The interactions between lasers and transparent materials, including nonlinear absorption and the origin of refractive index modification, are initially explained. Furthermore, an entire section is dedicated to waveguide fabrication using lasers. Some analyzing techniques and tools are also presented. However, the chapter focuses on two important photonic materials: glass and lithium niobate. Nevertheless, all demonstrations and explanations can be generalized to most linear and nonlinear transparent materials, which will be showcased throughout the chapter.

J. Lapointe Fabulas Laboratory, Department of Engineering Physics, Polytechnique Montreal, Montreal, QC, Canada H3C 3A7 e-mail: [email protected] R. Kashyap () Fabulas Laboratory, Department of Electrical Engineering, Polytechnique Montreal, Montreal, QC, Canada H3C 3A7 Fabulas Laboratory, Department of Engineering Physics, Polytechnique Montreal, Montreal, QC, Canada H3C 3A7 e-mail: [email protected] G. Marowsky (ed.), Planar Waveguides and other Confined Geometries: Theory, 129 Technology, Production, and Novel Applications, Springer Series in Optical Sciences 189, DOI 10.1007/978-1-4939-1179-0__6, © Springer ScienceCBusiness Media New York 2015

130

J. Lapointe and R. Kashyap

Finally, fabrication of photonic devices using laser ablation is also addressed in the last section, as an alternative technique for making specialist prototyping devices.

6.2 Nonlinear Energy Absorption of fs Laser Pulses When a femtosecond laser pulse is incident on a transparent material with an energy gap Eg larger than the energy of the photon emitted by the laser, there is no possibility for linear absorption. However, if the intensity is sufficiently high, absorption can occur via nonlinear effects such as multiphoton ionization and tunnel or avalanche ionization.

6.2.1 Multiphoton Ionization The ionization of an electron by multiple photons requires the simultaneous absorption of m photons of energy hv, where m is the smallest possible integer for which the total energy is sufficient to ionize an electron (mh > Eg , as shown in Fig. 6.1). Many photons are required to excite a single electron into the conduction band, because of the transparent materials’ large bandgap such as in LN.

6.2.2 Tunnel Ionization Tunnel ionization occurs when a laser impulse creates an intense electric field that reduces the Coulomb potential energy barrier, therefore allowing an electron to jump from the valence band to the conduction band. An important deformation of the material band structure promotes this ionization because of the intensity of the generated electric field. Under very high intensities, the aforementioned multiphoton and tunnel ionizations compete with each other, with the former gaining the upper hand in most interactions between fs lasers and dielectrics [1–4].

Fig. 6.1 Multiphoton ionization principle

6 Laser Processed Photonic Devices

131

Fig. 6.2 Avalanche ionization principle. Variation (solid arrows) and transfer (dashed arrows) of electrons energy

6.2.3 Avalanche Ionization This nonlinear ionization occurs when an electron, free at the bottom of the conduction band and exposed to an intense photon field, is accelerated and acquires substantial kinetic energy. When the total amount of energy surpasses the sum of the conduction band’s minimal gap energy, an electron can ionize another electron at the valence band. Both can now be accelerated in the electric field, henceforth causing an avalanche where the free electron density in the conduction band increases exponentially (see Fig. 6.2). When this density reaches a certain threshold, the dielectric becomes locally absorbent. With the intensity of fs laser pulses, avalanche ionization is negligible in comparison to multiphoton and tunnel effect ionizations. However, this ionization effect is the only option for ionization when the laser intensity is too low for the two other effects described above. As such, avalanche ionization is preferred when materials present impurities and dislocations. Depending on the type of defect present in a crystal, the significance of the avalanche effect can be increased, as the electrons could be at intermediate levels [3–5].

6.3 High and Low Repetition Rate Writing Regimes Nonlinear absorption in transparent materials occurs at intensities in the vicinity of 1013 W/cm2 , which for an impulse of 100 fs corresponds to energy densities of about a J/cm2 [5]. Such energy densities can be attained with the help of lasers, namely that of the Ti:Sapphire, with impulses of Js to tens of nJ (depending on the focus diameter, also called beam waist) and by varying the laser scan speed or repetition rate. The repetition rate of a laser is the number of pulses per second emitted by the laser. There are two distinct repetition rate regimes for fs laser writing: high and low. These regimes are characterized by the critical repetition rate at which the impulsion period is different than the time required for the diffusion of heat outside the focal volume. The critical repetition rates required range from kHz to MHz depending on the material’s thermal diffusivity.

132

J. Lapointe and R. Kashyap

This is precisely the reason why it is very difficult to write a waveguide by changing the refractive index at the focal point using a continuous wave (CW) laser such as with a CO2 laser. The laser can reach energies needed to be nonlinearly absorbed but energy accumulation is too high, which in turn results in internal cavitation or direct material ablation. However, CW lasers can be used to fabricate buried waveguide using photosensitivity of the material [6]. The latter is outside the scope of this chapter; however, waveguides also may be formed in thin films by ablation [7–12], as discussed in Sect. 6.11.

6.4 Two Types of Induced Index Modification To date, two concepts for index modification have been used for waveguide fabrication. Both can be adequately described within the framework of induced lattice defects [13]. In type I, which occurs at lower energies, heat accumulation at the focus induces a fast state transformation from the crystalline to the amorphous state. This results in stress that can increase the refractive index locally. The waveguide is therefore produced in the focal region of the laser [14]. This type of index modification produces good quality waveguides [15] but disappears at temperatures of over 150 ı C in a matter of hours [13, 14]. In type II, laser interactions result in a decrease in the refractive index. The waveguide is therefore produced in the region adjacent to the interaction volume. A simple method to produce these types of waveguides is to write multiple parallel lines; the guiding thus occurs between these lines [13, 16]. For this type of waveguide, the index modification occurs because of the photorefractive effect, which is naturally present in LN [17]. The effect consists of inducing a noninstantaneous and nonlocal refractive index variation in the crystal with laser illumination. This variation is due to the combination of multiple effects created by impurities that can be optically ionized. For example, in lithium niobate the most photoreactive impurities are Fe, Cu, and Mn. The beam ionizes these impurities, which can then move inwards in the crystal via charge transport mechanisms such as conduction band diffusion, with photovoltaic current and forces generated by the external field [18]. In LN, this photo-induced transport is principally linked to photovoltaic currents. These currents carry charges from illuminated areas to darker regions, which increases density, therefore increasing the index as well. Recently, waveguide writing inside an LN fiber using this principle combined with a vortex beam has proven successful [19].

6 Laser Processed Photonic Devices

133

6.5 Basic Steps for Fabricating Waveguides in Transparent Material Using a fs Pulse Laser and Analyzing Methods Fabricating waveguides using a femtosecond pulse laser is quick and simple. A laser beam with a power of 1 W (average), a focusing lens, and a translation stage are the three basic components required (shown in Fig. 6.3). Several variables can be controlled for laser beam, such as power, polarization, beam diameter, beam focus shape, etc., in order to produce an automated highquality waveguide writing system. Figure 6.4 shows the setup used at our FABULAS Laboratory located at Polytechnique Montreal, in Montreal, Canada. The laboratory includes ten different lasers that can be switched towards the sample. The most used laser for waveguide writing, the one seen on the picture, is a Pharos Altos at 1,030 nm (power 8 W, repetition rate from 1 to 600 kHz, pulse width from 50 to 300 fs). The setup includes a beam expander, shutter, half-wave plate, a beam splitter, and a power meter with feedback to automatically and precisely control the laser power. Before the focusing lens, apparatus, such as quarter-wave plates, can be added (or removed quickly using magnetic kinematic stages) to control the polarization of the laser beam. Finally, a high-precision, two-axis, horizontal motorized stage moves the sample and the vertical axis controls the lens position in order to minimize vibrations transmitted to the sample. The setup is mounted on a heavy granite block installed on a pneumatic optical table to further reduce vibrations. The whole setup is inside a HEPA filter system under a slight positive pressure to minimize dust accumulation. An extractor removes debris, should this be necessary.

6.5.1 Laser Beam Alignment, Polarization, and Shaping of the Laser Focus A perfect focusing shape is crucial to fabricate high-quality waveguides repeatably. First, the laser beam must have a symmetrical Gaussian shape, which is usually the case with commercial lasers. One can measure the beam profile using a CCD

Fig. 6.3 Waveguide fabrication

134

J. Lapointe and R. Kashyap

Fig. 6.4 The FABULAS laser fabrication system. 1. Femtosecond laser. 2. Beam expander. 3. Motorized half-wave plate. 4. Beam splitter acting as a polarizer. 5. Feedback power meter. 6. Shutter. 7. Quarter-wave plate. 8. Focusing lens installed on a motorized vertical stage. 9. Vacuum sample holder installed on a motorized horizontal 2-axis stage. The white lines show the beam path

camera or the knife-edge technique. Second, the beam must be right in the center and parallel to the axis of the focusing lens. This alignment can be long and arduous.

6 Laser Processed Photonic Devices

135

Fig. 6.5 (a) Beam evolution near the focus not using a slit, (b) energy distribution in YZ plane not using a slit, (c) beam evolution near focus using a slit, (d) energy distribution in YZ plane using a slit, and (e) schematic of a waveguide writing setup using cylindrical lenses. Adapted from [22, 23]

Note that in complex systems in which different lasers with different wavelengths are used, the mirrors must be changed every time and a good alignment method is essential. The polarization of the laser beam also affects the waveguide. Using a halfwave plate, one can choose the polarization to be parallel or perpendicular to the waveguide direction. A polarization perpendicular to the waveguide direction will produce a highly polarization-dependent waveguide while one parallel to the waveguide direction will produce a polarization-independent waveguide for linear propagation. As one of the advantages of using a laser to fabricate waveguides is to make 3D waveguides, the best way to make uniform waveguides independent to the direction of writing is to choose circular polarization with a quarter-wave plate. Unfortunately, at low repetition rates, even if we have a perfect beam with a perfectly symmetric shape of the spot at the focus as shown in Fig. 6.5a, the waveguide will not be symmetric. In fact, as shown in Fig. 6.5b, the waveguide size perpendicular to the laser beam along the y-axis will be about the size of the beam waist, as there is no energy outside of this area. Otherwise, parallel to the laser beam (z-axis), the waveguide size will be larger, as seen in the equation for the confocal parameter b D 2 ¨0 2 /œ. It was noticed, as shown on Fig. 6.6, that the number of scans influences the waveguides to become more symmetric. This phenomenon may be explained by the fact that multi-scans reduce the probability of irregularities that occur when performing a single scan. Nevertheless, several methods can be used to overcome this nonsymmetrical issue efficiently. Firstly, without the use of other devices, one can simply make the waveguide cross-section shape required by using several scans in which each scan is displaced slightly from the previous one [20]. This method,

136

J. Lapointe and R. Kashyap

Fig. 6.6 Microscope images of the end view (sample facet) of the waveguides, showing the tendency of waveguides to be symmetric by increasing the number of scans. Each column is for a scan speed noted at the top. The number of scan is noted at the bottom left corner of each picture

although efficient, multiplies the time it takes to fabricate waveguides and can generate complications when one wants to fabricate 3D waveguides or other complex devices. A second way is to use cylindrical lenses, which generate an elliptic beam just before the focusing lens, as shown in Fig. 6.5 [21, 22]. In addition, a quick and very effective solution is to introduce a slit of width about 500 m just before the focusing lens [23, 24]. After focusing, the beam shape generated by these two last solutions can be seen in Fig. 6.5c, d. Again, these two solutions are very good for straight waveguides but need to be motorized for 3D writing as the slit or the axes of the cylindrical lenses must remain parallel to the waveguide. This proves to be rather complex. At high repetition rates, this nonsymmetrical issue disappears, thanks to the isotropic heat diffusion out of the focal volume [25–27]. In fact, a circular symmetry of the waveguide cross section is achievable due to heat accumulation, which makes the waveguide larger than the focal point. Typically, the waveguide diameter increases with the repetition rate of the laser and can be up to ten times the focal diameter 2¨0 of the laser, 2¨0 D 4œF= D;

(6.1)

where œ is the wavelength of the laser, F is the focal length, and D is the beam diameter before the lens, as shown in Fig. 6.7.

6 Laser Processed Photonic Devices

137

Fig. 6.7 Laser-focusing parameters

The choice of the lens is therefore extremely important. The numerical aperture (NA) of the lens must be chosen and understood properly, as NA D n sin ™ D n D=2F

(6.2)

2¨0 D 2œn= NA

(6.3)

where n D 1 is the refractive index (if immersion oil is not used) of air. A beam expander can be used to match the lens diameter and then obtain the full NA of the lens. If the beam is larger than the lens, the power below the lens must be verified. When one wants to reproduce an experiment, the beam size must be considered. For example, in Table 6.1, Minoshima used a 100 magnification lens which has an NA typically above 1, but because of the use of a smaller beam diameter, this NA becomes 0.6 [26].

6.5.2 Analyzing Methods The physical properties and propagation efficiency are essential characteristics to be analyzed in order to understand guiding failures and to improve a waveguide. In this section, we explain some of the basic waveguide characterization methods. Note that several other specific characteristics can be also analyzed as far as waveguides are concerned. For example, Raman scatterings can provide information on deformation and strain in a waveguide [28].

Study (et al.) Davis (1996) [34] Davis (1996) [34] Hirao (1998) [44] Schaffer (2001) [25] Minoshima (2001) [26] Streltsov (2002) [4] Will (2002) [125] Cerullo (2002) [21] Osellame 2004 [126] Eaton (2005) [127] Ams (2005) [23]

œlaser (nm) 810

1

790

120

1

Phosphate

800

375

300

150

120

30

Borosilicate 1,045 1,000

1,040 166

1

800

Fused silica Er:Ybdoped

Er:Ybdoped

80,000

Borosilicate 400

100

25,000

80

120

200

4,000

120

200

470

Average power (mW) 470

1,500

520 1.5

520

448

0.04

15

0.1

–

Few J Few

270

0.025

Few J Few

10

20

0.01

80

125

0.02

0.1

1

1

1

1

1

1

1

1

10

10

Scan speed # of (mm/s) scans 0.1 1

160

2

20

5

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close